# 10. Appendix

### You also want an ePaper? Increase the reach of your titles

YUMPU automatically turns print PDFs into web optimized ePapers that Google loves.

<strong>Appendix</strong> A:<br />

Pioneers of Semiconductor Physics Remember...<br />

Semiconductor physics has a long and distinguished history. The early developments<br />

culminated in the invention of the transistor by Bardeen, Shockley,<br />

and Brattain in 1948. More recent work led to the discovery of the laser diode<br />

by three groups independently in 1962. Many prominent physicists have contributed<br />

to this fertile and exciting field. In the following short contributions<br />

some of the pioneers have recaptured the historic moments that have helped<br />

to shape semiconductor physics as we know it today. They are (in alphabetical<br />

order):<br />

Elias Burstein<br />

Emeritus Mary Amanda Wood Professor of Physics,<br />

University of Pennsylvania, Philadelphia, PA, USA.<br />

Editor-in-chief of Solid State Communications 1969–1992;<br />

John Price Wetherill Medal, Franklin Institute 1979;<br />

Frank Isakson Prize, American Physical Society, 1986.<br />

Marvin Cohen<br />

Professor of Physics, University of California, Berkeley, CA, USA.<br />

Oliver Buckley Prize, American Physical Society, 1979;<br />

Julius Edgar Lilienfeld Prize, American Physical Society, 1994.<br />

Leo Esaki<br />

President, Tsukuba University, Tsukuba, Japan.<br />

Nobel Prize in Physics, 1973.<br />

Eugene Haller<br />

Professor of Materials Science and Mineral Engineering,<br />

University of California, Berkeley, CA, USA.<br />

Alexander von Humboldt Senior Scientist Award, 1986.<br />

Max Planck Research Award, 1994.<br />

Conyers Herring<br />

Professor of Applied Physics, Stanford University, Stanford, CA, USA.<br />

Oliver Buckley Prize, American Physical Society, 1959;<br />

Wolf Prize in Physics, 1985.<br />

P.Y. Yu, M. Cardona, Fundamentals of Semiconductors, Graduate Texts in Physics, 4th ed.,<br />

DOI <strong>10.</strong>1007/978-3-642-00710-1, © Springer-Verlag Berlin Heidelberg 2010

554 <strong>Appendix</strong> A<br />

Charles Kittel<br />

Emeritus Professor of Physics, University of California, Berkeley, CA, USA.<br />

Oliver Buckley Prize, American Physical Society, 1957;<br />

Oersted Medal, American Association of Physics Teachers, 1978.<br />

Neville Smith<br />

Scientific Program Head, Advanced Light Source,<br />

Lawrence Berkeley Laboratory, Berkeley, CA, USA.<br />

C.J. Davisson and L.H. Germer Prize, American Physical Society, 1991.<br />

Jan Tauc<br />

Emeritus Professor of Physics and Engineering, Brown University,<br />

Providence, RI, USA.<br />

Alexander von Humboldt Senior Scientist Award, 1981;<br />

Frank Isakson Prize, American Physical Society, 1982.<br />

Klaus von Klitzing<br />

Director, Max-Planck-Institut für Festkörperforschung, Stuttgart, Germany.<br />

Nobel Prize in Physics, 1985.

Ultra-Pure Germanium 555<br />

Ultra-Pure Germanium:<br />

From Applied to Basic Research or<br />

an Old Semiconductor Offering New Opportunities<br />

Eugene E. Haller<br />

University of California, Berkeley, USA<br />

Imagine arriving one morning at the laboratory and somebody comes to ask<br />

you if single crystals of germanium with a doping impurity concentration in<br />

the 10 10 –10 11 cm 3 range can be grown! You quickly compare this concentration<br />

with the number of Ge atoms per cm 3 , which is close to 4 × 10 22 . Well,<br />

you pause and wonder how anybody can ask if a 99.999999999% pure substance<br />

can be made. The purest chemicals available are typically 6 or 7 nines<br />

pure. Robert N. Hall of the General Electric Company proposed in 1968 [1]<br />

that such crystals could be grown and that they would be most useful in fabricating<br />

very large volume (up to 400 cm 3 ) p-i-n junctions working as gammaray<br />

detectors [2].<br />

When I arrived at Berkeley as a postdoc I joined the group of F.S. (Fred)<br />

Goulding, who headed one of the leading groups of semiconductor detector<br />

and electronics experts at the Lawrence Berkeley Laboratory (LBL), then<br />

called the Radiation Laboratory. There I met W.L. (Bill) Hansen, who had<br />

started the race towards the ultra-pure Ge single-crystal goal believed to be attainable<br />

by Hall. Bill was extremely knowledgeable in chemistry, physics, and<br />

general laboratory techniques. In addition, he was the fastest-working experimentalist<br />

I had ever encountered. Somewhat overwhelmed, I started to work<br />

with Bill and Fred on these Ge crystals. When Bill tried out various Czochralski<br />

crystal growth configurations [3], he rigorously pursued ultra-purity by using<br />

the simplest crystal growth design, the purest synthetic silica (SiO2) container<br />

for the Ge melt, and hydrogen gas purified in a Pd diffusion system. I,<br />

on the other hand, tried to build up an arsenal of characterization techniques<br />

which would allow us to find out within hours the purity and crystalline perfection<br />

we had achieved. The IEEE meetings on nuclear science, which were<br />

held every fall, provided the forum where we “crossed swords” with Hall [4–<br />

7]. It was a close race. Hall had the advantage of enormous experience, which<br />

started way back when Ge was first purified and single crystals were grown<br />

for transistors. We had the advantage of blissful ignorance but also excellent<br />

and helpful colleagues. Furthermore, nobody could match Bill’s agility in trying<br />

out new purification and crystal growth methods. One major development<br />

for us was learning, through Hall, about a super-sensitive photoconductivity<br />

technique which was capable of identifying extremely small numbers of impurities<br />

in Ge single crystals. The technique had been discovered by Russian<br />

scientists at the Institute of Radio-engineering and Electronics in Moscow [8,<br />

6.85]; see Figs. 6.39 and 6.40. They found that a two-step ionization process of

556 <strong>Appendix</strong> A<br />

shallow hydrogenic donors or acceptors in a very cold crystal would lead to<br />

photoconductivity peaks which were very sharp and unique for each dopant<br />

species. Paul Richards, of the Physics Department at the University of California<br />

at Berkeley, had a home-built Fourier-transform far-infrared spectrometer<br />

and the necessary liquid helium temperature dewar. By the end of the first day<br />

of experimenting we had a spectrum of a p-type high-purity Ge crystal with<br />

only 10 10 cm 3 net amount of acceptors and we knew also that phosphorus<br />

and aluminum were the major residual impurities.<br />

In parallel with a number of novel and interesting physics studies we fabricated<br />

gamma-ray detectors at LBL. We broke records in the resolution of the<br />

gamma-ray photopeaks with our ultra-pure crystals [2]. Soon the commercial<br />

detector manufacturers became interested and started their own ultra-pure Ge<br />

crystal-pulling programs. In a few years several companies in the US and in<br />

Europe succeeded in developing large-diameter ( 8 cm) single crystals with<br />

incredibly good yield, excellent purity ( 2 × 10 10 cm 3 ) and very small concentrations<br />

(10 8 cm 3 ) of deep-level defects which would detrimentally affect<br />

the charge collection in large-size coaxial p-i-n diodes. In order to achieve the<br />

best spectral resolution, electrons and holes had to have mean-free-paths of<br />

up to several meters. Most semiconductor physicists simply shook their heads<br />

and could not comprehend these numbers.<br />

How pure is ultra-pure Ge? The person who cares only about electrically<br />

active impurities would say that crystals with a few 10 10 cm 3 of impurities<br />

are routinely grown. But are there other inactive impurities? Yes, of course<br />

there are. Hydrogen, oxygen, silicon and carbon are usually present at concentrations<br />

of up to 10 14 cm 3 , depending on the crystal growth conditions.<br />

These impurities do not interfere with Ge’s operation as radiation detectors<br />

provided certain rules are followed: no heating to temperatures above 350C<br />

and no rapid temperature changes. Can we reduce the concentration of these<br />

four electrically inactive impurities? Yes, we can, but we pay a price. Eliminating<br />

hydrogen by growing in vacuum leads to the introduction of impurities<br />

which can no longer be “flushed” out of the crystal puller. Furthermore, hydrogen<br />

will passivate the very small concentrations of deep-level defects and<br />

impurities which are always present. Free oxygen and silicon are generated<br />

by the reduction of the ultra-pure silica crucible by the liquid Ge. We do not<br />

know of any substance which can replace silica with, perhaps, the exception of<br />

graphite. Numerous attempts to grow ultra-pure Ge in graphite crucibles have<br />

failed so far because the resultant crystals contain too many Al acceptors.<br />

Most recently, the interest in Ge has sharply increased because isotopically<br />

pure Ge can be obtained from Russia. Isotopically pure Ge bulk crystals [9–<br />

12] and isotope superlattices [13] have been grown. New phonon physics and<br />

electronic transport studies are currently being pursued by several groups with<br />

these isotopically controlled crystals and multilayers.<br />

Have we arrived at the ultimately ideal material: isotopically and chemically<br />

pure and crystallographically perfect Ge single crystals? Perhaps the answer<br />

is no, but I certainly do not know of another parameter that can be controlled.

References<br />

Ultra-Pure Germanium 557<br />

1 R.N. Hall: in Proc. of the 12th Int. Conf. on Physics of Semiconductors, ed. by M.H.<br />

Pilkuhn (Teubner, Stuttgart 1974), p. 363<br />

2 E.E. Haller, F.S. Goulding: Handbook on Semiconductors, Vol. 4, ed. by C. Hilsum<br />

(Elsevier, New York 1993), Chap. 11, p. 937–963<br />

3 W.L. Hansen, E.E. Haller: Mater. Res. Soc. Proc. 16, 1 (1983)<br />

4 R.N. Hall, T.J. Soltys: IEEE Trans. Nucl. Sci. NS-18, 160 (1971)<br />

5 E.E. Haller, W.L. Hansen, F.S. Goulding: IEEE Trans. Nucl. Sci. NS-20, 481 (1973)<br />

6 E.E. Haller, W.L. Hansen, G.S. Hubbard, F.S. Goulding: IEEE Trans. Nucl. Sci. NS-<br />

23, 81 (1976)<br />

7 E.E. Haller, W.L. Hansen, F.S. Goulding: Adv. Phys. 30, 93 (1981)<br />

8 E.E. Haller: Physics 146B, 201 (1987)<br />

9 E.E. Haller: Semicond. Sci. Technol. 5, 319 (1990)<br />

10 E.E. Haller: Solid State Phenom. 32–33, 11 (1993)<br />

11 G. Davies, J. Hartung, V. Ozhogin, K. Itoh, W.L. Hansen, E.E. Haller: Semicond. Sci.<br />

Technol. 8, 127 (1993)<br />

12 H.D. Fuchs, P. Etchegoin, M. Cardona, K. Itoh, E.E. Haller: Phys. Rev. Lett. 70, 1715<br />

(1993)<br />

13 J. Spitzer, T. Ruf, M. Cardona, W. Dondl, R. Schorer, G. Abstreiter, E.E. Haller:<br />

Phys. Rev. Lett. 72, 1565 (1994)

558 <strong>Appendix</strong> A<br />

Two Pseudopotential Methods:<br />

Empirical and Ab Initio<br />

Marvin L. Cohen<br />

University of California, Berkeley, USA<br />

It took a relatively long time to develop methods capable of determining the<br />

detailed electronic structure of solids. In contrast, for gases, unraveling the<br />

mysteries of atomic energy levels went hand in hand with the development of<br />

quantum theory. Atomic optical spectra yielded sharp lines that could be interpreted<br />

in terms of excitations of electrons from occupied to empty states.<br />

These studies provided important tests of the theory. However, compared to<br />

atomic spectra, solid-state spectra are broad, since the interactions between<br />

the atoms spread the allowed occupied and empty energy levels into energy<br />

bands. This made interpretation of spectra in terms of electronic transitions<br />

very difficult. Trustable precise electronic energy band structures were needed<br />

to interpret solid-state spectra, but these were difficult to obtain.<br />

In principle, the Schrödinger equation can describe the behavior of electrons<br />

in solids; but without approximations, solutions for the electronic energy<br />

levels and wavefunctions are extremely difficult to calculate. Despite considerable<br />

effort, the situation around 1960 was still unsatisfactory. Creative models<br />

of solids had been introduced to explain many physical phenomena such as<br />

electronic heat capacities and superconductivity with spectacular success. However,<br />

calculations capable of yielding band structures and other properties for<br />

specific materials were not available.<br />

An important intermediate step was the introduction of the empirical<br />

pseudopotential model (EPM). Pseudopotentials had been around since 1934,<br />

when Fermi introduced the concept to examine the energy levels of alkali<br />

atoms. Since he was interested in highly excited atoms, he ignored the oscillations<br />

of the valence electron wavefunctions in the regions near the nucleus.<br />

By assuming a smooth wavefunction responding to a weak potential or pseudopotential,<br />

Fermi could easily solve for the outer electron energy levels.<br />

Since most solid-state effects, such as bonding, are principally influenced<br />

by the changes in the outermost electrons, this picture is appropriate. For the<br />

EPM it is assumed that the solid is composed of a periodic array of positive<br />

cores. Each core has a nucleus and core electrons. Each of the outer valence<br />

electrons moves in the electrostatic potential or pseudopotential produced by<br />

the cores and by the other valence electrons. In this one-electron model, each<br />

electron is assumed to respond to this average periodic crystalline pseudopotential.<br />

The periodicity allows Fourier decomposition of the potential and the<br />

EPM fits data to obtain Fourier coefficients. Usually only three coefficients per<br />

atom are needed.

Two Pseudopotential Methods: Empirical and Ab Initio 559<br />

The EPM stimulated interactions between theorists and experimentalists<br />

and the result was one of the most active collaborations in physics. Not only<br />

were optical and photoemission spectra of solids deciphered, the activities resulted<br />

in new experimental techniques and a much deeper understanding of<br />

the behavior of electrons in solids. The meeting ground between experiment<br />

and theory is usually response functions such as dielectric functions or reflectivity.<br />

In the early phases of this work the actual energy band structures, which<br />

are plots of energy versus wavevector, were the domain of theorists. However,<br />

the introduction of angular resolved photoemission spectroscopy (ARPES)<br />

gave energy bands directly and provided further tests of the EPM.<br />

The EPM band structures obtained in the 1960s and 1970s are still used today.<br />

In addition, the EPM produced the first plots of electronic charge density<br />

for crystals. These plots displayed covalent and ionic bonds and hence gave<br />

considerable structural information. Optical constants, densities of states, and<br />

many other crystal properties were obtained with great precision using EPMderived<br />

energy levels and wavefunctions.<br />

Despite the success of the EPM, there was still considerable motivation to<br />

move to a first-principles or ab initio model. The approach chosen was similar<br />

to Fermi’s. Instead of an EPM potential, the interaction of the valence<br />

electron with the core was described using an ab initio pseudopotential constructed<br />

from a knowledge of atomic wavefunctions. The valence electron–<br />

electron interactions were modeled using a density functional theory which,<br />

with approximations, allows the development of an electron–electron potential<br />

using the electronic charge density. However, the latter approach is appropriate<br />

only for calculating ground-state properties. Excited states such as those<br />

needed to interpret atomic spectra require adjustments to this theory. These<br />

adjustments are complex and require significant computer time compared to<br />

the EPM, but they are successful in reproducing the experimental data and<br />

the approach is completely ab initio.<br />

One of the most important applications of the ab initio pseudopotential<br />

model was the determination of structural properties. It became possible to<br />

explain pressure-induced solid–solid structural transitions and even to predict<br />

new structural phases of solids at high pressure using only atomic numbers<br />

and atomic masses. Bulk moduli, electron–phonon coupling constants, phonon<br />

spectra, and a host of solid-state properties were calculated. The results allowed<br />

microscopic explanations of properties and predictions. An example was<br />

the successful prediction that semiconducting silicon would become a superconducting<br />

hexagonal metal at high pressure.<br />

The two types of pseudopotential approaches, empirical and ab initio, have<br />

played a central role in our conceptual picture of many materials. Often the<br />

resulting model is referred to as the “standard model” of solids. Unlike the<br />

standard model of particle physics, which is sometimes called a theory of everything,<br />

the standard model of solids is most appropriate for those solids with<br />

reasonably itinerant electrons. Despite this restriction, the model is extremely<br />

useful and a triumph of quantum theory.

560 <strong>Appendix</strong> A<br />

The Early Stages of Band-Structures Physics<br />

and Its Struggles for a Place in the Sun<br />

Conyers Herring<br />

Stanford University, Stanford, USA<br />

It is universally recognized today that among the components necessary for<br />

a theoretical understanding of the properties of semiconductors, their specific<br />

electronic band structures have an extremely fundamental place. Textbooks<br />

on semiconductors typically have, among their earliest chapters, one on band<br />

structure, which contains diagrams of energy versus wavevector for important<br />

semiconductors, usually obtained from first-principles numerical calculations.<br />

But obviously these calculations would not be so conspicuously featured if<br />

they did not agree with a great body of experimental information. What the<br />

present-day student may not realize is that, despite the spurt of activity in<br />

the early post-transistor years – roughly 1948–1953 – the workers of this period<br />

had almost no knowledge of band structures, and had to muddle through<br />

as best they could without it. The evolution of this aspect of semiconductor<br />

physics provides a thought-provoking perspective on how science moves toward<br />

truth by erratic diffusional steps, rather than with military precision.<br />

The possible range of band structures had, of course, long been known in<br />

principle. The standard generalities about Bloch waves and their energy spectra<br />

had been known for a couple of decades; symmetry-induced degeneracies<br />

had been classified; early band-structure calculations, though not quantitatively<br />

reliable, had suggested that degenerate and multi-valley band edges might often<br />

occur. The trouble lay elsewhere. When so many possibilities for exciting<br />

work were opening up, people tended to avoid projects that would be tedious<br />

and time-consuming. Band-structure theorists, equipped only with mechanical<br />

calculators, often opted to use incomplete boundary conditions or limited basis<br />

sets. Experimentalists, despite rapid improvements in purity and perfection of<br />

materials, continued to focus mostly on properties whose interpretation did not<br />

depend critically on anisotropies and other special features of the energy bands.<br />

Much of the blame for this neglect must be cast on the theorists, not only for<br />

their failure to agree on calculated band structures, but also because, for too long,<br />

they shied away from the tedium of making detailed calculations of properties<br />

such as magnetoresistance for various kinds of nonsimple band structures.<br />

My own experience provides a typical example. In December 1953 I delivered<br />

an invited paper at an APS meeting with the title “Correlation of Electronic<br />

Band Structures with Properties of Silicon and Germanium”. In it I<br />

tried to reason as logically as possible from the existing experimental and theoretical<br />

literature, to draw plausible conclusions about the possible band-edge<br />

symmetries for these elements. While I got a few things right, it was distress-

The Early Stages of Band-Structures Physics and Struggles 561<br />

ing to learn over the next year or so that most of my inferences were wrong.<br />

How did I go astray?<br />

My first step, safe enough, was to classify the possible types of band-edge<br />

points: those at wavevector k 0, and those at k 0 (multi-valley); for each<br />

of these the states could be degenerate (two or more states of the same energy<br />

and k) or nondegenerate. In surveying the experimental and theoretical<br />

evidence bearing on the choices among these numerous alternatives, I began<br />

by trying to limit the possible choices to those that could occur for band structures<br />

qualitatively similar to that newly calculated by Herman [1] for diamond,<br />

which seemed more reliable than any others that had been made for any material<br />

with this crystal structure. Using the “k · p method” for qualitative estimations<br />

of the energy-band curvatures on moving away from k 0, this<br />

meant that I neglected perturbations of the p-like k 0 states °25 ′, °15 by the<br />

anti-bonding s-like level °2 ′, which is quite high in diamond but, contrary to<br />

my assumption, much lower in silicon and germanium. This neglect turned out<br />

to make me omit the possibility of conduction-band edges on the [111] axes in<br />

k-space for n-germanium, and to retain the possibility of valence-band edges<br />

on the [100] axes for p-silicon.<br />

From this flawed start I tried to narrow the possibilities further by appealing<br />

to experimental evidence, and especially to magnetoresistance. The nearvanishing<br />

of longitudinal magnetoresistance in [100]-type directions was obviously<br />

consistent with multi-valley band-edge regions centered on the [100]type<br />

axes in k-space, and this proved to be the correct identification for n-type<br />

silicon. But, lacking explicit calculations, I assumed that the energy surfaces of<br />

a degenerate hole band at k 0 would be so strongly warped as to preclude<br />

the near-zero [100] longitudinal magnetoresistance observed for p-silicon. So<br />

my predictions were all wrong here. Finally, I had the tedious task of calculating<br />

the complete anisotropy of magnetoresistance for multi-valley models,<br />

which a few months later were shown to give strong evidence for [111]-type<br />

valleys for n-germanium.<br />

What all this illustrates is that to achieve an acceptable understanding of<br />

band structures, each of three types of information sources had to reach a<br />

certain minimum level of sophistication. Band calculations from first principles<br />

had to be made with accuracy and self-consistency in an adequately large<br />

function space. Experimental measurements of properties sensitive to band<br />

structure had to be made under well-controlled conditions. And theoretical<br />

predictions of these properties for different band structure models had to be<br />

available. There were gaps in all three of these sources up to the end of 1953;<br />

it is thus not surprising that Shockley, in writing what was intended as a basic<br />

text for the coming semiconductor age [2], stated, in spite of his awareness of<br />

the diversity of possible band structures, that the theoretical reasoning in the<br />

book would all be based on the simple model with an isotropic effective mass.<br />

Remarkably, in a year or so starting in 1954, each of the three sources filled<br />

itself in sufficiently so that they could pull together (e. g., better theoretical<br />

bands [3], cyclotron resonance [4], magnetoresistance theory [5]) and bandstructure<br />

physics became a solid and accepted component of basic knowledge.

562 <strong>Appendix</strong> A<br />

References<br />

1 F. Herman: Phys. Rev. 88, 1210 (1952)<br />

2 W. Shockley: Electrons and Holes in Semiconductors (Van Nostrand, New York<br />

1950), esp. p. 174<br />

3 For an early review of progress 1953–1955, see, for example, F. Herman: Proc. IRE<br />

43, 1703 (1955)<br />

4 See the following contribution by C. Kittel<br />

5 B. Abeles, S. Meiboom: Phys. Rev. 95, 31 (1954); M. Shibuya, Phys. Rev. 95, 1385<br />

(1954)

Cyclotron Resonance and Structure of Conduction and Valence Band Edges 563<br />

Cyclotron Resonance and Structure of Conduction<br />

and Valence Band Edges in Silicon and Germanium<br />

Charles Kittel<br />

University of California, Berkeley, USA<br />

A prime objective of the Berkeley solid-state physics group (consisting of<br />

Arthur Kip and myself) from 1951 to 1953 was to observe and understand cyclotron<br />

resonance in semiconductors. The practical problems were to gain reliable<br />

access to liquid helium, and to obtain an adequate magnet and sufficiently<br />

pure crystals of Ge and Si. The liquid helium was obtained from the Shell Laboratories<br />

and later from the Giauque laboratory on campus. The magnet was<br />

part of a very early cyclotron (from what one may call the Ernest O. Lawrence<br />

collection), and the dc current for the magnet came from recycled US Navy<br />

submarine batteries. The semiconductor crystals were supplied by the Sylvania<br />

and Westinghouse Research Laboratories, and later by the Bell Telephone<br />

Laboratories. I think the microwave gear came from war surplus at MIT Radiation<br />

Laboratory. Evidently, very little of the equipment was purchased.<br />

The original experiments were on Ge [1], both n-type and p-type. There<br />

were too few carriers from thermal ionization at 4 K to give detectable signals,<br />

but the carriers that were present were accelerated by the microwave electric<br />

field in the cavity up to energies sufficient to produce an avalanche of carriers<br />

by impact ionization. This was true cyclotron resonance! A good question is,<br />

why not work at liquid hydrogen temperature, where the thermal ionization<br />

would be adequate? Hydrogen was then, and perhaps is still now, considered<br />

to be too hazardous (explosive) to handle in a building occupied by students.<br />

A better question is, why not work at liquid nitrogen temperature, where<br />

there are lots of carriers and the carrier mobilities are known to be much<br />

higher than at the lower temperatures? Cyclotron resonance at liquid nitrogen<br />

temperature had been tried at several other laboratories without success. The<br />

reason for the failures is that the plasma frequencies, being mixed with the<br />

cyclotron frequencies to produce a magnetoplasma frequency, are too high at<br />

the higher carrier concentrations – you are not measuring a cyclotron resonance<br />

but instead a magnetoplasma resonance [2]. Indeed, one can follow the<br />

plasma displacement of the original cyclotron lines when the cavity is allowed<br />

to warm up. In radio wave propagation in the ionosphere this effect is called<br />

magneto-ionic reflection, a subject I had learnt from the lectures of E.V. Appleton<br />

at Cambridge.<br />

A better way to produce carriers at 4 K was suggested by the MIT group.<br />

They irradiated the crystal with weak light sufficient to excite both electrons<br />

and holes. With this method both electrons and holes could be excited in the<br />

same crystal. Alternatively, one can excite a known carrier type by infrared

564 <strong>Appendix</strong> A<br />

irradiation of n- or p-type material. By modulating the optical excitation the<br />

detection of the absorption signal was made highly sensitive [3]. In addition,<br />

if there is any doubt about the sign of the carriers, circularly polarized microwaves<br />

can be (and were) used to distinguish the sense of rotation of the<br />

carriers in the magnetic field.<br />

The most surprising result of the original experiments was the observation<br />

of two effective masses (m ∗ ) for the Ge holes: m ∗ /m0 0.04 and 0.3, both approximately<br />

isotropic. Frank Herman and Joseph Callaway had calculated that<br />

the top of the valence band in Ge occurs at the center of thr Brillouin zone<br />

and is threefold degenerate (sixfold with spin), corresponding to p bonding orbitals<br />

on the Ge atoms. This would have given rise to three hole masses. We<br />

suggested [4,5] that the spin–orbit (s.o.) interaction splits the p orbitals into<br />

fourfold degenerate (related to p3/2 orbitals) and twofold degenerate (related<br />

to p1/2 orbitals) bands at the zone-center. We found that the most general form<br />

of the energy of the upper valence bands in the diamond structure to second<br />

order in wavevector k is (2.62)<br />

E(k) Ak 2 ± [B 2 k 4 C 2 (k 2 x k2 y k2 y k2 z k2 z k2 x )]1/2 .<br />

This was perhaps the first application of the spin–orbit interaction in semiconductors.<br />

The “s.o. split-off” or lower band in Ge is 0.30 eV below the top of the<br />

valence band edge. This s.o. splitting and the lower band itself are explored<br />

best by optical absorption. The analysis by Kahn [6] of the available experiments<br />

was an important confirmation of our model developed from cyclotron<br />

resonance.<br />

One of the early applications of the results of cyclotron resonance experiments<br />

in Si and Ge was to the theory of the ionization energies of the shallow<br />

donor and acceptor states in these materials. The approximate ionization energies<br />

are 0.04 eV for electrons and 0.05 eV for holes in Si, and 0.01 eV for<br />

both electrons and holes in Ge. The near equality of the ionization energies<br />

for both electrons and holes was astonishing, at the time, because their band<br />

edge structures were known to be completely different (thanks to cyclotron<br />

resonance). The problem was discussed in the summer of 1954 with visitors<br />

to Berkeley, notably Freeman Dyson and Joaquin Luttinger. The near equality<br />

turns out to be merely a matter of coincidence after the electron and hole<br />

ionization energies are calculated separately.<br />

The donor ionization energy was calculated first at Berkeley [7]. We used<br />

the hamiltonian for an ellipsoidal energy surface at any of the degenerate<br />

band edges for electrons and the dielectric constant of the bulk crystal. The<br />

calculated energies are in good agreement with experiment, at least for donors<br />

with atomic numbers close to that of the host crystal. For heavier donors, central<br />

cell corrections must be made. The acceptor problem is more difficult because<br />

of the fourfold degeneracy of the valence band edges at the zone center,<br />

and is reviewed by Walter Kohn [8], with satisfying results.

References<br />

Cyclotron Resonance and Structure of Conduction and Valence Band Edges 565<br />

1 G. Dresselhaus, A.F. Kip, C. Kittel: Phys. Rev. 92, 827 (1953)<br />

2 G. Dresselhaus, A.F. Kip, C. Kittel: Phys. Rev. 100, 618 (1955)<br />

3 G. Dresselhaus, A.F. Kip, C. Kittel: Phys. Rev. 98, 368 (1955)<br />

4 G. Dresselhaus, A.F. Kip, C. Kittel: Phys. Rev. 95, 568 (1954)<br />

5 R.J. Elliot: Phys. Rev. 96, 266 (1954)<br />

6 A.H. Kahn: Phys. Rev. 97, 1647 (1955)<br />

7 C. Kittel, A.H. Mitchell: Phys. Rev. 96, 1488 (1954)<br />

8 W. Kohn, in Advances in Solid State Physics, Vol. 5, ed. by F. Seitz, D. Turnbull (Academic,<br />

New York 1957), p. 257–320

566 <strong>Appendix</strong> A<br />

Optical Properties of Amorphous Semiconductors<br />

and Solar Cells<br />

Jan Tauc<br />

Brown University, Providence, USA<br />

In the early 1960s the foundations for an understanding of the optical properties<br />

of crystalline semiconductors were established. They were based on the<br />

existence of long-range order and k-vector conservation, which led to sharp<br />

structures in the spectra associated with the Van Hove singularities. My group,<br />

working in the Institute of Solid State Physics of the Czechoslovak Academy<br />

of Sciences in Prague, was making contributions to this ongoing effort which<br />

flourished throughout the 1960s. While on leave at Harvard in 1961–1962, I<br />

started thinking about what the optical properties should be like when longrange<br />

order is absent, and I began working on this problem after my return to<br />

Prague.<br />

There is a huge group of materials, called glasses, that lack long-range order;<br />

they are produced by quenching the melt, which of course does not have<br />

long-range order. In these materials the liquid has the same short-range order as<br />

the solid phase. This is not the case for semiconductors with tetrahedral bonding.<br />

The efficiency of this bond in lowering energy depends on the geometrical<br />

rigidity of the structure; once it is loosened at high temperature, the energetically<br />

favorable phase is a metallic one (some kind of close packing). So even if it<br />

were possible to quench, say, liquid Ge (which it is not), the short-range order of<br />

this “glass” would be completely different from crystalline Ge, and therefore a<br />

comparison of the optical properties would be meaningless. There are, however,<br />

ways to prepare amorphous Ge (a-Ge) (and other tetrahedral semiconductors)<br />

with the same short-range order as crystalline Ge (c-Ge) as a thin film, for example<br />

by condensing evaporated Ge on a cold substrate.<br />

In Prague, we first worked on the optical properties of some liquids, which<br />

clearly demonstrated the fact that the main optical properties depend on the<br />

short-range order. A breakthrough came when we learned that Radu Grigorovici<br />

had prepared thin films of a-Ge at the Institute of Physics of the Romanian<br />

Academy of Sciences. A close, fruitful and friendly collaboration soon<br />

developed, and for some years Radu regularly visited Prague. We spent long<br />

hours and days discussing amorphous semiconductors with tetrahedral bonding.<br />

At that time, we did not know of anyone else who would be interested<br />

in amorphous semiconductors of this kind (there was an important group in<br />

Leningrad which had been studying amorphous chalcogenide semiconductors<br />

since the 1950s, but these are real glasses and very different from tetrahedral<br />

semiconductors). Radu was interested in the preparation, structure and electronic<br />

transport, while we in Prague worked on the optical properties.

Optical Properties of Amorphous Semiconductors and Solar Cells 567<br />

From the reflection spectra, using Kramers-Kronig analysis, we determined<br />

the optical constants of a-Ge in the spectral range up to 12 eV and confirmed<br />

the expectation that there should be no sharp structures [1]. Instead<br />

of the three prominent peaks in the fundamental absorption band observed<br />

in c-Ge, there is just one band, which has the remarkable feature of having<br />

much larger absorption in the low energy region (a “red shift”). From the<br />

transmission spectra we determined the dependence of the absorption coefficient<br />

· on photon energy in the absorption edge region. The data gave a<br />

straight line when √ ˆ· was plotted as a function of photon energy ˆ[ √ ˆ· <br />

const. × (ˆ Eg)]. This plot defines an energy Eg, which it is natural to call<br />

the optical gap. Of course, it was the most obvious plot to try: if the k-vector<br />

is not conserved, if the density of electron states close to the valence and conduction<br />

band extrema is proportional to the square root of energy as in the<br />

crystal, and if the matrix element is a constant then · ∝ (ˆ Eg) 2 /ˆ, asis<br />

the case for phonon-assisted indirect transitions in crystalline semiconductors.<br />

In fact, in amorphous semiconductors there was no rigorous theoretical justification<br />

for this law at that time (and there is no generally accepted one today),<br />

so it must be considered as empirical. It is, however, most amazing that this<br />

plot works in many amorphous semiconductors. In the literature, this kind of<br />

edge is sometimes referred to as a “Tauc edge” and used as a definition of the<br />

“optical” gap, which is usually somewhat different from the gap determined<br />

from electrical conductivity measurements (“electrical gap”).<br />

The “red shift” mentioned above is observed also in a-Si and is the basis<br />

for the usefulness of this material for solar cell. Although Radu and I, during<br />

our walks in Prague (which was run down at that time but still beautiful), considered<br />

various possible applications of these materials, the truth is that they<br />

are useless as electronic materials because they are full of defects which act as<br />

traps, preventing n- and p-type doping. A prominent defect is a Si atom with<br />

only three neighbors, i. e., with an unpaired electron (a “dangling bond”). Our<br />

walks ended in 1968 after the tragic political events which put an end to what<br />

has since become known as the “Prague Spring”.<br />

In the 1970s the oil crisis hit the world, and thinking about renewable<br />

energy sources became popular. Among these, solar cells appeared very attractive.<br />

Cells made of c-Si are very good but too expensive for large scale<br />

deployment. The reason is that c-Si is an indirect-gap semiconductor and the<br />

absorption coefficient is small in the spectral region of the solar flux. To absorb<br />

it, the cell must be relatively thick (∼ 100 Ìm), which requires a large<br />

amount of a rather expensive material, in addition to the expensive technology<br />

(crystal growing, wafer cutting, polishing, etc.). Because of the red shift,<br />

a-Si absorbs solar light much more efficiently: the cells can be made much<br />

thinner, and thin film technology is much cheaper.<br />

A discovery dramatically improved the electronic properties of a-Si. It<br />

started with the work of Chittick and coworkers at Standard Telecommunications<br />

Laboratories in England in the late 1960s. A standard procedure for<br />

the crystal growth of a silicon layer on a Si substrate is the decomposition of<br />

SiH4 gas by the high temperature of the substrate. Instead, Chittick et al. [2]

568 <strong>Appendix</strong> A<br />

studied the decomposition of SiH4 by radio frequency glow discharge, which<br />

enabled them to deposit silicon on a cool noncrystalline substrate. They produced<br />

thin amorphous Si films whose electronic properties were radically improved<br />

through a reduced defect state density in the gap. They showed that<br />

the resistivity of these films could be lowered by two orders of magnitude by<br />

adding PH3 gas to SiH4 – the first demonstration of doping of an amorphous<br />

semiconductor. Their company did not let them continue the work. What is<br />

quite amazing is that Chittick told many of us about this work in 1969 and<br />

no one grasped the enormous significance of his result except Spear and Le<br />

Comber at the University of Dundee. They reported in 1975 [3] n- and pdoping<br />

and in 1976 production of p-n junctions. It was first believed that the<br />

good properties were due to an exceptionally gentle deposition technique, but<br />

the work of W. Paul and others showed that they were due to the presence of<br />

hydrogen in the films. Hydrogen in a-Si:H reduces the defect state density by<br />

compensating the dangling bonds.<br />

The gap of a-Si:H (about 1.8 eV) is larger than that of a-Si (1.4 eV) but<br />

the spectrum is also red-shifted with respect to c-Si, and therefore the films<br />

can be quite thin (1 Ìm) and still absorb a substantial part of the solar spectrum.<br />

One would think that with all these clues in hand someone would go<br />

ahead and design an a-Si:H solar cell. It did happen, but not in this way. Carlson<br />

and Wronski [4] discovered such cells independently at RCA in thin-film<br />

solar cells made of polycrystalline Si. They observed that when the substrate<br />

was cold enough the cells had a better efficiency and found that these better<br />

cells were amorphous rather than polycrystalline; only then did they realize<br />

the connection of their discovery to the current research on a-Si:H. These<br />

cells are today produced for small-scale applications and still remain a primary<br />

candidate for large-scale photovoltaic energy conversion plants which may be<br />

needed someday.<br />

References<br />

1 J. Tauc, A. Abraham, L. Pajasova, R. Grigorovici,A. Vancu: Non-Crystalline Solids<br />

(North-Holland, Amsterdam 1965), p. 606<br />

2 R.C. Chittick, J.H. Alexander, H.F. Sterlin: J. Electrochem. Soc. 116, 77 (1969)<br />

3 W.E. Spear, P.G. Le Comber: Solid State Commun. 17, 1193 (1975)<br />

4 D.E. Carlson, C.R. Wronski: Appl. Phys. Lett. 28, 671 (1976)

Optical Spectroscopy of Shallow Impurity Centers 569<br />

Optical Spectroscopy of Shallow Impurity Centers<br />

Elias Burstein<br />

University of Pennsylvania, Philadelphia, USA<br />

In the fall of 1948, Frank Isakson, head of the Physics Section of the Office<br />

of Naval Research, was a frequent visitor at the Naval Research Laboratory,<br />

where I was a member of the Crystal Branch. During one of our frequent discussions<br />

of projects of mutual interest, he informed me about the Navy’s interest<br />

in developing an infrared (IR) photoconductor with a response beyond<br />

7 Ìm, the long wavelength limit of PbS films, an intrinsic photoconductor developed<br />

in Germany during World War II. The properties of the III–V semiconductors<br />

were still unknown at that time. In the summer of 1949 I had the<br />

good fortune of being able to attend the annual Modern Physics Symposium<br />

at the University of Michigan, one of a series of symposia that started in 1928.<br />

The lecturers that summer were Luis Alvarez (High Energy Physics), Richard<br />

Feynman (Path Integral Method), Frederick Seitz (Solid State Physics) and<br />

Gordon B.B. Sutherland (Infrared Spectroscopy of Solids).<br />

In his lectures on semiconductors, Seitz discussed the nature of the impurity<br />

levels in Si and Ge and summarized the thermal ionization energies of<br />

group III acceptors and group V donors that had been obtained by Pearson<br />

and Bardeen at Bell Telephone Laboratories [1] from data on the temperature<br />

dependence of the carrier densities derived from resistivity and Hall measurements.<br />

He also discussed their conclusions that the ionization energies of the<br />

group III acceptors (0.048 eV) and group V donors (0.045 eV) were in reasonable<br />

agreement with a simple effective-mass hydrogen model. It was at that<br />

point in the lecture that the idea came to me to make use of the photoionization<br />

of un-ionized hydrogenic impurity centers in Si and Ge as the basis for<br />

IR detectors.<br />

Shortly after returning to Washington, DC, I went to see John Bardeen,<br />

who provided me with several Si samples. Together with John J. Oberly, James<br />

W. Davisson and Bertha Henvis, I started measurements of the low temperature<br />

IR absorption spectra of the Si samples. I wanted to study the absorption<br />

spectra associated with photoionization of un-ionized impurity centers before<br />

making an effort to observe the photoconductive response. Our first measurements,<br />

using a Perkin-Elmer model 12C spectrometer with interchangeable<br />

NaCl, KBr, KSR-5(TlBr+I) prisms and mirror optics, were carried out at 77 K,<br />

since a simple calculation based on the thermal ionization energy of impurities<br />

indicated that over 90% of the impurity centers would remain un-ionized<br />

at this temperature.

570 <strong>Appendix</strong> A<br />

The observed spectrum for a boron-doped Si sample was quite striking,<br />

since it exhibited peaks corresponding to transitions from the ground state to<br />

excited states of the acceptor centers, as well as the onset of a photoionization<br />

continuum [2,3] (Fig. 1). Moreover, the positions of the excitation peaks corresponded<br />

closely to the 1s–2p, 1s–3p and 1s–4p transitions of a hydrogenlike<br />

center and yielded an ionization energy of 0.046 eV, in good agreement with<br />

the thermal ionization data [4]. However, the oscillator strengths of the absorption<br />

peaks are markedly different from those for a hydrogenic center. In<br />

particular, the oscillator strength of the 1s–2p peaks is an order of magnitude<br />

smaller than that for a hydrogenic center. The widths of the excitation peaks<br />

decrease on cooling to liquid helium temperature, but there is no appreciable<br />

shift in the peak positions, indicating that Franck–Condon effects are small.<br />

Our data showed no obvious evidence of transitions from the ground state of<br />

Absorption cross section [10 –16 cm 2 ]<br />

40<br />

30<br />

20<br />

10<br />

20<br />

15<br />

10<br />

5<br />

3.0<br />

2.0<br />

1.0<br />

Boron-doped Silicon<br />

0 0.05 0.1 0.15<br />

Aluminum-doped Silicon<br />

0 0.1 0.2 0.3<br />

15<br />

Gallium-doped Silicon<br />

10<br />

5<br />

0 0.1 0.2 0.3<br />

Lattice<br />

Absorption<br />

Band<br />

><br />

Indium-doped Silicon<br />

0 0.1 0.2 0.3 0.4 0.5 0.6 0.7<br />

Photon energy [eV]<br />

Fig. 1. Photoexcitation and photoionization<br />

absorption spectra of group III acceptors<br />

in Si at liquid helium temperature<br />

[6]. For boron-doped Si, the dashed<br />

line is the theoretical photoionization<br />

absorption spectrum of the corresponding<br />

hydrogenic model

Optical Spectroscopy of Shallow Impurity Centers 571<br />

the split-off valence band, which is not unexpected since the spin–orbit interaction<br />

is small in Si and the optical spectra are broadened appreciably.<br />

Efforts to detect photoconductivity in n- and p-type Si at 77 K were unsuccessful,<br />

due to the presence of large numbers of thermally excited carriers.<br />

However, a photoconductive response was observed at liquid helium temperature.<br />

The spectral response of relatively pure n-Si is shown in Fig. 2 [5]. The<br />

dips in the photoconductive response between 8 and 24 Ìm correspond to lattice<br />

vibration absorption peaks. The data yielded a donor optical ionization<br />

energy of 0.04 eV. Photoconductivity studies were later carried out at liquid<br />

helium temperature on Ge doped with group III and V impurities. The photoconductive<br />

response was found to extend out to 38 Ìm, the limit of measurement<br />

at that time [6].<br />

Fairly complete optical studies were carried out for the group III acceptors<br />

(B, Al, Ga and In) and for the group V donors [7,8]. Absorption spectra<br />

for the group III centers are shown in Fig. 1. The variations in the ionization<br />

energy (Fig. 3) are accompanied by changes in the character of the excitation<br />

and photoionization absorption spectra. The positions of the excitation bands<br />

for Al, Ga and In centers, unlike B, do not correspond to a hydrogenic model,<br />

their oscillator strengths also differ appreciably from those of a hydrogenic<br />

model (Fig. 3). These deviations, which become more pronounced on going<br />

from B to In, are due to central cell corrections. The states with s character<br />

have their energies and wavefunctions rather strongly modified, since their<br />

wavefunctions are relatively large at the impurity atoms. The states with p<br />

characters, whose wavefunctions are small at the center of the impurity atom,<br />

are affected to a lesser degree. The agreement between the experimental ionization<br />

energy for B and the predictions of the hydrogenic model is probably<br />

due to a cancellation of different effects.<br />

Relative photoconductivity<br />

per incident photon<br />

10<br />

5<br />

1<br />

0.5<br />

0.1<br />

0.05<br />

0.01<br />

0.6 1.0 5.0 10 20 30 40<br />

Wavelength [µm]<br />

10<br />

α [cm –1 ]<br />

Fig. 2. The relative photoconductive response per incident photon of a relatively pure<br />

n-Si sample [4]. The dips in the photoconductive response between 8 and 24 Ìm correspond<br />

to the peaks in the optical absorption due to lattice vibrations

572 <strong>Appendix</strong> A<br />

Energy [eV]<br />

0.15<br />

0.10<br />

In<br />

Ga<br />

Al<br />

0.05 B H<br />

0<br />

Valence band<br />

1s<br />

2p<br />

3p<br />

4p<br />

Fig. 3. Suggested term scheme for group<br />

III acceptors in Si showing the levels<br />

whose energies are derived from the<br />

low temperature absorption spectra [6]<br />

The optical ionization energies for donors in Si were found to be 10%<br />

larger than the thermal ionization energies, due in part to the presence of<br />

low-lying excited states that were not taken into account in the calculation<br />

of the activation energies. The positions of the ground state relative to the<br />

conduction band are appreciably different for the three donors P, As and Sb,<br />

again due to central cell effects. However, their excited p-states are observed<br />

at about the same positions relative to the conduction band (see Fig. 3 and<br />

[7]). Moreover, they are in good agreement with the results of the effective<br />

mass formulation of the donor p levels by Kohn and Luttinger [9], which takes<br />

into account the fact that the conduction band of Si has six nondegenerate<br />

minima along the [100] and equivalent directions.<br />

The data obtained in these early investigations were limited by the relatively<br />

low quality of the Si Samples, the poor resolution of the spectrometers<br />

and by the electronics. There has been major progress in the IR spectroscopy<br />

of shallow impurity levels in semiconductors since then, made possible by<br />

significant improvements in crystal quality, spectrometers and detectors, by<br />

the development of photothermal conductance spectroscopy, which has much<br />

higher sensitivity than IR detectors, and by the availability of tunable IR lasers<br />

[10].<br />

References<br />

1 J. Bardeen, G.L. Pearson: Phys. Rev. 75, 865 (1949)<br />

2 E. Burstein, J.J. Oberly, J.W. Davisson, B.W. Henvis: Phys. Rev. 82, 764 (1951)<br />

3 E. Burstein, E.E. Bell, J.W. Davisson, M. Lax: J. Phys. Chem. 57, 849 (1953)

Optical Spectroscopy of Shallow Impurity Centers 573<br />

4 F.J. Morin, J.P. Maita, R.G. Schulman, N.B. Hannay: Phys. Rev. 97, 833 (1954)<br />

5 E. Burstein, J.J. Oberly, J.W. Davisson, Phys. Rev. 89, 331 (1953)<br />

6 E. Burstein, J.W. Davisson, E.E. Bell, W.J. Turner, H.G. Lipson: Phys. Rev. 93, 65<br />

(1954)<br />

7 E. Burstein, G. Picus, B.W. Henvis, R.F. Wallis: J. Phys. Chem. Solids 1, 65 (1956)<br />

8 G. Picus, E. Burstein, B.W. Henvis: J. Phys. Chem. Solids 1, 75 (1956)<br />

9 W. Kohn, J.M. Luttinger: Phys. Rev. 97, 883 (1954); ibid. 98, 915 (1955)<br />

10 See the review by A.K. Ramdas, S. Rodriguez: Rep. Prog. Phys. 44, 1297 (1981)

574 <strong>Appendix</strong> A<br />

On the Prehistory<br />

of Angular Resolved Photoemission<br />

Neville V. Smith<br />

Lawrence Berkeley Laboratory, Berkeley, USA<br />

Band mapping using angle-resolved photoemission started in the early 1970s.<br />

Interest in the angular dependence of the photoelectric effect, however, goes<br />

back much further. Figure 1 shows an apparatus used in the 1920s by Herbert<br />

Ives and coworkers [1] at the Bell Telephone Laboratories. These workers<br />

were definitely not concerned with band structures. Wave mechanics was a<br />

newfangled concept, and solid-state physics had yet to be invented. They were<br />

concerned rather with optimizing the efficiency of photocathodes for use in<br />

television and eventually videotelephony.<br />

The sample (C) sits at the center of a spherical collector (B). Application<br />

of retarding potentials to the collector permits measurement of the photoelectron<br />

energy spectra. A finger (F) moving around a slot in the collector permits<br />

measurements as a function of angle of emission. We recognize here a resemblance<br />

to modern experimental methods. More striking is the resemblance to<br />

the apparatus used by Clinton Davisson and Lester Germer in establishing the<br />

wave nature of the electron [2]. This is not surprising. These scientists were all<br />

working at the same time in the same building in Manhattan.<br />

It is diverting to speculate on the interactions between Ives and Davisson.<br />

It seems likely, on the artistic evidence, that they were using the services of<br />

the same glass blower! But what did they talk about? Would they have been<br />

pleased to know that their separate lines of research would converge half a<br />

century later into the indispensable technique of band mapping?<br />

Evan Kane proposed in a prescient paper published in 1964 that bands<br />

could in principle be mapped using the angular dependence of photoemission<br />

spectra [3]. A decade elapsed, however, before bands were actually mapped<br />

[4]. Mort Traum and I approached this problem in the early 1970s but with<br />

some hesitance. There were persuasive proponents of the view that photoelectrons<br />

would be so thoroughly scattered before emerging from the sample that<br />

all memory of angular information would be lost. We were so intimidated by<br />

this that we built only a minimal apparatus, essentially the same as that of<br />

Ives but with a channel electron multiplier in place of the finger F. To circumvent<br />

the indeterminacy of k⊥, we looked at two-dimensional materials,<br />

the layer compounds TaS2 and TaSe2. Frank DiSalvo was manufacturing single<br />

crystals of these compounds in his laboratory a few doors down the corridor.<br />

Len Mattheiss was calculating their band structures just a few further<br />

doors down the corridor, and we found beautiful agreement with his predictions<br />

[5].

On the Prehistory of Angular Resolved Photoemission 575<br />

Fig. 1. Apparatus used by Ives et al. [1]<br />

With these shortcuts and fine collaborators we were able to perform the first<br />

demonstration of band mapping [4]. In hindsight, it is embarrassing to contemplate<br />

our hesitance and timidity. It is all now so obvious and commonplace.<br />

References<br />

1 H.E. Ives, A.R. Olpin, A.L. Johnsrud: Phys. Rev. 32, 57 (1928)<br />

2 C.J. Davisson, L.H. Germer: Phys. Rev. 30, 705 (1927)<br />

3 E.O. Kane: Phys. Rev. Lett. 12, 97 (1964)<br />

4 N.V. Smith, M.M. Traum, F.J. DiSalvo: Solid State Commun. 15, 211 (1974)<br />

5 L.F. Mattheiss: Phys. Rev. B 8, 3719 (1973)

576 <strong>Appendix</strong> A<br />

The Discovery and Very Basics<br />

of the Quantum Hall Effect<br />

Klaus von Klitzing<br />

Max-Planck-Institut für Festkörperforschung, Stuttgart, Germany<br />

The discovery of the quantum Hall effect (QHE) was the result of basic research<br />

on silicon field effect transistors – the most important device in microelectronics.<br />

Unlike in other conductors, the electron concentration in these<br />

devices can be varied in a wide range just by changing the gate voltage. Therefore<br />

this system is ideal for an investigation of the Hall effect at different carrier<br />

densities by analyzing the Hall voltage as a function of the gate voltage.<br />

The experimental curves together with the notes of February 4, 1980, which<br />

characterize the birthday of the quantum Hall effect, are shown in Fig. 9.39.<br />

As expected qualitatively from the classical Hall effect, the Hall voltage UH<br />

varies (at a fixed magnetic field B 18 T) inversely proportional to the number<br />

N of free electrons (or gate voltage Vg). However, plateaus are visible<br />

if the ratio of the number N of electrons to the number Nº of flux quanta<br />

within the area of the device is an integer. For one electron per flux quantum<br />

(this corresponds to a fully occupied lowest Landau level with the filling<br />

factor 1) the Hall voltage divided by the current has the fundamental<br />

value RK h/e 2 (25812.807 ± 0.005) ø. This Hall plateau is barely visible<br />

in the upper left corner of Fig. 9.39 and distorted by the large device resistance<br />

due to localization phenomena at this relatively small electron density.<br />

The plateaus at 2 or 4 times larger electron concentration are much better<br />

resolved. Today, electronic systems with higher quality are available so that<br />

measurements at much smaller electron densities with filling factors smaller<br />

than one are possible. This is the region where the fractional quantum Hall<br />

effect is observed [9.70].<br />

A special situation seems to be present if two flux quanta are available<br />

for one electron (filling factor 1/2): Quasiparticles (composite fermions) are<br />

formed which behave like electrons moving in an effective magnetic field<br />

B ∗ 0. The Shubnikov–de Haas oscillations of these composite fermions are<br />

equivalent to the structures of the fractional quantum Hall effect.<br />

Already the first publication on the QHE [1] with the original title “Realization<br />

of a Resistance Standard Based on Fundamental Constants” indicated<br />

that an application similar to the Josephson effect may be possible. Today,<br />

it is known that different materials (silicon field effect transistors, GaAs/<br />

AlGaAs heterostructures) show the same value for the quantized Hall resistance<br />

within the experimental uncertainty of 3.5 × 10 10 , and since 1990 all<br />

calibrations of resistances are based on the quantum Hall effect with a fixed<br />

value RK1990 25812.807 ø for the von Klitzing constant RK.

The Discovery and Very Basics of the Quantum Hall Effect 577<br />

Different approaches can be used to deduce a quantized value for the Hall<br />

resistance. The calculation shown in Fig. 9.39, which led to the discovery of the<br />

QHE, is simply based on the classical expression for the Hall effect. A quantized<br />

Hall resistance h/e 2 is obtained for a carrier density corresponding to the<br />

filling factor one. It is surprising that this simple calculation leads to the correct<br />

result. Laughlin was the first to try to deduce the result of the QHE in<br />

a more general way from gauge invariance principles [2]. However, his device<br />

geometry is rather removed from the real Hall effect devices with metallic<br />

contacts for the injection of the current and for the measurement of the electrochemical<br />

potential.<br />

The Landauer–Büttiker formalism, which discusses the resistance on the<br />

basis of transmission and reflection coefficients, is much more suitable for analyzing<br />

the quantum Hall effect [3]. This formalism was very successful in explaining<br />

the quantized resistance of ballistic point contacts [4] and, in a similar<br />

way, the quantized Hall resistance is the result of an ideal one-dimensional<br />

electronic transport. In a classical picture this corresponds to jumping orbits of<br />

electrons at the boundary of the device. In the future, the textbook explanation<br />

of the QHE will probably be based on this one-dimensional edge channel<br />

transport (see Fig. 9.40).<br />

References<br />

1 K. v. Klitzing, G. Dorda, M. Pepper: Phys. Rev. Lett. 45, 494 (1980)<br />

2 R.B. Laughlin: Phys. Rev. B 23, 5632 (1981)<br />

3 M. Büttiker: Phys. Rev. Lett. 57, 1761 (1986)<br />

4 B.J. von Wees, H. van Houten, S.W.J. Beenakker, J.G. Williamson, L.P. Kouwenhoven,<br />

D. van der Marel, C.T. Foxon: Phys. Rev. Lett. 60, 848 (1988);<br />

D.A. Wharam, T.J. Thornton, R. Newbury, M. Pepper, H. Ahmed, J.E.F. Frost, D.G.<br />

Hasko, D.C. Peacock, D.A. Ritchie, G.A.C. Jones: J. Phys. C 21, L 209 (1988)

578 <strong>Appendix</strong> A<br />

The Birth of the Semiconductor Superlattice<br />

Leo Esaki<br />

University of Tsukuba, Tsukuba, Japan<br />

In 1969, research on artificially structured materials was initiated when Tsu<br />

and I [1,2] proposed an engineered semiconductor superlattice with a onedimensional<br />

periodic potential. In anticipation of advances in controlled epitaxy<br />

of ultrathin layers, two types of superlattices were envisioned: doping and<br />

compositional, as shown in Fig. 1.<br />

Before arriving at the superlattice concept, we had been examining the<br />

feasibility of structural formation of potential barriers and wells that were thin<br />

enough to exhibit resonant tunneling [3]. A resonant tunnel diode [4,5] appeared<br />

to have more spectacular characteristics than the Esaki tunnel diode<br />

[6], the first quantum electron device consisting of only a single tunnel barrier.<br />

It was thought that advanced technologies with semiconductors might be<br />

Electron energy<br />

Electron energy<br />

(a)<br />

(b)<br />

+ + + + + + +<br />

+<br />

Energy gap Eg – – –<br />

– – –<br />

Valence band<br />

compositional superlattice<br />

conduction band<br />

Energy gap E g1 E g2<br />

Valence band<br />

– – –<br />

0<br />

l<br />

2<br />

l<br />

3l<br />

2<br />

Distance<br />

2l<br />

5l<br />

2<br />

3l<br />

Fig. 1a,b. Spatial variations of<br />

the conduction and valence<br />

band edges in two types of<br />

superlattices: (a) doping, (b)<br />

compositional

The Birth of the Semiconductor Superlattice 579<br />

ready for demonstration of the de Broglie electron waves. Resonant tunneling<br />

(see Sect. 9.5) can be compared to the transmission of an electromagnetic<br />

wave through a Fabry–Perot resonator. The equivalent of a Fabry–Perot resonant<br />

cavity is formed by the semiconductor potential well sandwiched between<br />

the two potential barriers.<br />

The idea of the superlattice occurred to us as a natural extension of<br />

double-, triple- and multiple-barrier structures: the superlattice consists of a<br />

series of potential wells coupled by resonant tunneling. An important parameter<br />

for the observation of quantum effects in the structure is the phasecoherence<br />

length, which approximates the electron mean free path. This depends<br />

on the bulk quality as well as the interface quality of crystals, and also<br />

on the temperatures and values of the effective mass. As schematically illustrated<br />

in Fig. 2, if characteristic dimensions such as superlattice periods or well<br />

widths are reduced to less than the phase-coherent length, the entire electron<br />

system will enter a mesoscopic quantum regime of low dimensionality, on a<br />

scale between the macroscopic and the microscopic. Our proposal was to explore<br />

quantum effects in the mesoscopic regime.<br />

The introduction of the one-dimensional superlattice potential perturbs the<br />

band structure of the host materials, yielding a series of narrow subbands and<br />

forbidden gaps which arise from the subdivision of the Brillouin zone into<br />

a series of minizones. Thus, the superlattice was expected to exhibit unprecedented<br />

electronic properties. At the inception of the superlattice idea, it was<br />

recognized that the long, tailormade lattice period provided a unique opportunity<br />

to exploit electric-field-induced effects. The electron dynamics in the super-<br />

1 Ìm<br />

100 nm<br />

10 nm<br />

1 nm<br />

0.1 nm<br />

Superlattice<br />

or<br />

quantum wells<br />

Macroscopic regime<br />

Phase–coherent distance<br />

(electron mean free path)<br />

Interatomic spacing<br />

microscopic regime<br />

“Mesoscopic” quantum<br />

regime<br />

Crystal quality<br />

(decreasing temperature)<br />

Fig. 2. Schematic illustration<br />

of a “mesoscopic” quantum<br />

regime (shaded) with a superlattice<br />

of quantum wells (inset)

580 <strong>Appendix</strong> A<br />

lattice direction was analyzed for conduction electrons in a narrow subband of<br />

a highly perturbed energy–wavevector relationship. The result led to the prediction<br />

of a negative differential resistance at a modestly high electric field,<br />

which could be a precursor of Bloch oscillations. The superlattice allows us to<br />

enter the regime of electric-field-induced quantization: the formation of Stark<br />

ladders [7,8], for example, can be proved in a (one-dimensional) superlattice<br />

[9], whereas in natural (three-dimensional) crystals the existence and nature of<br />

these localized states in a high electric field have been controversial [10,11].<br />

This was, perhaps, the first proposal which advocated using advanced thinfilm<br />

growth techniques to engineer a new semiconductor material designed<br />

by applying the principles of quantum theory. The proposal was made to the<br />

US Army Research Office (ARO), a funding agency, in 1969, daringly stating,<br />

with little confidence in a successful outcome at the time, “the study of superlattices<br />

and observations of quantum mechanical effects on a new physical<br />

scale may provide a valuable area of investigation in the field of semiconductors”.<br />

Although this proposal was favorably received by ARO, the original version<br />

of the paper [1] was rejected for publication by Physical Review on the<br />

referee’s unimaginative assertion that it was “too speculative” and involved<br />

“no new physics”. The shortened version published in IBM Journal of Research<br />

and Development [2] was selected as a Citation Classic by the Institute<br />

for Scientific Information (ISI) in July 1987. Our 1969 proposal was cited as<br />

one of the most innovative ideas at the ARO 40th Anniversary Symposium in<br />

Durham, North Carolina, 1991.<br />

At any rate, with the proposal we launched a program to make a “Gedankenexperiment”<br />

a reality. In some circles, the proposal was criticized as close to<br />

impossible. One of the objections was that a man-made structure with compositional<br />

variations on the order of several nanometers could not be thermodynamically<br />

stable because of interdiffusion effects. Fortunately, however,<br />

it turned out that interdiffusion was negligible at the temperatures involved.<br />

In 1970, Chang, Tsu and I [12] studied a GaAs–GaAs0.5P0.5 superlattice<br />

with a period of 20 nm synthesized by CVD (chemical vapor deposition) by<br />

Blakeslee and Aliotta [13]. Although transport measurements failed to reveal<br />

any predicted effect, the specimen probably constituted the first strainedlayer<br />

superlattice having a relatively large lattice mismatch. Early efforts in<br />

our group to obtain epitaxial growth of Ge1xSix and Cd1xHgxTe superlattices<br />

were soon abandoned because of rather serious technical problems at<br />

that time. Instead, we focused our research effort on compositional GaAs–<br />

Ga1xAlxAs superlattices grown by MBE (molecular beam epitaxy). In 1972,<br />

we found a negative resistance in such superlattices [14], which was interpreted<br />

in terms of the superlattice effect.<br />

Following the derivation of the voltage dependence of resonant tunnel currents<br />

[5], Chang, Tsu and I observed current–voltage characteristics with a<br />

negative resistance [15]. Subsequently, Chang and I measured quantum transport<br />

properties in a superlattice with a narrow bandwidth, which exhibited an<br />

oscillatory behavior [16]. Tsu et al. performed photocurrent measurements on

Number of papers<br />

500<br />

200<br />

100<br />

50<br />

20<br />

10<br />

5<br />

2<br />

1<br />

1970<br />

The growth of papers on<br />

quantum heterostructures<br />

presented at the int. conf.<br />

on phys. of semiconductors<br />

72 74 76 78 80 82 84 86 88 90 92 1994 1<br />

Warsaw<br />

Stuttgart<br />

Rome<br />

Edinburgh<br />

Kyoto<br />

Montpellier<br />

San Francisco<br />

Stockholm<br />

The Birth of the Semiconductor Superlattice 581<br />

Fig. 3. Growth in relevant papers at the biennial International Conference on the Physics<br />

of Semiconductors<br />

superlattices subjected to an electric field perpendicular to the plane layers<br />

with the use of a semitransparent Schottky contact, which revealed their miniband<br />

configurations [17].<br />

Heteroepitaxy is of great interest for the growth of compositional superlattices.<br />

Innovations and improvements in epitaxial techniques such as MBE and<br />

MOCVD (metal-organic chemical vapor deposition) have made it possible to<br />

prepare high-quality heterostructures with predesigned potential profiles and<br />

impurity distributions having dimensional control close to interatomic spacing.<br />

This great precision has cleared access to the mesoscopic quantum regime<br />

[18,19].<br />

Since a one-dimensional potential can be introduced along with the growth<br />

direction, famous examples in the history of one-dimensional mathematical<br />

physics, including the above-mentioned resonant tunneling [3], Kronig–Penney<br />

bands [20], Tamm surface states [21], Zener band-to-band tunneling [22], and<br />

Stark ladders including Bloch oscillations [7–9], all of which had remained<br />

textbook exercises, could, for the first time, be practiced in a laboratory. Thus,<br />

do-it-yourself quantum mechanics is now possible, since its principles dictate<br />

the details of semiconductor structures [23].<br />

Warsaw<br />

Thessaloniki<br />

Beijing<br />

100<br />

50<br />

20<br />

10<br />

5<br />

2<br />

Percentage of total papers

582 <strong>Appendix</strong> A<br />

Our original proposal [1] and pioneering experiments have triggered a<br />

wide spectrum of experimental and theoretical investigations on superlattices<br />

and quantum wells over the last two decades. A variety of engineered structures<br />

now exhibit extraordinary transport and optical properties which do not<br />

exist in any natural crystal. This new degree of freedom offered in semiconductor<br />

research through advanced materials engineering has inspired many ingenious<br />

experiments, resulting in observations of not only predicted effects but<br />

also totally unknown phenomena. As a measure of the growth of the field, Fig.<br />

3 shows the number of papers related to the subject and the percentage of<br />

the total presented at the biennial International Conference on the Physics of<br />

Semiconductors. Following 1972, when the first paper [14] was presented, the<br />

field went through a short period of incubation before experiencing a phenomenal<br />

expansion in the 1980s. It appears that nearly half of all semiconductor<br />

physicists in the world are working in this area. Activity at this new frontier<br />

of semiconductor physics has in turn given immeasurable stimulus to device<br />

physics, provoking new ideas for applications. Thus, a new class of transport<br />

and opto-electronic devices has emerged.<br />

References<br />

1 L. Esaki, R. Tsu: IBM Res. Note RC-2418 (1969)<br />

2 L. Esaki, R. Tsu: IBM J. Res. Devel. 14, 61 (1970)<br />

3 D. Bohm: Quantum Theory (Prentice Hall, Englewood Cliffs, NJ 1951), p. 283<br />

4 L.V. Iogansen, Zh. Eksp. Teor. Fiz. 45, 207 (1963) [Sov. Phys. – JETP 18, 146 (1964)]<br />

5 R. Tsu, L. Esaki: Appl. Phys. Lett. 22, 562 (1973)<br />

6 L. Esaki: Phys. Rev. 109, 603 (1958)<br />

7 H.M. James: Phys. Rev. 76, 1611 (1949)<br />

8 G.H. Wannier: Elements of Solid State Theory (Cambridge University Press, Cambridge<br />

1959), p. 190; Phys. Rev. 117, 432 (1960)<br />

9 W. Shockley: Phys. Rev. Lett. 28, 349 (1972)<br />

10 J. Zak: Phys. Rev. Lett. 20, 1477 (1968); Phys. Rev. B 43, 4519 (1991)<br />

11 A. Rabinovitch, J. Zak: Phys. Rev. B 4, 2358 (1971)<br />

12 L. Esaki, L.L. Chang, R. Tsu: Proc. 12th Int. Conf. Low Temp. Phys., Kyoto, Japan<br />

1970, p. 551<br />

13 A.E. Blakeslee, C.F. Aliotta: IBM J. Res. Devel. 14, 686 (1970)<br />

14 L. Esaki, L.L. Chang, W.E. Howard, V.L. Rideout: Proc. 11th Int. Conf. Phys. Semiconductors,<br />

Warsaw, Poland 1972, p. 431<br />

15 L.L. Chang, L. Esaki, R. Tsu: Appl. Phys. Lett. 24, 593 (1974)<br />

16 L. Esaki, L.L. Chang: Phys. Rev. Lett. 33, 495 (1974)<br />

17 R. Tsu, L.L. Chang, G.A. Sai-Halasz, L. Esaki: Phys. Rev. Lett. 34, 1509 (1975)<br />

18 L. Esaki: IEEE J. Quantum Electron. QE-22, 1611 (1986)<br />

19 L. Esaki: in Highlights in Condensed Matter Physics and Future Prospects, ed. by L.<br />

Esaki (Plenum, New York 1991), p. 55<br />

20 R. de L. Kronig, W.G. Penney: Proc. R. Soc. London A 130, 499 (1931)<br />

21 I. Tamm: Phys. Z. Sowjetunion 1, 733 (1932)<br />

22 C. Zener: Proc. R. Soc. London 145, 523 (1934)<br />

23 L. Esaki, Phys. Scr. T42, 102 (1992)

<strong>Appendix</strong> B:<br />

Solutions to Some of the Problems<br />

Solution to Problem 2.2<br />

There are many ways to “verify” a character table. One way to do this is to calculate<br />

the character table starting with the given basis functions. This is what we<br />

shall do here. This approach can be used to solve both parts (a) and (b).<br />

We note that the character of a class can be obtained by applying one of<br />

the symmetry operations in the class listed in Chapter 2 to the basis function<br />

(or functions), thus finding the transformation matrices and then summing up<br />

their diagonal elements. To do this for all the classes it is convenient to create<br />

first a table listing the effect of the symmetry operations on the spatial coordinates<br />

x, y and z.<br />

For the Td group we obtain immediately the following list:<br />

{E}: identity; xyz → xyz<br />

{C2}: 2-fold rotation about the x-axis; xyz → x, y, z<br />

{C3}: 3-fold clockwise rotation about the [111]-axis; xyz → yzx<br />

{S4}: 4-fold clockwise rotation about the x-axis followed by a reflection onto<br />

the yz-plane; xyz → x, z, y<br />

{Û}: reflection onto the [110]-plane; xyz → yxz<br />

The effects of these operations on the different basis functions are summarized<br />

below:<br />

A1 Irreducible Representation with basis function: xyz<br />

Since all the symmetry operations either do not change the signs or change<br />

the signs in pairs it is clear that all of them leave the function xyz unchanged<br />

and therefore all the characters are equal to unity as expected for the identity<br />

representation. Combining these results we obtain the characters for A1 as:<br />

Classes {E} {C2} {S4} {s} {C3}<br />

Characters of A1 1 1 1 1 1<br />

A2 Irreducible Representation with basis function:<br />

x4 (y2 z2 ) y4 (z2 x2 ) z4 (x2 y2 )<br />

If a symmetry operation simply changes the cyclic permutation of |x|, |y| and<br />

|z| then it will not change the above basis function and the corresponding<br />

character should be unity. This is the case for the operation {E} and the two

584 <strong>Appendix</strong> B<br />

proper rotations: {C2} and {C3}. In the case of the other two improper rotations<br />

{S4} and {Û}, the cyclic order of |x|, |y| and |z| is reversed. This changes<br />

the sign of the basis function and therefore the characters are both 1. Combining<br />

these results we obtain the characters for A2 as:<br />

Classes {E} {C2} {S4} {Û} {C3}<br />

Characters of A2 1 1 1 1 1<br />

E Irreducible Representation with basis functions: f1 (x2 y2 )<br />

and f2 z2 1<br />

2 (x2 y2 )<br />

The operation {C2} changes only the signs of y and z and therefore leaves<br />

both f1 and f2 unchanged i.e. its character is 2. The operation {C3} changes<br />

the orders of x, y and z. It changes f1 into (y2 z2 ) ( 1<br />

2 )(f1 2f2) and f2<br />

into x2 1<br />

2 (y2z2 ) ( 1<br />

2 )f1(f2/2). The two diagonal elements are both 1<br />

2 and<br />

the character is 1. The operation {S4} interchanges y 2 and z 2 . It changes f1<br />

into (x2 z2 ) ( 1<br />

2 )(f1 2f2) and f2 into y2 1<br />

2 (x2 z2 ) ( 3<br />

4 )f1 (f2/2). Thus,<br />

the two diagonal elements are 1 1<br />

2 and 2 , respectively and the character is 0.<br />

The operation {Û} interchanges x2 and y2 . It changes f1 into (y2 x2 ) f1<br />

and f2 into z2 1<br />

2 (x2 y2 ) f2. The two diagonal elements are 1 and 1,<br />

respectively and the character is 0. Combining the above results we obtain the<br />

characters for E as:<br />

Classes {E} {C2} {S4} {Û} {C3}<br />

Characters 2 2 0 0 1<br />

The derivation of the characters for the remaining two irreducible representations<br />

are left as exercise.<br />

Solution to Problem 2.4<br />

In this problem we demonstrate that the symmetrized wave functions in Table<br />

2.9 indeed transform according to the irreducible representations given in that<br />

table. The readers should try to verify the symmetry of the wave functions<br />

in Table 2.<strong>10.</strong> To do this we note that the three functions: {sin x, sin y, sin z}<br />

transform like x, y, z under all the symmetry operations of the Td group. On<br />

the other hand, the functions {cos x, cos y, cos z} are “even” under C2 rotations<br />

so they have the same transformation properties as {x2 , y2 , z2 }. Based on these<br />

observations we see immediately that:<br />

(a) The function sin(2applex/a) sin(2appley/a) sin(2applez/a) transforms like xyz and therefore<br />

from Table 2.3 it belongs to the °1 representation.<br />

(b) Similarly, the function cos(2applex/a) cos(2appley/a) cos(2applez/a) transforms like<br />

(xyz) 2 or (°1) 2 and, therefore, belongs to the °1 representation also.<br />

(c) By the same argument, the three functions: {sin(2applex/a) sin(2appley/a)<br />

cos(2applez/a), sin(2applex/a) cos(2appley/a) sin(2applez/a), cos(2applex/a) sin(2appley/a) sin(2applez/a)}

Solution to Problem 2.6 585<br />

transform like {xyz 2 , xy 2 z, x 2 yz} xyz{z, y, x}. Since {xyz} transforms like<br />

°1 and {x, y, z} transform like °4 these three functions transform like °4.<br />

(d) The derivation of the symmetry of the three functions {sin(2applex/a)<br />

cos(2appley/a) cos(2applez/a), cos(2applex/a) sin(2appley/a) cos(2applez/a), cos(2applex/a) cos(2appley/a)<br />

sin(2applez/a)} is left as an exercise.<br />

Solution to Problem 2.6<br />

In this solution we demonstrate how to derive the compatibility relation between<br />

° and ¢. The reader should repeat the calculation for the remaining<br />

compatibility relations in this problem. First, we need to find the symmetry<br />

operations of the group of ° which are also symmetry operations of ¢. From<br />

Table 2.13 we find the following correspondence between the symmetry operations<br />

in those two groups.<br />

Operation in ° Corresponding Operation in ¢<br />

{E} {E}<br />

{C2} {C2 4 }<br />

{Û} {md}<br />

{Û ′ } {m ′ d }<br />

According to the definition on page 45, two representations are compatible<br />

if they have the same characters for the corresponding classes in the above<br />

table. Based on this definition °1 is compatible with ¢1 while °2 is compatible<br />

with ¢2.<br />

For °3 the characters of the above 4 classes are:<br />

{E} {C2} {Û} {Û ′ }<br />

°3 2 2 0 0<br />

From Table 2.14 we see that the characters of ¢1 ¢2 are exactly the same<br />

for the corresponding classes of °:<br />

{E} {C 2 4 } {md} {m ′ d }<br />

¢1 ¢2 2 2 0 0<br />

Hence °3 is compatible with ¢1 ¢2.

586 <strong>Appendix</strong> B<br />

Solution to Problem 2.8<br />

(a) Before we symmetrize the wavefunctions at the X point, it is important<br />

to note that the pseudopotential form factors in Table 2.21 have been defined<br />

with (1) the origin chosen at the mid-point between the two atoms in the zincblende<br />

structure, (2) the cation has been chosen to be the atom a located at<br />

the point (a/8)(111), and (3) the anti-symmetric form factor is proportional to<br />

Va Vb. The symmetry operations of the group of X have to be defined to<br />

conform to this particular choice of coordinate system (denoted by O and its<br />

axes by x, y, and z in Fig. 1). It should be noted that the symmetry operations<br />

listed on p. 47 and the corresponding character table (Table 2.15) on the same<br />

page have been defined with respect to the coordinate system in which one of<br />

the two atoms in the unit cell has been chosen to be the origin (denoted by O ′<br />

and its axes by x ′ , y ′ , and z ′ in Fig. 1).<br />

y'<br />

y<br />

Cation (Atom a)<br />

(1/8)(1,1,1)<br />

Anion O<br />

(Atom b) (0,0,0)<br />

O'<br />

x'<br />

(–1/8)(1,1,1)<br />

x<br />

Prob.2.8-Fig. 1 The relation between the coordinate<br />

systems O and O ′<br />

Some of the symmetry operations are identical in the two coordinate systems.<br />

for example the identity operation {E} is independent of the choice of<br />

coordinate system. Unfortunately most of the other operations are affected by<br />

the change in coordinate system. To see the relations between symmetry op-<br />

erations in O and O ′ , we shall consider the operation C 2 4<br />

as an example. In O′<br />

this operation is a 2-fold rotation, say about the y ′ -axis. The same operation in<br />

O will involve:<br />

(i) a translation T to move the origin from that of O to O ′ ,<br />

(ii) a 2-fold rotation with respect to the axis y ′ and then<br />

(iii)another translation T 1 to move the origin back to O.<br />

In general any symmetry operation P in O ′ will become P ′ T 1 PT in O. We<br />

shall now symmetrize the X point wave functions in O ′ by first forming the<br />

following six linear combinations out of the two |100〉 and four |011〉 wave-<br />

functions:<br />

⎧ ⎫<br />

2apple<br />

⎪⎨ cos x ⎪⎬<br />

a<br />

<br />

⎪⎩<br />

2apple<br />

i sin x<br />

⎪⎭<br />

a<br />

1<br />

2<br />

<br />

|100〉 |100〉<br />

|100〉 |100〉<br />

(2.8.1)

⎧ ⎫<br />

2apple<br />

⎪⎨ cos (y z) ⎪⎬<br />

a<br />

<br />

⎪⎩<br />

2apple<br />

i sin (y z)<br />

⎪⎭<br />

a<br />

1<br />

2<br />

<br />

|011〉 |011〉<br />

|011〉 |011〉<br />

Partial solution to Problem 2.8 587<br />

(2.8.2)<br />

⎧ ⎫<br />

2apple<br />

⎪⎨ cos (y z) ⎪⎬<br />

a<br />

<br />

⎪⎩<br />

2apple<br />

i sin (y z)<br />

⎪⎭<br />

a<br />

1<br />

<br />

|011〉 |011〉<br />

(2.8.1)<br />

2 |011〉 |011〉<br />

We shall denote these six symmetrized wave functions as:<br />

<br />

2apple<br />

æ1 ∼ cos (y z)<br />

a<br />

<br />

2apple<br />

æ2 ∼ sin (y z)<br />

a<br />

<br />

<br />

2apple<br />

2apple<br />

æ3 ∼ sin (y z) cos (y z)<br />

a<br />

a<br />

<br />

<br />

(2.8.4)<br />

2apple<br />

2apple<br />

æ4 ∼ sin (y z) cos (y z)<br />

a<br />

a<br />

<br />

2apple<br />

2apple<br />

æ5 ∼ cos x sin x<br />

a<br />

a<br />

<br />

2apple<br />

2apple<br />

æ6 ∼ cos x sin x<br />

a<br />

a<br />

To determine their irreducible representations we shall test their symmetry<br />

by applying the 2-fold rotation C2 4 (y′ ) to all these 6 wave functions. First we<br />

have to find out the effect of this operation on the point (x, y, z) inO. When<br />

refered to O ′ this point has the coordinate: x ′ x (a/8); y ′ y (a/8) and<br />

z ′ z (a/8). We may also say that the operation T transforms (x, y, z) to<br />

(x ′ , y ′ , z ′ ). The 2-fold rotation then transforms (x ′ , y ′ , z ′ ) into (x ′ , y ′ , z ′ ).<br />

Finaly T1 transforms this point into x ′ a<br />

8 , y′ a<br />

8 , z′ a<br />

<br />

a<br />

8 x 4 ,<br />

y, z a<br />

<br />

2<br />

4 . Thus the net effect of the operation C4 (y ′ ) on the crystal can be<br />

represented by the change:<br />

<br />

(x, y, z) → x a a<br />

<br />

, y, z . (2.8.5)<br />

4 4<br />

The effect of this operation on the six wavefunctions æ1 to æ6 can now be<br />

shown to be:<br />

æ1 ∼ cos(2apple/a)(y z) → cos(2apple/a)(y z a/4)<br />

sin(2apple/a)(y z) æ2<br />

æ2 ∼ sin(2apple/a)(y z) → sin(2apple/a)(y z a/4)<br />

cos(2apple/a)(y z) æ1<br />

(2.8.6a)<br />

(2.8.6b)

588 <strong>Appendix</strong> B<br />

æ3 ∼ sin(2apple/a)(y z) cos(2apple/a)(y z)<br />

→ sin[(2apple/a)(y z) apple/2] cos[(2apple/a)(y z) apple/2]<br />

cos(2apple/a)(y z) sin(2apple/a)(y z) æ3<br />

æ4 ∼ sin(2apple/a)(y z) cos(2apple/a)(y z)<br />

→ sin[(2apple/a)(y z) apple/2] cos[(2apple/a)(y z) apple/2]<br />

cos(2apple/a)(y z) sin(2apple/a)(y z) æ4<br />

æ5 ∼ cos(2apple/a)x sin(2apple/a)x<br />

→ cos(2apple/a)(x a/4) sin(2apple/a)(x a/4)<br />

(2.8.6c)<br />

(2.8.6d)<br />

(2.8.6e)<br />

sin(2apple/a)x cos(2apple/a)x æ5<br />

and æ6 → æ6. (2.8.6f)<br />

Therefore the characters of these 6 wavefunctions under the operation of C2 4<br />

are: ¯(æ1) ¯(æ2) 0; ¯(æ3) 1; ¯(æ4) 1; ¯(æ5) 1; and ¯(æ6) 1.<br />

if we compare these characters with those in Table 2.15 we conclude that:<br />

(1) æ1 and æ2 form a 2D representation X5;<br />

(2) æ3 and æ6 belong to either the X3 or X4 representation; and<br />

(3) æ4 and æ5 belong to either the X1 or X2 representation.<br />

To narrow down the choice of irreducible representations for wave functions<br />

æ3, æ4, æ5 and æ6 we need to apply another symmetry operation to them.<br />

Let us choose the operation S4. In particular we consider an opeation involving<br />

a 4-fold rotation about the x ′ -axis. Using the same procedures as for the<br />

operation C2 4 (y′ ), we can show that the effect of this operation on (x, y, z) is<br />

given by:<br />

<br />

(x, y, z) → x a a<br />

<br />

, z, y . (2.8.7)<br />

4 4<br />

The effect of the operation S4 on the six wave functions is summarized below:<br />

æ1 ∼ cos(2apple/a)(y z) → cos(2apple/a)(z y a/4)<br />

(2.8.8a)<br />

sin(2apple/a)(z y) æ2<br />

æ2 ∼ sin(2apple/a)(y z) → sin(2apple/a)(y z a/4)<br />

(2.8.8b)<br />

cos(2apple/a)(y z) æ1<br />

æ3 ∼ sin(2apple/a)(y z) cos(2apple/a)(y z)<br />

→ sin[(2apple/a)(z y) apple/2] cos[(2apple/a)(y z) apple/2] (2.8.8c)<br />

cos(2apple/a)(y z) sin(2apple/a)(y z) æ3<br />

æ4 ∼ sin(2apple/a)(y z) cos(2apple/a)(y z)<br />

→ sin[(2apple/a)(z y) apple/2] cos[(2apple/a)(y z) apple/2] (2.8.8d)<br />

cos(2apple/a)(z y) sin(2apple/a)(y z) æ3<br />

(2.8.8e)<br />

æ5 → æ6<br />

æ6 → æ6<br />

(2.8.8f)

Partial solution to Problem 2.8 589<br />

The characters of these 6 wave functions under the operation S4 are, therefore,<br />

¯(æ1) 0 ¯(æ2); ¯(æ3) 1; ¯(æ4) 1; ¯(æ5) 1; and ¯(æ6) 1.<br />

We note that the characters of æ1 and æ2 are consistent with those of the<br />

irreducible representation X5 we obtained for these two wave functions based<br />

on the operation C2 4 (y′ ). The additional characters now allow us to determine<br />

uniquely the irreducible representation of æ3 and æ6 as X3 and those of æ4<br />

and æ5 as X1. The reader should try to determine the characters for the remaining<br />

symmetries of the group of X so as to complete the character table<br />

for these 6 wave functions.<br />

(b) To calculate the matrix elements of the above six wave functions we shall<br />

first derive the following results. First we notice that with the conventions in<br />

Section 2.5 the pseudopotential form factor Vg is defined for GaAs by (2.33)<br />

as:<br />

Vg V s g cos(g · s) iVa g sin(g · s)<br />

where s (a/8)(1, 1, 1) and g is a reciprocal lattice vector. If g <br />

(2apple/a)(g1, g2, g3) then g · s (apple/4)(g1 g2 g3). Limiting ourselves to: g <br />

(2apple/a)(2, 0, 0); (2apple/a)(2, 2, 0); (2apple/a)(1, 1, 1) we obtain<br />

V (220) V a (220) cos apple Vs (220) sin apple Vs (220) vs g V (220) vs g (2.8.9a)<br />

V (220) V (220) V (220) ... V (022) v s g<br />

(2.8.9b)<br />

V (200) iV a (200) iva4 and its cyclic permutations (2.8.9c)<br />

V (200) iv a 4 V (200)<br />

V (111) 1 √ 2<br />

(2.8.9d)<br />

s<br />

1<br />

v iVa √2 (v (111) (111)<br />

s 3 iva3 ) (2.8.9e)<br />

V (111) 1 √ (v<br />

2 s 3 iva3 ) (2.8.9f)<br />

V (111) 1 √ (V<br />

2 s 3 iva3 ) (2.8.9g)<br />

v (111) 1 √ (v<br />

2 s 3 iva3 ) (2.8.9h)<br />

We shall now demonstrate the calculation of a few selected matrix elements<br />

of the pseudopotential V : 〈æi|V|æj〉 where i and j 1, ..., 6. In principle there<br />

are 36 matrix elements. The number of inependent elements is roughly halved<br />

by noting that 〈æi|V|æj〉 〈æj|V|æi〉 ∗ .<br />

〈æ1|V|æ1〉 1<br />

〈011 011|V|011 011〉<br />

1<br />

2<br />

2<br />

<br />

〈011|V|011〉 〈011|V|011〉 〈011|V|011〉 〈011|V|011〉<br />

(2.8.10)

590 <strong>Appendix</strong> B<br />

Noting that according to (2.25) 〈abc|V|a ′ b ′ c ′ 〉 V (aa ′ ,bb ′ ,cc ′ ) we find:<br />

〈æ1|V|„1〉 1<br />

2 (V (000) V (220) V (220) V (000))<br />

1<br />

2 (V (220) V (220) ) v s (2.8.11a)<br />

8<br />

In obtaining (2.8.11a) we have set V (000) 0. In a similar manner we can<br />

obtain:<br />

〈æ1|V|æ3〉 1<br />

2 √ <br />

〈011|V|011〉〈011|V|011〉〈011|V|011〉〈011|V|011〉<br />

2<br />

〈011|V|011〉 〈011|V|011〉 〈011|V|011〉 〈011|V|011〉 0<br />

〈æ3|V|æ3〉 v s 8 2va 4<br />

(2.8.11b)<br />

(2.8.11c)<br />

〈æ4|V|æ5〉 √ 2i(v s 3 va3 ) (2.8.11d)<br />

The readers are urged to calculate the rest of the matrix elements in the determinant<br />

on p. 94.<br />

(c) Once the 6 × 6 determinant on p. 94 is constructed, it is clear that the<br />

wave functions æ1 and æ2 are coupled. Similarly æ3 and æ6 are coupled and<br />

the same is true for æ4 and æ5. Hence the 6 × 6 determinant can be broken<br />

up into three 2 × 2 determinants. As an example the 2 × 2 determinant for the<br />

æ4 and æ5 wave functions is given by:<br />

<br />

<br />

<br />

4<br />

<br />

<br />

<br />

<br />

2apple2 ma2 E vs8 2va4 i √ 2(va 3 vs 3 )<br />

i √ 2(va 3 vs 3 )<br />

22apple2 ma2 E va <br />

<br />

<br />

<br />

0 (2.8.12)<br />

<br />

4 <br />

(2.8.12) can be expanded into the following quadratic equation:<br />

<br />

E 2 E<br />

<br />

<br />

6 2 apple 2<br />

ma 2 vs 8 3va 4<br />

<br />

8 2 apple 2<br />

ma 2 22 apple 2<br />

ma 2 (vs 8 4va 4 ) 2(vs 3 va 3 )2 v a 4 (vs 8 2va 4 )<br />

<br />

0<br />

(2.8.13)<br />

Solving (2.8.13) we obtain the energies E(X1) given on p. 94. The energies<br />

E(X3) and E(X5) can be obtained similarly.<br />

(d) The energy splittings in Fig. 2.28 are obtained by substituting the following<br />

values into the equations for E(X1), E(X3) and E(X5) on p. 94:<br />

a 5.642 ˚A and the pseudopotential form factors for GaAs from Table 2.21:<br />

vs 3 0.252 Ry, vs 8 0Ry, va 3 0.068 Ry and va 4 0.066 Ry. Since the split-<br />

ting of 0.74 eV between the X3 and X1 levels is the result of subtracting two<br />

large numbers, it is important to keep at least four significant figures in your<br />

calculations.

Partial solution to Problem 2.10 591<br />

(e) The next higher energy plane wave states at the X point are obtained by<br />

adding the reciprocal vectors [0, ±2, 0] and [0, 0, ±2] to the vector [±1, 0, 0].<br />

This gives rise to eight additional plane wave states:<br />

|120〉, |120〉, |120〉, |120〉, |102〉, |102〉, |102〉 and |102〉<br />

while the additional form factors are: v11, v12, v16 and v18. These four form factors<br />

correspond to: g11 (1, 3, 1) etc; g12 (2, 2, 2) etc; g16 (0, 4, 0) etc; and<br />

g18 (2, 4, 0) etc (using the notation on p. 58). For the face-centered cubic<br />

lattice all form factors with reciprocal lattice vector (h, k, l) where the components<br />

are a mixture of even and odd integers vanish. As a result we only need<br />

to include g11, g12, g16 and g18.<br />

Solution to Problem 2.10<br />

Let us denote the operator exp[i£Û · n/2] by O(ı). The operators Ûx, Ûy and<br />

Ûz are the Pauli matrices given in 2.6.2. The coordinate axes are assumed to<br />

be chosen with the z-axis parallel to the spin axis. In other words, the spin<br />

functions (to be denoted by · and ‚) are eigenfunctions of the operator Ûz<br />

with eigenvalues 1 and 1, respectively.<br />

(a) For a 2apple rotation about the z axis, we obtain the following results:<br />

O(2apple)· exp[i2appleÛz/2]· ·.<br />

O(2apple)‚ exp[i2appleÛz/2]‚ ‚.<br />

This gives a character of 2 for this symmetry operation.<br />

(b) For the Td group we will demonstrate how to obtain the character for the<br />

operations: {C2x}: 2-fold rotation about the x-axis; and {C2z}: 2-fold rotation<br />

about the z-axis. Normally we expect these two operations to belong to the<br />

same class and, therefore, should have the same character. In this case, because<br />

of the rather unusual nature of the rotation operators when applied to<br />

spin functions (which can change sign upon a 2apple rotation), we shall derive the<br />

results for both operators just to be absolutely sure. For {C2z} the axis of rotation<br />

is along the z-direction so n · Û Ûz. As the spin wave functions are<br />

eigenfunctions of Ûz, we find that:<br />

O(apple)· exp[iappleÛz/2]· i·.<br />

O(apple)‚ exp[iappleÛz/2]‚ i‚.<br />

Thus the character of {C2z} is (i i) 0.<br />

For {C2x} the axis of rotation is along the x-direction so n · Û Ûx. We<br />

note that: Ûx· ‚ and Ûx‚ · while (Ûx) 2 · Ûx‚ · and similarly<br />

(Ûx) 2 ‚ Ûx· ‚. From these results we can conclude that all even functions<br />

of (Ûx) will leave · and ‚ unchanged while all odd functions of (Ûx) will<br />

interchange · and ‚.<br />

The rotation operator corresponding to {C2x} is: exp[iappleÛx/2] <br />

cos[appleÛx/2] i sin[appleÛx/2]. From the above results we can deduce that the spin<br />

wave functions · and ‚ are eigenfunctions of the operator cos(appleÛx/2) with

592 <strong>Appendix</strong> B<br />

eigenvalues cos(apple/2) 0 since an expansion of the cosine function will contain<br />

only even functions of Ûx. On the other hand, the operator sin(appleÛx/2) contain<br />

only odd functions of Ûx and, therefore, will interchange the spin wave functions:<br />

sin[appleÛx/2]· ‚ and sin[appleÛx/2]‚ ·.<br />

Hence the character of the rotation matrix corresponding to {C2x} is again<br />

0 in agreement with the character of the rotation matrix corresponding to<br />

{C2z}.<br />

In principle, the characters for the other operators can be obtained similarly.<br />

In practice, the improper rotations deserve special attention. An improper<br />

rotation can usually be expressed as the product of a proper rotation<br />

and the inversion operator I. For example, a reflection onto the xy-plane (or<br />

md) can be thought of as a 2-fold rotation about the z-axis followed by I.<br />

Similarly, the S4 operation can be decomposed into a 4-fold rotation followed<br />

by I. In quantum mechanics the inversion operator is also referred to as the<br />

parity operator. Its eigenvalue is the parity of its eigenfunction. Except in processes<br />

where particles are created or annihilated, the parity of a vector (like<br />

the spatial coordinate r and the momentum p) are 1. On the other hand, the<br />

parity of the angular momentum l rxp is 1. Since spin is similar to l we expect<br />

its parity is also 1. It turns out that there is a subtle difference between<br />

ordinary angular momentum and spin. Angular momentum involves rotation<br />

about a fixed axis. Under a reflection onto a plane containing the axis of rotation<br />

the sense of rotation will change. For example, the adjacent figure shows<br />

how under reflection a clockwise rotation is changed into a counterclockwise<br />

rotation. The axis of rotation serves also as the axis for quantization of the zcomponents<br />

of the angular momentum vector(spatial quantization). However,<br />

spin is an intrinsic property of elementary particles and cannot be visualized<br />

in terms of a classical rotation. There is no such thing as “an axis of rotation”<br />

associated with spin. The axis of spatial quantization in the case of spin can be<br />

chosen arbitrarily. The effect of an inversion operation I on the spin functions<br />

· or ‚ can be expressed as: I(· or ‚) A(· or ‚) where the constant A can<br />

be 1, 1, i or –i.<br />

Reflection Plane<br />

Prob 2.10-Fig. 1 Effect of a reflection on a rotation when the reflection<br />

plane is parallel to the axis of rotation.<br />

This arbitrariness in the constant A does not pose a problem in quantum<br />

mechanics because the effect of I on any matrix element involving the spin<br />

functions will be proportional to |A| 2 1. For simplicity, we shall choose<br />

A 1. In other words, the spin wavefunctions are eigenfunctions of the inver-

Partial solution to Problem 2.12 593<br />

sion operator with eignenvalues: 1. Hence, the double group character of the<br />

improper rotations such as S4 can be obtained by first calculating the character<br />

for the corresponding proper rotation. In the book it was pointed out in 2.6.2<br />

that for some symmetry operations Ci both Ci and ÊCi belong to the same<br />

class. It can be shown [see H. Jones: The Theory of Brillouin Zones and Electronic<br />

States in Crystals, p. 251] that this is not true if the trace of the spin operator<br />

corresponding to Ci (i.e. Tr[O(Ci)]) is non-zero. In case Tr[O(Ci)] 0<br />

then Ci and ÊCi will belong to the same class if Ci contains a 2-fold rotation<br />

about an axis perpendicular to the axis n.<br />

Some references on the effect of symmetry operations on spin wave functions:<br />

E. Merzbacher: Quantum Mechanics. (John Wiley & Sons, Inc. New York, 1961).<br />

M. Tinkham: Group Theory and Quantum Mechanics. (McGraw-Hill, New York, 1964).<br />

V. Heine: Group Theory in Quantum Mechanics. (Dover, New York, 1993).<br />

Solution to Problem 2.12<br />

(a) The operator p has three components px, py and pz which transform under<br />

the symmetry operations of Td like the components of a vector x, y, and<br />

z. Similarly the °4 conduction and valence bands of the zincblende-type semiconductor<br />

are three-dimensional whose basis functions transform under the<br />

symmetry operations of Td like the components of a vector x, y, and z. We<br />

shall denote the valence band basis functions as |X〉, |Y〉 and |Z〉 respectively.<br />

The corresponding conduction band basis functions will be denoted by °4c(x),<br />

°4c(y) and °4c(z), respectively. Under a C2 or 180◦ rotation around say the<br />

x-axis the coordinate transformation can be represented as: xyz ⇒ xyz. Thus,<br />

under the C2 operation about the x-axis, any terms of the form xxy, xxz and<br />

yyy etc., which contain only an odd number of y or z will change sign and<br />

therefore vanish. The same will be true for terms of the form xyy, xxx etc<br />

which contain an odd number of x. Similarly all matrix elements of the form<br />

〈X|px|°4c(x)〉, 〈Y|px|°4c(x)〉 etc., can be shown to vanish under appropriate C2<br />

rotations.<br />

(b) In the case of matrix elements of the form 〈X|py|°4c(z)〉 which do not<br />

vanish since they do not transform like the matrix elements considered in (a),<br />

we can show that they transform into each other under the three-fold rotations<br />

C3. For example, a 120◦ rotation about the [111] axis will result in the<br />

following coordinate transformation: xyz ⇒ yzx and its effect on the matrix<br />

element 〈X|py|°4c(z)〉 would be to transform it into 〈Y|pz|°4c(x)〉. Since the<br />

crystal is invariant under this C3 rotation we conclude that: 〈X|py|°4c(z)〉 <br />

〈Y|pz|°4c(x)〉. The other cyclic permutations of 〈X|py|°4c(z)〉 can also be<br />

shown to be equal by using C3 rotations about the other equivalent [111] axes.<br />

(c) This remaining problem is left as an exercise.

594 <strong>Appendix</strong> B<br />

Partial solution to Problem 2.14<br />

In the book the matrix element H ′ 11 of the k · p Hamiltonian was worked out<br />

for the wave function º1. Here we will work out the matrix element: H ′ 12 .<br />

By definition (2.52):<br />

H ′ 12 H12 2<br />

m2 〈º1|k · p|°1c〉〈°1c|k · p|º2〉<br />

E0<br />

2<br />

m2E ′ 〈º1|k · p|°4c〉〈°4c|k · p|º2〉<br />

0<br />

Substituting into the first matrix elements the wave functions º1 and º2 we<br />

get:<br />

and<br />

〈º|k · p|°1c〉〈°1c|k · p|º2〉 〈3/2,3/2|k · p|°1c〉〈°1c|k · p|3/2,1/2〉<br />

<br />

1 <br />

√ 〈X iY|k · p|°1c〉〈°1c|k · p|Z〉<br />

<br />

3<br />

P2<br />

<br />

√ (ikx ky)(ikz)<br />

3<br />

<br />

P2<br />

<br />

√ (kxkz ikykz)<br />

3<br />

〈º1|k · p|°4c〉〈°4c|k · p|º2〉 〈3/2,3/2|k · p|°4c〉〈°4c|k · p|3/2,1/2〉<br />

<br />

1 <br />

√ 〈X iY|k · p|°4c〉〈°4c|k · p|Z〉<br />

<br />

3<br />

1 <br />

√ 〈X iY|kzpz|°4c(x)〉〈°4c(x)|kypy|Z〉<br />

<br />

3<br />

1 <br />

√ 〈X iY|kzpz|°4c(y)〉〈°4c(y)|kxpx|Z〉<br />

<br />

3<br />

Q2<br />

<br />

(kz)(iky) √ (ikz)(ikx)<br />

3<br />

<br />

<br />

Q2<br />

<br />

√ (kxkz ikykz)<br />

3<br />

H12 ∼〈3/2,3/2|k · p|3/2,1/2〉 <br />

<br />

<br />

X iY<br />

√ 2<br />

<br />

<br />

<br />

k · p<br />

2<br />

3 Z<br />

<br />

0<br />

Hence H ′ 12 <br />

<br />

1 <br />

<br />

√ (M L)(kxkz ikykz) <br />

3<br />

N <br />

√ (kxkz ikykz). The<br />

3<br />

remaining matrix elements can be obtained in a similar manner.

Solution to Problem 2.16<br />

Solution to Problem 2.16 595<br />

(a) The matrix elements of the tight-binding Hamiltonian are given by (2.78).<br />

Examples of the calculation of these matrix elements, such as Hs2,s2, are given<br />

in the book for the diamond structure. The results for the zincblende structure<br />

differ only slightly from that of the diamond structure in that the two atoms<br />

in the unit cell are different. Since the nearest neighbor tetrahedral arrangement<br />

is the same in the two structures, one would expect that the definition<br />

of the vectors d1, ..., d4 would be the same. The main difference would be the<br />

matrix elements 〈S1|int|S1〉 and 〈S2|int|S2〉 which are no longer equal. Similarly<br />

〈X1|int|X1〉 would not be equal to 〈X2|int|X2〉 etc. This means that<br />

in Table 2.25 it would be necessary to introduce an energy ES1 for the matrix<br />

element 〈S1|int|S1〉 and a different energy ES2 for the matrix element<br />

〈S2|int|S2〉. Similarly, one can introduce energies Ep1 and Ep2.<br />

(b) At k 0, g0(k) 1 and g1(k) g2(k) g3(k) 0. Hence, the s-band<br />

determinant derived from the modified Table 2.25 for the zincblende crystal is<br />

given by:<br />

<br />

<br />

<br />

Es1 Es(0) Vss<br />

V∗ ss<br />

<br />

<br />

<br />

Es2 Es(0) 0<br />

Evaluating this determinant one obtains a quadratic equation in Es(0):<br />

[Es(0)] 2 Es(0)(Es1 Es2) (Es1Es2) |Vss| 2 0<br />

The solutions for the s-band energies at k 0 are therefore:<br />

Es(0) [(Es1 Es2)]/2] ± (1/2)[(Es1 Es2) 2 4|Vss| 2 ] 1/2<br />

The solutions for the p-band energies at k 0 can be obtained similarly.<br />

Solution to Problem 2.18<br />

In this case the overlap parameter Vxx can be evaluated in the same way as<br />

〈px|H|px〉 in Fig. 2.23 of the book and the result is the same, except for replacing<br />

the angle £ by £x.<br />

The overlap parameter Vxy can be evaluated, in principle, by drawing the<br />

following diagram and decomposing the figure into a sum of two figures as<br />

shown in Prob. 2.18-Fig. 1.<br />

The first figure on the right is rather simple and easy to calculate since<br />

both orbitals are projected along the vector d. The projections of px and py<br />

along d are simply px cos £x and py cos £y, respectively. The resulting overlap<br />

integral is VppÛ cos £x cos £y.<br />

The second overlap integral is more difficult to evaluate from the second<br />

figure on the right, since the components of px and py perpendicular to d are<br />

not parallel to each other. Instead, we will decompose the unit vector along

596 <strong>Appendix</strong> B<br />

+<br />

z<br />

-<br />

d +<br />

- y<br />

y<br />

-<br />

z<br />

d +<br />

-<br />

+ y<br />

x<br />

x x<br />

x x x<br />

Prob. 2.18-Fig. 1 Decomposition of the overlap integral Vxy into two in which the two p<br />

orbitals are either parallel or perpendicular to the vector d joining the two atoms.<br />

the x-axis into two components: ˆx x || x⊥, where x || is parallel to d and x⊥<br />

is perpendicular to d. x⊥ is given by:<br />

x⊥ ˆx (ˆx · ˆd) ˆd<br />

where ˆd is a unit vector along d. Defining y || and y⊥ in similar ways we obtain:<br />

x⊥y⊥ ˆx (ˆx · ˆd) ˆd ˆy (ˆy · ˆd) ˆd (ˆx · ˆd)(ˆy · ˆd) cos £x cos £y<br />

Using these results it can be shown that the overlap integral from the second<br />

figure is given by: Vppapple cos £x cos £y. Hence Vxy (VppÛ Vppapple)<br />

cos £x cos £y.<br />

Solution to Problem 2.20<br />

(a) In the nearly-free electron model the lowest energy bands at the L-point<br />

are those with k (apple/a)(1, 1, 1) and (apple/a)(1, 1, 1) (see Fig. 2.9). According<br />

to group theory, the plane wave states: „1 exp[ik · x] and „2 <br />

exp[ik · x] can be symmetrized into one even parity state with L1 symmetry<br />

and one odd parity state with L2 ′ symmetry. The proper symmetrization depends<br />

on the choice of origin. In order to use (2.22), we have to choose the<br />

origin at the mid-point of the two atoms in the unit cell. The inversion operation<br />

we have to apply to „1,2 is then the standard inversion operation I,<br />

without any translation. However, this operation is the equivalent of the special<br />

operation I ′ when the origin is chosen at one of the atoms. For simplicity,<br />

we will neglect the coupling of these two plane waves with the higher energy<br />

states with wave vectors (apple/a)(3, 1, 1) etc.. As we will show later, the separation<br />

between the L2 ′ valence band and the L1 conduction band under the<br />

present approximation is given by the matrix element of the pseudopotential:<br />

(2) 1/2 |Vs 3 |. In the case of Si the magnitude of this term is only ∼4 eV which is<br />

much smaller than the value of ∼12 eV obtained by the full pseudopotential<br />

calculation including the other pseudopotential form factors and also coupling<br />

y<br />

+<br />

z<br />

-<br />

-<br />

d<br />

+<br />

y

Solution to Problem 2.20 597<br />

to the higher energy plane wave states. However, for the purpose of demonstrating<br />

the symmetry of the L wave functions the present approximation is<br />

adequate.<br />

Based on the above assumption, the only pseudopotential form factor<br />

which couples „1 and „2 is: Vg V s 3<br />

cos(g · s) from (2.33) where the vec-<br />

tors g (2apple/a)(1, 1, 1) and s (a/8)(1, 1, 1). Notice that in arriving at (2.33)<br />

we have chosen the origin to be at the mid-point between the two atoms in the<br />

diamond lattice. We note also that the symmetric pseudopotential form factor<br />

Vs 3 is negative for all diamond and zincblende-type semiconductors (see Table<br />

2.21) because of the attractive nature of the potential seen by the electrons.<br />

Thus Vg Vs 3 cos(g · s) Vs 3 cos(3apple/4) (1/√2)Vs 3 is 0.<br />

To calculate the eigenvalues and eigenfunctions we will set up the usual<br />

determinant:<br />

<br />

<br />

<br />

<br />

<br />

<br />

<br />

<br />

2k2 E Vg<br />

2m<br />

V∗ <br />

g<br />

2k2 <br />

<br />

<br />

<br />

and diagonalize it.<br />

<br />

E <br />

2m<br />

The resultant energies are: E± [2k2 /2m] ±|Vg| where [2k2 /2m] ± Vg.<br />

The corresponding wave functions are given by: (1/2) 1/2 [„1 „2].<br />

For the valence band we have to take the lower energy solution: „v <br />

C1„1 C2„2. Substituting back EV E into the linear equation for C1 and<br />

C2 we get:<br />

{[2k2 /2m] E}C1 VgC2 0orVgC1 VgC2 0.<br />

Since Vg is 0, we obtain: C1 C2. Thus „V (1/2) 1/2 [„1 „2] or the valence<br />

band has odd parity under inversion operation I and hence its symmetry<br />

is L2 ′.<br />

(b) To calculate the bonding and anti-bonding s-orbitals within the tightbinding<br />

approximation we will further simplify the results contained in 2.7.2.<br />

First, we neglect the overlap between the s- and p-orbitals. This has the effect<br />

of reducing the 8 × 8 matrix in Table 2.25 into a 2 × 2 matrix for the s-orbitals<br />

and a 6×6 matrix for the p-orbitals. The effect of this simplification will affect<br />

the accuracy of the bonding and anti-bonding orbital energies but should not<br />

change their parity. Within this approximation there are only 2 orbitals: |S1〉<br />

and |S2〉 corresponding to the s-orbitals of the two atoms inside the primitive<br />

unit cell. The secular equations for their eigenvalues (as obtained from Table<br />

2.25) are now:<br />

<br />

<br />

<br />

Es<br />

<br />

Ek Vssg1<br />

<br />

<br />

0<br />

Vssg ∗ 1<br />

Es Ek<br />

According to (2.82a) the factor<br />

g1 (1/4) exp[i(d1 · k)] exp[i(d2 · k)]<br />

exp[i(d3 · k)] exp[i(d4 · k)] <br />

cos(k1apple/2) cos(k2apple/2) cos(k3apple/2) i sin(k1apple/2) sin(k2apple/2) sin(k3apple/2) ,

598 <strong>Appendix</strong> B<br />

where k (2apple/a)(k1, k2, k3). For the L point of interest to us here: k1 k2 <br />

k3 1/2. Thus g1 cos 3 (apple/4) i sin 3 (apple/4) (1/2 √ 2)(1 i). We can also write<br />

g1 as (1/2) exp(iapple/4).<br />

Note that:<br />

(1) (2.82a) was obtained by assuming that the origin is located at one of the<br />

atoms (atom 1) in the unit cell and the second atom is located at (a/4)(1,1,1).<br />

(2) Vss is negative for all the diamond-type semiconductors according to Table<br />

2.26.<br />

The eigenvalues of the secular equations given above are: Ek Es ±<br />

|Vss||g1|. The lower energy level: E Es |Vss||g1| is identified as the<br />

bonding state. The corresponding wave function will be denoted by: „B <br />

A1|S1〉 A2|S2〉. As in part (a) we substitute Ek E into the above determinant<br />

and obtain the following linear equation for A1 and A2:<br />

A1|Vss||g1| A2Vssg1 0.<br />

Solving the above equation for A2/A1 |g1|/g1 exp(iapple/4) we obtain:<br />

„B (1/ √ 2)[|S1〉 exp(iapple/4)|S2〉].<br />

In principle, the tight-binding wave functions should be expressed in the form<br />

given by (2.74), with the index j running over all the nearest neighbors. To<br />

achieve this we simply note that when k (apple/a)(1, 1, 1) we get: ºsk(1) |S1〉<br />

for atom 1 located at the origin. For atom 2 we get:<br />

ºsk(2) |S2〉[exp(ik · d1) exp(ik · fkd2) exp(ik · d3) exp(ik · d4)]/4<br />

|S2〉[exp(i3apple/4) 3 exp(iapple/4)]/4<br />

exp(iapple/4)|S2〉.<br />

Thus the properly symmetrized tight-binding s-wave function corresponding to<br />

the valence band at the L-point is:<br />

„B (1/ √ 2)[ºsk(1) ºsk(2)] (1/ √ 2)[|S1〉 exp(iapple/4)|S2〉].<br />

By writing the wave function in this way the antisymmetric nature of the wave<br />

function is not obvious. To determine the parity of this wave function we have<br />

to apply the operation I ′ to „B. The effects of I ′ on |S1〉 are: (1) inversion and<br />

(2) translation by the vector T (a/4)(1, 1, 1). As a result of the translation<br />

|S1〉 becomes |S2〉 multiplied by the phase factor exp[ik · T] exp(3applei/4). This<br />

can be written as:<br />

|S1〉<br />

I ′<br />

→ e 3applei/4 |S2〉<br />

On the other hand, the effect of I ′ on |S2〉 is to bring the atom 2 to the origin<br />

or the original position of atom 1 via a translation of (a/4)(1, 1, 1). This<br />

can be represented as:<br />

|S2〉<br />

I ′<br />

→ e 3applei/4 |S2〉

Therefore the result of I ′ on „B is to change it to:<br />

(1/ √ 2)[exp(i3apple/4))|S2〉 exp(iapple/4) exp(i3apple/4)|S1〉]<br />

(1/ √ 2)[ exp(iapple/4))|S2〉 exp(apple)|S1〉]<br />

(1/ √ 2)[exp(iapple/4))|S2〉 |S1〉]<br />

Solution to Problem 2.20 599<br />

„B.<br />

Thus we find the lower energy bonding s-orbital to have odd parity under I ′ .<br />

Again the energy separating the bonding and anti-bonding s-orbitals in Si is<br />

only 2|Vss| 8.13 eV only. But the agreement with the full scale pseudopotential<br />

calculation is better than the result in (a).<br />

(c) One may ask then: what will the electron density look like for the odd<br />

parity (bonding) orbital when k is at the L point? Will this electron density<br />

have a maximum between the two atoms as we would expect for the bonding<br />

state? The answer is yes. To understand why the bonding electronic wave<br />

function has odd parity while the anti-bonding electronic wave function has<br />

even parity we will examine the parity of the zone-center acoustic and optical<br />

phonons in the diamond lattice. In Fig. 2.7 we have shown schematically<br />

the displacement vectors for both phonon modes. We notice that the displacement<br />

vectors point in the same direction for both atoms within the unit cell<br />

in the case of the acoustic phonon. Clearly, if we extrapolate the atomic displacement<br />

to the midpoint between the two atoms it will not be zero. In a<br />

sense the acoustic phonon is the analogue of a bonding electronic state and<br />

yet the acoustic phonon has odd parity under the operation I ′ . On the other<br />

hand, the displacement vectors for the optical phonon point in opposite directions<br />

at the two atoms inside the unit cell. When extrapolated to the midpoint<br />

of the two atoms in the unit cell we expect the phonon wave function should<br />

vanish as in an anti-bonding state but its parity is even under the operation<br />

I ′ . The reason why the parity of these phonon modes seems to be opposite to<br />

what one may expect intuitively lies in the translation by T of the lattice under<br />

the operation I ′ . This translation causes the parity of the phonon modes<br />

to change sign. Without this translation the acoustic phonon parity would indeed<br />

be even while the parity of the optical phonon would be odd. The same<br />

is true for the electron wave functions when k is at the L point. The translation<br />

operation T introduces a phase factor: exp[ik · T] to the electronic wave<br />

functions. When k (apple/a)(1, 1, 1) at the L point, this phase vector is equal to<br />

exp(i3apple/4) and causes the parity of the electron wave function to reverse sign<br />

as shown in (b). Thus the operation T causes both the phonon wave functions<br />

at k 0 and the electronic wave functions for k (apple/a)(1, 1, 1) to reverse<br />

the sign of their parity. This phase factor does not cause a problem when one<br />

consider the “compatibility” between the zone-center and L point electronic<br />

wave functions since this phase factor is zero when k (0, 0, 0). If we start at<br />

k 0 we find that the parity of the bonding state (where the electron density<br />

is non-zero at the mid-point between the two atoms in the unit cell) is even.<br />

The parity of the electronic wave function changes sign as k approaches the L<br />

point but the state remains a bonding state.

600 <strong>Appendix</strong> B<br />

Solution to Problem 3.1<br />

We will first choose the oxygen atom to be at the center of the unit cube as<br />

the origin and then label the six atoms in the primitive unit cell as:<br />

Atom [1] = oxygen atom at (0, 0, 0);<br />

Atom [2] = oxygen atom at (a/2)(1, 1, 1), where a is the size of the unit cube;<br />

Atom [3] = copper atom at (a/4)(1, 1, 1);<br />

Atom [4] = copper atom at (a/4)(1, 1, 1);<br />

Atom [5] = copper atom at (a/4)(1, 1, 1); and<br />

Atom [6] = copper atom at (a/4)(1, 1, 1).<br />

(a) To determine the characters for representations of the zone center (°)<br />

phonon modes we apply first the symmetry elements of the Td group to the<br />

six atoms and in each case count the number of atoms which are unchanged<br />

by the operation. For example, the symmetry operation C2(z) (a 2-fold rotation<br />

about the z-axis) will change atom [2] to the position (a/2)(1, 1, 1)<br />

which differs from its original position by a lattice vector. Because of the periodicity<br />

of the lattice, the atom [2] is considered unchanged. On the other<br />

hand, atoms [3] and [4] obviously will interchange their positions and similarly<br />

for atoms [5] and [6]. Thus, the total number of atoms unchanged by C2(z) is<br />

2 and hence the character of C2(z) is2.<br />

Similarly, the 3-fold rotation (C3) about the [111] axis will leave the oxygen<br />

atoms unchanged while permuting the position of all the copper atoms,<br />

except atom [3]. Thus its character is 3. The reflection md onto the [110] plane<br />

will leave atoms [1], [2], [3] and [4] unchanged while interchanging atoms [5]<br />

and [6] making its character equal to 4. Using similar method the readers can<br />

show easily that the character of the class {S4} is 2.<br />

Next, we consider the symmetry operation I ′ involving inversion followed<br />

by the translation of (a/2)(1, 1, 1). Under this operation the two oxygen atoms<br />

interchange their positions while atom [3] is unchanged. Under I ′ the position<br />

of atom [4] is changed to (a/4)(3, 3, 1). Applying the lattice translation<br />

(a/4)(4, 4, 0) atom [4] is returned to its original position. Similarly the other<br />

copper atoms are unchanged by I ′ so its character is 4.<br />

In summary, the characters of ° for the operations of the Td group and I ′<br />

are given by:<br />

{E} {C2} {S4} {md} {C3} {I ′ }<br />

6 2 2 4 3 4<br />

(b) Based on these characters and Table 2.16 we can determine that ° can be<br />

reduced to the following representations:<br />

2° ∗ 1 ⊕ ° 2 ⊕ ° 5 .<br />

(c) Again using Table 2.16 we can show that:<br />

(2° 1 ⊕ ° 2 ⊕ ° 5 ) ⊗ ° 4 ° 2 ⊕ ° 3 ⊕ 3° 4 ⊕ ° 5 ⊕ ° 5 .<br />

Reference<br />

K. Huang: The long wave modes of the Cu2O lattice. Zeitschrift für Physik, 171, 213–225<br />

(1963)

Solution to Problem 3.2(c)<br />

Solution to Problem 3.2(c) 601<br />

Let us assume that a pair of equal and opposite forces, F and F, are applied<br />

along the [111] direction: F (F/ √ 3)(1, 1, 1). These forces are applied to a<br />

pair of surfaces of area A whose normals are also oriented along the [111]<br />

directions. It is convenient to use a vector parallel to the normal of a surface<br />

to represent both its area and direction. In the case of the surface of a solid<br />

the convention we shall adopt is: a normal pointing away from the solid is<br />

positive. For example, the surface to which the above force F is applied can be<br />

represented by the vector: A (A/ √ 3)(1, 1, 1). Similarly, the force F would<br />

now be applied to a surface, represented by the vector A, on the opposite<br />

side of the solid. The combined effect of F and F would be to stretch the<br />

solid. Since the forces F and F lie along the same axis, the solid is said to be<br />

under a tensile uniaxial stress. The magnitude of the uniaxial stress X is equal<br />

to F/A. However, the stress on a solid cannot be represented, in general, by a<br />

scalar or a vector. Instead, we have to define a second rank tensor Xij, known<br />

as a stress tensor, such that when Xij is contracted with the vector A we obtain<br />

the force F. For the present case of F applied along the [111] direction to the<br />

area represented by A, the component of F along the direction x is Fx <br />

(F/ √ 3). We can decompose A into three mutually perpendicular components:<br />

Ax, Ay and Az. The tensor elements X11, X12 and X13 are defined by: Fx/Ax,<br />

Fx/Ay and Fx/Az, respectively. Since Ax Ay Az for the area A we have<br />

defined above, we expect that X11 X12 X13. Similarly, we find that X21 <br />

X22 X23 and X31 X32 X33. Finally, since Fx Fy Fz we find all the<br />

elements of the stress tensor Xij to be equal: X11 X22 X33 ... etc.. Thus,<br />

the second rank tensor Xij is given by:<br />

⎛ ⎞<br />

1 1 1<br />

C ⎝ 1 1 1⎠<br />

1 1 1<br />

where C is a constant to be determined. To obtain C we note that a contraction<br />

between the stress tensor Xij and the vector A would yield the force F<br />

or XijAj Fi. This implies 3C(A/ √ 3) F/ √ 3orC X/3. Thus, the stress<br />

tensor corresponding to a tensile stress applied along the [111] direction is:<br />

<br />

X<br />

3<br />

⎛ ⎞<br />

1 1 1<br />

⎝ 1 1 1⎠<br />

1 1 1<br />

Notice that our sign convention for the area vector A leads to the following<br />

sign convention for the stress: a tensile stress is positive.<br />

Solution to Problem 3.3<br />

To determine the non-zero and linearly independent components of the compliance<br />

tensor Sijkl we apply symmetry operations of the zincblende structure<br />

to Sijkl.

602 <strong>Appendix</strong> B<br />

As an example, consider a C3 rotation about the [111] axis. The change<br />

in the coordinate axes can be represented as: xyz ⇒ zxy. This operation is<br />

basically a cyclic permutation of the coordinates x, y and z. The fact that<br />

the crystal remains unchanged under this symmetry operation implies that:<br />

Sxxxx Syyyy Szzzz; similarly Sxxyy Szzxx Syyzz and Sxyxy Szxzx Syzyz<br />

and so on.<br />

By applying a reflection onto the (110) plane the coordinate axes are<br />

changed as: xyz ⇒ yxz. This operation essentially interchanges x and y so<br />

that: Sxxyy Syyxx etc and Sxyxy Syxyx, and so on.<br />

The remaining components which contain three identical indices, such as:<br />

Sxxxz, can be shown to be zero by applying the C2 rotation: xyz ⇒ x, y, z.<br />

This operation will change the sign of Sxxxz. The invariance of the crystal under<br />

this operation implies that: Sxxxz Sxxxz 0. The other components,<br />

like Sxxzx, Sxzxx etc., can also be shown to vanish by applying this C2 operation.<br />

Similarly, the remaining components Sxxxy etc., can be shown to vanish<br />

by applying other C2 operations.<br />

Solution to Problem 3.5<br />

By applying the symmetry operations of the zincblende structure to the 4 th<br />

rank stiffness tensor Cijkl as in Problem 3.3, we can show also that:<br />

Cxxxx Cyyyy Czzzz<br />

Cxyxy Cxzxz Cyzyz Cyxyx Czxzx Czyzy<br />

Cxxyy Cyyzz Czzxx Cyyxx Czzyy Cxxzz<br />

Using the same convention as for the compliance tensor in Problem 3.3, the<br />

stiffness tensor can be contracted into a 6 × 6 matrix:<br />

⎛<br />

⎞<br />

C11 C12 C12<br />

⎜ C12 C11 C12<br />

⎟<br />

⎜<br />

⎟<br />

⎜ C12 C12 C11<br />

⎟<br />

⎜<br />

⎟<br />

⎜<br />

C44<br />

⎟<br />

⎝<br />

⎠<br />

C44<br />

C44<br />

The easiest way to obtain the relations between the stiffness and compliance<br />

tensor components would be to assume that a stress belonging to an irreducible<br />

representation of the stress tensor is applied to the crystal. To demonstrate<br />

this procedure, we will consider the stress tensor Xij of a zincblende<br />

crystal. There are 6 linearly independent components in this tensor. Since the<br />

dimension of the irreducible representations of the zincblende crystal is at<br />

most three, this tensor is reducible. In 3.3.1 it has been shown that the second<br />

rank strain tensor eij of the zincblende crystal is reducible to these three<br />

irreducible representations:<br />

eij(°1) e11 e22 e33; eij(°3) e11 e22, e33 (e22 e11)/2 and eij(°4) e12,<br />

e23, e31.

Solution to Problem 3.5 603<br />

Similarly, we expect the stress tensor of the zincblende crystal to be reducible<br />

to three irreducible representations:<br />

Xij(°1) X11 X22 X33; Xij(°3) X11 X22, X33 (X22 X11)/2 and<br />

Xij(°4) X12, X23, X31.<br />

It is easily seen that the °1 component of the stress tensor is a hydrostatic<br />

stress. The two remaining °3 and °4 representations can be shown to correspond<br />

to shear stresses applied along the [100] and [111] axes, respectively.<br />

If we apply stresses represented by these irreducible representations to a<br />

zincblende crystal, the resulting strain tensors will also be irreducible and belong<br />

to the same irreducible representations as the stress tensors. In other<br />

words, the stress and strain tensors of the same irreducible representation<br />

will be related by a scalar. As an example, we apply a hydrostatic stress to<br />

a zincblende crystal. From Problem 3.2 this stress has the form:<br />

⎛<br />

P<br />

X ⎝ 0<br />

0<br />

0<br />

P<br />

0<br />

⎛ ⎞<br />

P<br />

⎞ ⎜ P ⎟<br />

0 ⎜ ⎟<br />

0 ⎠ ⎜ P ⎟<br />

⎜ ⎟<br />

⎜ 0 ⎟<br />

P ⎝<br />

0<br />

⎠<br />

0<br />

where P is the pressure. The resultant strain tensor is given by:<br />

⎛ ⎞ ⎛<br />

P S11 S12 S12<br />

⎜ P ⎟ ⎜ S12<br />

⎜ ⎟ ⎜<br />

⎜ P ⎟ ⎜ S12<br />

e ⎜ ⎟ ⎜<br />

⎜ 0 ⎟ ⎜<br />

⎝<br />

0<br />

⎠ ⎝<br />

S11<br />

S12<br />

S12<br />

S11<br />

S44<br />

0<br />

⎛ ⎞<br />

1<br />

⎜ 1 ⎟<br />

⎜ ⎟<br />

⎜ 1 ⎟<br />

(P)(S11 2S12) ⎜ ⎟<br />

⎜ 0 ⎟<br />

⎝<br />

0<br />

⎠<br />

0<br />

⎛<br />

1<br />

(P)(S11 2S12) ⎝ 0<br />

0<br />

1<br />

⎞<br />

0<br />

0⎠<br />

0 0 1<br />

which belongs to the °1 irreducible representation, as we expect. Thus, the<br />

strain tensor is identical in form to the stress tensor, except for the difference<br />

of a factor of (S11 2S12). If we had started with a strain tensor of the above<br />

form we would have ended with the stress tensor:<br />

S44<br />

S44<br />

⎞<br />

⎟<br />

⎠

604 <strong>Appendix</strong> B<br />

⎛ ⎞ ⎛<br />

1 C11 S12 C12<br />

⎞<br />

⎜ 1 ⎟ ⎜ S12<br />

⎜ ⎟ ⎜<br />

⎜ 1 ⎟ ⎜ C12<br />

X (P)(S11 2S12) ⎜ ⎟ ⎜<br />

⎜ 0 ⎟ ⎜<br />

⎝<br />

0<br />

⎠ ⎝<br />

C11<br />

C12<br />

C12<br />

C11<br />

C44<br />

C44<br />

⎟<br />

⎠<br />

0<br />

⎛ ⎞<br />

1<br />

C44<br />

⎜ 1 ⎟<br />

⎜ ⎟<br />

⎜ 1 ⎟<br />

(P)(S11 2S12)(C11 2C12) ⎜ ⎟<br />

⎜ 0 ⎟<br />

⎝<br />

0<br />

⎠<br />

0<br />

⎛<br />

1<br />

(P)(S11 2S12)(C11 2C12) ⎝ 0<br />

0<br />

1<br />

⎞<br />

0<br />

0⎠<br />

0 0 1<br />

This stress tensor must equal to the one we started with, so we must have<br />

(S11 2S12)(C11 2C12) 1or(C11 2C12) (S11 2S12) 1 .<br />

We need to apply uniaxial shear stress along the two symmetry directions:<br />

[100] and [111] to obtain the two remaining relations between Cij and Sij. Using<br />

again the results of Problem 3.2, we obtain the results that S44C44 1 for<br />

the [111] stress, while for the [100] stress we obtain (S11 S12)(C11 C12) 1.<br />

Solution to Problem 3.6 (a, b and c)<br />

(a) We shall adopt the convention: subscripts 1,2,3 correspond to x, y and z.<br />

Newton’s equation of motion for a small volume ¢x¢y¢z of the<br />

zincblende crystal along the x-axis can be written as:<br />

ρ(¢x)(¢y)(¢z) 2u1 net Force along the x-axis on a<br />

t2 unit volume (¢x)(¢y)(¢z)<br />

<br />

(¢y)(¢z) X11 X11<br />

x ¢x<br />

<br />

X11<br />

<br />

(¢x)(¢z) X12 X12<br />

y ¢y<br />

<br />

X12<br />

<br />

(¢x)(¢y) X13 X13<br />

z ¢z<br />

<br />

X13<br />

where ρ is the density, u (u1, u2, u3) is the displacement vector, t is the time<br />

and Xij is the stress tensor. There are two similar equations for u2 and u3. The<br />

above equation can be reduced to:<br />

ρ 2u1 X11<br />

<br />

t2 x1<br />

X12<br />

<br />

x2<br />

X13<br />

x3<br />

These three equations for u can be simplified as: ρ(2u/t2 ) ∇·X.

Solution to Problem 3.7 (b and c) 605<br />

The stress tensor can be expressed in terms of the strain tensor eij (or ei in<br />

the contracted notation) and the stiffness tensor Cijkl (or Ckl in the contracted<br />

notation). By using the results of Problem 3.5, the stress tensor in zincblende-<br />

type crystals can be expressed as:<br />

⎛<br />

⎞<br />

C11e1 C12e2 C12e3<br />

⎜ C12e1 C11e2 C12e3 ⎟<br />

⎜<br />

⎟<br />

⎜ C12e1 C12e2 C11e3 ⎟<br />

Xij ⎜<br />

⎟<br />

⎜ C44e4 ⎟<br />

⎝<br />

⎠<br />

C44e5<br />

C44e6<br />

Substituting these stress tensor elements into the above equation of motion<br />

for u1 we obtain the following equation:<br />

ρ 2u1 <br />

C11<br />

t2 2u1 x2 <br />

<br />

C44<br />

1<br />

2u1 x2 <br />

2<br />

2u1 x2 <br />

<br />

<br />

(C12 C44)<br />

3<br />

2u2 <br />

x1x2<br />

2 <br />

u3<br />

x1x3<br />

Two similar equations for u2 and u3 can be obtained from the equation of<br />

motions for u2 and u3.<br />

(b) To simulate the LA wave propagating along the [100] direction as a solution,<br />

we assume that u1 u0 exp[i(kx1 ˆt)], u2 0 and u3 0. By substituting<br />

this solution into the above equation for u1 we obtain: ρ(ˆ 2 )u0 <br />

C11(k 2 )u0. Therefore, the LA sound velocity along the [100] axis is given by:<br />

vl (ˆ/k) [C11/ρ] 1/2 .<br />

To obtain a solution representing a TA wave (polarized along the [010]<br />

direction) propagating along the [100] direction we assume that u2 <br />

u0 exp[i(kx1 ˆt)], u1 0 and u3 0. Substituting this solution into the<br />

equation of motion for u2 we obtain: ρ(ˆ 2 )u0 C44(k 2 )u0. Therefore, the<br />

corresponding TA sound velocity is: vt (ˆ/k) [C44/ρ] 1/2 .<br />

(c) To simulate a LA wave traveling along the [111] direction one has to assume<br />

solutions of the form: u1 u2 u3 u0 exp{i[(k/ √ 3)(u1u2u3)ˆt]}.<br />

Again by substituting this solution into the equation of motion for u1 one can<br />

obtain the LA sound velocity. The remaining cases are left as exercises.<br />

Solution to Problem 3.7 (b and c)<br />

(b) To determine the linearly independent and non-zero elements of the stress<br />

tensor in the wurtzite crystal we shall start by examining the stress tensor for<br />

a zincblende crystal and ask: what is the difference in symmetry between the<br />

two structures? We notice that if we choose the c-axis of a wurtzite crystal<br />

to be the z-axis then the properties along the z-axis are different from those<br />

along the x- and y-axes while the properties along the x, y and z directions<br />

are the same in the zincblende crystal. This leads us to conclude that in the<br />

wurtzite crystal the coefficients C11 and C22 are equal but they are not equal<br />

to C33. Similarly, C13 C23 but they are not equal to C12. While C1313

606 <strong>Appendix</strong> B<br />

C2323 C44 but they not necessarily equal to C1212 C66. To obtain the<br />

relation between C1212 and C1111 C2222 we have to consider some symmetry<br />

operations that transform x into y, such as a 3-fold rotation. If we rotate the<br />

coordinate axes by 120 ◦ in the counter-clockwise direction about the z-axis we<br />

will transform the axis (x, y, z) into (x ′ , y ′ , z ′ ) with the transformation matrix:<br />

⎛<br />

⎝ x′<br />

y ′<br />

z ′<br />

⎞ ⎛<br />

<br />

⎠ ⎝<br />

1<br />

√2 3<br />

2<br />

√<br />

3<br />

2<br />

1<br />

2<br />

⎞ ⎛<br />

0<br />

0 ⎠ ⎝ x<br />

⎞<br />

y ⎠<br />

z<br />

0 0 1<br />

or x ′ i aijxj.<br />

The effect of this operation on C1212 is given (as corresponds to a fourth<br />

rank tensor) by: C ′ 1212 a1ka2la1ma2nCklmn, with summation over repeated indices<br />

implied. In principle, the summation has to be performed over all values<br />

of k, l, m and n. This operation is greatly simplified by the observation that<br />

Cklmn is zero for many combination of k, l, m and n. The non-zero summands<br />

are: C1212, C2222, C2121, C1111, C1122, C2211, C1221, C2112, and C1212. In terms of<br />

the contracted notation we obtain:<br />

C ′ 66 C66(a 2 11a222 a212a221 2a11a22a12a21)<br />

C11(a 2 12a222 a211a221 ) C12(2a11a22a12a21)<br />

Substituting in the transformation coefficients aij, etc. we find:<br />

C ′ 66 C66[(1/4)(1/4) (3/4)(3/4) 2(1/4)(3/4)]<br />

C11[(3/4)(1/4) (1/4)(3/4)] C12[(1/4)(3/4) (1/4)(3/4)]<br />

C66(4/16) C11(6/16) C12(6/16).<br />

Since the crystal is invariant under this operation, we expect C ′ 66 C66. By<br />

substituting this result back into the above equation for C ′ 66 we obtain: C66 <br />

(1/2)(C11 C12).<br />

(c) We shall again adopt a coordinate system in which the z-axis is parallel to<br />

the c-axis of the wurtzite crystal. The subscripts 1, 2, 3 will correspond to x, y<br />

and z.<br />

Newton’s Equation of motion for a small volume xyz of the wurtzite crystal<br />

along the x-axis can be written as:<br />

ρ(¢x)(¢y)(¢z) 2u1 net Force along the x-axis on a<br />

t2 unit volume (¢x)(¢y)(¢z)<br />

<br />

(¢y)(¢z) X11 X11<br />

x ¢x<br />

<br />

X11<br />

<br />

(¢x)(¢z) X12 X11<br />

y ¢y<br />

<br />

X12<br />

<br />

(¢x)(¢y) X13 X13<br />

z ¢z<br />

<br />

X13<br />

where ρ is the density, u (u1, u2, u3) is the displacement vector, t is the time<br />

and Xij is the stress tensor. There are two other similar equations for u2 and

u3. The above equation can be reduced to:<br />

Solution to Problem 3.8 (a, c and d) 607<br />

ρ 2u1 X11<br />

<br />

t2 x1<br />

X12<br />

<br />

x2<br />

X13<br />

x3<br />

Using the results of part (b) the stress tensor can be expressed in terms of the<br />

strain tensor eij (or ei in the contracted notation) and the stiffness tensor Cijkl<br />

(or as Ckl in the contracted notation) as:<br />

⎛<br />

⎞<br />

C11e1 C12e2 C13e3<br />

⎜ C12e1 C11e2 C13e3 ⎟<br />

⎜<br />

⎟<br />

⎜ C13e1 C13e2 C33e3 ⎟<br />

Xij ⎜<br />

⎟<br />

⎜ C44e4 ⎟<br />

⎝<br />

⎠<br />

C44e5<br />

C11C12<br />

2<br />

e6<br />

Substituting these stress tensor elements into the equation of motion we obtain<br />

the following equation:<br />

ρ 2u1 <br />

C11<br />

t2 2u1 x2 <br />

1<br />

C11 C12 <br />

2<br />

2u1 x2 <br />

C44<br />

2<br />

2u1 x2 <br />

3<br />

C11 C12<br />

2<br />

(C13 C44) 2 u3<br />

x1x3<br />

with two similar differential equations for u2 and u3.<br />

Solution to Problem 3.8 (a, c and d)<br />

2 u2<br />

x1x2<br />

(a) In Prob. 3.4 (b) it was shown that a tensile uniaxial stress X applied along<br />

the [100] axis of a zincblende crystal will induce a strain tensor of the form:<br />

⎛<br />

˜e ⎝ S11X<br />

⎞<br />

0 0<br />

0 S12X 0 ⎠ .<br />

0 0 S12X<br />

This matrix can be decomposed into its irreducible components consisting of<br />

two matrices:<br />

a diagonal matrix (belonging to the °1 irreducible representation) of the form:<br />

⎛ ⎞<br />

1 0 0<br />

˜ehydrostatic ⎝ 0 1 0⎠<br />

(S11 2S12)(X/3)<br />

0 0 1<br />

which represents a hydrostatic strain; and the traceless matrix (belonging to<br />

the °3 irreducible representation):<br />

⎛<br />

⎞<br />

2 0 0<br />

˜eShear ⎝ 0 1 0 ⎠ (S11 S12)(X/3) .<br />

0 0 1<br />

This decomposition allows us to simplify the evaluation of the strain Hamltonian<br />

HPB in (3.23). [note that there is a difference of a factor of 3 in the second

608 <strong>Appendix</strong> B<br />

and third terms containing the deformation potentials b and d in (3.23) in the<br />

first and second editions, depending on definition].<br />

Since the first term in (3.23) contains the trace of the strain tensor,<br />

the traceless shear strain tensor ˜eshear does not contribute to this term and<br />

we obtain from the hydrostatic strain tensor ˜ehydrostatic a term of the form:<br />

a(S11 2S12)X. Similarly, the hydrostatic strain tensor will not contribute to<br />

the shear part of the Hamiltonian HPB. On the other hand, the contribution<br />

of the shear strain tensor to HPB is simply:<br />

(b)(S11 S12)(X/3)[(J 2 x J2 /3)2 (J 2 y J2 /3) (J 2 z J2 /3)]<br />

(b/3)(S11 S12)X[2J 2 x J2 y J2 z ]<br />

b(S11 S12)X[J 2 x (J2 /3)]<br />

Combining the above results we find that the form of the strain Hamiltonian<br />

for uniaxial stress along the [100] direction is:<br />

HPB(X) a(S11 2S12)X b(S11 S12)X[J 2 x (J2 /3)] .<br />

(c) To calculate the splitting in the J 3/2 states due to the uniaxial stress<br />

X along the [100] direction we note that the hydrostatic component of the<br />

stress Hamiltonian: a(S11 2S12)X will shift all the J 3/2 states by the same<br />

amount so we can neglect this term in calculating the splitting. From the form<br />

of the shear component of the stress Hamiltonian: b(S11 S12)X[J 2 x (J2 /3)]<br />

it is clear that the two mJ ±3/2 states will remain degenerate while the<br />

two mJ ±1/2 states also will not be split by the stress. Thus, we need only<br />

calculate the eigenvalues of b(S11 S12)X[J 2 x (J2 /3)] for the mJ 3/2 and 1/2<br />

states. Noting that:<br />

while<br />

〈3/2, 3/2|J 2 x|3/2, 3/2〉 (3/2) 2 9/4 and 〈3/2, 1/2|J 2 x|3/2, 1/2〉 (1/2) 2 1/4<br />

〈3/2, 3/2|J 2 |3/2, 3/2〉 (3/2)(5/2) 15/4 〈3/2, 1/2|J 2 |3/2, 1/2〉<br />

we obtain the following results:<br />

〈3/2, 3/2|b(S11 S12)X[J 2 x (J2 /3)]|3/2, 3/2〉<br />

b(S11 S12)X〈3/2, 3/2|J 2 x (J2 /3)|3/2, 3/2〉<br />

b(S11 S12)X[(9/4) (5/4)]<br />

b(S11 S12)X<br />

and similarly<br />

b(S11 S12)X〈3/2, 1/2|J 2 x (J2 /3)|3/2, 1/2〉<br />

b(S11 S12)X[(1/4) (5/4)] b(S11 S12)X .<br />

Thus the splitting between the mJ ±3/2 states and mJ ±1/2 states induced<br />

by the [100] uniaxial stress is: 2b(S11 S12)X.<br />

The results for the [111] uniaxial stress can be obtained similarly.

Solution to Problem 3.8 (a, c and d) 609<br />

(d) In case the spin orbit-coupling is zero, the Pikus-Bir Hamiltonian can be<br />

written as:<br />

<br />

L 2 L2<br />

x <br />

HPB a(exx eyy ezz) 3b ∗<br />

exx c.p.<br />

3<br />

6d∗<br />

<br />

1<br />

√<br />

3 2 (LxLy<br />

<br />

Lylx)exy c.p. .<br />

By repeating the calculation in (a) we obtain for [100] stress:<br />

HPB(X) a(S11 2S12)X 3b ∗ (S11 S12)X[L 2 x (L2 /3)] .<br />

The matrix elements corresponding to those in part (c) are:<br />

while<br />

〈1, 1|L 2 x|1, 1〉 〈1, 1|L 2 x|1, 1〉 1 and 〈1, 0|L 2 x|1, 0〉 0<br />

〈1, 1|L 2 |1, 1〉 〈1, 1|L 2 |1, 1〉 〈1, 0|L 2 |1, 0〉 2.<br />

Clearly, the mL ±1 states remain degenerate while these two states are split<br />

from the mL 0 state by the uniaxial stress. Calculating the matrix elements<br />

for the Pikus-Bir Hamiltonian we obtain:<br />

〈1, 1|3b ∗ (S11 S12)X[L 2 x (L2 /3)]|1, 1〉 3b ∗ (S11 S12)X[1 (2/3)]<br />

b ∗ (S11 S12)X<br />

and<br />

〈1, 0|3b ∗ (S11 S12)X[L 2 x (L2 /3)]|1, 0〉 3b ∗ (S11 S12)X[0 (2/3)]<br />

2b ∗ (S11 S12)X .<br />

Thus the three L 1 states split into a doublet (mL ±1 states) and a singlet<br />

(mL 0) with the energy of the splitting equal to 3b∗ (S11 S12)X.<br />

The reason why the stress induced splitting depends on the angular momentum<br />

can be traced to the degeneracy of the initial states. In case of semiconductors<br />

with a large spin-orbit coupling we can assume that the spin-orbit<br />

splitting ¢ will be much larger than the stress-induced splitting. Thus the initial<br />

state J 3/2 before stress is applied is 4-fold degenerate. [100] uniaxial stress<br />

splits these states into two doublets with a splitting equal to 2b(S11S12)X. On<br />

the other hand, if we neglect spin-orbit coupling then the initial state L 1is<br />

six-fold degenerate (including spin). [100] uniaxial stress splits them into two<br />

pairs of degenerate states (one is a spin doublet while the other is a fourfold<br />

degenerate state when spin degeneracy is included) with total splitting<br />

3b∗ (S11 S12)X. Thus, the splitting is larger than that for the J 3/2 states by<br />

a factor of (3/2) which is equal to the ratio of the degeneracy of their initial<br />

states.<br />

We have assumed in this book the general case where b and b∗ , d and d∗ may be different. Usually we can assume that the spin-orbit coupling is not dependent<br />

on strain. In this case, within this approximation b b∗ and d d∗ .<br />

It is with this approximation in mind that the strain Hamiltonians with and<br />

without the spin-orbit coupling are defined with a difference of a factor of 3<br />

in the shear terms.

610 <strong>Appendix</strong> B<br />

Note that in real situations one often has to diagonalize the Pikus-Bir<br />

Hamiltonian by assuming that the unperturbed states include both the J 3/2<br />

and J 1/2 states. In this case one can use the large spin-orbit coupling approximation<br />

only for low stress to obtain the linear stress-induced splitting<br />

2b(S11 S12)X. For high uniaxial stress the mJ ±1/2 states of both the<br />

J 3/2 and J 1/2 states will be coupled by the stress Hamiltonian and one<br />

obtains a nonlinear stress dependence of their energies. Students are urged to<br />

derive the 6×6 matrices for the two cases of a [100] and a [111] uniaxial stress<br />

and then diagonalize these matrices to obtain the stress dependent energies of<br />

the J 3/2 and 1/2 states.<br />

Solution to Problem 3.9<br />

From (2.84a) and (2.94b) we can express the zone-center conduction and valence<br />

band energies Ec and Ev as:<br />

Ec Es Es |Vss| and Ev Ep Ep |Vxx| .<br />

If we assume that both |Vss| and |Vxx| depend on the nearest neighbor distance<br />

d as d 2 and d is related to the lattice constant a by d (a/4) √ 3 then<br />

¢Vss<br />

Vss<br />

¢Vxx<br />

Vxx<br />

2 ¢a<br />

a 2<br />

3<br />

¢V<br />

V<br />

where ¢V<br />

V<br />

is the volume dilation.<br />

It can be expressed in terms of the trace of the strain tensor e : ¢V/V <br />

Trace(e). We can express the above results as:<br />

¢Ec <br />

2<br />

3<br />

<br />

|Vss|Trace(e); and ¢Ev <br />

2<br />

3<br />

<br />

|Vxx|Trace(e).<br />

The relative deformation potential (ac av) is then given by: ¢Ec ¢Ev <br />

(ac av)Trace(e) (2/3)[|Vss| |Vxx|]Trace(e). Hence the relative deformation<br />

potential (ac av) is given by: (2/3)[|Vss| |Vxx|].<br />

In the following table we compare the values of (ac av) inC,SiandGe<br />

obtained from the tight binding parameters in Table 2.26 and compare them<br />

with experimental values (all energies in units of eV).<br />

|Vss| |Vxx| (ac av)theoretical (ac av)experimental<br />

C 15.2 3.0 12.1<br />

Si 8.13 3.17 7.53 10<br />

Ge 6.78 2.62 6.07 12<br />

While this approach gives the right order of magnitude and sign for the deformation<br />

potentials, it is not accurate enough. As seen in the cases of Si and Ge<br />

the values obtained from the model are smaller than the experimental values<br />

by about a factor of two.

Solution to Problem 3.11(a,b and c)<br />

Solution to Problem 3.11(a,b and c) 611<br />

(a) By definition, a strain tensor e will induce a change in the vector r inside a<br />

crystal by an amount ¢r given by: ¢r r · e. Suppose a pure [111] shear strain<br />

is defined by the strain tensor:<br />

⎛ ⎞<br />

0 1 1<br />

e ‰ ⎝ 1 0 1⎠<br />

1 1 0<br />

For the vector d1 (a/4)(1, 1, 1) the change ¢d1 induced by e is equal to:<br />

<br />

a‰<br />

¢d1 <br />

4<br />

⎛ ⎞ ⎛<br />

0 1 1<br />

⎝ 1 0 1⎠⎝<br />

1 1 0<br />

1<br />

⎞<br />

<br />

1 ⎠<br />

a‰<br />

a‰<br />

(2, 2, 2) (1, 1, 1) .<br />

4<br />

2<br />

1<br />

For the vector d2 (a/4)(1, 1, 1) the change ¢d2 induced by e is equal to:<br />

<br />

a‰<br />

¢d2 <br />

4<br />

⎛ ⎞ ⎛<br />

0 1 1<br />

⎝ 1 0 1⎠⎝<br />

1 1 0<br />

1<br />

⎞<br />

<br />

<br />

1 ⎠<br />

a‰<br />

a‰<br />

(2, 0, 0) (1, 0, 0) .<br />

4<br />

2<br />

1<br />

Thus, an atom located at d1 in the unstrained solid will be displaced, in the<br />

strained solid, to d ′ 1 d1 ¢d1 (a/4)(1, 1, 1) (a‰/2)(1, 1, 1) (a/4)(1 <br />

2‰)(1, 1, 1) while another atom at d2 will be displaced to d ′ 2 d2 ¢d2 <br />

(a/4)(1, 1, 1) (a‰/2)(1, 0, 0) (a/4)(1 2‰, 1, 1).<br />

The displaced vectors d ′ 3 and d′ 4 can be calculated in a similar manner.<br />

Note that if we define a bond by connecting an atom located at the origin to<br />

the atom at d1 this bond will be stretched by the positive strain. On the other<br />

hand, the bonds to the other 3 atoms will be bent.<br />

(b) From the results in (a) it is clear that the ratio ¢d1/d1 (2‰) where<br />

¢d2 |d ′ 2| 2 |d2| 2 <br />

a<br />

√ <br />

a<br />

√ <br />

a<br />

<br />

√<br />

3 4‰ 3 ≈ 3 1<br />

4<br />

4 4<br />

2‰<br />

<br />

a<br />

√<br />

3.<br />

3 4<br />

or ¢d2/d2 (2‰/3). Furthermore, the direction of d ′ 2 is no longer parallel to<br />

d2.<br />

(c) To calculate the matrix elements in the strained crystal we will consider<br />

first the matrix element V ′ xx . For atom 1 located at d1 we can express the<br />

matrix element V ′ xx (1) as:<br />

V ′ xx (1) cos 2ı′ 1x V′ ppÛ sin 2ı′ 1x V′ ppapple<br />

where ı ′ 1x is the angle between the x-axis and the vector d′ 1 ; V′ ppÛ and V′ ppapple are<br />

the overlap parameters in the strained crystal. In the case of atom 1 the angle<br />

ı ′ 1x is the same as in the unstrained crystal so that cos 2ı′ 1x cos 2ı1x 1/3.<br />

Assuming that the overlap integral scales with atomic separation d as 1/d 2 ,<br />

both V ′ ppÛ and V′ ppapple are related to the overlap parameters VppÛ and Vppapple in<br />

the unstrained crystal by the factor [1 2(¢dl/d1)] [1 4‰]. Thus, we obtain:<br />

V ′ xx (1) (1/3)[VppÛ 2Vppapple][1 4‰]

612 <strong>Appendix</strong> B<br />

The calculation for V ′ xx (2) is essentially similar except that the angle ı′ 2x<br />

equal to ı2x. Instead<br />

cos ı ′ 2x<br />

1 2‰<br />

√ 3 4‰ .<br />

is not<br />

If we expand cos ı ′ 2x to the lowest order in ‰ we get: cos 2ı′ 2x ∼ (1/3)[1 <br />

(8‰/3)]. Using this result we can show that:<br />

V ′ <br />

xx (2) 1 2¢d2<br />

<br />

VppÛ<br />

1 <br />

d2 3<br />

8‰<br />

<br />

<br />

3<br />

2Vppapple<br />

<br />

1 <br />

3<br />

4‰<br />

<br />

3<br />

≈ VppÛ<br />

<br />

1 <br />

3<br />

4‰<br />

<br />

<br />

3<br />

2Vppapple<br />

<br />

1 <br />

3<br />

8‰<br />

<br />

3<br />

Similarly V ′ xx (3) V′ xx (4) can be shown to be given by:<br />

V ′ <br />

VppÛ<br />

xx (3) ≈ 1 <br />

3<br />

8‰<br />

<br />

<br />

3<br />

2Vppapple<br />

<br />

1 <br />

3<br />

2‰<br />

<br />

.<br />

3<br />

Finally<br />

V ′ xx <br />

4<br />

i1<br />

V ′ VppÛ 8Vppapple<br />

xx (i) <br />

3 3 O(‰2 ) ≈ Vxx .<br />

This proves that the deformation changes V ′ xx only by amounts that are of<br />

second order in ‰. This is not true for V ′ xy . To calculate the corresponding<br />

results for V ′ xy we can first show that: V′ xy (1) cos ı′ 1x cos ı′ 1y (V′ ppÛ V′ ppapple )<br />

where cos ı ′ 1x cos ı′ 1y 1/3. Thus we can show that V′ 1y (l) ∼ (l 4‰)(VppÛ <br />

Vppapple)/3 to the lowest order in ‰. The other matrix elements V ′ xy (2), V′ xy (3) and<br />

(4) can be calculated similarly. In particular the reader should show that:<br />

V ′ xy<br />

cos ı ′ 2y <br />

1<br />

√<br />

3 4‰<br />

so that cos ı ′ 2x cos ı′ 2y (1/3)[1 (2‰/3)] cos ı′ 3x cos ı′ 3y and<br />

cos ı ′ 4x cos ı′ 4y<br />

(1/3)[1 (4‰/3)] all to the lowest order in ‰. Combining these<br />

results one obtains<br />

V ′ xy ≈ 8‰<br />

9 (VppÛ Vppapple).<br />

In this way one can obtain the 6 × 6 determinant on p. 152. The solutions to<br />

the rest of this problem can be obtained by following the directions given in<br />

the problem.<br />

Solution to Problem 3.15<br />

We note first that the third rank electromechanical tensor (em)ijk is symmetric<br />

with respect to interchange of the indices i and j.<br />

(a) By applying the symmetry operations of the zincblende crystal to this third<br />

rank tensor as in Problem 3.5 we can show that:

Solution to Problem 3.16 613<br />

(1) All the components containing two identical indices, such as (em)xxy and<br />

(em)yyy, must be zero by applying the C2 rotations.<br />

(2) This leaves as the only non-zero elements to be those where all the three<br />

indices are different, such as (em)xyz (or (em)14 in the contracted notation).<br />

By applying C3 operations then all the non-zero elements can be shown to<br />

be identical.<br />

The form of the electromechanical tensor in the zincblende crystal can be expressed<br />

as a 3 × 6 matrix of the form:<br />

⎛<br />

⎝ 0 0 0 (em)14 0 0<br />

0 0 0 0 (em)14 0<br />

0 0 0 0 0 (em)14<br />

⎞<br />

⎠<br />

(b) Repeating the calculation by applying the symmetry operations of the<br />

wurtzite structure (assuming that the c-axis of wurtzite is chosen as the z-axis)<br />

we can show that the components (em)ijk containing x and y as indices satisfy<br />

the same constraint as in the zincblende crystal. This means: (em)xxx and<br />

(em)yyy are both zero but not (em)zzz ( (em)33). Similarly (em)xxy and (em)yyx<br />

are both zero but not (em)xxz and (em)yyz (these two components are both<br />

equal to (em)15) while (em)zxx and (em)zyy are also not zero (both equal to<br />

(em)31). However, there is now a new symmetry operation involving reflection<br />

onto the zy plane. This symmetry operation will change the sign of x while<br />

leaving those of y and z unchanged. As a result of this symmetry operation,<br />

the components (em)xyz etc., are now all zero. Thus (em) in wurtzite crystals<br />

can be expressed as:<br />

⎛<br />

⎝ 0 0 0 0 (em)15<br />

⎞<br />

0<br />

0 0 0 (em)15 0 0⎠<br />

(em)31 (em)31 (em)33 0 0 0<br />

Solution to Problem 3.16<br />

Using the result of Prob. 3.15 we will assume that the non-zero and linearly<br />

independent elements of the electromechanical tensor em in wurtzite crystals<br />

have the contracted form:<br />

⎛<br />

⎞<br />

em <br />

⎝ 0 0 0 0 e15 0<br />

⎠<br />

0 0 0 e15 0 0<br />

e31 e31 e33 0 0 0<br />

In the contracted notation the strain tensor e corresponding to a phonon with<br />

displacement vector u and wavevector q is given by:

614 <strong>Appendix</strong> B<br />

⎛ ux<br />

⎞<br />

⎜ x ⎟<br />

⎜ uy<br />

⎟<br />

⎜ ⎟<br />

⎜ y ⎟<br />

⎜ ⎟<br />

⎜ uz ⎟<br />

⎜ ⎟<br />

⎜ z ⎟<br />

e ⎜ ⎟<br />

⎜ uy uz ⎟<br />

⎜ ⎟<br />

⎜<br />

z x ⎟<br />

⎜ ux uz ⎟<br />

⎜<br />

⎟<br />

⎜ z x ⎟<br />

⎝ ux uy ⎠<br />

<br />

y x<br />

Once the strain tensor and the electromechanical tensor are known the polarization<br />

P induced by the strain can be calculated from the definition:<br />

Pi (e)ijej while the electric field E is related to P by: E ( 4appleP<br />

Â ), Â being<br />

the dielectric constant.<br />

To simply the notation we can assume that the z-axis is parallel to the<br />

c-axis of the wurtzite structure and the y-axis lies in the z-q plane so that<br />

q (0, q sin ı, q cos ı). With this notation we obtain the strain tensor as:<br />

⎛<br />

⎞<br />

0<br />

⎜ iuyq sin ı ⎟<br />

⎜<br />

⎟<br />

⎜ iuzq cos ı ⎟<br />

e ⎜<br />

⎟<br />

⎜ iq(uz sin ı uy cos ı) ⎟<br />

⎝<br />

iuxq cos ı<br />

⎠<br />

iuxq sin ı<br />

From this strain tensor we obtain the polarization:<br />

P e15iqux cos ı, e15iq(uz sin ı uy cos ı), iq(e31uy sin ı e33uz cos ı) <br />

and hence the electric field.<br />

In particular we are interested in the longitudinal component of this piezoelectric<br />

field since this will couple most strongly to an electron. The longitudinal<br />

electric field El is given by the projection of E along q:<br />

E · q<br />

El <br />

q<br />

4appleiq<br />

e15 sin ı(uz sin ı uy cos ı) e31uy cos ı sin ı e33uz cos<br />

Â<br />

2 ı <br />

From this longitudinal field we can define a scalar potential V such that<br />

Hpiezoelectric |e|V<br />

4apple|e| <br />

e15 sin ı(uz sin ı uy cos ı) e31uy cos ı sin ı e33uz cos<br />

Â<br />

2 ı <br />

Note that a factor of 4apple may be missing in some earlier editions of the book.

Solution to Problem 3.17<br />

Solution to Problem 3.17 615<br />

In real crystals the ionic interaction Hamiltonian (Hion in Eq. (3.1)) is a complicated<br />

function of the ion positions Rj. If one expands this Hamiltonian<br />

about the equilibrium positions Rj0 the expansion will contain terms of higher<br />

order than the second order term (‰Rj0) 2 . These higher order terms are known<br />

as anharmonic terms. When these anharmonic terms are present, the phonon<br />

modes calculated without them are no longer true normal modes of the crystal.<br />

One consequence of the lattice anharmonicity is that the phonons will decay<br />

via phonon-phonon interaction. For example, the third-order anharmonic<br />

term: (‰Rj0) 3 will allow a phonon to decay into two phonon modes. The anharmonic<br />

terms are important in determining the mean-free path of phonons<br />

and hence the thermal conductivity of a crystal (see, for example, Chapter 5<br />

of C. Kittel, Introduction to Solid State Physics, Wiley & Sons, New York).<br />

Another important effect of the lattice anharmonicity is to cause thermal expansion<br />

of the lattice. This effect will be discussed in part (b) of this problem.<br />

One not so obvious effect of the anharmonic terms is to effect a change of<br />

the phonon frequency with the equilibrium lattice volume. To understand this<br />

result we will consider the simple case of a one-dimensional anharmonic oscillator.<br />

The energy of this oscillator can be expanded around any point x0 as a<br />

Taylor series:<br />

E(x) E(x0) <br />

<br />

dV<br />

(x x0) <br />

dx x0<br />

<br />

1<br />

2<br />

<br />

d2V dx2 <br />

x0<br />

(x x0) 2 ... (3.17.1)<br />

In this expression V is the potential energy of the oscillator. If x0 is the equilibrium<br />

position of theoscillator, the linear term will vanish for x x0 and<br />

d<br />

the second derivative:<br />

2V dx2 <br />

becomes the spring constant (to be denoted<br />

x0<br />

by k). Often it is assumed that k is independent of x0. Suppose k is a function<br />

of x0. Since the frequency ˆ of the oscillator is related to k and the reduced<br />

mass m by ˆ (k/m) 1/2 , the fact that k changes with x0 implies that the frequency<br />

of oscillation also changes with x0.<br />

Next we continue the expansion of E(x) to the third order term: a(xx0) 3 ,<br />

which represents the anharmonic component of the potential. We assume that<br />

the constant a is small so that for small displacements (x x0) the potential is<br />

almost harmonic. This is known as the quasi-harmonic approximation. What it<br />

means is that: in the vicinity of x0 the potential is dominated by the quadratic<br />

term: (x x0) 2 and is, therefore, almost harmonic. Suppose we now change<br />

(say via a small pressure) the equilibrium position of the oscillator from x0 to<br />

x0 ‰. For weak anharmonicity we can assume that the constants k and a of<br />

the potential are not changed by ‰.The energy of the oscillator is now given<br />

by:<br />

E ′′ (x) E(x0 ‰) (k/2)(x x0) (1/3!)a(x x0) 3 . (3.17.2)

616 <strong>Appendix</strong> B<br />

(a) The mode Grüneisen parameter Áˆ of a phonon mode is defined as:<br />

Áˆ d(ln ˆ)/d(ln v) where v is the volume of the crystal. In the following<br />

table we list the mode Grüneisen parameter for various phonon modes in<br />

semiconductors.<br />

Table 1 of Problem 3.17. Mode Grüneisen parameter of phonons in selected diamondand<br />

zincblende-type semiconductors (TO transverse optical phonon, LO longitudinal<br />

optical phonon, TA transverse acoustic phonon and LA longitudinal acoustic<br />

phonon).<br />

Semiconductors Zone Center<br />

Phonons<br />

Zone Edge Phonons<br />

TO LO L X<br />

Si 0.98 0.9(LA) 1.3(TA) 0.9(LA) 1.4(TA)<br />

Ge 1.12 1.53(TA)<br />

GaAs 1.39 1.23 1.5(TO) 1.7(TA) 1.73(TO) 1.62(TA)<br />

GaP 1.09 0.9 1.5(TO) 0.81(TA) 1.0(LA) 0.72(TA)<br />

InP 1.44 1.24 1.4(TO) 2.0(TA) 1.4(TO) 2.1(TA)<br />

ZnS 0.95 1.0(TO) 1.5(TA) 1.0(TO) 1.2(TA)<br />

ZnTe 1.7 1.2 1.7(LO) 1.0(TA) 1.8(LO) 1.55(TA)<br />

The experimental values contained in this table are obtained from:<br />

B.A. Weinstein and R. Zallen: Pressure-Raman Effects in Covalent and Molecular Solids<br />

in Light Scattering in Solids IV, edited by Cardona and G. Güntherodt (Springer-Verlag,<br />

Berlin, 1984) p. 463–527. Citations to the original publications for these values can be<br />

found in this article’s references.<br />

This table shows that for most diamond- and zincblende-type semiconductors<br />

the value of Áˆ for the optical phonons is around 1, although it can be as large<br />

as 1.7 in ZnTe. However, the value of Áˆ is usually negative for the zoneedge<br />

TA phonons. This is related to the fact that the diamond and zincblende<br />

lattices are unstable against shear distortion except for the restoring forces due<br />

to the bond charges (see Section 3.2.4).<br />

(b) The linear thermal expansion coefficient · of a solid is defined usually as:<br />

· 1<br />

<br />

L<br />

where L is the length of the solid, T the temperature and P<br />

L T P<br />

the pressure. It is related to the volume thermal coefficient of expansion ‚ by<br />

the expression:<br />

‚ 1<br />

<br />

v<br />

3·<br />

v T P<br />

where v is the volume of the solid. To relate ‚ to the mode Grüneisen parameter<br />

of the solid we start with the thermodynamic relation between the<br />

pressure P and the Helmholtz free energy F:<br />

<br />

F<br />

P .<br />

v T<br />

For a semiconductor, where there are no free electrons, the free energy contains<br />

mainly two contributions: one, which we shall denote as º, is due to the

Solution to Problem 3.17 617<br />

forces holding the atoms together, and a second one stems from the vibration<br />

of the atoms. Since phonons are bosons (like photons), the calculation of<br />

the free energy term due to phonons is the same as that for photons and can<br />

be found in many standard textbooks on statistical mechanics (see, for example,<br />

C. Kittel and H. Kroemer: Thermal Physics, second edition. Freeman, San<br />

Francisco, 1980. p. 112). The contribution Fvib to the total free energy from<br />

the phonons can be calculated from the partition function Zvib of phonons:<br />

Fvib kBT ln Zvib where kB is the Boltzmann’s constant and<br />

Zvib <br />

1 (n<br />

e 2)<br />

i,n<br />

ˆi <br />

kBT e<br />

i<br />

ˆi 1<br />

2kBT 1 e ˆ <br />

i<br />

kBT 1<br />

(3.17.3)<br />

ˆi<br />

i 2 sinh<br />

2kBT<br />

with the summation i over all the phonon modes.<br />

From this partition function we obtain:<br />

Fvib kBT <br />

<br />

ˆi<br />

ln 2 sinh<br />

(3.17.4)<br />

2kBT<br />

i<br />

The energy º is assumed now to be a function of v only. Using (3.17.4) for<br />

Fvib we obtain an expression for P:<br />

<br />

dº<br />

P kBT<br />

dv<br />

<br />

<br />

ˆi dˆi<br />

coth<br />

(3.17.5)<br />

2kBT 2kBT dv<br />

i<br />

To simplify this expression we assume that the mode Grüneisen parameters<br />

for all the phonon modes are roughly the same and can be approximated by<br />

an average Grüneisen parameter 〈Á〉 ∼d(ln ˆi)/d(ln v) for all phonon modes.<br />

Within this approximation the expression for P simplifies to:<br />

<br />

dº 〈Á〉 <br />

<br />

ˆi ˆi<br />

P ≈ <br />

coth<br />

(3.17.6)<br />

dv v<br />

2kBT 2<br />

i<br />

i<br />

The average energy (like the average energy for photons) of a phonon mode<br />

with frequency ˆ is given by:<br />

U(ˆ) {n(1/2)}(ˆ) where n is the phonon occupancy or Bose-Einstein<br />

distribution function (see p. 126), given by: n [exp(ˆ/kBT)1] 1 . Using the<br />

result that {n (1/2)} (1/2) coth[(ˆ/2kBT)] we obtain:<br />

<br />

<br />

ˆi ˆi<br />

coth<br />

U (3.17.7)<br />

2kBT 2<br />

where U represents the internal energy of the crystal due to vibrational modes<br />

only. Hence we arrive at:<br />

P (dº/dv) 〈Á〉U/v (3.17.8)<br />

We can regard this relation between P and v as an equation-of-state of the<br />

crystal.<br />

Using this equation we can obtain the relation between the coefficient of<br />

thermal expansion ‚ and 〈Á〉 under a quasi-harmonic approximation. In this

618 <strong>Appendix</strong> B<br />

approximation we can expand the term º(v) as a function of v about the equilibrium<br />

volume v0 and keep only terms up to the quadratic term:<br />

º(v) ∼ º(v0) (dº/dv)v0 (v v0) (1/2)(d 2 º/dv 2 2<br />

)V0 (v v0)<br />

(3.17.9)<br />

By definition, the linear term (dº/dv)V0 vanishes at the equilibrium volume so<br />

we can take the derivative of º(v) with respect to v and obtain:<br />

(dº/dv) ∼ (d 2 º/dv 2 )v0 (v v0) . (3.17.10)<br />

On the other hand, if we have started from (3.17.8) and take the derivative<br />

with respect to v at equilibrium volume then we would obtain:<br />

(dP/dv)V0 ∼ (d2 º/dv 2 )v0 (3.17.11)<br />

by noting that U is proportional to v. (3.17.11) can be simplified by introducing<br />

the isothermal compressibility Î0 (1/v0)(dv/dP)T. The bulk modulus B<br />

defined on Page 139 is related to Î by: B 1/Î. With this simplification we<br />

arrived at:<br />

(dP/dv)T 1/Î0v0 . (3.17.12)<br />

Combining (3.17.10) – (3.17.12) we obtain:<br />

(dº/dv) (dP/dv)V0 (v v0) (v v0)/Î0v0<br />

(3.17.13)<br />

On substituting (3.17.13) back into (3.17.8) we obtain the equation-of-state<br />

within the quasi-harmonic approximation:<br />

P (v v0)/Î0v0 〈Á〉U/v . (3.17.14)<br />

This equation was first derived by Mie and later by Grüneisen.<br />

To obtain the coefficient of thermal expansion ‚ (1/v)(v/T)P we take<br />

the partial derivative of (3.17.14) with respect to T while keeping P constant:<br />

0 ‚v<br />

<br />

〈Á〉 <br />

Î0v0<br />

‚U<br />

<br />

U<br />

‚ <br />

v v T<br />

1<br />

<br />

U<br />

. (3.17.15)<br />

v T v<br />

The quantities inside the braces can be expressed in terms of measurable<br />

quantities, such as the heat capacity. For example, the constant volume heat<br />

capacity Cv is equal to (U/T)V. By differentiating the equation (3.17.7) for<br />

U with respect to v, we can show that:<br />

(U/v)T (〈Á〉CvT/v) (〈Á〉U/v) . (3.17.16)<br />

Actually this calculation is very similar to the one used to derive (3.17.5) by<br />

taking the derivative of Fvib in (3.17.4) with respect to v. Substituting back<br />

(3.17.16) into (3.17.15) we obtain:<br />

‚V<br />

<br />

Î0v0<br />

〈Á〉‚U<br />

<br />

CVT U<br />

‚〈Á〉2 <br />

v v v<br />

〈Á〉Cv<br />

(3.17.17)<br />

v<br />

Since we have assumed a weak anharmonic term we expect that terms<br />

quadratic in 〈Á〉 can be neglected. This means that at P 0 (when v v0)

Solution to Problem 4.1 619<br />

the above equation can be simplified to:<br />

‚ 〈Á〉CV<br />

<br />

v<br />

<br />

V Î0v0<br />

〈Á〉U<br />

1 ∼<br />

v<br />

〈Á〉Cv<br />

<br />

1<br />

<br />

v0 Î0<br />

〈Á〉U<br />

1 <br />

v0<br />

〈Á〉CvÎ0<br />

(3.17.18)<br />

v0<br />

This result shows that: the volume coefficient of thermal expansion is directly<br />

proportional to the average mode Grüneisen parameter and hence is a measure<br />

of the anharmonicity of the lattice, provided this anharmonicity is weak.<br />

References<br />

G.P. Srivastava: The Physics of Phonons. (Adamm Hilger, Bristol, 1990) p. 115.<br />

Ryogo Kubo, H. Ichimura, T. Usui, and N. Hashizume: Statistical Mechanics. (North-<br />

Holland Publishing Co., Amsterdam, 1965) p. 163.<br />

Solution to Problem 4.1<br />

(a) We have to first establish the characters of the six wave functions:<br />

X, Y, Z, X, Y and Z with respect to the symmetry operations of the point<br />

group Td. To do this we have to apply to them the symmetry operations belonging<br />

to the 5 classes of Td. As an example, we will apply the two-fold rotation<br />

C2(z) about the z-axis. This operation will leave only the functions Z<br />

and Z unchanged. Thus the character ¯ for C2 is 2. On the other hand, a S4(z)<br />

operation will interchange Z and Z so that the character ¯(S4) 0. The reflection<br />

operation onto a [110] plane will not change Z and Z so its character<br />

¯(Ûd) 2. Finally, a C3 rotation will permute all 6 wave functions so its character<br />

¯(C3) 0.<br />

In summary, the characters for the 6 conduction band minima wave functions<br />

in Si with respect to the symmetry operations of Td are given by:<br />

{E} {C2} {S4} {Ûd} {C3}<br />

6 2 0 2 0<br />

(b) By inspection one sees that the characters in the above table can be obtained<br />

by taking the following direct sum of the irreducible representations of<br />

Td listed in Table 2.3:<br />

A1 ⊕ E ⊕ T2 .<br />

(c) To obtain the proper linear combinations of the 6 Si conduction band wave<br />

functions that transform according to the above irreducible representations,<br />

we note first that a sum of all 6 functions must be invariant under all the<br />

symmetry operations of Td and therefore belongs to the A1 irreducible representation.<br />

The irreducible representation T2 is three dimensional and the three<br />

basis functions should transform into each other like the coordinate axes x, y<br />

and z. A possible choice for these three functions (with proper normalization)<br />

is clearly: [X X]/ √ 2; [Y Y]/ √ 2 and [Z Z]/ √ 2. Notice that under C2(x)<br />

rotation both y and z will change sign. This is also the case for [Y Y] √ 2 and<br />

[Z Z] √ 2. Finally, according to Table 2.3 the E irreducible representation is

620 <strong>Appendix</strong> B<br />

two-dimensional and a possible set of basis function has the form: x 2 y 2 and<br />

z 2 [x 2 y 2 ]/2. In this case y 2 and z 2 will not change sign under C2(x) rotation.<br />

To achieve the result with the Si wave functions we find that [Y Y] and<br />

[ZZ] will not change sign under the C2(x) rotation. Thus the normalized linear<br />

combination for the E irreducible representations are: {[XX][YY]}/2<br />

and {[2Z 2Z] [X X] [Y Y]}/ √ 12.<br />

Solution to Problem 4.5<br />

Assume that the imaginary part of an analytic function F(E) is given by:<br />

Im[F(E)] [(E E ′ ) 2 ° 2 ] 1 . (4.5a)<br />

Applying the Kramers-Kronig relation (4.56), we find that the real part of<br />

F(E) is given by:<br />

Re[f (E)] 1<br />

apple P<br />

1<br />

apple P<br />

∞<br />

∞ ∞<br />

∞<br />

Im[F(z)]<br />

z E dz<br />

(1)<br />

(z E)[(z E ′ ) 2 ° 2 ] dz<br />

(4.5b)<br />

One way to calculate this definite integral is to rewrite the integrand as a sum:<br />

1/(z E)[(z E ′ ) 2 ° 2 ] [A/(z E)] [B/(z E ′ i°)]<br />

[C/(z E ′ i°)]<br />

(4.5c)<br />

where i2 (1), A 1/[(E E ′ )2 ° 2 ], B (i/2°)[1/(E E ′ i°)]<br />

and C (i/2°)[1/(E E ′ i°)]. For each term in (4.5c) the corresponding<br />

integration in (4.5b) can be performed with the help of a contour integral. As<br />

an example, let us consider:<br />

∞<br />

dz<br />

P<br />

∞ z (E ′ (4.5d)<br />

i°)<br />

First, we will simplify the integral with a change in variable: x z E ′ so that<br />

(4.5d) becomes:<br />

∞<br />

dx<br />

P<br />

(4.5e)<br />

∞ x i°<br />

The integrand in (4.5e) has a pole at x i°. To obtain its principal value we<br />

consider an integral over a closed contour C in the complex z ′ -plane where<br />

z ′ x iy:

C<br />

dz ′<br />

z ′ i°<br />

Solution to Problem 4.5 621<br />

(4.5f)<br />

In order to avoid the pole at z ′ i°, we construct the contour C with the<br />

half-circle shown in the following figure:<br />

<br />

C<br />

y<br />

-R R<br />

R<br />

C<br />

dz ′<br />

z ′ i° <br />

R<br />

dx<br />

R x i° <br />

apple<br />

0<br />

x<br />

C consists of two parts: (1) a straight<br />

line along the x-axis connecting (R,0)<br />

and (R,0) and (2) a semi-circle in the<br />

lower half of the y-plane with radius R<br />

and centered at the origin. Since C does<br />

not enclose any pole we obtain from the<br />

Residue Theorem<br />

<br />

C<br />

dz ′<br />

z ′ i°<br />

0 (4.5g)<br />

We now explicitly decompose the integration<br />

over C into one integral over the horizontal<br />

axis and one over the semi-circle:<br />

Rieiı dı<br />

Re iı i°<br />

(4.5h)<br />

Next we take the limit R ⇒ ∞. The first integral of (4.5h) becomes<br />

∞<br />

dx<br />

P<br />

which is just what we want to calculate.<br />

∞ x i°<br />

In the limit RÊ ≫ °, the second integral becomes<br />

apple<br />

0<br />

Rieiı dı<br />

Re iı i° ⇒<br />

apple<br />

0<br />

Rie iı dı<br />

i(apple) (4.5i)<br />

iı<br />

Re<br />

Substituting these results back into (4.5g) we get:<br />

∞<br />

dx<br />

P<br />

iapple (4.5j)<br />

∞ x i°<br />

Similarly we can obtain:<br />

∞<br />

dx<br />

P<br />

iapple (4.5k)<br />

∞ x i°<br />

Finally, to evaluate the integral:<br />

∞<br />

P<br />

∞<br />

1<br />

x ′ E dx′ ∞<br />

P<br />

∞<br />

1<br />

dx (4.5l)<br />

x<br />

we have to use a different contour C as shown in the following figure.

622 <strong>Appendix</strong> B<br />

y<br />

-R R<br />

R<br />

C<br />

x<br />

In this case the pole occurs at the origin<br />

so we have to exclude the origin from C<br />

by adding another semicircle with radius<br />

‰. By applying the Residue Theorem we<br />

find that:<br />

<br />

C<br />

1<br />

dz 0 (4.5m)<br />

z<br />

To obtain the integral in (4.5l) we have<br />

to take the limits: R ⇒ ∞ and ‰ ⇒ 0.<br />

We note that the integrals over the two semicircles of radius R and ‰ cancel<br />

each other since the integration over the angle ı is from 0 to apple for the larger<br />

semicircle and from apple to 0 for the smaller semicircle.<br />

Thus<br />

∞<br />

1<br />

P<br />

∞ x ′ E dx′ 0 (4.5n)<br />

Putting all these integration results back into (4.5b) we obtain:<br />

Re[f (E)] 1<br />

<br />

i (iapple)<br />

apple 2° (E E ′ i iapple<br />

<br />

) i° 2° (E E ′ <br />

) i°<br />

1<br />

<br />

1<br />

2° (E E ′ ) i° <br />

1<br />

(E E ′ <br />

) i°<br />

<br />

1 (E E<br />

<br />

°<br />

′ )<br />

(E E ′ ) 2 ° 2<br />

(4.5o)<br />

For readers who are familiar with complex analysis and contour integrals,<br />

there is a faster way to obtain the same result. The first step is to make a<br />

transformation: z ′ z E ′ so that the integral in (4.5b) becomes:<br />

Re[f (E)] 1<br />

apple P<br />

∞<br />

(1)<br />

∞ (z ′ E ′ E)[(z ′ ) 2 ° 2 ] dz′<br />

(4.5p)<br />

The integrand now has three poles at E E ′ , i° and i°. To calculate the<br />

principal value of the integral one constructs two contours A and B as shown<br />

in the following figures.

R<br />

-R<br />

A<br />

y<br />

E’-E<br />

y<br />

E’-E<br />

R<br />

x<br />

Solution to Problem 5.1 623<br />

Let us first consider the contour integral:<br />

<br />

A<br />

dz ′<br />

(z ′ E ′ E)(z ′ i°)(z ′ i°)<br />

In the limits of R ⇒∞and ‰ ⇒ 0 the<br />

part of the contour integral over the xaxis<br />

will give us the principal value of:<br />

∞<br />

∞<br />

dz ′<br />

(z ′ E ′ E)(z ′ i°)(z ′ i°)<br />

-R<br />

R<br />

R<br />

x<br />

Similarly, when we perform the contour<br />

integral over B in the limits of R ⇒∞<br />

B<br />

and ‰ ⇒ 0, the part of the contour integral<br />

over the x-axis will give us again the<br />

same principal value of the above integral.<br />

On the other hand, the parts of the two contour integrals over the semicircles<br />

(whether of radius R or ‰) will exactly cancel each other since the directions<br />

of the integrations in A and B are opposite. Thus, the principal value<br />

of the integral becomes:<br />

∞<br />

dz<br />

∞<br />

′<br />

(z ′ E ′ E)(z ′ i°)(z ′ i°)<br />

1<br />

<br />

dz<br />

2 A<br />

′<br />

(z ′ E ′ E)(z ′ i°)(z ′ i°)<br />

<br />

dz<br />

<br />

B<br />

′<br />

(z ′ E ′ E)(z ′ i°)(z ′ (4.5q)<br />

<br />

i°)<br />

The value of the two contour integrals in (4.5q) can now be obtained by<br />

the Residue Theorem. For example, the contour integral over A is given by<br />

2applei times the residue of the integrand at the only pole: i°, and is equal to<br />

(2applei)(1/2apple°)[i° E ′ E] 1 . Similarly the contour integral over B is given by<br />

the residue at the pole: i° and is equal to (2applei)(1/2i°)[i° E ′ E] 1 .<br />

Substituting these results into (4.5q) one can obtain the same expression as in<br />

(4.5o).<br />

Solution to Problem 5.1<br />

[Note: (5.19) in the first, second and third editions has an error in the sign of<br />

gk. This error has led to errors in the sign of the term qÙkvk · F in Problem 5.1<br />

in those older editions].<br />

In Sect. 5.2.1 it is shown that, when a small enough electric field F is applied<br />

to a charge distribution with a distribution function f 0 k in the absence of

624 <strong>Appendix</strong> B<br />

F, the change in the distribution function gk is given by (5.19) as:<br />

<br />

gk <br />

f 0 k<br />

Ek<br />

qÙkvk · F<br />

within the relaxation time approximation. The new distribution function fk is<br />

given by (5.16): fk f 0 k gk. Thus<br />

<br />

fk f 0 k gk f 0 k (Ek) <br />

f 0 k<br />

Ek<br />

(qÙkvk · F) ≈ f 0 k (Ek qÙkvk · F)<br />

The physical meaning of this result is that: under the influence of the field, the<br />

functional form of the final distribution function fk is the same as the initial<br />

distribution function f 0 k (Ek). However, the energy E ′ k of each electron is now<br />

equal to its energy in the presence of the field, ie E ′ k Ek qÙkvk · F. Asa<br />

result we can write<br />

fk(E ′ k ) f 0 k (Ek) f 0 k (E′ k qÙkvk · F)<br />

If we consider the distribution function of the electron as a function of its<br />

velocity vk rather than its energy, then initially f 0 k is symmetric with respect<br />

to vk 0 in the absence of F. In the presence of F the entire distribution<br />

function would be displaced (without change in shape) along the vk axis by<br />

an amount: qÙkF/m (where m is the electron mass). The entire distribution<br />

appears to have acquired a drift velocity qÙkF/m. Hence f 0 k (Ek qÙkvk · F) is<br />

known as a drifted distribution.<br />

Solution to Problem 5.2(a)<br />

(a) As an example of the application of the results in Problem 5.1 we will<br />

consider the special case where f 0 k is the Boltzmann distribution function in<br />

the absence of F: f 0 k A exp[Ek/kBT]. In addition, we will assume that<br />

the electrons occupy a spherical band with the dispersion: Ek (1/2)m∗v2 k<br />

where m∗ is the electron effective mass. The resultant distribution is known<br />

as a Maxwell-Boltzmann distribution. Under the effect of the field F the perturbed<br />

distribution function fk is given by:<br />

fk ≈ f 0 k (Ek qÙkvk · F)<br />

<br />

m∗v2 k<br />

f 0 k<br />

<br />

≈ f 0 k<br />

2 qÙkvk · F<br />

<br />

m ∗ (vk vd) 2<br />

2<br />

<br />

f 0 k<br />

<br />

m ∗ (vk vd) 2<br />

2<br />

m∗ v 2 d<br />

2<br />

using the result of Prob. 5.1. This result can also be expressed as: fk <br />

A exp[m ∗ (vk vd) 2 /2kBT] where vd qÙkF/m ∗ is the drift velocity. This<br />

distribution function is known as a drifted Maxwell-Boltzmann distribu-

Solution to Problem 5.3(a) 625<br />

tion. The following figure shows schematically the “undrifted” (solid curve)<br />

and drifted (broken curve) Maxwell-Boltzmann distribution. Note that the<br />

Maxwell-Boltzmann distribution is a Gaussian function of vk.<br />

o<br />

fk 0<br />

Solution to Problem 5.3(a)<br />

v d<br />

f k<br />

v k<br />

(a) The interaction Hamiltonian between the electron and the longitudinal<br />

acoustic (LA) phonon is given by (3.21):<br />

HeLA ac(q · ‰R)<br />

(where ac is the conduction band deformation potential while q is the phonon<br />

wave vector). Substituting in the phonon displacement vector ‰R from (3.22)<br />

one obtains:<br />

<br />

HeLA ac<br />

q ′<br />

1/2 <br />

(q · eq<br />

2NVρˆ<br />

′)<br />

<br />

· C q ′ exp[i(q′ · r ˆt)] Cq ′ exp[i(q′ <br />

· r ˆt)]<br />

In the above expression ρ, N and V are, respectively, the density, the number<br />

of unit cells, and the volume of the crystal. eq is the phonon displacement vector<br />

and C and C are, respectively, the creation and annihilation operators<br />

for the phonon. In the case of the LA phonon propagating along high symmetry<br />

directions, such as along the [100] and [111] axes of the zincblende-type<br />

crystals, eq is parallel to q. Using the Fermi Golden Rule (6.43a) we can calculate<br />

the probability for an electron to scatter from state k to k ′ via emission<br />

or absorption of a LA phonon:<br />

P(k, k ′ ) (2apple/) 〈k, Nq|HeLA|k ′ , Nq ± 1〉 2 ρf<br />

where Nq is the occupation number of a LA phonon with wave vector q, Eq<br />

is its energy and ρf is the density of final electronic states. The and signs<br />

in the above equation represent, respectively, emission and absorption of a<br />

phonon by the electron during the scattering.

626 <strong>Appendix</strong> B<br />

As an example, we will calculate the probability for the scattering process<br />

in which the electron absorbs a phonon. In this case the electron-phonon matrix<br />

element is given by (under the simplifying assumption that eq is parallel<br />

to q):<br />

<br />

〈k, Nq|HeLA|k ′ , Nq 1〉 2 <br />

<br />

2 <br />

(ac) (q · eq) 2<br />

<br />

<br />

〈k, Nq|C q exp[i(q · r ˆt)]k′ <br />

<br />

, Nq 1〉<br />

(ac)<br />

q<br />

<br />

2<br />

q<br />

2NVρˆ<br />

<br />

2NVρˆ<br />

<br />

(q) 2 Nq‰(Ek Ek ′ Eq)‰(k k ′ q)<br />

In obtaining the above expression we have used the result that the probability<br />

of absorbing a phonon is proportional to Nq. Substituting this matrix element<br />

into the Fermi Golden Rule we obtain the total scattering rate of the electron<br />

out of the state k via absorption of phonon:<br />

<br />

2apple <br />

2<br />

P(k) (ac)<br />

<br />

k ′ <br />

<br />

2NVρˆ<br />

,q<br />

<br />

2apple<br />

(ac)<br />

<br />

2<br />

<br />

<br />

2NVρ<br />

q<br />

<br />

(q) 2 Nq‰(Ek Ek ′ Eq)‰(k k ′ q)<br />

<br />

q<br />

2 Nq‰(Ek Ekq Eq)<br />

ˆ<br />

It should be noted that the LA phonon frequency ˆ vsq where vs is the<br />

LA phonon velocity and therefore cannot be taken outside the summation<br />

over q in the above expression. Notice that P(k) is essentially the same as<br />

(5.41). In the high temperature limit, where kBT ≫ ˆ and Nq ≫ 1, we can<br />

approximate Nq ∼ kBT/(vsq) so that the q 2 term inside the summation sign<br />

is cancelled by the Nq/ˆ term. The final result can be reduced to:<br />

P(k) ∼ ‰(Ek Ekq Eq)<br />

except for a constant of proportionality which depends on material properties,<br />

such as the density, sound velocity, and the deformation potential. The<br />

way to calculate the allowed values of q is shown geometrically in Fig. 5.1(a).<br />

The summation over q can be converted into an integral over q as shown in<br />

(5.42a). The resultant expression is:<br />

P(k) <br />

<br />

a 2 c kBT<br />

8apple 2 ρv 2 s<br />

<br />

2appleq 2 dq d cos £‰<br />

<br />

2 q<br />

2m ∗<br />

<br />

(q 2k cos £) v2q<br />

After integration over cos £ and q the final expression becomes:<br />

<br />

a<br />

P(k) <br />

2 <br />

∗<br />

ckBTm q2 <br />

max<br />

2k<br />

4appleρ 3 v 2 s<br />

where qmax represents the maximum value of the wave vector of the phonon<br />

absorbed. We will now make the approximation that qmax ∼ 2k as in 5.2.4.<br />

With this simplification the probability of absorbing a phonon is given by:<br />

<br />

a<br />

P(k) <br />

2 √<br />

∗<br />

2<br />

ckBTm 2ackBT(m k <br />

∗ ) 3/2<br />

<br />

E 1/2<br />

2appleρ 3 v 2 s<br />

2appleρ 4 v 2 s<br />

2

Solution to Problem 5.5 627<br />

To obtain the total scattering rate of the electron by the LA acoustic phonon<br />

we have to add the rate of phonon emission (which is proportional to Nq 1)<br />

to the above rate of phonon absorption. For kBT ≫ ˆ, Nq ≫ 1soNq <br />

1 ∼ Nq. In other words: the rate of phonon emission is the same as the rate<br />

of phonon absorption. Thus the rate of scattering of electron by LA phonon<br />

(1/Ùac) is:<br />

1<br />

Ùac<br />

<br />

√ 2a 2 c (m ∗ ) 3/2 kBT<br />

apple 4 ρv 2 s<br />

Solution to Problem 5.5<br />

<br />

E 1/2<br />

(a) Let Ek, E ′ k and ELO be, respectively, the initial and final electron energies,<br />

and the LO phonon energy. In the case of emission of a LO phonon, energy<br />

and wave vector conservation requires that: Ek E ′ k ELO ˆLO and k <br />

k ′ q where ˆLO and q are, respectively, the LO phonon frequency and wave<br />

vector. For a parabolic band with mass m ∗ and a dispersionless LO phonon<br />

these two equations can be combined to yield:<br />

( 2 /2m ∗ )[k 2 (k q)] 2 ] ˆLO<br />

Let £ be the angle between k and q. Then the above equation can be rewritten<br />

as:<br />

( 2 /2m ∗ )[2kq cos £ q 2 ] ˆLO or q 2 2kq cos £ (2m ∗ /)ˆLO 0<br />

The roots of this quadratic equation are:<br />

<br />

2k cos £ ± (2k cos £)<br />

q <br />

2 <br />

8m∗ <br />

<br />

⎛<br />

2<br />

<br />

k ⎝cos £ ± cos2 £ ˆLO<br />

⎞<br />

⎠<br />

Ek<br />

ˆLO<br />

The maximum and minimum values of q (to be denoted as q2max and q2min)<br />

are obtained when cos £ 1. They correspond, respectively, to the and

628 <strong>Appendix</strong> B<br />

signs in the above solutions: q2max k[1 f (Ek)] and q2min k[1 f (Ek)]<br />

where f (Ek) [1 (ˆLO/Ek)] 1/2 .<br />

Note that the above derivation is valid as long as k (and hence Ek) is<br />

not zero. When k 0 one cannot define the angle £ between k and q. For<br />

LO phonon emission, the minimum value for Ek is ELO so Ek has to be 0<br />

always. When Ek ELO, f 0 and q2max q2min k. This can be easily seen<br />

in the following figure.<br />

q 1max<br />

E<br />

2min<br />

0<br />

q<br />

q 1min<br />

k<br />

LO phonon absorption<br />

q<br />

LO phonon emission<br />

k<br />

(b) The above results can be applied to the calculation for the absorption of a<br />

LO phonon by an electron by simply changing q to q and ELO to ELO in<br />

the appropriate places. For example, the quadratic equation for q is now:<br />

q 2 2kq cos £ (2m ∗ /)ˆLO 0<br />

and the solutions to this quadratic equation become:<br />

⎛ <br />

q k ⎝ cos £ ± cos2 £ ˆLO<br />

⎞<br />

⎠<br />

Ek<br />

while the maximum and minimum values of q (to be denoted by q1max and<br />

q1min) are given by: q1max k[1 f ′ (Ek)] and q1min k[f ′ (Ek) 1] where<br />

f ′ (E ′ k) [1 (ˆLO/Ek)] 1/2 .<br />

Again, the results are valid as long as Ek 0. For phonon absorption the<br />

minimum value of Ek is 0. k becomes 0 also when this happens. In this special<br />

case one has to go back to the equation: (2 /2m∗ )[k2 (k q)] 2 ] ˆLO and<br />

substitute in k 0. The only solution for q is then:<br />

q [2m ∗ ˆLO/] 1/2<br />

and therefore both q1max and q1min are equal to [2m ∗ ˆLO/] 1/2 .<br />

Also note that in the above figure both q1min and q2min decrease to 0 when<br />

Ek ⇒∞.<br />

(c) In the relaxation time approximation, the momentum relaxation rate<br />

(1/Ùm) is given by:<br />

(1/Ùm) [(k ′ k)/k]P(k, k ′ )

Ùm<br />

∞<br />

NLOq<br />

0<br />

2 apple<br />

dq<br />

0<br />

∞<br />

Solution to Problem 5.5 629<br />

where P(k, k ′ ) is the probability per unit time for the electron to be scattered<br />

from the initial state k to the final state k ′ . The summation over k ′ can be<br />

converted into an integration over q by invoking wave vector conservation. In<br />

the case of scattering by LO phonons the expression for PLO is then given by<br />

(5.48). The corresponding expression for (k/Ùm) then becomes:<br />

<br />

k<br />

q<br />

∝<br />

d cos £<br />

2<br />

(q2 q2 0 )<br />

<br />

q cos £‰(Ek ′ (Ek ELO))<br />

<br />

·<br />

0<br />

apple<br />

0<br />

(NLO 1)q 2 dq<br />

<br />

q<br />

d cos £<br />

2<br />

(q2 q2 0 )<br />

<br />

(q cos £)‰(Ek ′ (Ek ELO))<br />

To eliminate the integration over cos £ one notes that the ‰-functions can be<br />

written as:<br />

and<br />

‰[Ek ′ (Ek ELO)] (2m ∗ / 2 )‰[(2kq cos £ q 2 ) (2m ∗ / 2 )ELO]<br />

‰[Ek ′ (Ek ELO)] (2m ∗ / 2 )‰[(2kq cos £ q 2 ) (2m ∗ / 2 )ELO]<br />

After integration over cos £, one eliminates the delta functions and obtains:<br />

k<br />

Ùm<br />

∝<br />

q1max<br />

q1min<br />

<br />

NLO dq q 2m∗ELO 2 <br />

<br />

q<br />

q2max<br />

q2min<br />

<br />

(NLO 1) dq q 2m∗ELO 2 <br />

q<br />

Using the results from (a) and (b) for the limits of integration, we can perform<br />

the integration over q. The above results have been obtained under the<br />

assumption that the screening wave vector q0 can be set to zero. This assumption<br />

is valid when q1min and q2min are both larger than q0 or if the concentration<br />

of electrons is low. [Note that in case of scattering by acoustic phonons<br />

via the piezoelectric interaction it is impossible to neglect q0 since the minimum<br />

value of q is zero]. For LO phonons we have shown that both q1min and<br />

q2min can never be zero (except in the limit Ek ⇒∞) so this problem will<br />

not arise. To obtain (5.51) we have to perform the integration and put in the<br />

appropriate limits in the above expression. The result is:<br />

1<br />

∝ NLO<br />

Ùm<br />

<br />

q 2 1max q2 1min<br />

(NLO 1)<br />

k 2<br />

ELO<br />

Ek<br />

ln<br />

q1max<br />

<br />

q1min<br />

<br />

q2 2max q2 2min<br />

k2 ELO<br />

<br />

q2max<br />

ln<br />

Ek q2min

630 <strong>Appendix</strong> B<br />

The final step involves substituting in the expressions for q1min, q1max, q2min<br />

and q2max from parts (a) and (b) and replacing k2 by (2m∗ /2 )Ek to obtain:<br />

Ek 1/2 1<br />

ELO<br />

sinh 1<br />

<br />

1/2<br />

Ek<br />

∝ NLO<br />

Ùm<br />

(NLO 1)<br />

<br />

Ek<br />

ELO<br />

Ek<br />

Ek 1/2 ELO<br />

Ek<br />

ELO<br />

Ek<br />

ELO<br />

sinh 1<br />

Ek ELO<br />

ELO<br />

1/2 <br />

(d) Readers are urged to substitute the parameters for GaAs into the above<br />

expression to calculate Ùm.<br />

Solution to Problem 5.6<br />

(a) Starting with (5.72) we can write the drift velocity vd of charges q in an<br />

applied electric field F and an applied magnetic field B as:<br />

(m ∗ /Ù)vd q[F vd × B/c] (5.6a)<br />

where m ∗ is the carrier effective mass and Ù is its scattering time. Let Ì <br />

(qÙ/m ∗ ) represent the mobility of the charges. Then (5.6a) can be written as:<br />

vd Ì[F vd × B/c] (5.6b)<br />

Let N be the charge density, then the current density J is given by<br />

J Nqvd qÌ[F vdxB/c] q [F (J × B/Nqc)] (5.6c)<br />

For a magnetic field B applied along the z-direction (5.6c) can be written as:<br />

Jx NqÌ[Fx (JyBz/Nqc)] (5.6d)<br />

Jy NqÌ[Fy (JxBz/Nqc)] and (5.6e)<br />

Jz NqÌFz<br />

(5.6f)<br />

The two equations (5.6d) and (5.6e) can be solved for the two unknowns:<br />

Jx and Jy to give:<br />

Jx NqÌ[Fx (ÌFyBz/c)]/[1 (ÌBz/c) 2 ] and (5.6g)<br />

Jy NqÌ[Fy (ÌFxBz/c)]/[1 (ÌBz/c) 2 ] (5.6h)<br />

To simplify the notation we introduce · NqÌ and ‚ ·Ì/c so that<br />

(5.6g) and (5.6h) are rewritten as:<br />

Jx [·Fx ‚FyBz)]/[1 (ÌBz/c) 2 ] and (5.6i)<br />

Jy [·Fy ‚FyBz)]/[1 (ÌBz/c) 2 ] (5.6j)

plus<br />

Jz ·Fz<br />

Solution to Problem 5.7 631<br />

(5.6k)<br />

If there are both electrons and holes we have to add their contributions to J.<br />

Notice that · depends on the charge as q2 so ·n and ·p will both be positive.<br />

Similarly (5.6i) to (5.6k) are valid for both electrons and holes. Finally, if we<br />

assume that Bz is small then the B2 z terms can be neglected and the answer<br />

for J is:<br />

and<br />

Jx (·n ·p)Fx (‚n ‚p)FyBz<br />

Jy (·n ·p)Fy (‚n ‚p)FxBz<br />

Jz (·n ·p)Fz<br />

(b) In the Hall configuration Jy 0 in (5.6j) so that<br />

Fy Fx[(‚n ‚p)Bz/(·n ·p)] and<br />

Jx Fx[(·n ·p) 2 (‚n ‚p) 2 B 2 z ]/(·n ·p)<br />

The Hall Coefficient is RH Fy/JxBz (‚n ‚p)/[(·n ·p) 2 (‚n ‚p) 2B2 z ].<br />

Again, at low magnetic field, we can neglect the B2 z term so that<br />

RH (‚n ‚p)/(·n ·p) 2 .<br />

In terms of Nn and Np etc., the Hall Coefficient is equal to:<br />

RH (1/qc)[Np (Ìn/Ìp) 2 Nn]/[(Ìn/Ìp)Nn Np] 2<br />

Solution to Problem 5.7<br />

For samples where the electron distribution is given by f (E) the ensemble<br />

average of the current density is given by (5.88a) to(5.88c):<br />

and<br />

〈jx〉 ·Fx ÁBzFy<br />

〈jy〉 ·Fy ÁBzFx<br />

〈jz〉 〈Û0〉Fx<br />

where F and B are the electric and magnetic fields, respectively; · and Á are<br />

defined in (5.89a) and (5.89b). To obtain the Hall Coefficient RH we set 〈jy〉 <br />

0 so that Fy (Á/·)BzFx. Substituting back into RH Fy/〈Jx〉Bz we obtain:<br />

RH (Á/· 2 )Fx/[·Fx ÁBzFy] (Á/· 2 )/[1 (ÁBz/·) 2 ].

632 <strong>Appendix</strong> B<br />

Solution to Problem 6.6<br />

Van Hove singularities in the density-of-states (DOS) occur at energies E0 at<br />

which the gradient of E with respect to the electron wave vector k vanishes<br />

or |∇kE| 0. This means that E0 is either an extremum (a maximum or minimum)<br />

or a saddle point as a function of k. In general one can expand E as<br />

a Taylor series of k in the vicinity of E0. Without loss of generality, we can<br />

assume that E0 occurs at k 0. Since ∇kE vanishes at E0, the expansion has<br />

the form: E E0 ·k2 ... in 1D; E E0 ·k2 1 ‚k2 2 ... in 2D and E <br />

E0 ·k2 ‚k2 2 Ák2 3 ... in 3D.<br />

In the 1D case, the result is the simplest, since there is only one coefficient<br />

· whose sign will determine whether E0 is a maximum (corresponding to<br />

· 0) or a minimum (corresponding to · 0). If E0 is a minimum, there are<br />

no states with E E0 so the DOS must be zero when E E0. ForE E0<br />

the derivative |∇kE| is simply 2·|k|. To calculate the DOS we need to evaluate<br />

the integral in (6.52) over the constant energy surface Sk. In 1D a constant energy<br />

“surface” Sk defined by the energy E consists of two points only! These<br />

2 values of k are given by: k ±(1/·)[E E0] 1/2 . Thus an integral over Sk<br />

reduces to a summation over these two points of the integrand: 1/(2·|k|). If<br />

we convert k back to a function of E we find that the DOS is a function of<br />

1/[E E0] 1/2 . A similar divergence of the DOS at E0 of the form: 1/[E0 E] 1/2<br />

is obtained when E0 is a maximum. Thus the DOS of a 1D system diverges at<br />

the van Hove singularities. This result has a significant effect on the electronic<br />

and optical properties of quasi-1D materials such as semiconductor nanowires,<br />

and carbon nanotubes etc.<br />

In a 2D system there are two non-zero coefficients · and ‚. As a result, there<br />

are 3 possibilities:<br />

(a) both · and ‚ 0 so that E0 is a minimum.<br />

(b) both · and ‚ 0 so that E0 is a maximum.<br />

(c) ·‚ 0 so that E0 is a saddle point (in this case E increase in one direction<br />

but decreases in the other).<br />

Let us consider the case (a) where E0 is a minimum. As in the 1D case, there<br />

are no states with E E0 so the DOS must be zero for E E0. ForEE0 one can scale k1 and k2 so that · ‚ and the derivative |∇kE| is simply 2·|k|<br />

again. The constant energy “surface” (or, more appropriately, a curve) Sk in<br />

2D is a circle with radius k (1/·)[E E0] 1/2 . The result of an integration of<br />

1/|∇kE| over this circle is simply: 2apple(k/|∇kE|) apple/·. Therefore, the DOS in<br />

2D is a constant independent of k for E E0.<br />

If E0 corresponds to a maximum, the DOS is again a constant for E E0.<br />

The case of the saddle point (c) is rather interesting since the constant<br />

energy “surface” is a hyperbola. A hyperbola extends to ±∞ in k-space so,<br />

in principle, the integration of 1/|∇kE| over this hyperbola may diverge. In<br />

reality, the integration over the k-space for a real crystal must be limited to<br />

k kB (the size of the Brillouin zone). To illustrate this point, let us assume<br />

that the E(k) E0 k2 1 k2 2 after a proper transformation of the coordinate

Solution to Problem 6.7 633<br />

axes. For E E0 the constant energy curve is shown schematically in the<br />

following figure.<br />

k 2<br />

2 2 1/2<br />

2 k 1 2<br />

1<br />

k 1<br />

2 2<br />

E=E o+k 1– k 2<br />

The DOS is proportional to:<br />

<br />

dSk<br />

|∇kE| <br />

<br />

kB (dk1)<br />

0<br />

2 (dk2) 2<br />

<br />

k2 1 k2 2<br />

Using the result that:<br />

<br />

dx<br />

√<br />

x2 a2 log <br />

e x √ x2 a2 <br />

<br />

k2 B (E E0)<br />

<br />

kB<br />

0<br />

dk2<br />

|k1| <br />

kB<br />

0<br />

dk2<br />

<br />

k2 2 (E E0)<br />

We obtain the DOS as proportional to:<br />

<br />

<br />

<br />

loge kB <br />

loge E E0 ∼ C loge E E0<br />

The dependence on E of the first term in the above expression can be neglected<br />

since k 2 B ≫ (EE0). As a result, it can be approximated by a constant<br />

C. The dependence of the DOS is, therefore, determined by the second term<br />

which diverges logarithmically at E E0.<br />

The results we have obtained in this problem show that the energy dependence<br />

of the DOS is strongly dependent on the functional relation between<br />

the energy E and the wave vector k which, in turn, depends strongly on the<br />

dimensionality of the k-space and real space under consideration.<br />

Solution to Problem 6.7<br />

(c) A good starting point to solve this problem would be [6.44], the classic paper<br />

by R.J. Elliott, on the intensity of optical absorption by excitons. For direct<br />

excitons the transition probability per unit time (P) for an incident radiation

634 <strong>Appendix</strong> B<br />

of energy density ρ(˘) and frequency ˘ is given by:<br />

P (1/˘ 2 ) 〈i|HXR|f 〉 2 ‰(Ei Ef ˘)ρ(˘)<br />

HXR represents the exciton-photon interaction, |i〉 the initial state with the<br />

exciton in the ground state and |f 〉 the final state of the exciton. Ei and Ef<br />

are, respectively, the exciton initial state and final state energies. For absorption<br />

to the continuum state of the exciton, the exciton wave functions |f 〉 are<br />

expressed in terms of the hypergeometric functions within the hydrogenic approximation.<br />

These continuum wave functions can be decomposed into the<br />

product of a radial wave function R(r) and the spherical harmonic. R(r) is<br />

indexed by the exciton kinetic energy E and wave vector K and has the form:<br />

R(r) exp(apple·/2)/V 1/2 (2l 1)! |°(l 1 i·)|(2Kr) l<br />

· exp(iKr)F(i· l 1; 2l 2; 2iKr)<br />

In this expression l is the usual angular momentum quantum number of the<br />

exciton. · is a dimensionless quantity related to the exciton kinetic energy<br />

E(K) (K) 2 /2M (M is the exciton mass) and the R∗ exciton Rydberg constant<br />

(defined in (6.81)) by<br />

· (R ∗ /E) 1/2 .<br />

° is the Gamma function and F is the confluent hypergeometric function.<br />

Some references in physics textbooks on the hypergeometric functions are:<br />

L.D. Landau and E.M. Lifshitz, Quantum Mechanics, Nonrelativistic Theory<br />

(Addison-Wesley, Reading, MA 1958), Mathematical Appendices.<br />

N.F. Mott and H.S.W. Massey, Theory of Atomic Collisions (Clarendon Press,<br />

Oxford, 1949), second edition, p. 52.<br />

They are defined by an infinite series of the form:<br />

F(a; b; z) 1 a z a(a 1) z<br />

<br />

b 1! b(b 1)<br />

2<br />

...<br />

2!<br />

From this definition it is clear that b cannot be 0 or a negative integer. For<br />

b 0 the series will converge for all finite z provided both a and b are real.<br />

We are, however, only interested in direct and allowed excitonic optical transitions.<br />

As shown in (6.86) the transition matrix element depends on the magnitude<br />

of the final exciton wave function |f 〉 at r 0. For direct and allowed<br />

transitions l 0. The radial wave function of |f 〉 simplifies to:<br />

R(0) exp(apple·/2)/V 1/2 |°(1 i·)|F(i· 1; 2; 0)<br />

exp(apple·/2)/V 1/2 |°(1 i·)|<br />

The magnitude of this radial function is therefore:<br />

|R(0)| 2 [exp(apple·)/V] |°(1 i·)| 2<br />

Our problem now is to calculate the magnitude of the Gamma function with a<br />

complex argument. First, we will recall the properties of the Gamma function

which can be found in standard textbooks on mathematical analysis:<br />

°(1 n) n°(n);<br />

°(n)°(1 n) apple/ sin(napple) provided 0 n 1;<br />

and the Weierstrass definition of °(n):<br />

∞<br />

1<br />

<br />

zeÁz 1 <br />

°(z) z<br />

<br />

z <br />

e m .<br />

m<br />

m1<br />

Solution to Problem 6.11 635<br />

In this definition Á is the Euler constant, equal to 0.5772157...<br />

Next, we use analytic continuation to extend these results to complex arguments.<br />

From the above results one can show that:<br />

°(1 i·) (i·)°(i·)<br />

and hence:<br />

°(i·)°(i·) <br />

apple<br />

(i·) sin(i·apple)<br />

From the Weierstrass definition we can show that the complex conjugate of<br />

1/°(i·) is1/°(i·). Combining these results together we find the magnitude<br />

of the Gamma function with an imaginary argument:<br />

|°(1 i·)| 2 |·| 2 |°(i·)| 2 ·apple/ sinh(·apple).<br />

Substituting this result back into the relation between °(i·) and °(1 i·)<br />

we obtain:<br />

|°(1 i·)| 2 |·| 2 |°(i·)| 2 ·apple/ sinh(·apple).<br />

Finally, when we substitute this expression for |°(1 i·)| 2 into |R(0)| 2 we<br />

obtain:<br />

|R(0)| 2 ·apple exp(apple·)/[V sinh(·apple)]<br />

For a given photon energy ˆ bigger than the energy gap Eg, energy conservation<br />

leads to the relation: E ˆEg and · [R ∗ /(ˆEg)] 1/2 . We obtain<br />

(6.153) when we replace ·apple by Ù and use the atomic units for which 1.<br />

Solution to Problem 6.11<br />

(a) Let us start with the wave equation for the electric field: ∇ 2 E <br />

(Â/c 2 )( 2 E/t 2 ) 0 in a medium with dielectric constant Â. Without loss of<br />

generality we can assume that the interface corresponds to z 0 and the vacuum<br />

is given by z 0 and the solid fills z 0. The wave equation applies to

636 <strong>Appendix</strong> B<br />

both media with the appropriate value for Â (keeping in mind that the dielectric<br />

constant for a solid is a function of the frequency of the electromagnetic<br />

wave ˆ). As trial we assume a plane wave solution:<br />

E(x, y, z) E0 exp[i(kxx kyy kzz ˆt)].<br />

Since both media are isotropic we can choose, without loss of generality, the<br />

direction of propagation of the wave to be in the yz-plane. Substituting this<br />

plane wave solution into the wave equation we obtain the dispersion relation:<br />

k 2 yn k2 zn (ˆ/c)2 Ân where n A ⇔ vacuum and n B ⇔ solid.<br />

For the special case where ÂB is 0 and ÂA is 0, k 2 zB (ˆ/c)2 ÂB k 2 yB<br />

is also<br />

0 and kzB is purely imaginary. We will define kzB ±i· such that · is 0.<br />

If we choose kzB i· we obtain a solution whose dependence on z varies<br />

as exp(·z). This solution represents a surface wave since its amplitude decays<br />

exponentially to 0 as z decreases from 0 to ∞. However, the condition that<br />

ÂB 0 is necessary but not sufficient for a surface wave to exist.<br />

To obtain the necessary and sufficient condition we will try to obtain the<br />

relation between the wave vector of the wave ky and its frequency ˆ (ie the<br />

dispersion relation). In the absence of any sources of charge and current at<br />

the interface, Maxwell’s Equations for a nonmagnetic medium can be written<br />

as:<br />

div D 0; div H 0; curl E (1/c)H/t; and curl H (1/c)D/t,<br />

where E and H are the electric and magnetic field vectors, respectively. In addition,<br />

we have to include the constitutive equation D ÂBE for the solid.<br />

The boundary conditions imposed on E, D and H by the Maxwell Equations<br />

become:<br />

zx(EAEB)0; zx(HAHB)0; z · (DADB)0 and z · (HAHB)0.<br />

The subscripts A and B now denote the electric and magnetic fields at the<br />

interface, lying within the vacuum and the solid, respectively. For example, EA<br />

represents the electric field at z 0 ‰ with ‰ 0 in the limit ‰ ⇒ 0.<br />

Again we assume plane wave solutions of the form:<br />

E and H ∼ exp[i(kyy ˆt)] exp[ikzz]<br />

for waves in both media but with the understanding that kzB i·, so that<br />

these solutions represent surface waves. To determine the amplitudes of the<br />

waves in the two media we apply the above boundary conditions. As an example,<br />

we take the simple case of a transverse magnetic solution (a transverse<br />

electric solution will give similar results):<br />

Hy Hz 0 and<br />

HxA CA exp[i(kyAy ˆt)] exp[ikzAz];<br />

HxB CB exp[i(kyBy ˆt)] exp[ikzBz].

Solution to Problem 6.11 637<br />

The continuity of the tangential component of H at z 0 implied by the<br />

equation: zx(HA HB) 0 means that kyA kyB (which we will now denote<br />

as k ||) and CA CB.<br />

The corresponding solution for E can be obtained from the equation:<br />

curl H (1/c)D/t. Substituting the solution of Ey F exp[i(k ||y <br />

ˆt)] exp[ikzz] and Ez G exp[i(k ||y ˆt)] exp[ikzz] for both media A and<br />

B into the boundary conditions we obtain the following relations:<br />

kzCn (ˆÂn/c)Fn and k ||Cn (ˆÂn/c)Gn, where n A or B.<br />

The continuity of Ey at z 0 implies that<br />

FA FB or kzA/ÂA kzB/ÂB,<br />

while the continuity of Ez at the interface is trivially satisfied and generates<br />

no additional nontrivial equation.<br />

When this result is substituted back into the two expressions: k 2 || k2 zA <br />

(ˆ/c) 2 ÂA and k 2 || k2 zB (ˆ/c)2 ÂB to eliminate kzA and kzB one obtains an<br />

expression containing k || only:<br />

<br />

ˆ<br />

2 ÂAÂB k<br />

c<br />

2 || (ÂA ÂB)<br />

By taking the square root of both sides of this equation we obtain the dispersion<br />

of the surface wave:<br />

<br />

ˆ<br />

<br />

ÂAÂB<br />

k || <br />

c (ÂA ÂB)<br />

Since we have assumed ÂB 0 and ÂA 0, ÂAÂB is 0. In order that k ||<br />

be real we find that another condition, ÂA ÂB 0, has to be satisfied. If<br />

A is vacuum, then ÂA 1 and we find that the medium B must satisfy the<br />

condition that ÂB 1.<br />

For metals the dielectric function corresponding to the free electrons can<br />

be written as (see Problem 6.3):<br />

Â 1 4appleNe2<br />

mˆ2 1 ˆ2 p<br />

ˆ2 where ˆp is the bulk plasmon frequency of the metal. In analogy to the bulk<br />

plasmon oscillation, the frequency ˆsp at which a long wave length plasma oscillation<br />

can exist on the surface of the metal is known as the surface plasmon<br />

frequency. This frequency is given by:<br />

ˆsp <br />

4appleNe 2<br />

2m<br />

ˆp<br />

√2<br />

We can obtain the surface plasmon dispersion by replacing ÂA with 1 and<br />

ÂB with the expression for the dielectric function of the metal in the surface<br />

electromagnetic wave dispersion. Notice that in the special case of k || ∞,<br />

ÂB 1 and the frequency of the surface electromagnetic wave is equal<br />

to ˆsp. In this limit the photon (or electromagnetic wave in free space) and

638 <strong>Appendix</strong> B<br />

the surface plasmon are completely decoupled since the photon frequency<br />

approaches infinity when the wave vector becomes infinite while the surface<br />

plasmon frequency remains finite. Hence, retardation of the surface plasmon<br />

is completely negligible. When k || is finite there is coupling between the surface<br />

plasmon and the photon and therefore the surface plasmon is known as<br />

a surface-polariton in analogy to the phonon-polariton discussed in 6.4.1.<br />

(c) The dispersion of the surface phonon-polariton can be obtained simply by<br />

substituting ÂA by 1 and ÂB by the expression for the dielectric function of<br />

the optical phonon (6.110b). To obtain the surface phonon frequency without<br />

retardation we again set ÂB 1. Since ÂB approaches ∞ for ˆ slightly<br />

larger than ˆT and ÂB 0asˆ approaches ˆL, ÂB must be equal to 1 at<br />

some ˆ lying between ˆT and ˆL.<br />

Solution to Problem 6.13<br />

(a) In Figure 3.1 we found that the symmetry of the zone center optical<br />

phonon of Si is °25 ′ (this is true for any material with the diamond crystal<br />

structure, including Ge and gray tin). From the character table for the ° point<br />

in the diamond structure (Table 2.16) we find that the wave function of the<br />

°25 ′ optical phonon is triply degenerate. The crystal symmetry is lowered when<br />

the crystal is subjected to a uniaxial strain causing the triply degenerate optical<br />

phonon to split.<br />

For a [100] applied strain the crystal symmetry is lowered from cubic to<br />

tetragonal. Before the crystal is strained the optical phonons whose vibrations<br />

are polarized along the [100], [010] and [001] directions are degenerate. After<br />

the crystal is strained, the vibrations polarized along the [100] axis are expected<br />

to have a different frequency than those polarized perpendicular to the<br />

strain axis. Since the crystal remains invariant under S4 symmetry, operations<br />

of the strained crystal (provided the four-fold axis of rotation is parallel to<br />

the [100] axis) we expect the optical phonons polarized along the [010] and<br />

[001] axes to remain degenerate. Thus we conclude that the optical phonon<br />

in Ge will split into a doublet (polarized perpendicular to the strain axis) and<br />

a singlet (with polarization parallel to the strain axis). The effect of an [100]<br />

uniaxial strain on the symmetry of the q 0 optical phonons is similar “in a<br />

sense” to making the phonon wave vector q non-zero and directed along the<br />

[100] axis. In both cases the triple degeneracy of the phonon is split. As shown<br />

in Fig. 3.1, when the optical phonons propagate along the ¢ direction their<br />

frequencies split into two, corresponding to symmetries ¢2 ′ and ¢5. The character<br />

table of the group of ¢ (Table 2.20) shows that ¢2 ′ is a singlet while ¢5<br />

is a doublet. Using similar arguments we can show that a tensile stress along<br />

the [111] direction will split the optical phonon in Ge into a doublet (§3) and<br />

a singlet (§1). Whether the singlet or triplet phonon state will have a lower<br />

frequency cannot be determined by symmetry alone. This and also the magnitude<br />

of the splitting between the singlet and triplet states can be determined

Solution to Problem 6.19(a) 639<br />

if the phonon deformation potentials are known. See Problem 6.23 (new for<br />

the 4 th edition) for a discussion of the strain Hamiltonian for optical phonons.<br />

(b) Along high symmetry directions in a zincblende-type crystal, such as<br />

GaAs, the “nearly zone-center” optical phonons are split by the Coulomb interaction<br />

between the transverse effective charges e∗ of the ions into TO and<br />

LO phonons. The polarization of the LO phonon is along the direction of<br />

propagation of the phonon while the TO phonon is polarized perpendicular to<br />

the direction of propagation. When the crystal is subjected to a uniaxial strain,<br />

it is necessary to specify the direction of the uniaxial strain relative to that of<br />

the phonon propagation direction. Since, in many experiments, the strain direction<br />

is perpendicular to that of the phonon propagation (the exceptional<br />

case being a forward scattering experiment), let us consider the case of an<br />

uniaxial strain along the [100] direction while the phonon wave vector q is<br />

along the [010] direction. Without strain the TO phonon polarized along the<br />

[100] and [001] directions are degenerate. After the application of the strain<br />

along the [100] direction this degeneracy is removed. The LO phonon which<br />

is polarized along [010] is non-degenerate and, therefore, cannot exhibit any<br />

strain-induced splitting. The spring constant of the LO phonon involves two<br />

contributions: a “short-range mechanical” restoring force which is equal to<br />

that of the TO phonon and a long range Coulomb force which depends on e∗ .<br />

If the uniaxial strain does not affect the Coulomb force we expect the straininduced<br />

shift to be similar to that of the TO phonon along the [001] axis. In<br />

case the strain changes also e∗ then we will find the strain-induced shift of the<br />

LO phonon to be different from that of the [001] polarized TO phonon. Thus<br />

the difference between the stressed-induced shifts of the LO phonon and TO<br />

phonons in zincblende-type semiconductors can be used to study the effect of<br />

strain on e∗ . See the following references for further details:<br />

(1) F. Cerdeira, C.J. Buchenauer, F.H. Pollak and M. Cardona: Stress-induced<br />

Shifts of First-Order Raman Frequencies of diamond- and Zinc-Blende-Type<br />

Semiconductors. Phys. Rev. B5, 580 (1972).<br />

(2) E. Anastassakis and M. Cardona in Semiconductors and Semimetals Vol.<br />

55 (1998).<br />

One should note that it is possible to separate the optical phonons into TO<br />

and LO modes only for q along high symmetry directions. For the zincblendetype<br />

semiconductors the only other direction (in addition to the [100] and<br />

[111] directions) for which this is possible is the [110] direction. How a uniaxial<br />

strain along the [110] direction will affect the optical phonons is left as<br />

an exercise.<br />

Solution to Problem 6.19(a)<br />

Figure 6.44 shows the temperature (T) dependence of the direct band gap<br />

(Eg) ofGefrom0Kto600K.Thiscurve is representative of the temperature<br />

dependence of the fundamental band gap of most direct gap semiconductors

640 <strong>Appendix</strong> B<br />

with the diamond- and zincblende-type crystal structure. The main features of<br />

this curve are that: Eg is almost independent of T for T 100 K and then decreases<br />

linearly with T at higher temperatures. There are a few notable exceptions<br />

to this behavior. For example, the direct band gap of IV–VI chalcogenide<br />

semiconductors like PbS, PbSe and PbTe increases with T (see Fig. 6.14(b)).<br />

The band gaps of the chalcopyrite semiconductors AgGaS2 and AgGaSe2 exhibit<br />

a small blue-shift with increase in T at T 100 K before decreasing with<br />

T (see, for example, P.W. Yu, W.J. Anderson and Y.S. Park: Anomalous temperature<br />

dependence of the energy gap of AgGaS2, Solid State Commun. 13,<br />

1883 (1973)). Finally, the exciton energy (whose temperature dependence is<br />

similar to the band gap at low T) in cuprous iodide shows a shallow minimum<br />

as a function of T at low temperatures (see: J. Serrano, Ch. Schweitzer, C.T.<br />

Lin, K. Reimann, M. Cardona, and D. Fröhlich: Electron-phonon renormalization<br />

of the absorption edge of the cuprous halides. Phys Rev B65125110<br />

(2002)).<br />

Because the temperature dependence of Eg shown in Fig. 6.44 is highly<br />

nonlinear, especially around the “knee” at 100 K, it is not possible to derive<br />

(6.161) by simply expanding Eg(T) as a Taylor series in T. Instead, one has<br />

to consider what are the effects of T on Eg. In general, T can change Eg via<br />

one of these two effects. The first effect is associated with thermal expansion,<br />

an effect that results from the anharmonicity of the lattice. In other words, it<br />

involves phonon-phonon interaction (see, for example, C. Kittel: Introduction<br />

to Solid State Physics (Wiley, New York, 1995)). Typically, at T ∼ 300 K this<br />

effect is small since the coefficient of linear expansion is ∼ 5 × 106 K1 .For<br />

a semiconductor with these typical parameters: bulk modulus ∼100 GPa and<br />

pressure coefficient dEg/dP ∼ 100 meV/GPa (see Table of Physical Parameters<br />

of Tetrahedral Semiconductors in the inside cover), the contribution of<br />

this effect to the temperature coefficient is ∼0.15 meV/K. This is about a factor<br />

of 3 smaller than the typically observed value of dEg/dT ∼ 0.5 meV/K. The<br />

second effect is present even if the size of the unit cell does not change with T<br />

and arises directly from the electron-phonon interaction (whose Hamiltonian<br />

Hep is discussed in Chapter 3). Of the two effects, usually the second effect<br />

has a larger magnitude although they may have different sign. This happens in<br />

the case of the indirect band gap of Si where the gap increases with thermal<br />

expansion. One approach to estimate the electron-phonon effect is to assume<br />

that Hep is weak enough for the change in Eg to be calculated by second-order<br />

perturbation theory (see, for example, Eq. (2.38)). Using perturbation theory<br />

one obtains:<br />

Eg(T) Eg(0) <br />

<br />

〈g,0|Hep|i, ∓q〉〈i, ∓q|Hep|g,0〉<br />

n(ˆk,q) 1<br />

<br />

1<br />

±<br />

2 2<br />

i,k,q<br />

Eiq Eg ± ˆk,q<br />

In this expression |g,0〉 represent the electronic initial state of the system<br />

where an electron is in the conduction band and a hole is in the valence<br />

band at zone-center. |i, q〉 represents an intermediate electronic state where<br />

the electron-hole pair has been scattered to the state i by either emitting ()<br />

or absorbing () a phonon with wave vector q and belonging to the branch

Solution to Problem 6.19(a) 641<br />

k. ˆk,q and n(ˆk,q) are, respectively, the energy and occupancy of the this<br />

phonon mode. The summation in the above expression is over all the intermediate<br />

electron states and phonon branches. Notice that energy does not have<br />

to be conserved in the transition to the intermediate state (this is called a virtual<br />

transition) while the wave vector has to be conserved: this has already<br />

been taken into account in the summation. We have purposely put a minus<br />

sign in front of the second term on the right hand side of the above equation<br />

to emphasize that this term is always positive. The reason is that Eg is<br />

the lowest possible energy state of an electron-hole pair in the semiconductor<br />

(when excitonic effects are neglected). Most of the possible intermediate<br />

states will have higher energies than Eg so the energy denominator will usually<br />

be positive (one exception is when the electron or hole scatters back into<br />

the same initial state via the emission of a zone-energy optical phonon). The<br />

above equation can be simplified by considering only electron-hole pair states<br />

near the band gap since the energy denominator will make contributions from<br />

the high energy states negligible. In addition, one can limit the summation to<br />

only intraband scattering processes (ie |i〉 involves the same bands as those<br />

forming the gap). This approach is sometimes referred to as the Fan mechanism<br />

after H.Y. Fan (H.Y. Fan: Temperature Dependence of the Energy Gap<br />

in Semiconductors. Phys. Rev. 82, 900 (1951)). Another simplification is to assume<br />

that one phonon branch dominates the scattering. For example, the longitudinal<br />

optical phonon in zincblende-type semiconductors tends to have the<br />

strongest interaction with the electron-hole pairs near the band gap via the<br />

Fröhlich interaction. Using this approximation, one can limit the summation<br />

over phonon modes to essentially over one “average phonon mode” with energy<br />

ˆ. The net result of all the above simplifications is that:<br />

Eg(T) Eg(0) A[n(ˆ) 1] An(ˆ) Eg(0) A[2n(ˆ) 1]<br />

where the phonon occupancy n(ˆ) is given by:<br />

1<br />

n(ˆ) <br />

exp(ˆ/kBT) 1<br />

kB being the Boltzmann constant and A is a negative parameter. The term<br />

[2n(ˆ) 1] results from the probabilities for phonon emission (proportional<br />

to n 1) and absorption (proportional to n). Usually this expression gives a<br />

fairly good fit to the experimental result provided ˆ is adjustable.<br />

One should note that in some special cases the interband scattering contributions<br />

to the electron-phonon scattering may become as important as the<br />

intraband scattering. When this happens it becomes difficult to estimate even<br />

just the sign of the electron-phonon effect because the interband scattering<br />

terms can be either positive or negative. In principle, scattering to the lower<br />

energy band tends to increase the gap while scattering to the higher energy<br />

bands will decrease the gap. Which process will win out may depend on the<br />

detailed band structure and the electron-phonon interaction. In other words, it<br />

is difficult to calculate the temperature dependence of the band gap from first<br />

principles.

642 <strong>Appendix</strong> B<br />

How to explain a Positive Eg/T?<br />

We note that the above approach based on a second-order perturbation treatment<br />

of electron-phonon interaction tends to predict a decrease in Eg with<br />

increase in T. Clearly a different approach is necessary to explain the increase<br />

in Eg with T observed experimentally in the lead chalcogenides (even after<br />

deduction of the effect of thermal expansion) . This approach has been proposed<br />

by Antončik [E. Antončik, Czech. J. Phys. 5, 449 (1955)]. The main idea<br />

of this approach is that one starts with the pseudopotential method for calculating<br />

the energy gap Eg at T 0 (to be more precise, with the atoms at rest,<br />

so as to avoid quantum-mechanical zero-point vibrations) and then calculates<br />

Eg(T) from the temperature dependent pseudopotential form factors Vg. Let<br />

us assume that we define the T 0 pseudopotential form factors by (2.25):<br />

Vg(0) 1<br />

<br />

V(r) exp[ig · r]dr<br />

ø ø<br />

At T 0 we would expect that both V(r) and the unit cell volume ø would<br />

change with T. Again, we neglect the effect of thermal expansion on the lattice<br />

constant so ø remains unchanged. Under this assumption the effect of T<br />

is simply to cause the atoms to vibrate with amplitude ¢R(t) about the T 0<br />

equilibrium position R0. In principle, this vibration will cause V to be a function<br />

of time t and hence Vg also becomes time dependent. Since the period<br />

of atomic vibration is typically much shorter than the time of measurement<br />

of Eg in an experiment, Eg can be assumed to depend on the time-averaged<br />

pseudopotential 〈V〉 only. It is not easy to calculate this average 〈V〉 since we<br />

do not know how V will change as a result of the atomic vibration. Even if<br />

we can assume that the ion cores vibrate as a rigid body there is no reason to<br />

assume that the charge distribution of the valence electrons will rigidly follow<br />

the ion cores. One way to understand this is to think of what happens when<br />

we shake an egg. The egg yolk will not necessarily follow the shell rigidly.<br />

For simplicity, one can assume that the whole atom, including all the valence<br />

electrons, will vibrate as a rigid body. This means that when the atom moves<br />

from R0 to R0 ¢R(t) the pseudopotential changes from V to V ′ where V ′<br />

is related to V simply by a displacement of the coordinate system by ¢R(t).<br />

If we define a new coordinate system so that the origin is displaced by ¢R(t)<br />

and a point r in the old system becomes: r ′ r ¢R in the new system then<br />

V ′ (r ′ ) V(r). The new pseudopotential form factor Vg(T) is given by:<br />

Vg(T) 1<br />

<br />

V<br />

ø ø<br />

′ (r) exp[ig · r]dr<br />

1<br />

<br />

V(r<br />

ø ø<br />

′ ) exp[ig · (r ′ ¢R)dr ′<br />

<br />

[exp ig · ¢R]<br />

V(r<br />

ø<br />

′ ) exp[ig · r ′ ]dr ′<br />

ø

Solution to Problem 6.19(a) 643<br />

The terms inside the integral are now time-independent and so the time average<br />

of Vg(T) is given by:<br />

〈Vg(T)〉〈exp(ig · ¢R)〉Vg(0)〈1 (ig · ¢R) (1/2)(ig · ¢R) 2 ...〉Vg(0).<br />

Since g ∼ 1/lattice constant and ¢R ≪ lattice constant, g · ¢R ≪ 1. The above<br />

expansion can be terminated at the first non-zero term beyond 1. The time<br />

average of the first order term involving ¢R is zero for sinusoidal oscillations.<br />

Thus the first non-trivial and non-zero term is the second order term: 〈(g ·<br />

¢R) 2 〉. It is convenient to write 〈Vg(T)〉 as:<br />

〈Vg(T)〉 ∼[1 (1/2)〈(g · ¢R) 2 〉]Vg(0)<br />

∼ exp[〈(g · ¢R) 2 〉/2]Vg(0)<br />

exp[g 2 ¢R 2 /6]Vg(0).<br />

We note that the exponential factor exp[g2 ¢R2 /3] is known as the Debye-<br />

Waller Factor (see, for example, C. Kittel: Introduction to Solid State Physics<br />

(Wiley, New York, 1995), <strong>Appendix</strong> A). In studying the effect of temperature<br />

on the x-ray diffraction pattern, it was found that the sharpness of the x-ray<br />

peaks is not changed by the thermal vibration of the atoms. Instead, only the<br />

intensities of the peaks decrease while a constant background increases. The<br />

explanation for this result is that the thermal vibration does not change the<br />

time-averaged lattice constant and hence leaves the sharpness of the diffraction<br />

peaks unchanged. However, the thermal vibration decreases the magnitude<br />

of the structure factors causing the intensity to decrease by a Debye-<br />

Waller Factor. For the same reason, the magnitude of the pseudopotential<br />

form factors always decreases when the temperature increases. This decrease<br />

can lead to either a decrease or an increase in energy gaps which are formed<br />

when the pseudopotentials are turned on. It is easy to see how this decrease<br />

in pseudopotential form factors with T can cause the band gap Eg to decrease.<br />

What is not so clear is how it may lead to an increase in Eg under some special<br />

circumstances. In the case of PbTe and PbSe the positive Eg/T has been<br />

explained, at least partially, by this “Debye-Waller” mechanism.<br />

Additional References:<br />

Y.W. Tsang and M.L. Cohen: Calculation of the temperature dependence of the energy<br />

gaps in PbTe and SnTe. Phys. Rev. B3, 1254 (1971).<br />

M. Schlüter, G. Martinez and M.L. Cohen: Pressure and temperature dependence of electronic<br />

energy levels in PbSe and PbTe. Phys. Rev. B12, 650 (1975).<br />

P.B. Allen and M. Cardona: Temperature dependence of the direct gap of Si and Ge.<br />

Phys. Rev. B27, 4760 (1988). This paper includes both the Fan and “Debye-Waller”<br />

mechanisms.<br />

M. Cardona and M.L.Thewalt: Isotope effects on the optical spectra of semiconductors.<br />

Rev Mod Phys. 77, 1173 (2005).<br />

Ibrahim et al.: Temperature dependence of the optiocal response: Applications to GaAs<br />

using first-principles molecular dynamics. Phys Rev. B77, 125218 (2008)<br />

A. Marini: Ab initio finite temperature excitons, Phys. Rev. Letters 101, 106405 (2008).

644 <strong>Appendix</strong> B<br />

Solution to Problem 6.21<br />

The ratio ¢0/¢1 in Table 6.2 is not close to 3/2 for the two compounds GaN<br />

and InP. To understand why the ratio of the spin-orbit (S-O) splittings deviates<br />

from 3/2 for these compounds we have to find the reason why this ratio should<br />

be equal to 3/2 in the first place. Quantum mechanics teaches us that the S-O<br />

coupling is a relativistic effect described by the Hamiltonian: (see (2.45a)):<br />

HSO [/4c 2 m 2 ][(∇Vxp) · Û]<br />

Where V is the potential seen by the electron, p and Û are, respectively, the<br />

electron momentum operators and the Pauli spin matrices. In atoms the nuclear<br />

potential has spherical symmetry so one can express the S-O coupling in<br />

terms of the electron orbital angular momentum operator L and spin operator<br />

S as:<br />

HSO ÏL · S<br />

where Ï is known as the S-O coupling constant. In cubic semiconductors with<br />

the zincblende and diamond structure we find that the top valence band wave<br />

functions at k 0 are “p-like”. As a result we can “treat” these wave functions<br />

as if they were eigenfunction of L with eigenvalue L 1. Within this<br />

model, we can define a total angular momentum operator J L S. Following<br />

the results of atomic physics we symmetrize the k 0 valence band<br />

wave functions to correspond to J 3/2 and J 1/2. Using the relation that<br />

L · S (1/2)[J 2 L 2 S 2 ] we can show that:<br />

〈J 3/2|HSO|J 3/2〉 Ï/2 while 〉J 1/2|HSO|J 1/2〉 Ï.<br />

The S-O splitting ¢0 given by the separation between the J 3/2 and 1/2<br />

states is, therefore, 3Ï/2. In atoms the parameter Ï depends on the atomic orbitals<br />

involved. In crystals, we have pointed out on p. 59 that the conduction<br />

and valence band wave functions contain two parts: a smooth plane-wave like<br />

part which is called the pseudo-wave function and an oscillatory part which<br />

is localized mainly in the core region. Since HSO depends on ∇V most of<br />

the contribution to Ï comes from the oscillatory part of the wave function.<br />

Hence we expect that HSO in a semiconductor will depend on the S-O coupling<br />

of the core states (p and d states only since s states do not have S-O<br />

coupling) of its constituent atoms. In the cases of atoms with several p and<br />

d core states, the outermost occupied states are expected to make the biggest<br />

contribution to Ï of the conduction and valence bands. This is because the<br />

deeper core states tend to be screened more and hence contribute less to<br />

the valence and conduction electrons. For example, in Ge atoms the deep 2p,<br />

3d and 3p cores states all have larger S-O constants than the outermost 4p<br />

state. However, most of the S-O interaction in the valence band of Ge crystal<br />

at k 0 comes from the 4p atomic state. For the diamond-type semiconductors,<br />

such as Si and Ge, one may expect that S-O coupling in the crystal<br />

is related to the S-O coupling of the outermost occupied atomic p states

Solution to Problem 6.21 645<br />

by a simple constant Í. The valence electron wave functions in an atom are<br />

normalized to the total number of valence electrons/atom over the entire<br />

space. However, the valence band wave functions in a crystal are normalized<br />

over a unit cell by the total number of valence electrons/unit cell. Thus,<br />

the probability of finding a valence electron near the atomic nuclei will be<br />

enhanced in the crystal leading to a stronger S-O coupling. In other words:<br />

¢crystal Í¢atom with Í 1. As an example, ¢atom 0.219 eV for the 4p<br />

electrons in Ge (see, for example, the Atomic Spectra Database at the NIST<br />

website: http://physics.nist.gov/PhysRefData/ASD/index.html). The corresponding<br />

¢0 for the p-like top valence band at k 0 in Ge crystal is 0.296 eV. Thus,<br />

the enhancement factor Í is about 1.4, which is quite substantial.<br />

For a binary compound semiconductor, like GaAs, we expect that that<br />

S-O coupling for the valence electrons will depend on the S-O coupling of<br />

the outermost filled core electrons in both the cation and the anion. A simple<br />

approach would be to assume that ¢crystal Í1¢atom1 Í2¢atom2. If the electron<br />

spends equal time around the cation and the anion one would expect the<br />

ratio Í1/Í2 1. In ionic compounds this is usually not the case. For example,<br />

in GaAs the valence electrons spend more time around the As atoms so one<br />

expects that ÍAs/ÍGa 1. Indeed a ratio of ÍV/ÍIII 1.86 has been suggested<br />

for III-V compounds. An even larger ratio is expected for the II-VI semiconductors.<br />

So far we have been considering the effect of HS-O on the degenerate plike<br />

valence band states at the zone center. When the electron wave vector k<br />

increases from the zone center along a general direction, one would not expect<br />

the above model based on a spherical potential to be valid. Hence one<br />

may not be able to predict the contribution of HS-O to the band splitting. Using<br />

the k · p approach, the orbital part of the Hamiltonian of the electron as<br />

given by (2.35) is:<br />

H H0 [(k) 2 /2m] (/m)k · p<br />

Where H0 is the Hamiltonian for k 0. The k · p term now appears as an<br />

additional contribution to the crystal potential term and as a result HSO becomes<br />

k dependent. Instead of changing the crystal potential in response to<br />

the non-zero value of k we can interpret this effect as the electron now moving<br />

with velocity v k/m. We will choose a moving coordinate system O ′<br />

which is traveling with the electron (the electron rest frame). In this moving<br />

frame O ′ the spin-orbit Hamiltonian is again given by: HSO(v 0) <br />

[(/4c2m2 ][(∇V × p) · Û]. However, the electron momentum p ′ in the stationary<br />

(or laboratory frame) O is now given by p ′ p k. Thus the spin-orbit<br />

Hamiltonian in the frame O is:<br />

HSO(k) [h/4c 2 m 2 ][(∇V × p ′ ) · Û]<br />

[/4c 2 m 2 ][(∇V × p) · Û (∇V × k) · Û]<br />

In this Hamiltonian V and p both refer to the electron rest frame and, therefore,<br />

are calculated just as for the zone center electrons. In general, the second<br />

term is much smaller than the first one. The reasoning is like this: when the

646 <strong>Appendix</strong> B<br />

electron is close to the core where V is large the electron wave function ˇ<br />

will be varying rapidly over a distance which is of the order of the Bohr radius.<br />

On the other hand, (1/k) is of the order of the lattice constant which is<br />

much larger than the Bohr radius. Therefore 〈ˇ|p|ˇ〉 ∼〈ˇ|∇|ˇ〉 tends to be<br />

much larger than k (see, for example, E.O. Kane: Energy band structure in<br />

p-type germanium and silicon. J. Phys. Chem. Solids 1, 83 (1956)). When the<br />

second term is neglected we obtain again (2.45a) for the S-O coupling. However,<br />

for a general point k in the Brillouin Zone one finds the k · p term to be<br />

the dominant interaction which mixes the k 0 electron states so the effect<br />

of HSO on the electrons is no longer discernible. There are two exceptional<br />

cases though. They are when k is along the [111] or [100] directions.<br />

In Sections 2.4.1 and 2.4.2 we learn that the group of § in both the<br />

zincblende and diamond structure has three-fold rotational symmetry about<br />

the [111] axis. This symmetry is high enough that in the diamond-type semiconductor<br />

the triply degenerate p-like wave functions at k 0 splits into a<br />

doublet with symmetry §3 and a singlet with symmetry §1. See Fig. 2.10 for<br />

the band structure in Si neglecting S-O splitting and Table 2.12 for the character<br />

table (same for diamond and zincblende crystals along the [111] direction<br />

as long as k is inside the Brillouin zone). This degeneracy of the §3 state can<br />

be split by the S-O coupling.<br />

In fact, we can model the valence band electron in this case as a “p-like”<br />

electron in a cylindrical potential. In case of the L 1 state we expect the<br />

three degenerate states to be split into a doublet with Lz ±1 and a singlet<br />

with Lz 0 We will assume that the axis of quantization of the angular<br />

momentum vector L to be the [111] axis which will be labeled as the z-axis<br />

to simplify the notation. We can identify the doubly degenerate §3 states as<br />

corresponding to the Lz ±1 states. The wave functions for the §3 state can<br />

then be represented as [|X〉 i|Y〉]/ √ 2 and [|X〉 i|Y〉]/ √ 2 to correspond to<br />

the Lz ±1 states. Again |X〉 and |Y〉 are shorthand notations for the two §3<br />

wave functions which transform into each under the symmetry operations of<br />

the group of § like the spatial coordinates x and y. In this coordinate system<br />

the S-O interaction is given by: HSO Ï ′ L · S Ï ′ LzSz. We will assume at<br />

first that the spin-orbit coupling constant Ï ′ is not the same as Ï. We can show<br />

that:<br />

〈Lz 1, Sz 1/2|HSO|Lz 1, Sz 1/2〉 Ï ′ /2 while<br />

〈Lz 1, Sz 1/2|HSO|Lz 1, Sz 1/2〉 Ï ′ /2.<br />

Similarly 〈Lz 1, Sz 1/2|HSO|Lz 1, Sz 1/2〉 Ï ′ /2 while<br />

〈Lz 1, Sz 1/2|HSO|Lz 1, Sz 1/2〉 Ï ′ /2.<br />

In other words, along the [111] direction the Jz ±3/2 states are split<br />

from the Jz ±1/2 states by the spin-orbit coupling. The magnitude of the<br />

S-O coupling ¢1 is equal to Ï ′ .IfÏ Ï ′ then we obtain the “two-thirds rule”:<br />

¢1/¢0 2/3.<br />

The reason why one may expect Ï to differ from Ï ′ is that the k · p perturbation<br />

term mixes the k 0 wave functions. For example, the k · p term<br />

will mix the anti-bonding °15 conduction band wave function with the bonding

Solution to Problem 6.21 647<br />

°25 ′ valence band wave function. The anti-bonding and bonding states sample<br />

different amount of the core potential and hence contribute slightly different<br />

amounts to the S-O coupling. This mixing of the k 0 wave functions by the<br />

k·p term explains the small deviations from the “two-thirds rule” in Si and Ge.<br />

In case of III-V semiconductors the situation is complicated by the fact that<br />

there are two kinds of atoms which sometimes have quite different atomic S-<br />

O coupling strengths. In a simple-minded approach one can assume that the<br />

coefficients Í1 and Í2 are now k dependent so that we can write:<br />

¢1 (2/3)[Í1(k)¢atom1 Í2(k)¢atom2] with ¢0 Í1(0)¢atom1 Í2(0)¢atom2.<br />

Assuming that the admixture of anti-bonding states to the §3 wave functions<br />

is small we can expand Í1(k) ∼ Í1(0) ¢Í1 and similarly Í2(k) ∼ Í2(0) ¢Í2.<br />

¢Í1 (or ¢Í2) represents the change in Í1 (or Í2) as a result of the variation<br />

in the probability of finding the electron near the atom1 (or atom 2) as k<br />

increases along the [111] direction. To first order, we expect that a decrease in<br />

Í1 will be compensated by an increase in Í2. Thus we conclude that:<br />

¢1/¢0 (2/3)[1 ¢Í1(¢atom1 ¢atom2)/¢0].<br />

This argument shows that when the atomic S-O couplings for the two atoms in<br />

the unit cell are quite different one would expect a larger deviation from the<br />

“two-thirds rule”. Since the size of the atomic S-O coupling depends mainly<br />

on the atomic number Z, we expect the “two-thirds rule” not to be valid when<br />

the cation and anion have significantly different Z. This explains why ¢0/¢1<br />

for GaN and InP are not ∼ 1.5. In both compounds the cation has much larger<br />

Z than the anion. For the same reason one would expect the “two-thirds rule”<br />

not to be valid for BAs where Z for the anion is much larger than that of the<br />

cation. Although there is no experimental determination of the S-O couplings<br />

in BAs, there are reliable theoretical calculations of the band structure of BAs.<br />

See, for example, Gus L.W. Hart and Alex Zunger: Electronic structure of<br />

BAs and boride III-V alloys. Phys. Rev. B62, 13522 (2000). The theoretical<br />

values of ¢0 and ¢1 are, respectively, 0.22 and 0.1 eV with a ratio of ¢0/¢1 ∼<br />

2.2.<br />

Based on the above analysis, one may expect the same arguments to apply to<br />

the S-O coupling for k ||[100]. Along the [100] direction the triply degenerate<br />

p-like wave functions are split into a doublet with symmetry ¢5 and a sin-<br />

glet with symmetry ¢2 ′ as shown in Fig. 2.<strong>10.</strong> However, the “two-thirds rule”<br />

does not apply along the [100] direction even in the diamond-type semiconductors.<br />

The reason is: the group of X in the diamond structure contains the<br />

non-symorphic operation TÛz. As a result, all the states at the X point are<br />

doubly degenerate (not including the spin degeneracy) as shown on p. 56-57.<br />

This means that the effect of S-O coupling has to vanish at the zone boundary<br />

along the [100] direction. Similarly the ¢5 state has to become doubly degenerate<br />

as k ⇒ 0. As a result, the splitting of the ¢5 state induced by the S-O<br />

interaction becomes smaller than (2/3)¢0 and dependent on k. This large qualitative<br />

difference in the effect of HS-O on the valence bands along § and ¢ is<br />

clearly shown in the band structure of Ge in Fig. 2.13.

648 <strong>Appendix</strong> B<br />

References<br />

L. Liu: Effects of spin-orbit coupling in Si and Ge. Phys. Rev. 126, 1317 (1962).<br />

M.Cardona: Modulation Spectrosocopy, Solid State Physics, Suppl. 11 (Academic, New<br />

York, 1969) p. 66-73.<br />

Solution to Problem 7.1<br />

For simplicity, we assume that the two levels n and m (with energies En and<br />

Em) are both non-degenerate, although it is rather straightforward to generalize<br />

the result to the degenerate case. Let Nn and Nm be, respectively, the<br />

occupancies of these two levels. First, for the sake of argument, let us assume<br />

that there is no stimulated emission. If the rate of spontaneous emission from<br />

level n to level m is Anm then the rate of depopulation of the level n via emission<br />

is: NnAnm since Nn of the level n states are occupied. Similarly, if the<br />

rate of absorption from level m to level n induced by a radiation field of frequency<br />

Ó and energy density u(Ó) isuBmn then the rate of depopulation of<br />

level m due to absorption is: uBmnNm. At thermal equilibrium the principle of<br />

detailed balance (see p. 208) requires that the two rates be equal. This means:<br />

NnAnm uBmnNm or Nn/Nm uBmn/Anm<br />

At thermal equilibrium the ratio of the occupancies: Nn/Nm has to be equal to<br />

exp[(En Em)/kBT] at temperature T according to the Boltzmann’s distribution<br />

law (kB is Boltzmann’s constant). Equating these expressions for Nn/Nm<br />

one obtains:<br />

uBmn/Anm exp[(En Em)/kBT]<br />

Combining these results one obtains:<br />

u(Ó) [Anm/Bmn] exp[(En Em)/kBT]<br />

which, after equating hÓ to (En Em), disagrees with Planck’s Radiation Law:<br />

u(Ó) <br />

8applehÓ 3 n 3 r<br />

c 3 {exp[hÓ/(kBT)] 1}<br />

except for kBT ≪ hÓ.<br />

The way Einstein removed this disagreement between the classical result<br />

and Planck’s Radiation Law is to postulate that, in addition to the spontaneous<br />

emission processes between level n and m, there are stimulated emission<br />

processes induced by u(Ó). If we denote the rate of stimulated emission as Bnm<br />

then the only change we have to make to include the stimulated emission processes<br />

is to replace the rate of depopulation of level n by: Nn(Anm uBnm).<br />

Applying the principle of detailed balance again we obtain:<br />

Nn/Nm uBmn/(Anm uBnm).

Equating the two expressions for Nn/Nm one obtains now:<br />

u(Ó) Anm/{Bmn exp[(En Em)/kBT] Bnm}.<br />

Solution to Problem 7.5 649<br />

This expression becomes equal to Planck’s Radiation Law when one assumes<br />

that:<br />

Bmn Bnm and Anm<br />

Bnm<br />

Solution to Problem 7.5<br />

8applehÓ3 n 3 r<br />

c 3<br />

According to Problem 3.7 the wurtzite crystal structure possesses 4 atoms<br />

per primitive unit cell (double the number in the zincblende structure). As<br />

a result, there are 9 zone-center optical phonon modes with symmetries:<br />

°1 ⊕2°3 ⊕°5 ⊕2°6 (or A1 ⊕2B1 ⊕E1 ⊕2E2 using the C6v point group notation).<br />

One should note that the E modes are doubly degenerate and not all of these<br />

optical phonons are Raman-active.<br />

To determine the symmetry of the Raman-active phonon modes we note<br />

that, unlike absorption, Raman scattering involves two electromagnetic (EM)<br />

waves: one incident and one scattered wave. If we want to annihilate a photon<br />

and generate a phonon, as in optical absorption, then the phonon must<br />

have the same symmetry as the photon (which belongs to the same representation<br />

as a vector). We have already obtained this result as one of the many<br />

applications of group theory (see Section 2.3.4). In Raman scattering we annihilate<br />

the incident photon and create a scattered photon with the generation<br />

or annihilation of a phonon. The symmetry of the phonons involved is going<br />

to be the same as in the case where two photons are annihilated to generate<br />

one phonon (i.e. a two-photon absorption process). The reason is that the matrix<br />

elements describing the photon creation and annihilation processes are the<br />

same except for a term involving the photon occupancy factor Np (see Section<br />

7.1). Thus the representation of the phonon (or phonons) involved in Raman<br />

scattering must be contained within the direct product of the representations of<br />

two vectors.<br />

For example, a vector in zincblende-type crystals belongs to the °4 irreducible<br />

representation. Thus the representation of the Raman-active phonons<br />

must belong to the direct product:<br />

°4 ⊗ °4 °1 ⊕ °2 ⊕ °4.<br />

Although the zone-center optical phonons in zincblende-type crystals have °4<br />

symmetry, Raman scattering from phonon modes with the °1 and °2 symmetry<br />

can also be observed in the two-phonon spectra of zincblende-type crystals.<br />

See, for example, Fig. 7.22 for the various symmetry components of the twophonon<br />

Raman spectra of Si.

650 <strong>Appendix</strong> B<br />

To determine the symmetry of the Raman-active phonons in wurtzite crystals,<br />

we need to determine the irreducible representations of a vector in the<br />

wurtzite structure. From Problem 3.7 we find that the character table for the<br />

wurtzite structure becomes identical to that of point group C6v in the limit<br />

when the phonon wave vector approaches zero. Assuming that one chooses<br />

the z-axis to be parallel to the C6 axis of this point group or the c-axis of the<br />

wurtzite structure (this axis will also be labeled as 3 in subsequent tensor subscripts,<br />

while the x and y axes will be labeled as 1 and 2, respectively). Since<br />

the largest dimension of irreducible representations in C6v is 2, the representation<br />

of a vector in 3D (with components x, y and z) has to be reducible. One<br />

way this representation can be reduced is to separate {z} from {x, y}. {z}<br />

must belong to the A1 irreducible representation since it is invariant under all<br />

the symmetry operations of C6v. The remaining components {x} and {y} form<br />

a 2D irreducible representation. Whether this irreducible representation is of<br />

symmetry E1 or E2 can be decided by applying to {x, y} the C2 operation (a<br />

rotation by 180 ◦ about the z-axis): xy → xy. The character for this operation<br />

is 2. Hence {x, y} belongs to the E1 irreducible representation. The above<br />

result can be summarized as: the irreducible representations to which a vector<br />

in the group C6v belongs are A1 and E1.<br />

Based on this result we can predict that the zone-center phonons of symmetry<br />

°1 and °5 in the wurtzite crystal (corresponding to A1 and E1 representations,<br />

respectively, in C6v) are infrared-active. To obtain the symmetry of the<br />

corresponding Raman active phonons we have to calculate the direct product:<br />

(A1 ⊕ E1) ⊗ (A1 ⊕ E1). By inspection of the character table of C6v in Problem<br />

3.7 it can be shown that: E1 ⊗ E1 A1 ⊕ A2 ⊕ E2. Thus one obtains the result:<br />

(A1 ⊕ E1) ⊗ (A1 ⊕ E1) 2A1 ⊕ A2 ⊕ 2E1 ⊕ E2.<br />

In summary, in systems with C6v point group symmetry the Raman-active<br />

phonon modes must belong to the A1, A2, E1 or E2 irreducible representations.<br />

Similarly, the Raman-active zone-center optical phonons in the wurtzite<br />

crystal structure must belong to the °1, °2, °5, or°6 irreducible representations.<br />

Thus, of all the 9 zone-center optical phonons in the wurtzite structure the<br />

ones with °1 and °5 symmetries are both infrared and Raman active; the two<br />

phonons with °6 symmetry are only Raman-active while the two phonons with<br />

°3 symmetry are neither infrared nor Raman active (such modes are said to<br />

be silent).<br />

To obtain the Raman tensor for the Raman-active phonons we have to<br />

derive, in principle, the form of the phonon displacement vector Qk and the<br />

electric susceptibility tensor ¯ and then apply Eq. (7.37) to obtain the Raman<br />

tensor Rij. In reality, we can choose any basis function in lieu of the phonon<br />

displacement vectors, provided they belong to the same irreducible representation.<br />

As, an example, let us consider the °1 optical phonon. As shown in Problem<br />

3.15 the third order electromechanical tensor (em) in the wurtzite crystal<br />

has only three linearly-independent and non-zero elements: (em)15, (em)31,<br />

and (em)33. Since the third rank tensor (¯/Q) has the same symmetry prop-

Solution to Problem 7.5 651<br />

erties as (em) we expect that its linearly-independent and non-zero elements<br />

are: c (¯/Q)15, a (¯/Q)31, and b (¯/Q)33. The number of non-zero<br />

elements for the °1 optical phonon will be further reduced since we can put<br />

Q1 Q2 0 and Q3 z. Thus the second rank Raman tensor is obtained by<br />

the contraction of (¯/Q) with (0, 0, z):<br />

⎛ ⎞<br />

az<br />

⎛<br />

⎞ ⎜ az ⎟ ⎛ ⎞<br />

0 0 0 0 c 0 ⎜ ⎟ a 0 0<br />

(0 0 z) ⎝ 0 0 0 c 0 0⎠<br />

⎜ bz ⎟<br />

⎜ ⎟ ⇔ ⎝ 0 a 0 ⎠ z<br />

⎜ 0 ⎟<br />

a a b 0 0 0 ⎝<br />

0<br />

⎠ 0 0 b<br />

0<br />

The final form of the Raman tensor for the °1 mode, after dividing by the<br />

phonon amplitude z, is therefore:<br />

⎛ ⎞<br />

a 0 0<br />

Rij(°1) ⎝ 0 a 0 ⎠<br />

0 0 b<br />

The Raman tensor for the 2D °5 modes can be obtained similarly by assuming<br />

that Q (x, 0, 0) for one of the two modes and (0, y, 0) for the remaining<br />

mode. The second rank Raman tensor obtained by the contraction of (¯/Q)<br />

with (x, 0, 0) is:<br />

⎛ ⎞<br />

0<br />

⎛<br />

⎞ ⎜ 0 ⎟ ⎛ ⎞<br />

0 0 0 0 c 0 ⎜ ⎟ 0 0 c<br />

(x 00) ⎝ 0 0 0 c 0 0⎠<br />

⎜ 0 ⎟<br />

⎜ ⎟ ⇔ ⎝ 0 0 0⎠x<br />

.<br />

⎜ 0 ⎟<br />

a a b 0 0 0 ⎝<br />

cx<br />

⎠ c 0 0<br />

0<br />

The final form of the Raman tensor for the °5(x) mode, after dividing by the<br />

phonon amplitude x, is therefore:<br />

⎛ ⎞<br />

0 0 c<br />

Rij(°5(x)) ⎝ 0 0 0⎠<br />

.<br />

c 0 0<br />

Similarly, the Raman tensor for the °5(y) mode is:<br />

⎛ ⎞<br />

0 0 0<br />

Rij(°5(y)) ⎝ 0 0 c ⎠ .<br />

0 c 0<br />

Finally, the °6 mode is also doubly degenerate. However, there is an important<br />

difference between this mode and the °5 mode. While the °5 mode is<br />

infrared-active and can be represented by the components of a vector, the °6<br />

mode is not infrared-active and it cannot be represented by a vector (it can<br />

be represented instead by a pseudovector). As a result, we cannot deduce the<br />

symmetry of the Raman tensor for the °6 mode by taking advantage of the<br />

known symmetry of the third rank tensor in the wurtzite structure. Instead,<br />

we have to derive the symmetry of the Raman tensor by first finding some<br />

basis functions to represent the °6 modes. It is easier to do this for the C6v

652 <strong>Appendix</strong> B<br />

point group. We notice that one important difference between the E1 and E2<br />

irreducible representation is that under a C2 operation the character of the<br />

E1 mode is 2 while the corresponding character for the E2 mode is 2. This<br />

suggests that both basis functions of the E2 mode remain invariant under a<br />

C2 operation, On the other hand, the character for the E2 mode under a C6<br />

operation is 1 while that of the E1 mode is 1.<br />

Functions of x and y that remain invariant under a rotation by 180◦ about<br />

the z-axis (C2 symmetry operation) are: {xy and x2 y2 }. Thus, their character<br />

is 2 for a C2 operation. To verify that these two functions indeed form an<br />

irreducible 2D representation of E2 symmetry, we consider a 6-fold rotation<br />

about the z-axis. Under this symmetry operation x and y transform according<br />

to: x ⇒ (x/2) ( √ 3y/2) while y ⇒ ( √ 3x/2) (y/2).<br />

From these two transformation equations we find the character of the 2D<br />

representation {x, y} to be: ( 1 1<br />

2 ) ( 2 ) 1 consistent with the fact that the<br />

symmetry of this representation is E1. Under the same symmetry operation<br />

{xy, x 2 y 2 } transform according to the following equations:<br />

xy ⇒ [(x/2) ( 3y/2)][( √ 3x/2) (y/2)] <br />

<br />

1<br />

2<br />

<br />

xy ( √ 3/4)(x 2 y 2 )<br />

while<br />

x 2 y 2 ⇒[(x/2)( 3y/2)] 2 [( √ 3x/2)(y/2)] 2 <br />

3xy 1<br />

<br />

(x<br />

2<br />

2 y 2 ).<br />

These results show that {xy, x2 y2 } forms a 2D representation whose character<br />

is 1 under a C6 symmetry operation. It is easy to show that the characters<br />

of {xy, x2 y2 } under the other symmetry operations of the C6v point group<br />

are all consistent with the E2 irreducible representation. Thus {xy, x2 y2 }<br />

form a set of basis functions for the E2 mode.<br />

Next we have to deduce the non-zero and linearly independent elements<br />

of the Raman tensor of a phonon belonging to the E2 irreducible representation.<br />

We will illustrate this process by showing that the Raman tensor component<br />

R13 has to vanish. For simplicity, we will define f1 xy and f2 x2 y2 .<br />

By definition<br />

R13 ∼ (¯13/f1)f1 (¯13/f2)f2<br />

Consider the effect of a symmetry operation Ûd (reflection in the plane containing<br />

the y and z axes): xyz → xyz. Under this operation f1 ⇒ f1 while<br />

f2 ⇒ f2. The second rank tensor component (¯13) ⇒ (¯13). Thus R13 ⇒ R13<br />

under this symmetry operation and hence R13 0. By similar symmetry arguments<br />

one can conclude that R23 0 also.<br />

Next, we consider the diagonal term: R33 ∼ (¯33/f1)f1 (¯33/f2)f2<br />

Under the same operation Ûd, ¯33 is invariant while f1 changes sign. Thus<br />

(¯33/f1) changes sign and hence is zero. By considering another reflection<br />

operation in which f2 changes sign we can show similarly that (¯33/f2) 0<br />

and hence R33 0.<br />

The derivation of the remaining non-zero components of the Raman tensor<br />

for the E2 or °6 mode is left as an exercise.

A Short Cut to the Calculation of the Raman tensor for the °6 mode<br />

Solution to Problem 7.5 653<br />

For readers who have worked out Problem 3.7(b) to derive the symmetry<br />

properties of the stiffness tensor for the wurtzite crystal, the above derivation<br />

should look very familiar. The reason is that the stiffness component Cijkl<br />

can be defined as:<br />

Cijkl Xij/ekl where Xij and ekl are, respectively, the second rank, symmetric<br />

stress and strain tensors.<br />

The two functions f1 xy and f2 x2 y2 happen to be related to the<br />

components of the second rank tensor:<br />

⎛<br />

⎞<br />

xx xy xz<br />

⎝ yx yy yz ⎠<br />

zx zy zz<br />

We should note that the above second rank tensor is not symmetric. However,<br />

as we have seen in the case of the strain tensor, we can always symmetrize<br />

(xy yx)/2. As long as we consider<br />

this tensor by defining a new function f ′ 1<br />

symmetry operations within the C6 point group f1 and f ′ 1<br />

will have the same<br />

symmetry properties. This observation allows us to map f ′ 1 into exy or e6 and<br />

f2 into exx eyy or e1 e2. Now we apply this mapping to the Raman tensor<br />

components. For example, for the mode f1 the Raman tensor should be given<br />

by:<br />

⎛ ¯11 ¯12 ¯13<br />

⎞<br />

⎜ f1<br />

⎜ ¯21<br />

Rij(f1) ⎜ f1<br />

⎝<br />

f1<br />

¯22<br />

f1<br />

f1 ⎟<br />

¯23 ⎟<br />

f1 ⎟<br />

⎠<br />

¯31<br />

¯32<br />

¯33<br />

f1 f1 f1<br />

Next we can apply the mapping: ¯ij/f1 ⇔ ¯ij/f ′ 1 ⇔ Xij/e6 Ci6 where i <br />

1...6. From the results of Problem 3.7 we see that the only non-zero element<br />

of the form Ci6 is C66. Thus, based on the results of Problem 3.7 we conclude<br />

that the Raman tensor for the f1 mode has the form:<br />

⎛ ⎞<br />

0 d 0<br />

Rij(°6(xy)) ⎝ d 0 0⎠<br />

0 0 0<br />

To obtain the Raman tensor for the f2 mode we map ¯ij/f2 into (Xij/exx <br />

Xij/eyy) (Xij/e1 Xij/e2). Again using the results of Problem 3.7 we<br />

conclude that all the off-diagonal elements of the Raman tensor vanish. The<br />

only non-vanishing elements are of the form: (X11/e1 X11/e2) C11 C12<br />

and (X22/e1 X22/e2) C21 C22 (C11 C12). Thus, the Raman tensor<br />

for the f2 mode is of the form:<br />

Rij(°6(x 2 y 2 ⎛ ⎞<br />

e 0 0<br />

)) ⎝ 0 e 0 ⎠<br />

0 0 0<br />

In Problem 3.7 the stiffness tensor components C66 (C11 C12)/2. Similarly,<br />

one can show that d e.

654 <strong>Appendix</strong> B<br />

Solution to Problem 7.6<br />

Figure 7.26(b) shows the scattering geometry used by Henry and Hopfield in<br />

determining the polariton dispersion of GaP.<br />

(a) From this figure it is clear that the minimum value of the polariton wave<br />

vector q for a given value of kL and the scattering angle ı is: qmin kL sin ı.<br />

(b) From Pythagoras Theorem one obtains that q2 a2 q2 min .ora [q2 <br />

q2 min ]1/2 . Since ks a kL cos ı one obtains the result: ks kL cos ı a <br />

kL cos ı [q2 q2 min ]1/2 .<br />

(c) Using the result in (b) we can write:<br />

kL ks kL (kL cos ı [q 2 q 2 min ]1/2 )<br />

kL(1 cos ı) q[1 (qmin/q) 2 ] 1/2<br />

Since ˆL hckL and ˆS hckS (where c is the speed of light inside the<br />

crystal) the Raman frequency ˆL ˆS hc(kL ks) ˆL(1 cos ı) <br />

hcq[1 (qmin/q) 2 ] 1/2 .Forq ≫ qmin one obtains the dependence of ˆL ˆS on<br />

q as hcq. This is the reason why the series of broken curves in Fig. 7.26(a) are<br />

“nearly” parallel straight lines for different values of ı. Forq near qmin these<br />

lines are not really straight lines since ˆL ˆS depends on q as [q 2 q 2 min ]1/2 .<br />

Solution to Problem 7.8<br />

(a) The solution to this part of the problem can already be found in Fig.<br />

7.28. The results of translating the various Feynman diagrams into perturbation<br />

terms can be found in (7.50). The correspondence between the diagrams<br />

and the terms in (7.50) is simply: (a) ⇔ term 1; (b) ⇔ term 2; (c) ⇔ term 3<br />

etc. Students are urged to work through each diagram to learn the “art” of<br />

translating Feynman diagrams into perturbation theory expressions. In addition,<br />

notice how some of the terms are related by permutation of the timeorder<br />

of the vertices. This is a very convenient way to generate all the diagrams<br />

by first starting with a few diagrams and then use them to generate<br />

all the remaining diagrams via permutation of the order in which the vertices<br />

occur in time.<br />

(b) To write down all the Feynman diagram contributing to a phonon-assisted<br />

optical transition in an indirect bandgap semiconductor, let us start with the<br />

schematic diagram in Fig. 6.16. The Feynman diagram corresponding to the<br />

process labeled as (1) in Fig. 6.16 is:

The diagram for the process labeled (2) is:<br />

Solution to Problem 7.8 655<br />

These diagrams translate into perturbation terms similar to that in (6.61).<br />

In both of the above diagrams the vertex for the electron-photon interaction<br />

occurs first. We can generate other diagrams in which the electron(hole)phonon<br />

interaction occurs first. For example, the following is a diagram in<br />

which the electron-phonon interaction excites an electron from an intermediate<br />

valence band (°v ′) to the conduction band (¢c) and then the photon<br />

excites another electron from the final valence band state (°v) to fill the hole<br />

in °v ′.<br />

This diagram can also be translated into an expression similar to (6.61). However,<br />

since the electron-hole pair has to be created via emission of a phonon<br />

the energy denominator in this case has the form: Ecv ′ ˆphonon and this term<br />

is highly non-resonant.<br />

(c) The Feynman diagrams for two-phonon Raman scattering processes can be<br />

divided into three types. These are labeled (a) to (c) in the following figure.

656 <strong>Appendix</strong> B<br />

All the diagrams have corresponding diagrams in which the holes are scattered<br />

by phonons rather than electrons.<br />

Solution to Problem 7.10<br />

This problem is another illustration of the power of group theory. The yellow<br />

exciton in Cu2O is electric-dipole forbidden. However, optical excitation via<br />

an electric quadrupole transition of representation ° 5 (or ° 25 ) is allowed. This<br />

opens up the possibility of a resonant Raman process in which the incident<br />

photon excites the yellow exciton via an electric quadrupole transition, the<br />

exciton is scattered via the creation or annihilation of a phonon and finally a<br />

scattered photon is emitted via an electric dipole transition of representation<br />

° 4 (or ° 15 ). According to the Matrix Element Theorem the phonon in this<br />

case should have the same representation as the direct product of ° 5 and<br />

° 4 (see also the solution to Problem 7.5). The character table for the space<br />

group of Cu2O (O4 h ) is nonsymmorphic (see Problem 3.1) but its factor group<br />

isomorphic to the factor group of the space group of diamond (O7 h ). Thus we<br />

can use the characters for the space group of diamond in Table 2.16 to obtain<br />

the characters of ° 5 ⊗ ° 4 :<br />

{E} {C2} {S4} {Ûd} {C3} {i ′ } {i ′ C2} {i ′ S4} {i ′ Ûd} {i ′ C3}<br />

° 5 3 1 1 1 0 3 1 1 1 0<br />

° 4 3 1 1 1 0 3 1 1 1 0<br />

° 5 ⊗ ° 4 9 1 1 1 0 9 1 1 1 0<br />

By inspection we can show that the direct product: ° 5 ⊗° 4 is reducible to the<br />

direct sum: ° 1 ⊕ ° 3 ⊕ ° 4 ⊕ ° 5 . When combined with the results of Problem<br />

3.1 we find that all the odd-parity phonons in Cu2O should become Ramanactive<br />

via this quadrupole-dipole transition mechanism whenever the incident

Solution to Problem 7.12 657<br />

or scattered photon is resonant with the electric-quadrupole allowed yellow<br />

exciton. An example of the application of this resonant Raman process involving<br />

the odd-parity ° 3 (or ° 12 ) phonon mode to map out the yellow excitonic<br />

series in Cu2O is shown in Fig. 7.34.<br />

Solution to Problem 7.12<br />

For a [100] uniaxial stress of magnitude X the strain tensor is given by (as<br />

shown in Problem 3.4):<br />

⎛<br />

eij ⎝ S11<br />

⎞<br />

0 0<br />

0 S12 0 ⎠ X<br />

0 0 S12<br />

In a diamond-type semiconductor the zone-center optical phonons are threefold<br />

degenerate at X 0. Under the [100] uniaxial stress the crystal symmetry<br />

is lowered to tetragonal so we expect the phonon to be split into a singlet and<br />

doublet as discussed also in Problem 6.13. To obtain the magnitude of the<br />

stress-induced shift in the phonon frequencies we will first substitute the elements<br />

of the above strain tensor into the determinant of the secular equation<br />

given in Problem 6.23. We obtain:<br />

<br />

<br />

<br />

(pS112qS12)X Ï 0 0 <br />

<br />

<br />

0 [pS12q(S11S12)]X Ï 0 <br />

<br />

0 0 [ ( pS12<br />

... S12)]X <br />

The three solutions of the corresponding secular equations consist of a nondegenerate<br />

(singlet) solution:<br />

Ï1 ˆ 2 1 ˆ2 0 X(pS11 2qS12)<br />

and a doubly degenerate (doublet) solution:<br />

Ï2 ˆ 2 2 ˆ2 0 X[pS12 q(S11 S12)].<br />

Under the small strain (and therefore low stress) condition we have assumed,<br />

we can approximate Ï ˆ 2 ˆ 2 0 by (ˆ ˆ0)(ˆ ˆ0) ∼ 2ˆ0(ˆ ˆ0). The<br />

shifts of the singlet and doublet optical phonons are thus given, respectively,<br />

by:<br />

¢ˆs X<br />

[pS11 2qS12]<br />

2ˆ0<br />

and<br />

¢ˆd X<br />

[pS12 q(S11 S12)]<br />

2ˆ0<br />

The average of the three phonon modes: ¢ˆH (ˆs 2ˆd)/3 shifts with stress<br />

as: ¢ˆH (X/6ˆ0)(p 2q)(S11 2S12) while the splitting between the two

658 <strong>Appendix</strong> B<br />

modes ¢ˆ ˆsˆd is given by ¢ˆ (X/2ˆ0)(pq)(S11S12). The stress dependence<br />

of the singlet and doublet phonon modes can be expressed in terms<br />

of ¢ˆH and ¢ˆ as:<br />

¢ˆs ¢ˆH (2/3)¢ˆ and ¢ˆd ¢ˆH (1/3)¢ˆ.<br />

Another way of obtaining the above results is to first decompose the strain<br />

tensor into a hydrostatic component plus a traceless shear component as discussed<br />

in Problem 3.4:<br />

⎛<br />

eij ⎝ S11<br />

0<br />

0<br />

S12<br />

0<br />

0<br />

⎞<br />

⎠ X<br />

0 0 S12<br />

⎛<br />

1<br />

[(S11 2S12)X/3] ⎝ 0<br />

0<br />

1<br />

⎞<br />

⎛<br />

0<br />

2<br />

0⎠<br />

[(S11 S12)X/3] ⎝ 0<br />

0<br />

1<br />

0<br />

0<br />

⎞<br />

⎠<br />

0 0 1<br />

0 0 1<br />

It is then straightforward to show that the hydrostatic strain produces the average<br />

shift ¢ˆH while the shear strain splits the degenerate optical phonons<br />

into a singlet and a doublet separated by ¢ˆ. Using the same approach and<br />

the results of Problem 3.4 the splitting of the optical phonons induced by a<br />

[111] oriented stress can be calculated easily.<br />

Note: The Raman tensors of a diamond-type crystal are, in principle, altered<br />

by the application of a uniaxial stress. For low stress one can, however, neglect<br />

the effect of the stress on the magnitude of the Raman tensor. This is particularly<br />

true for a scattering geometry where the Raman tensor is non-zero at<br />

zero stress and is most likely much larger than the strain-induced change.<br />

As an example of the effect of uniaxial strain on Raman modes, we will consider<br />

the case of backscattering from a [100] surface of a diamond-type crystal<br />

under a uniaxial stress along the [001] direction. Based on the above discussions<br />

we would expect that the optical phonon polarized along the [001] direction<br />

to be the singlet mode while the ones polarized along the [100] and [010]<br />

axes to be the doublet mode. For the singlet mode the non-zero Raman tensor<br />

component are: Rxy and Ryx. For the backscattering geometry from the [100]<br />

surface the light polarization cannot lie along the x-axis or [100] direction so<br />

the singlet mode is always forbidden. For the doublet mode the non-zero Raman<br />

tensor components are: Rxz, Rzx, Ryz and Rzy. Thus the doublet mode is<br />

allowed for the scattering geometries: (||, ⊥) and (⊥, ||) where || and ⊥ refers<br />

to the [001] stress axis. The reader should work out the Raman selection rules<br />

for backscattering from a surface under [111] stress. The results can be found<br />

also in:<br />

F. Cerdeira, C.J. Buchenauer, F.H. Pollak and M. Cardona: Stress-induced<br />

shifts of first-order Raman frequencies of diamond- and zinc-blende-type semiconductors.<br />

Phys. Rev. B5, 580 (1972).

Solution to Problem 8.1<br />

Solution to Problem 8.1 659<br />

There are several units of pressure in use nowadays. When we try to inflate<br />

our tires we find that the unit for pressure most commonly used in the US is<br />

pounds per square inch (PSI). When the meteorologists report their weather<br />

forecast they quote the atmospheric pressure in terms of inches of mercury<br />

(Hg). The SI unit for pressure is the Pascal (Pa). However, when one is dealing<br />

with vacuum systems and pumps the most common unit for pressure is the<br />

torr. The conversion from torr to Pa and the cgs units (which we use here)<br />

can be found in the inside back cover table.<br />

Let us recall that a torr is the pressure exerted by a column of Hg 1 mm<br />

high. Since the density of Hg 13.6 g/cm 3 , and the acceleration due to gravity<br />

is 981 cm/sec 2 , 1 torr 1.33 × 10 3 dyn/cm 2 in cgs units. Thus, a pressure of<br />

10 6 torr corresponds to 1.33 × 10 3 dyn/cm 2 .<br />

Next we determine the density of oxygen molecules at this pressure and a<br />

temperature of 300 K using the equation of state of ideal gases:<br />

p NkBT,<br />

where p is the pressure (in dyn/cm 2 ), N is the number of molecules per cm 3 ,<br />

kB is the Boltzmann’s constant (1.38×10 16 erg/K, from the inside back cover)<br />

and T the temperature in Kelvin. From this equation we obtain N 3.22 ×<br />

10 10 molecules/cm 3 for the pressure and temperature under consideration.<br />

Using the kinetic theory of gases (see e.g., F.J. Blatt, Principles of Physics,<br />

(Allyn and Bacon, 1983), p. 262) we find that the pressure p is related to the<br />

average velocity v of one molecule by the equation:<br />

v 2 3p/NM,<br />

where M is the mass of the molecule (we take M to be the oxygen molecule<br />

mass: 2 × 16 × 1.67 × 10 24 gm 5.34 × 10 23 gm). Hence the average<br />

oxygen molecule velocity v 4.82 × 10 4 cm/sec. The number of molecules<br />

impinging on a surface area of 1 cm 2 per second is obtained by multiplying v<br />

by N. However, one must take into account that the velocity can point along<br />

six different directions: x, y, z, x, y, z. If the surface is perpendicular to say<br />

the z-direction, then only the molecules with velocities along the z direction<br />

will contribute to collisions with the surface. Hence, we have to divide N by 6<br />

in order to obtain the total number of molecules colliding with 1 cm 2 of the<br />

surface per second. The result is:<br />

(1/6)v.N 2.62 × 10 14 /cm 2 sec.<br />

Let us now consider the (001) silicon surface. Since there are two atoms per<br />

unit lattice square on this surface, the surface density of Si atoms is: 2/a 2 0 ,<br />

where a0, the lattice constant, is equal to 0.543 nm. The surface density of<br />

atoms is, therefore, 6.78×10 14 atoms/cm 2 . Assuming that the oxygen molecules<br />

split into two oxygen atoms upon collision with the surface, then after 1 Langmuir<br />

(L) of exposure the Si surface should be 77.3% covered if the sticking

660 <strong>Appendix</strong> B<br />

coefficient of oxygen atoms to Si atoms is one. Typically an exposure of ∼1 L<br />

is needed to cover a surface with a monolayer of adatoms.<br />

Students are urged to repeat the calculation for a (111) and a (110) Si<br />

surface.<br />

Solution to Problem 8.2<br />

We refer for notation to Fig. 8.9.<br />

The average radius of the analyzer is Ra. The applied voltage is Va, the<br />

kinetic energy of the electrons under consideration is Ee. The electron band<br />

pass energy, being non-relativistic, is obtained by equating the electron centripetal<br />

force mv 2 /Ra to the force eVa/2¢Ra exerted by the electric field on<br />

the electron (of charge e and mass m):<br />

mv 2<br />

Ra<br />

eVa<br />

2¢Ra<br />

i.e., Ee eVa<br />

4<br />

Ra<br />

¢Ra<br />

For some typical values: Va 1V,Ra 10 cm and ¢Ra 0.5 cm we find that<br />

Ee 5eV.<br />

The resolution of the hemispherical analyzer is defined by the change in<br />

the band pass energy ¢Ee induced by a small change ‰Ra in Ra: From the<br />

above result ¢Ee/‰Ra (eVa/4¢Ra). In case of the typical hemispherical analyzer<br />

values given above the resolution is 0.05 eV/mm.<br />

Solution to Problem 8.5<br />

A model of the zincblende crystal structure would be helpful in visualizing this<br />

problem<br />

Let us first consider a (100) surface. It involves atoms of only one of the<br />

two sublattices discussed in Chap. 2 as constituting diamond or zincblende<br />

crystals. Hence no operations transforming an atom in one of the sublattices<br />

into one in the other can exist and a single flat surface layer must have a symmorphic<br />

space group. One may at first sight think that C4, a fourfold rotation<br />

about the [100] axis, is a symmetry operation. This is not the case: the atoms<br />

have tetrahedral, not fourfold symmetry because of the sp 3 bonding. The only<br />

symmetry operations of the diamond (Table 2.5) or the zincblende (Table 2.3)<br />

point groups that survive when we consider the (100) surface are: a C2 rotation<br />

around the [100] axis and two reflections across the (011) and (01-1)<br />

planes. The point group is C2v whose characters are shown in Table 2.14.<br />

Similar considerations concerning a (111) surface lead to the point group<br />

C3v. Note, however, that there are two possible non-equivalent flat (111) surfaces.<br />

One of them has “dangling bonds” sticking out of the crystal perpendicular<br />

to (111). In the other, each atom has three “dangling bonds” at an angle

Solution to Problem 8.9 661<br />

of 19.5 ◦ with the surface. Show that the former is energetically favorable when<br />

cleaving a crystal parallel to one of the equivalent (111) surfaces.<br />

The primitive translation vectors of a (100) surface are (a/2)(011) and<br />

(a/2)(01-1).<br />

The two corresponding reciprocal lattice vectors can be obtained from<br />

(2.9) by defining a3 a(001). Using these two vectors it is easy to draw the<br />

corresponding Brillouin zone.<br />

The groups of the k-vector at the center of the Brillouin.zone. are also C2v<br />

and C3v.<br />

Solution to Problem 8.9<br />

Let us start with the simplest case, that of a zincblende crystal (point group at<br />

°: Td).<br />

We will discuss the hexagonal faces first and then the tetragonal faces.<br />

The point in a tetragonal face with the highest symmetry is the X-point:<br />

(2°/a0)(100). The corresponding group of the k-vector is D2d (Table 2.15). The<br />

slope of a given band perpendicular to this face is proportional to the expectation<br />

value of px according to (2.35). It is easy to check with Table 2.15 that<br />

px has X3 symmetry. All bands are non-degenerate (we are neglecting spin at<br />

this point) at the X point except those of X5 symmetry which are twofold degenerate<br />

(see Fig. 2.14. In this figure the X5 bands are split into X6 and X7<br />

by spin-orbit interaction. In the absence of spin-orbit interaction these bands<br />

remain doubly degenerate along the ¢ direction because of time reversal invariance).<br />

Any nondegenerate bands will approach the X-point along ¢ with<br />

zero slope because the product of two nondegenerate representations is the<br />

identity representation, X1 in our case. Since px belongs to X3, its expectation<br />

value for a nondegenerate representation must vanish. Since the X5 degeneracy<br />

does not split along ¢, both bands belonging to it act as a single band<br />

which also end at the X point with zero slope. The only other high symmetry<br />

point on the (100) face is the W-point, (1, 0, 1<br />

2 ). Its point group is S4 [2.4]. It is<br />

easy to see that the matrix elements of px do not vanish by symmetry at this<br />

point and thus no one-dimensional van Hove singularities occur there.<br />

Let us consider now a face perpendicular to the [111] axis. The highest<br />

symmetry point of k-space on this surface is L. The corresponding group is<br />

C3v (see Table 2.12). The component of p along the [111] direction is invariant<br />

under all operations of C3v and, therefore, we cannot use an argument<br />

similar to that used for the (100) face to prove that the bands have zero slope<br />

perpendicular to the (111) face. An examination of Figs. 2.14 and 2.15, however,<br />

suggests that this is still the case. In order to prove it, we use the following<br />

arguments. Let us move along the § axis, perpendicular to the (111)<br />

face, by an infinitesimally small amount ‰. The resulting point we label as<br />

(apple/a0)(1 ‰)(111). Using time reversal symmetry we can show that the energy<br />

of a given band at this point is equal to that at (apple/a0)(1 ‰)(111). Adding to

662 <strong>Appendix</strong> B<br />

the latter k the reciprocal lattice vector (2apple/a0)(111) we find that the energy at<br />

the point (apple/a0)(1 ‰)(111) should be the same as that of (apple/a0)(1 ‰)(111).<br />

Hence the slope of the energy vs. ‰ vanishes. There are no other symmetry<br />

points (U, W, orK) for which the slope perpendicular to the (111) faces vanishes.<br />

In the case of germanium the group of the k vector at L is isomorphic to<br />

D3d (see p. 55). This group has even higher symmetry than C3v. Hence, the<br />

slope under consideration also vanishes. In the case of the X-point matters<br />

are more complicated because of the non-symmorphic nature of the groups<br />

as discussed in 2.4.2. The relevant k-vector representations are all two-fold<br />

degenerate (X1, X2, X3, X4 in Table 2.19). With the exception of X4 these representations<br />

split along ¢ becoming non-degenerate. The representations that<br />

split have equal and opposite slopes along ¢ (so that the average slope remains<br />

zero). Hence for them no van Hove singularities are obtained. All the<br />

others reach the X point with zero slope.<br />

Solution to Problem 8.10<br />

Let us first consider the case of the d orbital states (l 2) under a tetrahedral<br />

field (point group symmetry Td, which is equivalent to the ° point of a<br />

zincblende crystal). The splitting pattern is the same for a cubic field of point<br />

group symmetry Oh (similar to the ° point of the diamond crystal) although<br />

the corresponding representations may be labeled differently, according to Tables<br />

2.3 (Td) or2.5 (Oh). The d-functions are even upon inversion, hence reflections<br />

and C2 rotations must have the same characters, given by (8.24) when<br />

considering the full rotation group. These characters are, for the five operations<br />

relevant to the Td group:<br />

E C2 S4 Û C3<br />

5 1 1 1 1<br />

(8.25)<br />

In order to decompose the fivefold degenerate orbital d states into those belonging<br />

to irreducible representations of the Td point group we use the orthogonality<br />

relations (2.11) and the Table 2.3 of characters of the Td group.<br />

Performing the appropriate multiplications and sums, the right hand side<br />

of (2.11) becomes: h (the number of Td group operations 24) for the °3(E)<br />

and °4(T2) representations and zero for all others. Hence, the fivefold d orbital<br />

states split into a triplet °4(T2) and a doublet °3(E) in a field of either<br />

tetrahedral or cubic symmetry. In the case of electronic band structures this<br />

will happen for the d states at k 0.<br />

Let us consider d-orbital states with a spin of 1<br />

2<br />

attached to them (one-<br />

electron states). Multiplication of angular momentum l 2 (orbit) with<br />

s 1/2 (spin) gives rise to two sets of states, a sextuplet with J 5/2 and<br />

a quadruplet with J 3/2. In order to investigate the effect of a field of either<br />

Td (the case we are considering here) or Oh symmetry we must use the

Solution to Problem 8.10 663<br />

corresponding double groups. These have, besides the operations mentioned<br />

above, rotations by 2apple which reverse the sign of the spin (because s 1<br />

2 ). The<br />

representations of the double group fall into two classes, those with the same<br />

character for E and E (a rotation by 2apple) and those for which ¯(E) ¯(E).<br />

The latter operations introduce a set of so-called additional representations.<br />

The counterpart of (8.25) for the double group of the J 5/2 functions is (use<br />

(8.24)):<br />

E E C2 C2 S4 S4 Û Û C3 C3<br />

J (5/2) 6 6 0 0 √ 2 √ (8.26)<br />

2 0 0 0 0<br />

In order to find out the effect of a Td symmetry field on the (5/2) wave functions.<br />

We use the characters of the additional representations of the Td group<br />

given in Ref. 2.4:<br />

°6<br />

°7<br />

E<br />

2<br />

2<br />

E<br />

2<br />

2<br />

3C2<br />

0<br />

0<br />

3C2<br />

0<br />

0<br />

6S4 √<br />

2<br />

<br />

6S4 √<br />

2<br />

6Û<br />

0<br />

6Û<br />

0<br />

8C3<br />

1<br />

8C3<br />

1<br />

√ 2 √ 2 0 0 1 1<br />

°8 4 4 0 0 0 0 0 0 1 1<br />

(8.27)<br />

The numbers on the first row indicate the number of corresponding operations,<br />

which have to be used in the evaluation of (2.11). This evaluation gives<br />

for the product of the J (3/2) representation and the additional ones of Td:<br />

(5/2) × °6 0<br />

(5/2) × °7 48<br />

(5/2) × °8 48<br />

(48 is the total number of operations of the Td double group)<br />

This implies that the J 5/2 sextuplet splits into a quadruplet (°8) and a<br />

doublet (°7).<br />

Multiplying the characters of the J 3/2 representation by those in Table<br />

(8.27) and contracting them as required by (2.11) we obtain:<br />

(3/2) × °6 0<br />

(3/2) × °7 0<br />

(3/2) × °8 48,<br />

Hence the J 3/2 quadruplet does not split under the action of a field of either<br />

Td or Oh symmetry.<br />

Another interesting exercise consists of introducing spin, and applying<br />

spin-orbit interaction (2.45a), to the °4 and °3 functions into which J 5/2<br />

splits. We assume that the orbital splitting is much larger than the spin-orbit<br />

splitting so that no coupling between °4 and °3 takes place. The effect of spin<br />

is obtained by multiplying the orbital representations by °6, the double group<br />

representation which corresponds to J 1/2. By applying the orthogonality<br />

relation (2.11) one will find that the sextuplet consisting of °4 with either up<br />

or down spin split into a quadruplet (°8) and a doublet (°7). The °3 orbital<br />

doublet becomes a °8 quadruplet and does not split.<br />

An interesting observation is that, in the absence of a Td or Oh field but<br />

in the presence of spin-orbit interaction, the sextuplet (J 5/2) state is usually

664 <strong>Appendix</strong> B<br />

higher in energy than the J 3/2 quadruplet. However, if one includes spin in<br />

the split °4 state, it splits further into °8 and °7, the former being below the<br />

latter.<br />

Readers may want to consult:<br />

K. Shindo, A. Morita and H. Kamimura: Spin-orbit coupling in ionic crystals with zincblende<br />

and wurtzite structures. Proc. Phys Soc Japan 20, 2054 (1965), and errata in<br />

Proc. Phys Soc Japan 21, 2748 (1966)<br />

For further discussions.<br />

Another exercise will be to show that the spin-orbit interaction does not split the °3<br />

orbital doublet which becomes a °8 quadruplet when spin is included.<br />

Solution to Problem 8.11<br />

The problem is of interest in connection with the calculation of core level<br />

shifts discussed in pages 453 and 454.<br />

We consider a uniformly charged spherical shell with outer radius rm and<br />

inner radius °rm with 0 ° 1. We impose the boundary condition on the<br />

potential V → 0 for r (the distance from the center of the shell) →∞.We<br />

use Gauss’s theorem: the electric field E is directed towards (or away from)<br />

the center of the shell and has, at the distance r from that center and outside<br />

of the shell (r rm) the magnitude E q/r 2 where q is the total charge in<br />

the shell, taken to be negative for an electron (note that cgs units are used in<br />

this problem). For r rm the magnitude of the field is q ∗ /r 2 , where q ∗ is the<br />

charge within a sphere of radius r∗ rm.<br />

q ∗ q[r 3 (°rm) 3 ]/[r 3 m (°rm) 3 ].<br />

In order to calculate V(r) we integrate the field E(r) from infinity to rm and<br />

add to the resulting V(rm) q/rm, the integral of E(r) between rm and °rm.<br />

The result is:<br />

V(0) q<br />

rm<br />

<br />

q<br />

[r3 m (°rm) 3 <br />

°rm<br />

r <br />

] rm<br />

q q<br />

<br />

rm [r3 m (°rm) 3 ]<br />

<br />

<br />

(°rm) 2<br />

2<br />

3 (°rm)<br />

r2 <br />

dr<br />

(°rm) 2 r2 m<br />

2 r2 m °3<br />

It is of interest to check the value of V(0) for the two extreme cases, ° 0<br />

(uniformly charged sphere) and ° 1 (infinitesimal thickness of the shell.<br />

In the former case we find V(0) q/rm. In the latter case we find V(0) <br />

(3/2)q/rm.

Solution to Problem 9.2<br />

Solution to Problem 9.2 665<br />

This 1D periodic potential (known as the Kronig-Penney Potential) is so wellknown<br />

that the solutions can be found in textbooks on Solid State Physics<br />

(see, for example, Ref. [7.14]) or Quantum Mechanics (see, for example,<br />

Ref. [9.19]).<br />

First, to simplify the problem we will assume that the solutions are Bloch<br />

waves of the form: Ê exp(ikx)u(x) where u(x) is a periodic function.<br />

Next we assume that the origin x 0 is chosen to be the beginning of one<br />

well. In this coordinate system the potential V(x) 0 for 0 x a (the well)<br />

and V(x) V for a x b. The period of the potential a b is defined as<br />

d.<br />

The boundary conditions imposed by the periodicity of the potential on<br />

u(x) are: u(0) u(d) and u ′ (0) u′ (d).<br />

We have defined u(0) u(‰) and u(d) u(d ‰) where, in both cases,<br />

‰ is 0 and in the limit ‰ ⇒ 0. When the particle is inside the well we expect<br />

its wave function to satisfy the Schrödinger Equation for a free particle (since<br />

V(x) 0):<br />

Ê(x) A exp(ik1x) B exp(ik1x) (9.2a)<br />

where E (k1) 2 /2m is the particle energy. We will now assume that E V<br />

so that classically the particle will be confined inside the well. In this case the<br />

particle cannot penetrate into the barrier under the laws of classical physics.<br />

Thus, its wave function has to decay exponentially with distance into the barrier.<br />

Let us assume solutions of the form:<br />

Ê(x) C exp(Îx) D exp(Îx) (9.2b)<br />

where V E (Î) 2 /2m.<br />

By writing u(x) exp(ikx)Ê(x) and imposing the boundary conditions<br />

on u(x) and u ′ (x) atx 0 and at x a we can obtain four linear equations<br />

relating A, B, C and D:<br />

A B exp(ikd))[C exp(Îd) D exp(Îd)] (9.2c)<br />

ik1(A B) Î exp(ikd)[C exp(Îd) D exp(Îd)] (9.2d)<br />

A exp(ik1a) B exp(ik1a) C exp(Îa) D exp(Îa) (9.2e)<br />

ik1[A exp(ik1a) B exp(ik1a)] Î[C exp(Îa) D exp(Îa)] (9.2f)<br />

These 4 homogenous equations have non-trivial solutions when their determinant<br />

vanishes:<br />

<br />

<br />

1<br />

<br />

<br />

<br />

<br />

<br />

1 ed(Îik) ed(Îik) k1 k1 Î<br />

i<br />

ed(Îik)<br />

Î<br />

i ed(Îik)<br />

eik1a eik1a eÎa eÎa <br />

<br />

<br />

<br />

<br />

0<br />

<br />

<br />

(9.2g)<br />

k1e ik1a k1e ik1a Î<br />

i eÎa<br />

Î<br />

i eÎa

666 <strong>Appendix</strong> B<br />

After a bit of algebra we obtain from (9.2g) the secular equation:<br />

(cos k1a)(cosh Îb) [(k 2 1 Î2 )/2k1Î](sin k1a)(sinh Îb) cos kd. (9.2h)<br />

This equation contains the unknown k as a function of k1 and Î. Both<br />

k1 and Î are functions of E and are related by: k 2 1 Î2 2mV/ 2 . By<br />

combining k1 and Î in a way so that the above equation (9.2h) contains<br />

only E and k we can obtain the dispersion relation i.e. E as a function<br />

of k. The results in the following figure and table are obtained by using<br />

the program Mathcad. The program codes are shown in a separate file labeled<br />

as Problem9.2 Codes.mcd which can be downloaded from the website:<br />

http://pauline.berkeley.edu/book/SolutionsNew.html.<br />

Figure 9.2.1 was obtained for a b 5 nm and for an effective mass<br />

m 0.1 times the free electron mass m0.<br />

The Left Hand Side of Eq. (9.2h)<br />

Electron Energy (eV)<br />

Figure 9.2.1 The relation between E and k can be determined by setting the y-axis (equal<br />

to L(E) Left Hand Side expression of Eq. 9.2h)) to cos(kd) and reading off the value<br />

of E from the x-axis. This process can be greatly simplified if we notice that the curves<br />

in the above figure can be approximated by straight lines. Let E0 be the minimum energy<br />

when L(E) 1 and W be the band width of the lower energy branch. If we assume that<br />

the curve is a straight line then it can be written as: E [E0 (W/2)] (W/2)L(E) or:<br />

E [E0 (W/2)] (W/2) cos(kd)<br />

In the Table 9.2.1 we show the values of E for some simple values of L(E) and the corresponding<br />

E0 and W.

Solution to Problem 9.4 667<br />

Table 9.2.1 The eigenvalues E of the Kronig-Penney Model for two different sets of values<br />

of the well (a) and barrier width (b) assuming that the effective mass of the electron<br />

in the well and barrier is 0.1m0 (free electron mass). When there are two bands they are<br />

shown in separate columns under the same values of a and b.<br />

cos[k(a b)] E(a b 3 nm) in eV E(a b 5 nm) in eV<br />

1 0.13176 0.07563 0.291<br />

0 0.14465 0.07637 0.28154<br />

1 0.16068 0.07713 0.27352<br />

E0 (eV) 0.13176 0.07563 0.27352<br />

W (meV) 29 1.5 16<br />

Additional eigenvalues for other values of a and b can be calculated similarly.<br />

Solution to Problem 9.4<br />

For the case of k 0, the equations in (9.22) reduce to:<br />

mAˆ 2 v f [x 2v u];<br />

mBˆ 2 x f [y 2x v];<br />

mBˆ 2 y f [x 2y u]; and<br />

mAˆ 2 u f [v 2u y].<br />

One can solve this system of four linear and homogeneous equations by setting<br />

its determinant:<br />

<br />

<br />

mAˆ<br />

<br />

<br />

<br />

<br />

<br />

2 2f f 0 f<br />

f mAˆ2 2f f 0<br />

0 f mBˆ2 2f f<br />

f 0 f mBˆ2 <br />

<br />

<br />

<br />

<br />

<br />

<br />

2f <br />

equal to zero. A simpler and more elegant way to solve this problem would<br />

be to note that this linear chain of atoms has reflection symmetry with respect<br />

to a plane passing through the center between any two atoms (such as the<br />

midpoint between two B atoms). As a result, the k 0 phonons must have<br />

definite parity under this reflection operation. The displacement pattern of the<br />

atoms would either remain unchanged or change sign upon reflection. To symmetrize<br />

the displacement patterns we define new displacement vectors: U, V,<br />

X and Y in terms of the displacements u, v, x and y shown in Fig. 9.14:<br />

U (u v), V (u v); X (x y) and Y (x y).<br />

With these new definitions the equations of motion become:<br />

mAˆ 2 V f [Y 3V];<br />

mBˆ 2 X f [U X];<br />

mBˆ 2 Y f [V 3Y]; and<br />

mAˆ 2 U f [X U].

668 <strong>Appendix</strong> B<br />

Now V and Y form two linear homogeneous equations while U and X form<br />

another set of two linear homogeneous equations. The fact that the modes<br />

represented by U and X are decoupled from those represented by V and<br />

Y means that the atoms of both kinds are moving either in phase or out of<br />

phase.<br />

For<br />

<br />

the X and U modes we obtain the determinant:<br />

<br />

<br />

mBˆ2 f f<br />

f mAˆ2 <br />

<br />

<br />

f <br />

By setting this determinant to be zero we can obtain the equation:<br />

ˆ 4 ˆ 2<br />

<br />

1<br />

<br />

mA<br />

1<br />

<br />

f 0.<br />

mB<br />

By solving this equation we obtain the eigenvalues:<br />

ˆ 0 and ˆ 2 f [(1/mA) (1/mB)]. (see(9.23))<br />

By calculating the eigenvectors one can show that: for the ˆ 0 acoustic<br />

mode X U i.e. the displacement of the A and B layers are in the same direction<br />

as one may expect for an acoustic mode. Furthermore, this displacement<br />

pattern is odd under reflection. Similarly, one can show that the eigenvector<br />

for the other mode is given by: mAU mBX or mA(u v) mB(x y) 0.<br />

In this mode the A and B layers vibrate against each other but their center of<br />

gravity remains constant. Their displacement patterns are shown in Fig. 9.14 as<br />

that of the 348 cm 1 mode. Again, one can show that this mode is odd under<br />

reflection (since only modes of same parity can be coupled with each other in<br />

the equations of motion).<br />

The determinant of the remaining (even parity) Y and V modes is given<br />

by: mBˆ 2 f f<br />

f mAˆ 2 f<br />

<br />

<br />

<br />

<br />

The eigenvalues are obtained by the solving the following equation:<br />

ˆ 4 ˆ 2<br />

<br />

1<br />

<br />

mA<br />

1<br />

<br />

2 8f<br />

f 0<br />

mB mAmB<br />

or<br />

ˆ 2 f 3(mA mB) ± 9(mA mB) 2 4mAmB<br />

2mAmB<br />

as given in (9.24). The corresponding eigenvectors will give the displacement<br />

patterns of the remaining two modes in Fig. 9.14.<br />

When k apple/d, the phase factors exp[±ikd] exp[±iapple] (1).<br />

Thus, the equations of motion become:<br />

mAˆ 2 v f [x 2v u];<br />

mBˆ 2 x f [y 2x v];<br />

mBˆ 2 y f [x 2y u]; and<br />

mAˆ 2 u f [v 2u y].

Solution to Problem 9.14 669<br />

Again by symmetrizing u, v, x and y as in the case of k 0 one can simplify<br />

the 4 × 4 determinant into two 2 × 2 determinants from which the eigenvalues<br />

and eigenvectors can be calculated. The parity of the modes can be deduced<br />

from the eigenvectors afterwards. This is left as an exercise for the readers.<br />

Solution to Problem 9.14<br />

The double barrier structure relevant to Fig. 9.34 is shown schematically below:<br />

V d1<br />

d2<br />

d2<br />

The height of the barrier V 1.2 eV. The widths of the barrier (d2) and of<br />

the well (d1) are equal to 2.6 and 5 nm, respectively. The zero bias transmission<br />

coefficient T(E) can be calculated with the transmission matrix method<br />

described in section 9.5.1.<br />

To apply the transfer matrix technique we will divide the potential into 5<br />

regions to be labeled as 1, ..., 5 from left to right. To define these 5 regions we<br />

will label the horizontal axis as the x-axis and define the five regions by:<br />

x [∞, d2 (d1/2)], [d2 (d1/2), (d1/2)], [(d1/2), (d1/2)],<br />

[(d1/2), d2 (d1/2)], [d2 (d1/2), ∞].<br />

We will choose the origin for the potential such that the potential Vi is equal<br />

to 0 inside the regions i 1, 3 and 5 and equal to V in the regions 2 and 4.<br />

The incident wave is assumed to arrive in region 1 from the left while the<br />

transmitted wave emerges into region 5. Let Ai and Bi be the amplitudes of<br />

the incident and reflected wave in region i. In region i 1, 3 and 5 we can<br />

define the generalized wave vector k1 by:<br />

2 k 2 1 /2m1 E (9.14a)<br />

where E is the energy of the incident electron and is assumed to be less than<br />

V in this problem. In regions i 2 and 4 we will define k2 by:<br />

2 k 2 2 /2m2 E V (9.14b)<br />

m1 and m2 are, respectively, the electron masses in the well and in the barrier.<br />

The wave vector k2 in Eq. (9.14b) is imaginary since E is smaller than the<br />

barrier V. The wave amplitudes An1 and Bn1 in the final region is related

670 <strong>Appendix</strong> B<br />

to the waves A1 and B1 via a product of transfer matrices M1, M2, ..., Mn1:<br />

<br />

<br />

A1<br />

An1<br />

M1M2...Mn<br />

B1<br />

Bn1<br />

Each transfer matrix Mi isa2× 2 matrix of the form:<br />

Mi <br />

<br />

Mi(1, 1)<br />

<br />

Mi(1, 2)<br />

Mi(2, 1) Mi(2, 2)<br />

whose elements are given in Eqs. (9.59a) to (9.59d):<br />

M1(1, 1) <br />

M1(1, 2) <br />

M1(2, 1) <br />

M1(2, 2) <br />

<br />

1 m1k2<br />

exp i(k2 k1) d2 <br />

2 2m2k1<br />

d1<br />

<br />

2<br />

<br />

<br />

1 m1k2<br />

exp i(k2 k1) d2 <br />

2 2m2k1<br />

d1<br />

<br />

2<br />

<br />

1 m1k2<br />

exp i(k2 k1) d2 <br />

2 2m2k1<br />

d1<br />

<br />

2<br />

<br />

<br />

1 m1k2<br />

exp i(k2 k1) d2 <br />

2 2m2k1<br />

d1<br />

<br />

2<br />

(9.14c)<br />

(9.14d)<br />

(9.14e)<br />

(9.14f)<br />

(9.14g)<br />

(9.14h)<br />

The transfer matrices M2, M3, and M4 can be obtained similarly. The product<br />

(Mij) of the four matrices M1, ..., M4 can be calculated with a computer<br />

program, such as Mathematica, Mathcad etc. T(0) can obtained by assuming<br />

that there will be no reflected wave in region 5 so B5 0 and A1 M11A5:<br />

T(0) |A5/A1| 2 |1/M11| 2 .<br />

The following plot of T(0) vs E has been obtained by using the program<br />

Mathcad. The program codes are shown in a separate file labeled<br />

as Problem9.14 Codes.mcd which can be downloaded from the website:<br />

http://pauline.berkeley.edu/book/SolutionsNew.html.

Solution to Problem 9.14 671<br />

Note that in obtaining this plot we have assumed that the electron effective<br />

masses in the well (m1) and in the barrier (m2) are equal, respectively, to<br />

0.037 and 0.0023 times the free electron mass.<br />

Electron Energy (eV)<br />

Transmission curve obtained for m1=0.037mo and m2=0.0023mo.<br />

To calculate the transmission coefficient under applied bias one has to tilt the<br />

barrier and the well and approximate the tilted potential with piece-wise constant<br />

potentials. With slight variation in the computer program this computation<br />

can be done easily and is left as an exercise for the students. The students<br />

are also urged to vary the effective masses and other parameters to see their<br />

effects on the transmission curve.

<strong>Appendix</strong> C:<br />

Recent Development<br />

A4.1 A Prototypical Deep Center in N-Type<br />

Zincblende-Type Semiconductors: The DX Center<br />

A4.1.1 Introduction<br />

So far the hydrogenic impurities have been very attractive from the viewpoint<br />

of understanding their properties. By applying the effective mass theory we<br />

have been able to explain the properties of a large family of impurities using<br />

only the physical properties of the host lattice, without regard to the chemical<br />

nature of the impurities. The relevant physical properties of the host are<br />

its dielectric constant and the effective mass parameters of the nearest band<br />

extrema. We have defined deep centers as defects whose properties cannot be<br />

understood within the effective mass theory. We expect, therefore, their properties<br />

to be sensitive to their chemical and physical nature, such as their ionic<br />

radii and/or electronegativities. It has been relatively difficult to explain the<br />

properties of deep centers in terms of those of the host lattice alone. The vacancy<br />

without lattice relaxation and the isovalent impurities discussed in 4.3.2<br />

and 4.3.3 are two exceptions we have encountered so far. The utility of the<br />

vacancy model is unfortunately reduced by its neglect of lattice relaxation. In<br />

this addition we shall present a class of deep centers known as the DX centers<br />

which was first mentioned in 4.2.2. This family of defects is technologically<br />

important because it has strong effects on the electrical properties of the<br />

host crystal. It has interesting features found in other deep centers, such as<br />

large lattice relaxation, strong electron-phonon coupling, and the existence of<br />

metastable excited states. It is also an interesting example of a many-body effect<br />

known as negative-U, already mentioned in 4.3.<br />

The outline of this addition is as follows. We shall start with some historical<br />

background on how the DX centers were discovered and in so doing<br />

summarize also their important features. This is followed by a simple qualitative<br />

description of the theoretical model of the DX center first proposed by<br />

Chadi and Chang. This model has successfully explained many of the characteristics<br />

of the DX centers. It has also made predictions about properties<br />

which were subsequently verified experimentally. One important prediction of<br />

the Chadi and Chang model (to be abbreviated as the CCM) is that the DX<br />

centers have a negative correlation energy U. We conclude by discussing the<br />

experimental results which have confirmed this prediction.

674 <strong>Appendix</strong> C<br />

A4.1.2 Historical Background<br />

The DX center was discovered in 1979 by Lang and coworkers [Lang79a] in<br />

the ternary alloys n-AlxGa1xAs with Al concentration x 0.22. As shown in<br />

4.2.2, Group IV dopants like Te substituting atoms on the Group VI sublattice<br />

of III-V semiconductors like GaAs form hydrogenic donors. Lang et al. found<br />

that the substitutional Te atoms suddenly behave more like deep centers in<br />

AlxGa1xAs when x is 0.22. For example, the energy required to thermally<br />

ionize the Te impurities (known as the thermal ionization energy) increases<br />

from the hydrogenic donor binding energy of ∼5 meV by more than one order<br />

of magnitude to ∼0.1 eV. The center exhibits a higher-energy, metastable<br />

(or long-lived) and conducting state which can be excited optically. As a result,<br />

samples containing these centers exhibit persistent photoconductivity at low<br />

temperatures (such as T 100 K), i.e. their conductivity is greatly increased<br />

by light irradiation but, unlike ordinary photoconductivity, the sample remains<br />

in this conducting state for a very long time even after the light is turned<br />

off. These unusual properties of the Te donors in AlGaAs have been demonstrated<br />

by Lang et al. with two different kinds of capacitance transient techniques.<br />

These techniques are known as Deep Level Transient Spectroscopy<br />

(or DLTS) and Thermally Stimulated Capacitance (TSCAP). Their results are<br />

shown in Fig. A4.1.<br />

DLTS Signal (arb. units)<br />

TOTAL DIODE CAPACITANCE (pF)<br />

+<br />

0<br />

-<br />

80<br />

60<br />

40<br />

20<br />

0<br />

iii<br />

h<br />

i<br />

ii<br />

(a) DLTS<br />

Al xGa 1-xAs(Te)<br />

x=0.36<br />

(b) TSCAP<br />

0 100 200 300<br />

TEMPERATURE (K)<br />

Fig. A4.1 The DLTS(a) and thermally<br />

stimulated capacitance (TSCAP) results<br />

(b) in AlGaAs:Te obtained<br />

by Lang et al. Reproduced from<br />

[Lang79a].

A4.1 A Prototypical Deep Center in N-Type Zincblende-Type Semiconductors 675<br />

A detailed description of these techniques is beyond the scope of this book.<br />

Interested readers are referred to many reviews found in the literature<br />

[Lang74, Sah75, Lang84, Li94]. The basic idea behind these two techniques<br />

involves the use of a semiconductor containing deep centers as the insulating<br />

layer between two conductors to form a parallel-plate capacitor. For example,<br />

a reverse-biased pn-junction forms such a capacitor [see, for example,<br />

Wang89a]. The highly doped p-type and n-type regions form the conductors<br />

while the depletion layer between them forms the insulator. Unlike a standard<br />

insulator whose thickness is fixed, the thickness of the semiconductor<br />

space-charge layer can be varied by applying an electric field to populate or<br />

depopulate the deep centers. This change in the thickness of the space-charge<br />

layer can be monitored accurately by measuring the corresponding change in<br />

capacitance. A Schottky Barrier formed at a metal/semiconductor junction as<br />

a result of Fermi Level pinning (see 8.3.3) is another example of a variablecapacitance<br />

condenser [see, for example, Wang89b]. In both cases the charge<br />

state of the deep centers in study (assumed to be the only kind in the sample)<br />

affects the junction capacitance. For example, the deep centers can be filled<br />

by applying an appropriate electrical pulse (sometimes referred to as a filling<br />

pulse). Suppose this deep level is normally above the Fermi Level in the depletion<br />

layer. A filling pulse will change the band bending so as to lower the<br />

deep level towards the Fermi level. Whenever a deep level is below the Fermi<br />

level it becomes filled with electrons. Since these electrons have to come from<br />

the filled shallow donors in the n-type region, the depletion layer expands.<br />

As a result, the junction width increases and the capacitance decreases. When<br />

the applied field is removed the deep centers return to their equilibrium occupancy<br />

by emission of carriers and, correspondingly, the junction capacitance<br />

increases. However, in many deep centers the rate of this emission is usually<br />

thermally activated and strongly dependent on temperature. The emission<br />

process can be monitored by measuring the junction capacitance either as a<br />

function of time at fixed temperature or for a fixed time interval as a function<br />

of temperatures.<br />

In the case of DLTS experiments one fixes the time interval (known as the<br />

time window) defined by two times t1 and t2 and then measures the difference<br />

in capacitance C given by ¢C C(t2) C(t1) while sweeping the temperature.<br />

The resulting ¢C (labeled as the DLTS signal in Fig. A4.1) versus temperature<br />

curves are known as the DLTS spectra. As seen in Fig. A4.1 dips and peaks<br />

can appear in these spectra. A dip in capacitance indicates a sudden decrease<br />

in the capacitance which results when the emission rate of carriers from the<br />

deep centers falls within the time window. Typically by selecting several time<br />

windows appropriately and measuring the corresponding temperature of the<br />

dip in the DLTS spectra one can construct an Arrhenius plot (see 7.1.2 for<br />

definition) for the emission rate of carriers from the deep centers. A variation<br />

of the DLTS technique can be used to measure the capture rate of carriers by<br />

deep centers. Figure A4.2 shows Arrhenius plots for the emission and capture<br />

rates of the deep centers in AlGaAs:Te obtained by Lang et al.. The corresponding<br />

activation energies for emission and capture of electrons determined

676 <strong>Appendix</strong> C<br />

from the slopes of these plots are 0.33 eV and 0.26 eV, respectively. Notice<br />

that the emission activation energy Eem is not the same as the capture activation<br />

energy Ecap. Their difference Eem Ecap is equal to the thermal ionization<br />

energy which is defined as the energy required to thermally ionize carriers out<br />

of the deep center. The relation between the three energies will become clear<br />

when we discuss the large lattice relaxation model.<br />

ELECTRON EMISSION OR CAPTURE RATE (sec -1)<br />

10 7<br />

10<br />

10<br />

10<br />

10<br />

10<br />

5<br />

3<br />

10<br />

-1<br />

-3<br />

-5<br />

0.33 eV<br />

0.26 eV<br />

Al Ga As(Te)<br />

0.36 0.64<br />

ELECTRON EMISSION<br />

RATE<br />

ELECTRON CAPTURE<br />

RATE<br />

THERMAL<br />

QUENCHING OF<br />

PHOTOCONDUCTIVITY<br />

0.18 eV<br />

5 7 9 11 13 15 17<br />

1000/T (1/K)<br />

Fig. A4.2 The Arrhenius plots<br />

for the emission and capture<br />

rates of the deep centers in Al-<br />

GaAs:Te obtained by Lang et al.<br />

Reproduced from [Lang79a].<br />

In the TSCAP measurement shown in Fig. A4.1(b) the total capacitance (as<br />

distinct from the capacitance difference measured in DLTS) is measured as a<br />

function of temperature. An increase in capacitance indicates that a smaller<br />

number of electrons are trapped at the deep centers. The curve labeled as (1)<br />

is the steady-state state zero-bias capacitance curve. This curve is reversible for<br />

increasing and decreasing temperatures. Curves labeled as (2) and (3) are irreversible<br />

with respect to temperature cycling. Curve (2) is obtained by first<br />

cooling the sample in the dark from about 200 K to 50 K with a bias of<br />

1 V. This positive bias causes electrons to be trapped on the deep centers<br />

thus returning them to the neutral charged state. At the lowest temperature<br />

the bias voltage is set to zero so that the electrons want to escape from the<br />

deep centers. However, the emission rate at low temperature is very slow and,<br />

therefore, the deep centers remain in a non-equilibrium state. As the sample<br />

is warmed above 100 K the emission process is thermally activated and be-

A4.1 A Prototypical Deep Center in N-Type Zincblende-Type Semiconductors 677<br />

comes much faster than at low temperatures. The result is a sudden rise in<br />

the capacitance. If the sample is now cooled back to 50 K under zero bias,<br />

the capacitance will follow curve (1) rather than retrace curve (2). The reason<br />

why electrons are not re-captured into the deep centers under zero bias<br />

is because the electrons have to overcome a barrier of 0.2 eV in order to<br />

be re-captured by the deep centers. Thus, at temperatures below 100 K the<br />

capture rate is too small for a significant number of electrons to return to the<br />

deep centers. Curve (3) is obtained by illuminating the sample with a broadband<br />

light source after it has been cooled to low temperature in the dark and<br />

under zero bias. The rise in capacitance indicated by the arrow (labeled hÓ)<br />

in Fig. A4.1(b) suggests that the deep centers are photo-ionized. However,<br />

the capacitance remains high even when the light is turned off. This indicates<br />

that carriers have been photo-excited into a metastable state. If the sample is<br />

now warmed up in the dark, the capacitance will follow curve (3). The sudden<br />

decrease in the capacitance at less than 100 K can be explained by the thermal<br />

activation of the capture of electrons from the metastable state back onto<br />

the deep centers. At still higher temperatures the emission process becomes<br />

thermally activated and results in the rise of the capacitance. Thus, the results<br />

obtained by Lang et al. for the behavior of Te in AlGaAs are completely different<br />

from those expected from shallow donors.<br />

Lang et al. named this newly discovered deep defect the DX center because<br />

they thought that it involved a complex consisting of a donor atom D<br />

and an unknown constituent X. Since this center was first observed in alloys<br />

of AlGaAs only, it was believed that X is an intrinsic defect, such as a vacancy<br />

or an interstitial, which are abundant in alloys. Another characteristic of the<br />

DX centers which distinguishes them from the shallow impurities is that their<br />

optical ionization energy (i.e. the minimum photon energy necessary to ionize<br />

the defect, usually denoted by Eop) is much larger than the thermal ionization<br />

energy. For shallow impurities, these two energies are identical and we have,<br />

therefore, not made a distinction between them. In case of the DX centers Eop<br />

is ∼1 eV as shown in Fig. A4.3.<br />

Lang et al. explained qualitatively many of the unusual properties of the<br />

DX centers with a large lattice relaxation model. We shall discuss this model<br />

in greater detail in A4.1.4. The results of Lang et al. in AlGaAs:Te were soon<br />

confirmed by other authors using different donors. For example, Chand et al.<br />

[Chand84] studied the DX centers in AlGaAs:Si using temperature-dependent<br />

Hall-effect measurements. They determined the thermal activation energy of<br />

the Si DX centers as a function of alloy concentration. They found that the<br />

DX center energy level does not follow the lowest conduction band minima<br />

as a function of Al mole fraction. Instead, it appears to follow the conduction<br />

band minima at the L point of the Brillouin Zone as shown in Fig. A4.4. The<br />

fact that the DX center does not follow the nearest conduction band minimum<br />

suggests that it is not a shallow impurity. Lifshitz et al. [Lifshitz80] made<br />

the interesting observation that pressure has the same effect in converting

678 <strong>Appendix</strong> C<br />

Fig. A4.3 The electron photo-ionization cross-section of the DX center in AlGaAs:Te<br />

obtained by Lang and Logan. Reproduced from [Lang79b].<br />

shallow Sn donors in Al0.15Ga0.85As into DX centers as increasing the Al<br />

fraction. 1<br />

A.4.1.3 Identification of DX Centers as Substitutional Deep Donors<br />

An important experiment which eventually led to the correct identification of<br />

the DX centers was performed by Mizuta et al. in 1985[Mizuta85]. Unlike Lifshitz<br />

et al. [Lifshitz80], who started with n-type AlGaAs, these authors applied<br />

hydrostatic pressure to a Si-doped GaAs sample. They found that they could<br />

convert the Si shallow donors into DX centers by applying pressure larger<br />

than 2.4 GPa. Their results are shown in Fig.A4.5. Subsequently many exper-<br />

1 It is interesting to note that William Paul has reported anomalies in the pressure dependence<br />

of resistivity in both n-type GaAs and n-GaSb as early as 1961 [Paul61]. In those<br />

early days of semiconductor research, these anomalies (involving a sudden increase by<br />

more than one order of magnitude at the pressure of around 2.5 GPa in case of GaAs)<br />

were explained in terms of the pressure effect on the conduction band minima. Now,<br />

in hindsight, one can attribute these resistivity anomalies to the conversion of shallow<br />

donors to deep DX centers under pressure.

A4.1 A Prototypical Deep Center in N-Type Zincblende-Type Semiconductors 679<br />

iments have firmly established that the deep centers induced by pressure in<br />

GaAs have the same properties as the DX center found in AlGaAs and, furthermore,<br />

this conversion of shallow donors to DX centers occurred also for<br />

other group IV donors, such as Ge and Sn, and group VI donors like S, Se<br />

and Te. In fact, it has been shown that the effect of a hydrostatic pressure of<br />

0.1 GPa on the DX in GaAs is almost equivalent to adding 1% of Al [Wei89].<br />

It has been known that both pressure and alloying with Al have the similar<br />

effect of lowering the conduction band minima at the X point of the Brillouin<br />

zone in GaAs relative to the zone-center conduction band valley. With<br />

sufficient pressure or Al concentration GaAs can be converted from a direct<br />

band gap semiconductor into an indirect one. At ambient pressure the DX<br />

level associated with donor atoms in GaAs is actually a resonant state above<br />

the conduction band. As a result of the change in the conduction band structure<br />

caused by alloying or by pressure, the DX level emerges from the conduction<br />

band into the band gap and becomes the stable ground state of the<br />

donor. Thus, one can conclude that the DX center is the result of a so-called<br />

“shallow-to-deep transformation” of substitutional donors in GaAs induced by<br />

changes in the conduction band structure. In this transformation the chemical<br />

nature of the impurity plays only a secondary role.<br />

E (eV)<br />

2.5<br />

2.0<br />

1.5<br />

Al Ga As<br />

x 1-x<br />

1.4<br />

0 0.2 0.4 0.6 0.8 1.0<br />

GaAs AlAs Mole Fraction x AlAs<br />

Γ<br />

L<br />

X<br />

E(eV)=0.54x+1.57<br />

Fig. A4.4 The DX center energy<br />

level (open squares) determined by<br />

Chand et al. from temperature-dependent<br />

Hall effect measurement on<br />

Si doped AlGaAs as a function of<br />

the AlAs mole fraction. For comparison<br />

the solid curves labeled as °,<br />

L and X show, respectively, the corresponding<br />

dependence of the direct<br />

band gap energy at the zone center,<br />

the indirect band gap energies between<br />

the conduction valleys at the<br />

L and X points and the zone-center<br />

valence band maximum. Reproduced<br />

from Chand et al. [Chand84].

680 <strong>Appendix</strong> C<br />

Fig. A4.5 (a)–(d)The Deep Level Transient Spectroscopy (DLTS) results in GaAs:Si measured<br />

at different pressures. From the temperature of the dip in the spectra and experimental<br />

conditions it is possible to deduce the thermal ionization energy (EI) of the deep<br />

center. The absence of a dip in the spectra (a)–(c) indicates the absence of any center<br />

with EI larger than 0.2 eV. Spectrum (e) was obtained from a AlGaAs:Si sample under<br />

similar experimental conditions except that no high pressure was applied to that sample.<br />

From the size of the dip in the spectrum (d) an approximate concentration of the deep<br />

center more than 10 17 cm 3 could be deduced. The inset shows the appearance of a persistent<br />

effect in the photoconductivity in GaAs:Si under pressure exceeding 2.5 GPa. The<br />

solid curves were measured with the sample in the dark before any light illumination<br />

while the broken curves were measured after the sample was illuminated momentarily by<br />

light. Reproduced from Mizuta et al. [Mizuta85].<br />

A.4.1.4 Theoretical Models of the DX Centers<br />

Many theoretical models of the DX centers have been proposed. At one time<br />

there were controversies surrounding the atomic and electronic configurations<br />

of the DX center. One such controversy involves the question of whether<br />

there are large [Lang79a, Chadi88, Khachaturyan89] or small lattice relaxations<br />

[Hjalmarson86, Henning87, Bourgoin89, Yamaguchi90] associated with<br />

the formation of the DX center. Another issue is whether the DX center has

A4.1 A Prototypical Deep Center in N-Type Zincblende-Type Semiconductors 681<br />

a negative on-site Coulomb interaction U (abbreviated as -U) between two<br />

electrons localized on the same impurity (as a result of a large lattice relaxation).<br />

It is now generally accepted that the model proposed by Chadi and<br />

Chang in 1988 [Chadi88] is the correct one. One modification to this original<br />

model, referred to as the Chadi-Chang model (or CCM), is the idea proposed<br />

by Yamaguchi et al. [Yamaguchi90] that, in addition to the ground state with<br />

large relaxation, the DX center has also a metastable resonant state with small<br />

lattice relaxation and symmetry A1. The existence of this state which is neutral<br />

rather than negatively charged has now been confirmed by several theoretical<br />

calculations [Dabrowski92] and experiments [Suski94].<br />

The CCM which used the approach based on a super-cell self-consistent pseudopotential<br />

calculation has two important features:<br />

1. When the DX center becomes the stable ground state of the substitutional<br />

donor impurity in GaAs or AlGaAs (as a result of either high pressure or<br />

alloying), the DX center is formed by one neutral donor capturing an electron<br />

from another neutral donor atom. This process can be represented by the<br />

“reaction”:<br />

2d 0 → d DX <br />

where d 0 and d represent, respectively, a fourfold-coordinated substitutional<br />

donors in the neutral and ionized state. The resultant DX center is negatively<br />

charged and contains two electrons localized on the same donor atom. Normally<br />

two electrons will repel each other via the Coulomb interaction U (see<br />

4.3, p. 182). In special cases, such as encountered in the DX center, two electrons<br />

can attract each other as a result of electron-lattice interaction. Such<br />

defect centers exhibiting attractive Coulomb interaction between electrons are<br />

referred to as negative-U centers [Baraff80].<br />

2. The DX defect formation involves a large bond-rupturing displacement of<br />

either the defect atom or the host lattice atoms. For donors on cation sites,<br />

such as SiGa, the donor atom is displaced as shown in Figs. A4.6(a) and (b).<br />

In the case of donors located on anion sites, such as SAs, one of its nearestneighbor<br />

Ga (or Al) atoms along a bond axes, is displaced. This is illustrated<br />

in Figs. A4.6(c) and (d). Thus the local symmetry of a donor is charge dependent.<br />

When the electron occupancy of the donor is 0 or 1, corresponding to<br />

the positively charged d or neutrally charged d 0 states, the local symmetry of<br />

the donor in the vicinity of the donor atom is tetrahedral (i.e., the point group<br />

symmetry is Td) and there is no lattice relaxation. When the electron occupancy<br />

is increased to 2, corresponding to the negatively charged DX state,<br />

the defect symmetry is lowered to trigonal (the point group symmetry is C3v)<br />

as a result of a bond-breaking lattice relaxation.<br />

The reason why a deep and localized state becomes favorable in GaAs<br />

under pressure or alloying with Al is the near degeneracy between the three<br />

conduction minima at °, L and X. The contribution of all these conduction<br />

minima to the deep DX state manifests itself in its alloy and pressure dependence.<br />

Instead of following either the °, L or X conduction valleys as a func-

682 <strong>Appendix</strong> C<br />

tion of alloying (see Fig. A4.4) or pressure, the deep DX state roughly follows<br />

an average (weighted by the degeneracy of each kind of valley) of the dependence<br />

of all the valleys. Because of this degeneracy in reciprocal space, itis<br />

energetically favorable for the electron wave function to become delocalized<br />

in reciprocal space while becoming localized in real space. This localization is<br />

achieved via a large lattice distortion. In other words, the defect electron can<br />

lower its energy by “trading-off” lattice energy with electronic energy. In order<br />

to maximize the gain in electronic energy the DX center attracts an extra<br />

electron when it undergoes lattice relaxation so that the total gain in electronic<br />

energy is doubled while the lattice energy spent remains the same. The idea<br />

that the DX center may be a negative-U center was proposed independently<br />

by Khachaturyan et al. [Khachaturyan89].<br />

Fig. A4.6 The displacement of the donor atoms or<br />

the surrounding host atoms in forming the DX center.<br />

In (a) and (c) the substitutional atoms are in<br />

their neutral states and located in tetrahedral sites.<br />

In (b) the substitutional Si atom is shown displaced<br />

along one of the Si-As bonds into a site where it is<br />

surrounded by only three As atoms. In (d) the substitutional<br />

S atom is not displaced but, instead, one<br />

of its three Ga neighbors is relaxed in a pattern<br />

similar to the Si donor in (b). Reproduced from<br />

[Chadi88].<br />

A4.1.5 Experimental Evidence in Support of the Chadi-Chang Model<br />

The CCM was not immediately accepted because initial attempts to measure<br />

the large lattice relaxation associated with the DX center turned out<br />

to be quite difficult. On one hand, it was possible to introduce only around<br />

10 18 cm 3 of such centers. Techniques for measuring lattice displacements such<br />

as x-ray diffraction and extended x-ray absorption fine structures (or EXAFS)<br />

are not sensitive enough for low atomic number atoms like Si. Heavier atoms,<br />

like Sn, induce smaller lattice displacements. On the other hand, measurement<br />

of the -U properties of the DX centers was easier and the correctness of the<br />

CCM became accepted based on its correct prediction of the properties of the<br />

DX centers including their -U nature.<br />

The -U nature of the DX centers has now been established by several experiments.<br />

Perhaps the most convincing ones are those based on the concept<br />

of co-doping. As we noted earlier, most DX centers exhibit similar properties,

A4.1 A Prototypical Deep Center in N-Type Zincblende-Type Semiconductors 683<br />

independent of their chemical nature. However, there is a “chemical shift” in<br />

their activation energies. For example, Si DX centers have larger activation<br />

energies than Sn. Similarly, S DX centers have larger activation energies than<br />

Te. This chemical shift makes it possible to convert one donor specie into the<br />

deep DX center while a different donor specie remains shallow. When this<br />

shallow-to-deep conversion occurs for one donor specie it can capture free<br />

electrons from the specie which remains shallow. Such a co-doping experiment<br />

was performed by Baj et al. [Baj93]. These authors co-doped a GaAs sample<br />

with both Te and Ge. A hydrostatic pressure of over 1.0 GPa converts Ge into<br />

a DX center while Te remains as a shallow donor level in the gap. Normally<br />

these Ge donors contribute free carriers to the conduction band and the free<br />

electron concentration can be measured accurately by Hall effect (see 5.5.2).<br />

When the Ge donors transform to DX centers there is a drop in the free electron<br />

concentration. This drop should be exactly equal to the Ge concentration<br />

if the deep state captures only one electron per Ge atom. On the other hand,<br />

if the deep state has a negative U then each Ge atom will capture two electrons<br />

with the extra electron coming from the Te donors which remain shallow<br />

at 1 GPa. As a result, the total free carrier concentration will decrease by twice<br />

the total number of Ge donors. Such a co-doping experiment can, therefore,<br />

probe not only the negatively charged DX state but also the neutral A1 state<br />

with small lattice relaxation.<br />

To realize the above idea Baj et al. utilized a combination of light irradiation<br />

and temperature to control the number of electrons trapped on the DX<br />

centers. The Hall effect is used to measure the free carrier concentration as<br />

a function of pressure at 77 K and 100 K, respectively. Light illumination was<br />

used to excite carriers into the persistent photo-conducting states. Their results<br />

are shown in Figure A4.7. Both curves exhibit a step at a pressure between<br />

0.5 GPa and 1.0 GPa. The step in the 77 K curve is smaller and has a magnitude<br />

of ∼ 1 × 10 17 cm 3 . This step is explained by the trapping of electrons<br />

from the conduction band into the shallower A1 level of Ge. Thus, the concentration<br />

of Ge impurities is determined accurately to be 1 × 10 17 cm 3 since<br />

each A1 state captures only one electron. The deeper -U DX level associated<br />

with the Ge impurities does not capture electrons at 77 K because of its large<br />

capture barrier height. However, at 100 K the capture rate of Ge DX center<br />

becomes much larger. If the DX center were really a -U center, then one<br />

would expect to see a bigger drop in the carrier concentration due to trapping<br />

into the DX state. Indeed Baj et al. found that the step in the 100 K curve<br />

in Fig. A4.7 is ∼ 2 × 10 17 cm 3 or exactly twice the Ge impurity concentration.<br />

This experiment unambiguously demonstrates that each DX level of the<br />

Ge impurity in GaAs captures two electrons. The beauty of this experiment<br />

is that the result is independent of the existence of any compensating acceptors.<br />

Also, no prior information on doping concentrations is needed. The only<br />

requirement is that the concentration of the Te shallow donor which provides<br />

the electrons for the Ge DX centers be higher than that of the Ge donors so<br />

that Te can provide enough electrons to fill the -U DX ground states.

684 <strong>Appendix</strong> C<br />

17 -3<br />

Hall Concentration (10 cm )<br />

3<br />

2<br />

1<br />

T=100K<br />

T=70K<br />

0<br />

0 0.5 1.0 1.5<br />

Pressure (GPa)<br />

Fig. A4.7 Plots of the Hall carrier concentration<br />

in GaAs co-doped with Ge and Te<br />

measured as a function of hydrostatic pressure<br />

at T 77 and 100 K. The open<br />

symbols are the experimental points. The<br />

solid lines are theoretical fits based on a -U<br />

model. Reproduced from Baj et al. [Baj93].<br />

Many other experiments [Mooney88,90; Calleja90, Wolk92, Zeman95] have<br />

helped to firmly establish the properties of the DX center to the point that<br />

it is one of the best understood deep centers in semiconductors.<br />

References for A4.1<br />

[Baraff80] G. A. Baraff, E. O. Kane and M. Schlüter: Theory of the silicon vacancy: an<br />

Anderson negative-U system. Phys. Rev. B21, 5662–5686 (1980).<br />

[Baj93] M. Baj, L. H. Dmowski and T. Stupinski: Direct Proof of two-electron occupation<br />

of Ge-DX centers in GaAs codoped with Ge and Te. Phys. Rev. Lett., 71, 3529–3532<br />

(1993).<br />

[Bourgoin89] J. C. Bourgoin, Solid State Phenomena, 10, 253 (1989).<br />

[Calleja90] E. Calleja, F. Garcia, A. Gomez, E. Munoz, P. M. Mooney, T. N. Morgan and<br />

S. L. Wright: Effects of the local environment on the properties of DX centers in Sidoped<br />

GaAs and dilute AlxGa1xAs alloys. Appl. Phys. Lett., 56, 934–936 (1990).<br />

[Chadi89] D. J. Chadi, and K. J. Chang: Theory of the atomic and electronic structure of<br />

DX centers in GaAs and AlxGa1xAs alloys. Phys. Rev. Lett. 61, 873–876 (1988); and<br />

Energetics of DX-center formation in GaAs and AlxGa1xAs alloys. Phys. Rev. B39,<br />

10063–10074 (1989).<br />

[Chand84] N. Chand, T. Henderson, J. Klem, W. T. Masselink, R. Fischer, Y.-C. Chang and<br />

H. Morkoç: Comprenhensive analysis of Si-doped AlxGa1xAs (x 0 to 1): Theory and<br />

Experiment. Phys. Rev. B30, 4481 (1984).<br />

[Dabrowski92] For a discussion on the theory of the do state see, for example, J.<br />

Dabrowski and M. Scheffler, in Defects in Semiconductors 16, Materials Science Forum,<br />

83–87 (Trans Tech Publ., Switzerland, 1992) p. 735.<br />

[Henning87] J. C. M. Henning and J. P. M. Ansems: A new model of deep donor centres<br />

in AlxGa1xAs. Semicond. Sci. Tech. 2, 1–13 (1987).<br />

[Hjalmarson86] H. P. Hjalmarson and T. J. Drummond: Deep donor model for the persistent<br />

photoconductivity effect. Appl. Phys. Lett. 48, 656–658 (1986).<br />

[Khachaturyan89] K. Khachaturyan, E. R. Weber and M. Kaminska: Two electron D-state<br />

of DX-centers. Defects in Semiconductors, 15 (Trans. Tech., Switzerland, 1989), p. 1067–<br />

1071.

A4.1 A Prototypical Deep Center in N-Type Zincblende-Type Semiconductors 685<br />

[Lang74] D. V. Lang: Deep-level transient spectroscopy: a new method to characterize<br />

traps in semiconductors. J. Appl. Phys., 45, 3023–3032 (1974).<br />

[Lang79a] D. V. Lang, R. A. Logan and M. Jaros: Trapping characteristics and a donorcomplex<br />

(DX) model for the persistent-photoconductivity trapping center in Te-doped<br />

AlxGa1xAs. Phys. Rev. B19, 1015 (1979).<br />

[Lang79b] D. V. Lang, and R. A. Logan: Chemical shifts of DX centers in AlxGa1xAs.<br />

Physics of Semiconductors 1978 (Inst. Phys. Conf. Ser. No. 43, 1979) p. 433–436.<br />

[Lang85] D. V. Lang: DX centers in III-V alloys, in Deep Centers in Semiconductors, ed.<br />

by S. T. Pantelides (Gordon and Breach, New York, 1985) p. 489–539.<br />

[Li87] M. F. Li, P. Y. Yu, E. R. Weber and W. L. Hansen: Photocapacitance Study of<br />

Pressure-induced deep donors in GaAs:Si. Phys. Rev. B36, 4531 (1987).<br />

[Li94] M. F. Li: Modern Semiconductor Quantum Physics, (World Scientific, Singapore,<br />

1994 ), p.280-286.<br />

[Lifshitz80] N. Lifshitz, A. Jayaraman and R. A. Logan, and H. C. Card. Pressure and<br />

compositional dependences of the Hall coefficient in AlxGa1xAs and their significance.<br />

Phys. Rev. B21, 670–678 (1980).<br />

[Mizuta85] M. Mizuta, M. Tachikawa, H. Kukimoto and S. Minomura: Direct evidence<br />

for the DX center being a substitutional donor in AlGaAs alloy system. Jpn. J. Appl.<br />

Phys. 24, L143–L146 (1985).<br />

[Mooney88] P. M. Mooney, T. N. Theis and S. L. Wright: Effect of local alloy disorder on<br />

emission kinetics of deep donors (DX centers) in AlxGa1xAs of low Al content. Appl.<br />

Phys. Lett., 53, 2546–2548 (1988).<br />

[Mooney90] P. M. Mooney: Deep donor levels (DX centers) in III-V semiconductors, J.<br />

Appl. Phys. 67, R1 (1990).<br />

[Paul61] W. Paul. Band Structure of the Intermetallic Semiconductors from Pressure Experiments.<br />

J. Appl. Phys. Suppl. 32, 2082 (1961).<br />

[Sah75] C. T. Sah: Bulk and interface imperfections in semiconductors. Solid State Electronics,<br />

19, 975–990 (1976).<br />

[Shan89] W. Shan, P. Y. Yu, M. F. Li, W. L. Hansen and E. Bauser: Pressure Dependence<br />

of the DX Center in Ga1xAlxAs:Te. Phys. Rev. B40, 7831 (1989).<br />

[Suski94] For discussions on experimental results see, for example, T. Suski: Hydrostatic<br />

pressure investigations of metastable defect states. Defects in Semiconductors 17, Materials<br />

Science Forum, 143–147 (Trans Tech Pub., Switzerland, 1994) p. 975–982.<br />

[Wang89a] Shyh Wang: Fundamentals of Semiconductor Theory and Device Physics<br />

(Prentice Hall, New Jersey, 89] Chapter 8.<br />

[Wang89b] Shyh Wang: Fundamentals of Semiconductor Theory and Device Physics<br />

(Prentice Hall, New Jersey, 89] Section 9.7.<br />

[Wolk92] See, for example, J. A. Wolk, W. Walukiewicz, M. L. Thewalt and E. E. Haller:<br />

Formation of a DX center in InP under hydrostatic pressure. Phys. Rev. Lett. 68, 3619–<br />

3622 (1992) for a description of the infrared vibrational study.<br />

[Yamaguchi90] E. Yamaguchi, K. Shiraishi and T. Ohno: First principle calculation of the<br />

DX-center ground-states in GaAs, AlxGa1xAs alloys and AlAs/GaAs superlattices. J.<br />

Phys. Soc. Japan, 60, 3093–3107 (1991).<br />

[Zeman95] See J. Zeman, M. Zigone and G. Martinez: Optical investigation of the DX<br />

centers in GaAs under hydrostatic pressure. Phys. Rev. B51, 17551–17560 (1995) for a<br />

review of the Raman investigation of the DX center under pressure inside the DAC.

<strong>Appendix</strong> D:<br />

Recent Developments and References<br />

Chapter 1<br />

Many new techniques for growing semiconductors have been developed recently<br />

in response to interests in nanostructures of semiconductors and their<br />

alloys. The following list contains some of these techniques and appropriate<br />

references.<br />

The Vapor-Liquid-Solid (VLS) Method<br />

This is a very popular method for growing one-dimensional structures known<br />

as nanorods or nanowires. It is one of a few techniques that can grow a large<br />

array of nanorods and also nanorods which contain a core different from an<br />

outer shell (core-shell nanowires). This technique usually requires a liquified<br />

metal, such as Au, as a “catalyst”. However, it has also been found that, without<br />

a “catalyst”, tapered nanocrystals known as nanoneedles can be grown.<br />

R. S. Wagner and W. C. Ellis: Vapor-Liquid-Solid Mechanism Of Single Crystal<br />

Growth. Appl. Phys. Lett. 4, 89–91 (1964).<br />

L. J. Lauhon, M. S. Gudiksen, D. Wang and C. M. Lieber: Epitaxial core-shell<br />

and core-multishell nanowire heterostructures. Nature, 420, 57–61 (2002).<br />

C. W. Blackledge, J. M. Szarko, A. Dupont, G. H. Chan, E. L. Read, S. R.<br />

Leone: Zinc oxide nanorod growth on gold islands prepared by microsphere<br />

lithography on silicon and quartz. J. of Nanoscience and Nanotechnology, 7,<br />

3336–3339 (2007).<br />

M. J. Tambe, S. K. Lim, M. J. Smith, L. F. Allard and S. Gradecak: Realization<br />

of defect-free epitaxial core-shell GaAs/AlGaAs nanowire heterostructures.<br />

Appl. Phys. Lett., 93, 151917–151919, (2008).<br />

K. Tateno, G. Zhang and H. Nakano: InP nanostructures formed in GaPbased<br />

nanowires grown on Si(111) substrates. J. Crystal Growth, 310, 2966–9<br />

(2008).<br />

M. Moewe, L. C. Chuang, S. Crankshaw, C. Chase, and C. Chang-Hasnain:<br />

Atomically sharp catalyst-free wurtzite GaAs/AlGaAs nanoneedles grown<br />

on silicon. Appl. Phys. Lett. 93, 023116–023118 (2008).

688 <strong>Appendix</strong> D<br />

The “TOPO” and related Method of Growing Nanocrystals<br />

This technique starts with solutions in tri-n-octyl-phosphine oxide (TOPO)<br />

of the desired chemical species for forming the semiconductor, such as Cd<br />

and Se compounds (or precursors) to produce CdSe. After reacting to form<br />

CdSe the size of the resultant nanocrystals is limited due to capping by TOPO<br />

molecules. The size of the almost spherical nanocrystals can be controlled to<br />

certain extent by selecting the temperature of the reagents and by performing<br />

further size sorting afterwards. This method can produce large quantities<br />

of nanocrystals with size spread of 5% for industrial application. Core-shell<br />

nanocrystals have also been successfully grown. The discovery of many other<br />

chemical agents to replace TOPO has greatly broadened the choice of nanostructured<br />

semiconductor which can be grown by this technique.<br />

C. B. Murray, D. J. Norris and M. G. Bawendi: Synthesis and Characterization<br />

of Nearly Monodisperse CdE (E=S, Se, Te) Semiconductor Nanocrystallites.<br />

J. Am. Chem. Soc. 115, 8706–8715 (1993).<br />

J. E. B. Katari, V. L. Colvin and A. P. Alivisatos: X-ray Photoelectron spectroscopy<br />

of CdSe nanocrystals with applications to studies of the nanocrystal<br />

surface. J. Phys. Chem. 98, 4109–4117 (1994).<br />

K. Hashizume, M. Matsubayashi, M. Vacha1 and T. Tani: Individual mesoscopic<br />

structures studied with sub-micrometer optical detection techniques:<br />

CdSe nanocrystals capped with TOPO and ZnS-overcoated system. J. of Luminescence,<br />

98, 49–56 (2002).<br />

J.-Yu Zhang and W. W. Yu: Formation of CdTe nanostructures with dot, rod,<br />

and tetrapod shapes. Appl. Phys. Lett. 89, 123108 (2006).<br />

P. Dagtepe, V. Chikan, J. Jasinski and V. J. Leppert: Quantized growth of<br />

CdTe quantum dots; observation of magic-sized CdTe quantum dots. J. Phys.<br />

Chem. C, 111, 14977–83 (2007).<br />

N. O. V. Plank, H. J. Snaith, C. Ducati, J. S. Bendall, L. Schmidt-Mende and<br />

M. E. Welland: A simple low temperature synthesis route for ZnO-MgO<br />

core-shell nanowires. Nanotechnology, 19, 465603–465610 (2008).<br />

Growth Of Nanocrystals In Glass<br />

In the middle ages stained glass was fabricated by dissolving metals in molten<br />

glass following by quenching and annealing to form metallic nanocrystals. Today<br />

this method can be used to produce nanocrystals of semiconductors embedded<br />

in a glass matrix. First the semiconductor is dissolved in the molten<br />

glass which is then quenched to room temperature. By annealing, the dispersed<br />

semiconductor molecules or atoms coalesce into nanocrystals which are<br />

approximately spherical. This method is inexpensive and can produce industrial<br />

size glass containing semiconductor nanocrystals for optical applications<br />

(neutral density filters, color filters in photography are some examples). A<br />

variation of this method involves implanting ions into the glass and then heat-

Chapter 1 689<br />

ing up the glass to allow the ions to react to form the semiconductor nanocrystals.<br />

L. C. Liu and S. H. Risbud: Quantum-dot size-distribution analysis and precipitation<br />

stages in semiconductor doped glasses. J. Appl. Phys. 68, 28–32 (1990).<br />

S. A. Gurevich, A. I. Ekimov, I. A. Kudryavtsev, O. G. Lyublinskaya, A. V.<br />

Osinskii, A. S. Usikov, N. N. Faleev: Growth of CdS nanocrystals in silicate<br />

glasses and in thin SiO2 films in the initial stages of the phase separation of<br />

a solid solution. Semiconductors, 28, 486–93 (1994).<br />

S. Guha, M. Wall and L. L. Chase: Growth and Characterization of Ge<br />

nanocrystals. Nuclear Instru. Meth. in Phys. Research B (Beam Interactions<br />

with Materials and Atoms) 147, 367–372 (1999).<br />

H. Bernas and R. E. de Lamaestre: Ion beam-induced quantum dot synthesis<br />

in glass. Nuclear Instru. Meth. in Phys. Research B (Beam Interactions with<br />

Materials and Atoms) 257, 1–5 (2007).<br />

Pulsed Laser Deposition<br />

This technique is similar to evaporation except it uses a uv laser producing<br />

high power nanosecond long pulses to ablate a source into a plume. The short<br />

duration of the pulse will not dissociate the semiconductor unlike evaporation<br />

by an oven. Contamination by the crucible is avoided since only the source is<br />

heated. By depositing nanometer metal catalyst particles on the substrate it is<br />

possible to grow an array of nanowires just as the LVS technique.<br />

N. Wang, Y. F. Zhang, Y. H. Tang, C. S. Lee and S. T. Lee: SiO2-enhanced synthesis<br />

of Si nanowires by laser ablation. Appl. Phys. Lett. 73, 3902–4 (1998).<br />

Y. Y. Wu, Rong Fan and P. D. Yang: Block-by-block growth of single-crystalline<br />

Si/SiGe superlattice nanowires. Nano Letters, 2, 83-6 (2002).<br />

S. Neretina, R. A. Hughes, N. V. Sochinski, M. Weber, K. G. Lynn, J. Wojcik,<br />

G. N. Pearson, J. S. Preston, and P. Mascher: Growth of CdTe/Si(100) thin<br />

films by pulsed laser deposition for photonic applications. J. Vac. Sci. Technol.<br />

A24, 606–611 (2006).<br />

C. V. Cojocaru, A. Bernardi, J. S. Reparaz, M. I. Alonso, J. M. MacLeod, C.<br />

Harnagea, and F. Rosei: Site-controlled growth of Ge nanostructures on<br />

Si(100) via pulsed laser deposition nanostenciling. Appl. Phys. Lett. 91,<br />

113112–113114 (2007).<br />

A. Rahm, M. Lokenz, T. Nobis, G. Zimmirmann, M. Grundmann, B. Fuhrmann<br />

and F. Syrowatka: Pulsed-laser deposition and characterization of<br />

ZnO nanowires with regular lateral arrangement. Applied Physics A88,<br />

31–4 (2007).<br />

X. W. Zhao, A. J. Hauser, T. R. Lemberger and F. Y. Yang. Growth control of<br />

GaAs nanowires using pulsed laser deposition with arsenic over-pressure.<br />

Nanotechnology, 18, 485608-1-6 (2007).

690 <strong>Appendix</strong> D<br />

Review articles<br />

L. Brus: Chemical Approaches to Semiconductor Nanocrystals. J. Phys. Chem.<br />

Solids, 59, 459–465 (1998).<br />

Y. N. Xia, P. D. Yang, Y. G. Sun, Y. Y. Wu, B. Mayers, B. Gates, Y. D. Yin, F.<br />

Kim and H. Q. Yan: One-dimensional Nanostructures: Synthesis, Characterization,<br />

and Applications. Adv. Materials 15, 353–389 (2003).<br />

N. Wang, Y. Cai and R. Q. Zhang: Growth of nanowires. Materials Science &<br />

Engineering R: 60, 1–51 (2008).<br />

Carbon Nanotubes and Graphene<br />

In earlier editions of this book carbon nanotubes, semiconducting as well as<br />

(semi)-metallic, had already been mentioned (1.1.5) and some references<br />

given. The field has reached an enormous development since the beginning<br />

of the present century: according to the Web of Science nearly 35 000 articles<br />

have appeared to date in source journals mentioning carbon nanotubes<br />

either in the title or in the abstract. Single wall nanotubes can now be grown<br />

readily and are available commercially. However, the control over chirality<br />

of the tube, which determines the size of the bandgap, is lacking. A related<br />

development which started around 2004 concerns single graphene sheets. For<br />

symmetry reasons they are semimetallic, with Dirac-type massless electrons at<br />

the Fermi energy. Nearly 3500 articles, cited to date (Dec. 2008) about 63000<br />

times, have been published on graphene. While single graphene sheets can be<br />

obtained by simple techniques, such as pealing, a well-controlled and reproducible<br />

growth technique is still lacking. We give next a few recent references<br />

on carbon nanotubes and graphene with the understanding that these are still<br />

fast developing fields:<br />

X. Fan, R. Buczko, A. A. Puretzky, D. B. Geohegan, J. Y. Howe, S. T. Pantelides,<br />

S. J. Pennycock: Nucleation of Single Walled Carbon Nanotubes.<br />

Phys. Rev. Letters 90, 145501 (2003).<br />

M. Monthioux, Who should be given credit for Nanotubes? Carbon 44, 1621<br />

(2006).<br />

M. J. Height, J. B. Howard, J. W. Tester, J. B. V. Sande: Flame Synthesis of Carbon<br />

Nanotubes. Carbon 42, 2295 (2004).<br />

K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, Y. Zhang, S. V. Dubonos,<br />

I. V. Grigoreva and A. A. Firsov: Carbon Wonderland, Scientific American<br />

298, 90 (2008).<br />

K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelsov, S. V.<br />

Dubonos, I. V. Grigoreva, S. V. Dubonos, and A. A. Firsov: Two–Dimensional<br />

Gas of Massless Dirac Fermions in Graphene, Nature 438, 197 (2005).<br />

General Reading<br />

Jorio, A., Dresselhaus, M. S., Dresselhaus, G. (ed.): Carbon Nanotubes: advanced<br />

topics in synthesis, structure, properties, and applications, Topics in<br />

Applied Physics, Vol. 111 (Springer, New York, 2008).

Chapter 2 691<br />

Popov, V. N., Lambin, P. (ed): Carbon Nanotubes: from basic research to technology,<br />

(Kluwer Acad. Pub., Doordrecht, 2006).<br />

Thomsen, C., Reich, S.: Raman Scattering in Carbon Nanotubes, in Springer<br />

Topics in Applied Physics, ed. by M. Cardona and R. Merlin (Springer, Heidelberg,<br />

2007).<br />

Chapter 2<br />

During the past two decades so-called ab initio techniques have become increasingly<br />

important as already mentioned in p. 333. This fact is due partly<br />

to the enhanced power of available computers and partly to the increasing<br />

sophistication of the computer codes available for the calculation of electronic<br />

structures. The latter now include free and commercial ones. Most of<br />

these computer codes are based on the so-called density functional theories<br />

which allow the conversion of the intractable many electron interactions into<br />

tractable one electron potentials. Among these functionals, the most commonly<br />

used ones are the local density approximation (LDA) and, more recently,<br />

the generalized gradient approximation (GGD). Some of these approaches<br />

start with one-electron ionic potentials which are reduced to ab initio<br />

pseudopotentials derived from the corresponding atomic wavefunctions. Plane<br />

waves or augmented plane waves (APW) are used as trial functions for solving<br />

the appropriate Schrödinger equation. In semiconductors containing partially<br />

filled d and f shells, the strong Coulomb repulsion between these highly<br />

localized electrons cannot be represented by pseudopotentials alone. One approach<br />

is to add an additional Coulomb repulsion term (U) for these localized<br />

electrons leading to approximations known as LDAU or GGAU. Most<br />

of these approaches are now implemented via a plethora of computer codes<br />

available through the web (on the basis of free access or for an annual fee)<br />

under acronyms such as:<br />

ABINIT (www.abinit.org),<br />

QUANTUM-EXPRESSO (www.quantum-espresso.org),<br />

SIESTA which stands for Spanish Initiative for Electronic Simulations with<br />

Thousands of Atoms (www.uam.es/departamentos/ciencias/fismateria),<br />

VASP which stands for Vienna Ab-initio Simulation Package<br />

(cms.mpi.univie.ac.at/vasp/),<br />

WIEN 2K (www.wien2k.at)<br />

and others.<br />

These methods have proven to be rather accurate for determining ground<br />

state energies and properties but have limited success when dealing with excited<br />

states properties, like the band gaps, and exciton energies in the dielectric<br />

response spectra (see p. 333). A number of highly sophisticated correction<br />

schemes have been developed to overcome these difficulties. They include<br />

the GW approximation to the electron self-energy and the time dependent

692 <strong>Appendix</strong> D<br />

density functionals, as well as direct solutions of the Bethe-Salpeter equation<br />

which take into account the Coulomb (excitonic) interaction between an excited<br />

electron and the hole left behind (see Fig. 6.55). Unfortunately, most<br />

of these calculations are quite computation intensive and require the use of<br />

super-computers. Even then, most of these calculations do not include the effect<br />

of electron-phonon interaction, which can be non-negligible in many cases<br />

even at zero temperature (because of the zero-point vibrations, see Fig. 6.44).<br />

We give below a list of articles and books related to the theory and practice of<br />

ab initio electronic band structure calculations including their recent updates.<br />

The acronyms of some of the codes used are given in red.<br />

P. Hohenberg and W. Kohn: Inhomogeneous electron gas. Phys. Rev. 136,<br />

B864–B871 (1964).<br />

W. Kohn and L. J. Sham: Self-consistent equations including exchange and correlation<br />

effects. Phy. Rev. 140, A1133–A1138 (1965). (Walter Kohn shared<br />

the 1998 Nobel Prize in Chemistry for his development of the densityfunctional<br />

theory.)<br />

M. S. Hybertson and S. G. Louie: Electron correlation in semiconductors and<br />

insulators: band gaps and quasiparticle energies. Phy. Rev. B34, 5390–5413<br />

(1986).<br />

A. Rubio, J. L. Corkill, M. L. Cohen, E. L. Shirley, and S. G. Louie: Quasiparticle<br />

Band Structure of AlN and GaN. Phys. Rev. B48, 11810–11816 (1993).<br />

B. Wenzien, P. Kackell, F. Bechstedt, G. Capellini: Quasiparticle Band Structure<br />

of Silicon Carbide Polytypes. Phys. Rev. B52, 10897–10905 (1995).<br />

D. Vogl, P. Krüger, J. Pollmann: Self-Interaction and Relaxation-Corrected<br />

Pseudopotentials for II-VI Semiconductors. Phys. Rev. B54, 5495–5511<br />

(1996).<br />

F. Bechstedt, P. Kackell, A. Zywietz, K. Karch, B. Adolph, K. Tenelsen, J.<br />

Furthmüller: Polytypism and Properties of Silicon Carbide. Phys. Stat. Solidi<br />

B 202, 35–62 (1997) (VASP).<br />

S. Albrecht, L. Reining, R. del Sole and G. Onida: Ab Initio Calculations of<br />

Excitonic Effects in the Optical Spectra of Semiconductors. Phys. Rev. Lett.<br />

80, 4510–4513 (1998).<br />

C. Stampfl and C. G. Van de Walle: Density-Functional Calculation of III–V<br />

Nitrides Using Local-Density Approximation and the Generalized Gradient<br />

Approximation. Phys. Rev. B59, 5521–5535 ( 1999).<br />

D. Sánchez-Portal, E. Artacho, J. M. Soler, A. Rubio, P. Ordejón: Ab Initio<br />

Structural, Elastic and Vibrational Properties of Carbon Nanotubes. Phys.<br />

Rev. B59, 12678–12688 (1999).<br />

K. Labniczak-Jablonska, T. Suski, I. Gorczyca, N. E. Christensen, K. E. Attenkofer,<br />

R. C. C. Perera, E. M. Gullikson, J. H. Underwood, D. L. Ederer,<br />

and Z. Liliental Weber: Electronic States in Valence and Conduction Bands<br />

of Group III Nitrides: Experiment and Theory. Phys. Rev. B61, 16623–16632<br />

(2000).<br />

L. E. Ramos, L. K. Teles, L. M. R. Scolfaro, J. L. P. Castineira, A. L. Rosa,<br />

J. R. Leite: Structural, Electronic, and Effective-Mass Properties of Silicon

Chapter 2 693<br />

and zinc-blende group III Nitride Semiconductors. Phys. Rev. B63, 165210–<br />

165219 (2001).<br />

F. Bechstedt and J. Furthmüller: Do We Know the Fundamental Gap of InN?<br />

J. Cryst. Growth 246, 315–319 (2002) (VASP).<br />

D. Sánchez-Portal, P.Ordejón, E. Canadell: Computing the Properties of Materials<br />

from First Principles with SIESTA. Structure and Bonding 113, 103–170<br />

(2004).<br />

M. Cardona: Electron-Phonon Interaction in Tetrahedral Semiconductors.<br />

Solid State Commun. 133, 3–18 (2005).<br />

M. Cardona and M. L. W. Thewalt: Isotope Effects on Optical Spectra of Semiconductors.<br />

Rev. Mod. Phys. 77, 1173–1224 (2005).<br />

A. Sucivara, B. R. Sahu, L. Kleinman: Density Functional Study of the Effect<br />

of Pressure on Ferroelectric GeTe. Phys. Rev. B73, 214105–214110 (2006)<br />

(VASP).<br />

R. Laskovski and N. E. Christensen: Ab Initio Calculation of Excitons in ZnO.<br />

Phys. Rev. B73, 045201 (2006).<br />

A. N. Chantis, M. Cardona, N. E. Christensen, D. L. Smith, M. van Schilfgaarde,<br />

T. Kotami, A. Svane, and R.C. Albers: Strain-Induced Conduction-<br />

Band Splitting in GaAs from First Principles Calculations. Phys. Rev. B78,<br />

075208–075214 (2008).<br />

A. Marini: Ab initio Finite-Temperature Excitons, Phys. Rev. Lett. 101,<br />

106405–106408 (2008) (YAMBO).<br />

Z. A. Ibrahim, A. I. Shkrebtii, M. J. G. Lee, K. Vynck, T. Teatro, W. Richter,<br />

T. Trepk, and T. Zettler: Temperature Dependence of the Optical Response:<br />

Application to bulk GaAs Using First-Principles Molecular Dynamics Simulations.<br />

Phys. Rev. B77, 125218–125222 (2008) (QUANTUM-EXPRESSO).<br />

M. Verstraete: First-Principles Computation of the Electronic and Dynamical<br />

Properties of Solids and Nanostructures with ABINIT. J. Phys.: Cond. Matter<br />

20, 064212 (2008).<br />

General Reading<br />

Dresselhaus M. S., Dresselhaus G., Jorio A.: Group Theory: Application to the<br />

Physics of Condensed Matter (Springer; Heidelberg, Berlin, 2008).<br />

Evarestov R. A.: Quantum Chemistry of Solids: The LCAO First Principles<br />

Treatment of Crystals (Springer, Berlin, Heidelberg, New York, 2007). In<br />

page 526 there is a list of computer codes for periodic systems that use a<br />

localized orbital basis.<br />

Fiolhais C., Nogueira F., and Marques M. A. L. (eds.): A Primer in Density<br />

Functional Theory (Lecture Notes in Physics) (v.620) (Springer, Heidelberg,<br />

Berlin, 2003).<br />

Marques M. A. L., Ullrich C. A., Nogueira F., Rubio A., Burke K., Gross<br />

E. K. U. (eds.): Time-Dependent Density Functional Theory (Springer, Heidelberg,<br />

Berlin, 2006).<br />

Martin R. M.: Electronic Structure: Basic Theory and Practical Methods (Cambridge<br />

University Press, Cambridge, 2004).

694 <strong>Appendix</strong> D<br />

Chapter 3<br />

Ab initio phonon calculations<br />

The discussion of phonon dispersion relations in Chap. 3 was based on semiempirical<br />

models of the force constants. In Fig. 3.3, however, an example of<br />

ab initio calculations was shown for the dispersion relations of GaN. These<br />

results are based on the total energy calculations obtained from an ab initio<br />

electronic band structure. The atomic positions are then perturbed and<br />

the corresponding changes in the total energy are used to obtain restoring<br />

forces. This can be done either by using static atomic displacements (i.e.<br />

time independent phonon eigenvectors), which correspond to frozen phonons,<br />

or by energy functional perturbation theory. During the past decade several<br />

of the ab initio computer codes mentioned in the update to the references<br />

of Chap. 2, (e.g. ABINIT, CASTEP, VASP) and others (MedeA is the<br />

name of a software platform which works with VASP for the computation<br />

of materials properties including phonons. Further details can be found at<br />

the URL:www.materialsdesign.com/), have been expanded so as to allow the<br />

calculation of phonon dispersion relations. In the references that follow, the<br />

reader will find examples of ab initio calculations of the lattice dynamics of<br />

semiconductors. Whenever standard codes were used in these calculations, the<br />

corresponding acronyms are given in red.<br />

S. Baroni, S. de Gironcoli, A. del Corso, P. Giannozzi: Phonons and Related<br />

Crystal Properties from Density-Functional Perturbation Theory. Rev. Mod.<br />

Phys 73, 515–562 (2001).<br />

M. D. Segall, P. J. D. Lindan, M. J. Probert, C. J. Pickard, P. J. Hasnip, S. J.<br />

Clark and M. C. Payne: First-principles simulation: ideas, illustrations and the<br />

CASTEP code. J. Phys.: Condens. Matter 14, 2717–2744 (2002).<br />

X. C. Gonze: A Brief Introduction to the ABINIT software package. Z. für<br />

Kristallographie, 220, 558–562 (2005).<br />

S. J. Clark, M. D. Segall, C. J. Pickard, P. J. Hasnip, M. I. J. Probert, K. Refson<br />

and M. C. Payne: First Principles Methods Using CASTEP. Z. für Kristallographie<br />

220, 567–570 (2005).<br />

K. Parlinski: First-Principle Lattice dynamics and Thermodynamics of Crystals.<br />

J. Physics: Conference Series 92, 012009-012013 (2007). (VASP) (In this article<br />

references to calculations for a number of semiconductors such as BN, GaN,<br />

HgSe, ZnTe, AgGaS2 etc. can be found.)<br />

A. H. Romero, M. Cardona, R. K. Kremer, R. Lauck, G. Siegle, J. Serrano,<br />

X. C. Gonze: Lattice Properties of PbX (X=S, Se, Te): Experimental studies<br />

and ab initio calculations including spin-orbit effects. Phys. Rev. B78,<br />

224302–224310 (2008). (ABINIT) (In this work, evidence for the influence<br />

of electronic spin-orbit coupling on the lattice dynamics and related properties<br />

is presented.)

Chapter 3 695<br />

Inelastic x-ray Scattering (IXS)<br />

As discussed in Chap. 7, laser Raman scattering yields very precise information<br />

about the frequencies and line widths of phonons at or near the center of<br />

the Brillouin zone. However, it cannot access phonons throughout the whole<br />

Brillouin zone because the laser wavelength is much larger than the typical lattice<br />

constants. The measured dispersion relations shown in this chapter were<br />

obtained by inelastic neutron scattering (INS), taking advantage of the fact<br />

that the wavelength of thermal neutrons is close to the lattice constants. This<br />

technique, however, is slow, cumbersome, requires large samples and has poor<br />

energy resolution. Within the past decade, these problems have been circumvented<br />

(except for the poor resolution) by using IXS, with monochromatized<br />

x-rays from a synchrotron radiation source. An example of these measurements<br />

is given in Fig. 3.3. IXS allows the use of small samples ( 1mmin<br />

size) and is thus suitable for measurements under pressure in diamond anvil<br />

cells (DAC). A discussion can be found in the following articles:<br />

M. Krisch: Status of Phonon Studies at High Pressure by inelastic X-ray scattering.<br />

J. Raman Spectr. 34, 628–632 (2003).<br />

M. Krisch and F. Sette: Inelastic X-ray Scattering from Phonons, in Light Scattering<br />

in Solids IX, edited by M.Cardona and R. Merlin (Springer, Heidelberg,<br />

2007) p. 317–369.<br />

Effects of Hydrostatic Pressure on Phonons<br />

The large samples required by INS limits the highest hydrostatic pressure that<br />

can be reached to about 1 GPa. With IXS much smaller samples can be used<br />

and, with the help of DACs pressures as high as a few hundred GPa can be<br />

reached at the expense of the resolution. The pressure effects of main interest<br />

are the shift in phonon frequencies (related to the mode Grüneisen parameters<br />

discussed in Problem 3.17) and changes in phonon line widths. These “anharmonic”<br />

effects are amenable to ab initio calculations. The phase transitions<br />

which take place at high pressures are also evinced in the phonon spectra.<br />

Recent advances in the field can be found in the following publications:<br />

A. Debernardi: Anharmonic Èffects in the Phonons of III-V Semiconductors:<br />

First Principles Calculations. Solid State Commun. 113, 1–10 (1999).<br />

J. Camacho, K. Parlinski, A. Cantarero, and K. Syassen: Vibrational Properties<br />

of the high pressure Cmcm phase of ZnTe. Phys. Rev. B70, 033205–033208<br />

(2004).<br />

J. Kulda, A. Debernardi, M. Cardona, F. de Geuser, and E. E. Haller: Self-<br />

Energy of Zone- Boundary Phonons in Germanium: Ab initio Calculations<br />

versus Neutron Spin-Echo Measurements. Phy. Rev. B69, 045209–045213<br />

(2004).<br />

J. Serrano, A. H. Romero, F. J. Manjon, R. Lauck, M. Cardona and A. Rubio:<br />

Pressure Dependence of the Lattice Dynamics of ZnO, an ab initio approach.<br />

Phys. Rev. B69, 094306–094319 (2004). (ABINIT)

696 <strong>Appendix</strong> D<br />

Effects of Isotopic Substitution on Phonons<br />

During the pass 15 years isotopically pure constituents of many semiconductors<br />

have become available at affordable prices. With them it has become possible<br />

to grow semiconductor crystals with tailor-made isotopic compositions.<br />

A number of interesting experiments have thus become possible. In p. 117<br />

(footnote) it has already been mentioned that elimination of strongly neutron<br />

absorbing isotopes (e.g. 113Cd) allows INS measurements on cadmium compounds<br />

such as CdS. Isotopic substitution also yields information about anharmonic<br />

effects, among others the dependence of the lattice parameters on<br />

isotopic mass. The interested reader should consult:<br />

N. Vast and S. Baroni: Effects of Isotopic Disorder on the Raman Spectra of<br />

Crystals: Theory and ab initio Calculations for Diamond and Germanium.<br />

Phys. Rev. B61, 9387–9392 (2000).<br />

M. Cardona and M. L. W. Thewalt: Isotope Effects on Optical Spectra of Semiconductors.<br />

Rev. Mod. Phys 77, 1173–1224 (2005).<br />

Electron Phonon Interactions<br />

In Sect. 3.3 we have discussed the effects of phonons on the electronic states<br />

on the basis of semi-empirical models of the electronic band structures and the<br />

lattice dynamics. As expected, these effects can also be calculated using the ab<br />

initio approach from both the electronic band structures and lattice dynamics.<br />

Such calculations are the simplest for long wavelength acoustic phonons; they<br />

correspond to the effects of uniform (either uniaxial or hydrostatic) strains on<br />

the electronic band structure. More general electron-phonon interaction effects,<br />

including intervalley scattering, have since been calculated also by ab<br />

initio techniques. We mention two recently articles on this subject.<br />

S. Sjakste, V. Tyuterev and N. Vast: Ab initio Study of °-X intervalley scattering<br />

in GaAs under pressure. Phys. Rev. B74, 235216–235222 (2006).<br />

S. Sjakste, N. Vast, V. Tyuterev: Ab initio Method for Calculating Electron-<br />

Phonon Scattering Times in Semiconductors: Application to GaAs and GaP.<br />

Phys. Rev. Lett. 99, 236405–236408 (2007).<br />

Chapter 4<br />

The study of defects in semiconductors is one of the most important fields<br />

in semiconductor physics and new developments appear constantly. For example,<br />

it has been found that large band gap semiconductors tend to be n-type.<br />

It was thought that there might be fundamental reasons preventing the incorporation<br />

of acceptors in them. By now it has been demonstrated via the<br />

p-doping of GaN and related alloys that no insurmountable barriers exist to<br />

prevent the p-doping of the large band gap semiconductors. This breakthrough

Chapter 4 697<br />

results from a better understanding and control of intrinsic defects which often<br />

compensate the acceptors. Another interesting development involves the discovery<br />

that alloying GaAs with high concentration of N (as shown in Section<br />

4.3.3 low concentration of nitrogen isoelectronic impurities produce resonant<br />

states inside the conduction band of GaAs) can lower the band gap of GaAs<br />

rather than increasing it as one may expect from the much larger band gap of<br />

GaN than that of GaAs. A related development is the incorporation of high<br />

concentration of magnetic ions, such as Mn, into a III-V host to produce ferromagnets<br />

with Curie temperature above room temperature. Much of these recent<br />

advances would not have been possible without the development of new<br />

“non-equilibrium” growth techniques (see updates in references of Chapter 1).<br />

Equally important for the study of deep centers in semiconductors has been<br />

the application of ab initio approaches to calculate the electronic properties of<br />

defects. A good case in point is the deep center known as the DX center (see<br />

Section 4.3). This deep center has been studied extensively, both experimentally<br />

and theoretically, so that its nature can be said to be completely understood.<br />

An appendix has been devoted in this book to this important deep center.<br />

The following is a list of references on the above topics except for the DX<br />

center. References to work on the DX center can be found in the <strong>Appendix</strong>.<br />

A few words of caution are in order though. There are still confusions and<br />

controversies in the study of dilute magnetic III-V semiconductors because<br />

many of the samples are inhomogeneous and poorly characterized. Nevertheless,<br />

our understanding of the properties of magnetic ions in semiconductors<br />

has greatly improved recently.<br />

Intrinsic and Deep Centers in Large Gap Semiconductors<br />

G. Y. Zhang, Y. Z. Tong, Z. J. Yang, S. X. Jin, J. Li and Z. Z. Gan: Relationship<br />

of background carrier concentration and defects in GaN grown by metalorganic<br />

vapor phase epitaxy. Appl. Phys. Lett., 71, 3376–3378 (1997).<br />

K. H. Chow. G. D. Watkins, A. Usui and M. Mizuta: Detection of interstitial<br />

Ga in GaN. Phys. Rev. Lett., 85, 2761–2764 (2000).<br />

C. H. Park, S. B. Zhang and S.-H. Wei: Origin of p-type doping difficulty in<br />

ZnO: The impurity perspective. Phys. Rev. B66, 073202/1–3 (2002).<br />

C. G. Van de Walle and J. Neugebauer: First-principles calculations for defects<br />

and impurities: applications to III-nitrides. J. Appl. Phys., 95, 3851–79 (2004).<br />

K. H. Chow, L. S. Vlasenko, P. Johannesen, C. Bozdog, G. D. Watkins, A. Usui,<br />

H. Sunakawa, C. Sasaoka and M. Mizuta: Intrinsic defects in GaN. I. Ga<br />

sublattice defects observed by optical detection of electron paramagnetic<br />

resonance. Phys. Rev. B69, 045207/1–5 (2004).<br />

P. Johannesen, A. Zakrzewski, L. S. Vlasenko, G. D. Watkins, A. Usui, H.<br />

Sunakawa and M. Mizuta: Intrinsic defects in GaN. II. Electronically enhanced<br />

migration of interstitial Ga observed by optical detection of electron<br />

paramagnetic resonance, Phys. Rev. B69, 045208/1–9 (2004).

698 <strong>Appendix</strong> D<br />

A. Janotti and C. G. Van de Walle: Oxygen vacancies in ZnO. Appl. Phys.<br />

Lett., 87, 122102/1–3 (2005)<br />

P. Dev, Y. Xue, and P. H. Zhang: Defect-induced intrinsic magnetism in widegap<br />

III-nitrides. Phys. Rev. Lett. 100, 117204–117206 (2008).<br />

Electronic Structure of GaAsN and related alloys<br />

W. Shan, K. M. Yu, W. Walukiewicz, J. W. Ager III, E. E. Haller, M. C. Ridgway:<br />

Reduction of band-gap energy in GaNAs and AlGaNAs synthesized by<br />

N implantation. Appl. Phys. Lett., 75, 1410–12 (1999).<br />

S. B. Zhang and S.-H. Wei: Nitrogen solubility and induced defect complexes<br />

in epitaxial GaAs: N. Phys. Rev. Lett., 86, 1789–92 (2001).<br />

P. R. C. Kent and A. Zunger: Evolution of III-V nitride alloy electronic structure:<br />

the localized to delocalized transition. Phys. Rev. Lett., 86, 2613–16<br />

(2001); Theory of electronic structure evolution in GaAsN and GaPN alloys.<br />

Phys. Rev. B64, 115208/1–23 (2001).<br />

L.-W. Wang: Large-scale local-density-approximation band gap-corrected<br />

GaAsN calculations. Appl. Phys. Lett., 78, 1565–7 (2001).<br />

Magnetic impurities in semiconductors and III-V dilute magnetic<br />

semiconductors<br />

H. Ohno: Making nonmagnetic semiconductors ferromagnetic. Science, 281,<br />

951–614 (1998).<br />

T. Dietl and H. Ohno:Ferromagnetism in III-V and II-VI semiconductor structures,<br />

Physica E.9, 185–93 (2001).<br />

M. A. Scarpulla, B. L. Cardozo, R. Farshchi, W. M. Oo, M. D. McCluskey, K. M.<br />

Yu, and O. D. Dubon: Ferromagnetism in Ga1xMnxP: Evidence for Inter-<br />

Mn Exchange Mediated by Localized Holes within a Detached Impurity<br />

Band. Phys. Rev. Lett. 95, 207204 (2005).<br />

E. Malguth, A. Hoffmann, W. Gehlhoff, O. Gelhausen, M. R. Phillips and X.<br />

Xu: Structural and electronic properties of Fe 3 and Fe 2 centers in GaN<br />

from optical and EPR experiments. Phys. Rev. B74, 165202/1–12 (2006).<br />

T. Jungwirth, J. Sinova, A. H. MacDonald, B. L. Gallagher, V. Novak, K. W.<br />

Edmonds, A. W. Rushforth, R. P. Campion, C. T. Foxon, L. Eaves, E. Olejnik,<br />

J. Masek, S.-R. E. Yang, J. Wunderlich, C. Gould, L. W. Molenkamp,<br />

T. Dietl and H. Ohno: Character of states near the Fermi level in<br />

(Ga,Mn)As: Impurity to valence band crossover. Phy. Rev. B76, 125206/1–9<br />

(2007).<br />

L. Liu, P. Y. Yu, Z. X. Ma, and S. S. Mao: Ferromagnetism in GaN:Gd: A Density<br />

Functional Theory Study. Phys. Rev. Lett. 100, 127203–127206 (2008).<br />

A. Ney, T. Kammermeier, V. Ney, S. Ye, K. Ollefs, E. Manuel, S. Dhar, K. H.<br />

Ploog, E. Arenholz, F. Wilhelm and A. Rogalev: Element specific magnetic<br />

properties of Gd-doped GaN: Very small polarization of Ga and paramagnetism<br />

of Gd. Phy. Rev. B77, 233308/1–4 (2008).

Chapter 5 699<br />

K. Alberi, K. M. Yu, P. R. Stone, O. D. Dubon, W. Walukiewicz, T. Wojtowicz,<br />

X. Liu, and J. K. Furdyna: Formation of Mn-derived impurity band in<br />

III-Mn-V alloys by valence band anticrossing Phys. Rev. B78, 075201/1–7<br />

(2008).<br />

General Reading<br />

Dietl T., Awschalom D. D., Kaminska M., Ohno H. (ed.): Spintronics, Volume<br />

82 (Semiconductors and Semimetals), (Academic Press; New York, 2008).<br />

Drabold D. A., Estreicher S. (ed.): Theory of Defects in Semiconductors (Topics<br />

in Applied Physics, Vol. 104), (Springer, Heidelberg, Berlin, 2006).<br />

Norbert H. N., Terukov E. (ed.): Zinc Oxide – A Material for Micro- and Optoelectronic<br />

Applications (NATO Science Series II: Mathematics, Physics and<br />

Chemistry) (Springer; Heidelberg, Berlin, 2005).<br />

Tilley R. J. D.: Defects in Solids (Special Topics in Inorganic Chemistry) (Wiley-<br />

Interscience, New York, 2008).<br />

Chapter 5<br />

In Chapter 5 we have studied the transport of electrons under an applied electric<br />

field based on the assumption that the mean-free-paths of the electrons<br />

are much smaller than the dimensions of the sample. This assumption allows<br />

us to treat the motion of the electron classically, similar to the diffusion of particles<br />

in the presence of an external perturbation. In reality, electrons behave<br />

as Bloch waves in a crystal. Although predictions of the effect of the wave<br />

nature of electrons on their transport can be traced back to F. Bloch, they<br />

were not realized until advances in the fabrication of nanometer size samples<br />

(see updated references for Chapter 1) make their observation possible. When<br />

the mean-free-paths of the carriers are much longer than the dimension of the<br />

sample, the motion of the carriers is said to be ballistic (as compared to diffusive).<br />

In this regime, the transport of carriers through a sample has to be<br />

described in terms of the transmission of quantum mechanical waves. This approach<br />

has already been applied in Section 9.5 to describe resonant tunneling.<br />

With the recent interest in low-dimensional structures, quantum transport has<br />

become a topic of great interest for both its basic science and electronic device<br />

applications. Some of the important phenomena discovered include: the<br />

observation of quantized conductance (the reciprocal of a quantum of conductance:<br />

the “quantum of resistance” has been defined on p. 541 in relation<br />

to the Quantum Hall Effect which is clearly an example of quantum transport).<br />

Another phenomenon is Coulomb Blockade which influences quantum<br />

transport through a double-barrier quantum well or quantum dot. This effect<br />

plays an important role in the operation of single electron transistors (or<br />

SET). One interesting consequence of the long mean-free-path of the electron

700 <strong>Appendix</strong> D<br />

is that electrons can be reflected many times within a superlattice sample just<br />

like light inside a Fabry-Perot interferometer. The resultant interference of the<br />

electron wave under a dc applied field can give rise to high frequency oscillations<br />

known as Bloch oscillations.<br />

The following list contains references to some of the theoretical and experimental<br />

papers related to quantum transport of charged carriers in semiconductors<br />

and metals. Additional references on more recent work including carbon<br />

nanotubes and graphene can be found in the updated references for Chapter 9.<br />

Theory<br />

M. Büttiker, Y. Imry, R. Landauer, S. Pinhas: Generalized many-channel Conductance<br />

Formula with Application to small Rings. Phys. Rev. B31, 6207–<br />

6215 (1985).<br />

S. Horiguchi, Y. Nakajima, Y. Takahashi, M. Tabe: Energy eigenvalues and<br />

quantized conductance values of electrons in Si quantum wires on {100}<br />

plane. Japan. J. of Appl. Phys., (Part 1) 34, 5489–5498 (1995).<br />

J.-L. Mozos, C. C. Wan, G. Taraschi, J. Wang, H. Guo: Quantized conductance<br />

of Si atomic wires. Phys. Rev. B56, R4351–4354 (1997).<br />

S. K. Lyo: Magnetic-field-induced V-shaped quantized conductance staircase in<br />

a double-layer quantum point contact. Phys. Rev. B60, 7732–7735 (1999).<br />

Y. Imry, R. Landauer: Conductance viewed as transmission. Rev. Mod. Phys.<br />

71, S306–312 (1999).<br />

W. Magnus, W. Schoenmaker: Quantized conductance, circuit topology, and<br />

flux quantization. Phys. Rev. B61, 10883–10889 (2000).<br />

B. Dwir, D. Kaufman. E. Kapon, A. Palevski: Quantized conductance and<br />

inter-subband scattering in serially connected quantum wires. Europhys.<br />

Lett., 55, 80–85 (2001).<br />

Quantized Conductance Experiments<br />

M. A. Kastner: Mesoscopic physics and artificial atoms. AIP Conference Proceedings,<br />

no. 275, 573–851 (993).<br />

E. B. Foxman, P. L. McEuen, U. Meirav, N. S. Wingreen, Y. Meir, P. A. Belk,<br />

N. R. Belk, M. A. Kastner, S. J. Wind: Effects of quantum levels on transport<br />

through a Coulomb island. Phys. Rev. B 47, 10020–10023 (1993).<br />

D. Dixon, L. P. Kouwenhoven, P. L. McEuen, Y. Nagamune, J. Motohisa, H.<br />

Sakaki: Linear and non-linear transport through coupled quantum dots. Surf.<br />

Sci., 361–362, 636–9 (1996).<br />

S. J. Koester, B. Brar, C. R. Bolognesi, E. J. Caine, A. Patlach, E. L. Hu, H.<br />

Kroemer, M. J. Rooks: Length dependence of quantized conductance in ballistic<br />

constrictions fabricated on InAs/AlSb quantum wells. Phys, Rev, B53,<br />

13063–13073 (1996).

Chapter 5 701<br />

P. Ramvall, N. Carlsson, I. Maximov, P. Omling, L. Samuelson, W. Seifert, Q.<br />

Wang, S. Lourdudoss: Quantized conductance in a heterostructurally defined<br />

Ga0.25In0.75As/InP quantum wire. Appl. Phys. Lett., 71, 918–920 (1997).<br />

B. E. Kane, G. R. Facer, A. S. Dzurak, N. E. Lumpkin, R. G. Clark, L. N.<br />

Pfeiffer, K. W. West: Quantized conductance in quantum wires with gatecontrolled<br />

width and electron density. Appl. Phys. Lett., 72, 3506–3508<br />

(1998).<br />

L. Worschech, F. Beuscher, A. Forchel,: Quantized conductance in up to 20 Ìm<br />

long shallow etched GaAs/AlGaAs quantum wires. Appl. Phys. Lett., 75,<br />

578–580 (1999).<br />

O. Klochan, W. R. Clarke, R. Danneau, A. P. Micolich, L. H. Ho, A. R. Hamilton,<br />

K. Muraki, Y. Hirayama: Ballistic transport in induced one-dimensional<br />

hole systems. Appl. Phys. Lett., 89, 92105/1–3 (2006).<br />

P. J. Simmonds, F. Sfigakis, H. E. Beere, D. A. Ritchie, M. Pepper, D. Anderson,<br />

G. A. C. Jones: Quantum transport in In0.75Ga0.25As quantum wires. Appl.<br />

Phys. Lett., 92, 152108/1–3 (2008).<br />

Coulomb Blockade and SET<br />

H. Matsuoka, S. Kimura: Transport properties of a silicon single-electron transistor<br />

at 4.2 K. Appl. Phys. Lett., 66, 613–615 (1995).<br />

K. Murase, Y. Takahashi, Y. Nakajima, H. Namatsu, M. Nagase, K. Kurihara,<br />

K. Iwadate, S. Horiguchi, M. Tabe, K. Izumi: Transport properties of silicon<br />

nanostructures fabricated on SIMOX substrates. Microelect. Eng., 28, 399–<br />

405 (1995).<br />

H. Ishikuro, T. Hiramoto: Quantum mechanical effects in the silicon quantum<br />

dot in a single-electron transistor. Appl. Phys. Lett., 71, 3691–3693 (1997).<br />

D. Goldhaber-Gordon, H. Shtrikman, D. Mahalu, D. Abusch-Magder, U.<br />

Meirav, M. A. Kastner: Kondo effect in a single-electron transistor. Nature<br />

391, 156–159 (1998).<br />

J. W. Park. K. S. Park, B. T. Lee, C. H. Lee, S. D. Lee, J. B. Choi, K.-H. Yoo,<br />

J. Kim, S. C. Oh, S. I. Park, K. T. Kim, J. J. Kim: Enhancement of Coulomb<br />

blockade and tunability by multidot coupling in a silicon-on-insulator-based<br />

single-electron transistor. Appl. Phys. Lett., 75, 566–568 (1999).<br />

L. P. Rokhinson, L. J. Guo, S. Y. Chou, D. C. Tsui: Kondo-like zero-bias<br />

anomaly in electronic transport through an ultrasmall Si quantum dot. Phys.<br />

Rev. B60, R16319–16321 (1999).<br />

L. Geppert: Quantum transistors: toward nanoelectronics. IEEE Spectrum, 37,<br />

46–51 ( 2000).<br />

T. W. Kim, D. C. Choo, J. H. Shim, S. O.Kang: Single-electron transistors operating<br />

at room temperature, fabricated utilizing nanocrystals created by<br />

focused-ion beam. Appl. Phys. Lett., 80, 2168–2170 (2002).<br />

C. Thelander, T. Mårtensson, M. T. Björk, B. J. Ohlsson, M. W. Larsson, L. R.<br />

Wallenberg, L. Samuelson: Single-electron transistors in heterostructure<br />

nanowires. Appl. Phys. Lett., 83, 2052–2054 (2003).

702 <strong>Appendix</strong> D<br />

S. M. Goodnick, J. Bird: Quantum-effect and single-electron devices. IEEE<br />

Transactions on Nanotechnology, 2, 368–385 (2003).<br />

L. J. Klein, K. A. Slinker, J. L. Truitt, S. Goswami, K. L. M. Lewis, S. N. Coppersmith,<br />

D. W. van der Weide, M. Friesen, R. H. Blick, D. E. Savage, M. G. Lagally,<br />

C. Tahan, R. Joynt, M. A. Eriksson, J. O. Chu, J. A. Ott, P. M. Mooney:<br />

Coulomb blockade in a silicon/silicon-germanium two-dimensional electron<br />

gas quantum dot. Appl. Phys. Lett., 84, 4047–4049 (2004).<br />

L. Y. Gorelik, S. I. Kulinich, R. I. Shekhter, M. Jonson, V. M. Vinokur:<br />

Coulomb promotion of spin-dependent tunneling. Phys. Rev. Lett., 95,<br />

116806/1–4 (2005).<br />

T. Nakaoka, S. Kako, Y. Arakawa, S. Tarucha: Coulomb blockade in a selfassembled<br />

GaN quantum dot. Appl. Phys. Lett., 90, 162109/1–3 (2007).<br />

Bloch Oscillations<br />

J. Rotvig, A.-P. Jauho, H. Smith: Bloch oscillations, Zener tunneling, and<br />

Wannier-Stark ladders in the time domain. Phys. Rev. Lett., 74, 1831–1834<br />

(1995).<br />

A. M. Bouchard, M. Luban: Bloch oscillations and other dynamical phenomena<br />

of electrons in semiconductor superlattices. Phys. Rev. B52, 5105–5123<br />

(1995).<br />

M. M. Dignam: Excitonic Bloch oscillations in a terahertz field. Phys. Rev.<br />

B59, 5770–5783 (1999).<br />

Y. Shimada, K. Hirakawa, S. W. Lee: Time-resolved Terahertz Emission Spectroscopy<br />

of Wide Miniband GaAs/AlGaAs Superlattices, Appl. Phys. Lett.,<br />

81, 1642–1644 (2002).<br />

S. K. Lyo: Bloch oscillations and nonlinear transport in a one-dimensional<br />

semiconductor superlattice. Phys. Rev. B77, 195306/1–8 (2008).<br />

General Reading<br />

J. H. Davis: The Physics of Low Dimensional Semiconductors (Cambridge University<br />

Press, Cambridge, 1998).<br />

T. Ihn: Electronic Quantum Transport in Mesoscopic Semiconductor Structures<br />

(Springer Tracts in Modern Physics) (Springer, Berlin, Heidelberg, 2004).<br />

S. Datta: Quantum Transport: Atom to Transistor (Cambridge University Press,<br />

Cambridge, 2005).<br />

R. Tsu: Superlattice to Nanoelectronics (Elsevier Science, 2005).<br />

A. Glatz, V. I. Kozub, and V. M. Vinokur (Editors): Theory of Quantum Transport<br />

in Metallic and Hybrid Nanostructures (NATO Science Series II: Mathematics,<br />

Physics and Chemistry), (Springer, Berlin, Heidelberg, 2006).

Chapter 6<br />

Ab initio calculations of the bulk dielectric response of semiconductors<br />

Chapter 6 703<br />

In the additional references to Chap. 2 we have already mentioned the possibility<br />

of calculating fully ab initio the dielectric response (Â1 and Â2 vs. ˆ).<br />

There was already in the 3rd edition (Fig. 6.55) an example of such calculations<br />

for GaN, compared with experimental results. During the past decade<br />

this topic has received considerable attention. Some examples have been listed<br />

among the additional references to Chap. 2, such as the book: Time Dependent<br />

Density Functional Theory, ed. by M. A. L. Marques et al.. Most extant<br />

calculations, however, do not include spin-orbit interaction nor the effect of<br />

electron-phonon interaction (i.e., the dependence on temperature and on isotopic<br />

masses). Since much of the information on these two effects has been<br />

obtained from optical measurements, we have added references to pertinent<br />

recent articles in this chapter. We also take advantage of this update to include<br />

references to ab initio calculations of the second-harmonic generation<br />

at surfaces, and on the Burstein-Moss shift of the band gap with increasing<br />

doping.<br />

K. Nakamura, Y. Yoshimoto, R. Arita, S. Tsuneyuki, M. Imada: Optical Absorption<br />

Study by ab initio downfolding approach: Application to GaAs,<br />

Phys. Rev. B77, 195126/1–13 (2008).<br />

L. E. Ramos, J. Paier, G. Kresse, F. Bechstedt: Optical Spectra of Si Nanocrystallites:<br />

Bethe-Salpeter Approach Versus Time-Dependent Density Functional<br />

Theory. Phys. Rev. B78, 195423/1–9 (2008).<br />

A. Walsh, J. L. F. Da Silva, S. H. Wei: Origins of Band Gap Renormalization in<br />

Degenerate Doped Semiconductors, Phys. Rev. B78, 075211/1–5 (2008)<br />

M. Shishkin and G. Kresse: Self-Consistent GW Calculation for Semiconductors<br />

and Insulators. Phys. Rev. B75, 235102/1–9 (2007).<br />

O. Onida, L. Reining and A. Rubio: Electronic Excitations: Density-Functional<br />

vs. Many-Body Green’s-function Approaches. Rev. Mod. Phys. 74, 601–659<br />

(2002).<br />

V. Olevano and L. Reining: Excitonic Effects on the Silicon Plasmon Resonance.<br />

Phys. Rev. Lett. 86, 5962–5965 (2001).<br />

B. S. Mendoza, M.Palummo, G. Onida, R. del Sole: Ab Initio Calculation of<br />

Second Harmonic Generation at the silicon [100] surface. Phys. Rev. B63,<br />

205406/1–6 (2001).<br />

Dependence of bandgaps on Temperature and Isotopic Masses:<br />

Electron-Phonon Interaction<br />

Most calculations of Â(ˆ) available in the literature imply that they apply to<br />

T 0. This is, however not correct: even at T=0 the electron-phonon interaction,<br />

not included in the calculation, can significantly alter the corresponding<br />

electronic states. This fact has already been mention in Problem 6.19, in con-

704 <strong>Appendix</strong> D<br />

nection with Fig. 6.44. The effects of the zero –point vibrations (i.e. at T 0)<br />

can be found for many semiconductors in TABLE III of the article by Thewalt<br />

and Cardona mentioned in the additional references of Chap. 2.<br />

Note that with increasing temperature energy gaps usually (but not always:<br />

see PbS) decrease. Some additional references were already given for Chap. 2.<br />

We add a few more:<br />

R. Ramírez, C. P. Herrero: Path Integral Molecular Dynamics Simulation of<br />

Diamond. Phys. Rev. B73, 245202/1–8 (2006).<br />

H. J. Liang, A. Yang, M. L. W. Thewalt, R. Lauck and M. Cardona: Effect<br />

of Sulfur Isotopic Composition on the Band Gap of PbS. Phys. Rev. B73,<br />

233202/1–4 (2006).<br />

S. Tsoi, H. Alawadhi, X. Lu, J. W. Ager III, C. Y. Liao, H. Riemann, E. E.<br />

Haller, S. Rodríguez and A. K. Ramdas: Electron-Phonon Renormalization<br />

of the Electronic Band Gap of Semiconductors: Isotopically Enriched Silicon:<br />

Phys. Rev. B70, 193201/1–4 (2004); erratum: Phys. Rev. B72, 249905<br />

(2005).<br />

M. Cardona, T. A. Meyer, and M. L. W. Thewalt: Temperature Dependence of<br />

the Energy Gap of Semiconductors in the Low-Temperature Limit. Phys.<br />

Rev. Letters 92, 196403–196406 (2004).<br />

D. Olguín, M. Cardona and A. Cantarero: Electron-Phonon Effects on the<br />

Direct Band Gap of Semiconductors: LCAO calculation. Sol. State Comm.<br />

122, 575–589 (2002)<br />

Optical Properties of Semiconductor Mixed Crystals<br />

Mixed Crystals or alloys have been mentioned in connection with Fig. 4.8.<br />

Their energy gaps vary usually continuously from one end to the other of the<br />

composition range. They are used by technologists for bandgap engineering<br />

(see Fig. 9.2). The literature in the field has an old and distinguished history<br />

(see Chap. 9). Recent work involves ab initio calculations of the so-called<br />

“bowing” in the dependence of bandgaps on composition. A few recent references<br />

are:<br />

C. Mitra and W. R. L. Lambrecht: Band-Gap Bowing in AgGa(Se1xTex)2 and<br />

its effect on second–order response coefficients and refractive indices. Phys.<br />

Rev. B76, 205206/1–5 (2007).<br />

V. R. D’Costa, C. S. Cook, J. Menéndez, J. Tolle, J. Kouvetakis and S. Zollner:<br />

Transferability of bowing optical parameters between binary and ternary<br />

group-IV alloys. Solid State Commun. 138, 309 (2006)<br />

Z. H. Sun, W. S. Yan, H. Oyanagi, Z. Y. Pan, S. H. Wei: Local Lattice Distortion<br />

of Ge-Dilute Ge-Si alloy: Multiple-Scattering EXAFS Study. Phys. Rev.<br />

B74, 092101/1–4 (2006).

Chapter 6 705<br />

Strain-induced birefringence and intrinsic birefringence of cubic<br />

semiconductors<br />

Equation (6.158) describes the effect of an electric field on the dielectric function.<br />

A similar tensor equation can be used to describe the effect of a tensorial<br />

strain. Whereas a cubic crystal is usually assumed to be optically isotropic, a<br />

finite wavevector q breaks this isotropy (p. 246 and Refs. [6.7, 8]). This effect<br />

has recently received attention as determining the resolution of lenses used<br />

for uv lithography. In the past few years ab initio calculations of strain induced<br />

and q induced birefringence have been performed:<br />

G. Bester, X. Wu, D. Vanderbilt and A. Zunger: Importance of Second order<br />

Piezoelectric Effects in Zinc-Blende Semiconductors. Phys. Rev. Lett. 96,<br />

187602–187605 (2006)<br />

J. H. Burnett, Z. H Levine and E. L. Shirley: Photoelastic and Elastic Properties<br />

of the Fluorite Structure Materials, LiF and Si. Phys. Rev. B68,<br />

155120/1–12 (2003); erratum: Phys. Rev. B70, 239904 (2004).<br />

J. H. Burnett, Z. H. Levine and E. L. Shirley: Intrinsic Birefringence in calcium<br />

fluoride and barium fluoride. Phys. Rev. B64, 241102/1–4 (2001).<br />

Optical Response of Semiconductor Surfaces<br />

During the past decade many studies have concentrated on the optical response<br />

of surfaces. This is due to advances in ab initio computational techniques<br />

as well as development of highly sensitive experimental methods based<br />

on ellipsometry and reflectometry. The results have proven to be useful for<br />

the in situ characterization of epitaxial layers during growth.<br />

The calculations are often performed on fictitious samples obtained by repetition<br />

of thin layers so as to generate in the computer a three-dimensional<br />

crystal. Many experiments are of the reflectance difference variety, which take<br />

advantage of the fact that even on cubic crystals some surfaces (e.g. (110)) are<br />

anisotropic. Recent theoretical and experimental references are as follows:<br />

O. Pulci, O. Onida, R. del Sole and L. Reining: Ab Initio Calculation of Selfenergy<br />

Effects on Optical Properties of GaAs(110). Phys. Rev. Lett. 81,<br />

5374–5377 (1998).<br />

P. Chiaradia, and R. del Sole: Difference-Reflectance Spectroscopy and<br />

Reflectance-Anisotropy Spectroscopy on Semiconductor Surfaces. Surface<br />

Review and Letters 6, 517–528 (1999).<br />

W. G. Schmidt, F. Bechstedt, and J. Bernholc: Understanding Reflectance<br />

Anisotropy: Surface-State Signatures and Bulk Related Features. J. Vac. Sci.<br />

Technol. B18, 2215–2223 (2000).<br />

W. G. Schmidt, N. Esser, A. M. Frisch, P. Vogl, J. Bernholc, F. Bechstedt, M.<br />

Zorn, Th. Hannappel, S. Visbeck, F. Willig, and W. Richter: Understanding<br />

Reflectance Anisotropy: Surface-State Signatures and Bulk-Related Features<br />

in the Optical Spectrum of InP(001)(2×4). Phys. Rev. B61, R16335–8 (2000).

706 <strong>Appendix</strong> D<br />

J. Pollmann, P. Kruger, A. Mazur, and M. Rohlfing: Electron, Phonon and Excitons<br />

at Semiconductor Surfaces in Advances in Solid State Physics, Volume<br />

42 (Springer, Berlin, Heidelbery, 2002) 189–206.<br />

W. G. Schmidt, K. Seino, P. H. Hahn, F. Bechstedt, W. Lu, S. Wang, and J.<br />

Bernholc: Calculation of Surface Optical Properties: from Qualitative Understanding<br />

to Quantitative Predictions. Thin Solid Films, 455–456, 764–771<br />

(2004).<br />

P. Weightman, D. S. Martin, R. J. Cole, and T. Farrell: Reflection Anisotropy<br />

Spectroscopy. Rep. Prog. Phys. 68, 1251–1341 (2005).<br />

L. F. Lastras-Martínez, J. M. Flores-Camacho, A. Lastras-Martínez, R. E.<br />

Balderas-Navarro and M.Cardona: Measurement of the Surface Strain Induced<br />

by Reconstructed Surfaces of GaAs(001) using Photoreflectance and<br />

Reflectance-Difference Spectroscopies. Phys. Rev. Letters 96, 047402–047405<br />

(2006).<br />

M. Marsili, O. Pulci, F. Fuchs, F. Bechstedt, and R. del Sole: Many Body Effects<br />

in the Electronic and Optical Properties of the (111) Surface of Diamond.<br />

Surface Science 601, 4097–4101 (2007).<br />

K. F. Mak, M. Y. Sfeir, Y. Wu, C. H. Lui, J. A. Misewich, and T. F. Heinz: Measurement<br />

of the Optical Conductivity of Graphene. Phys. Rev. Lett. 101,<br />

196405–196408 (2008).<br />

Dielectric Response due to Vibrational Excitations:<br />

Born Effective Charges<br />

The first order infrared absorption related to the excitation of phonons in polar<br />

materials is discussed in Sect. 6.4. Its strength is related to the Born effective<br />

charge e ∗ shown in Eq. (6.119). This effective charge has been calculated<br />

for many semiconductors during the past 15 years using ab initio techniques.<br />

e ∗ and other polarization related properties have been described by several<br />

authors using the so-called Berry’s phase. Ab initio methods also allow the<br />

calculation of the dependence of e ∗ on strain. Although a non-zero e ∗ is characteristic<br />

of polar crystals and thus vanishes for crystalline Si, in amorphous<br />

Si deviations from the regular lattice positions induce dynamic charges and,<br />

consequently, ir absorption. Several references are listed as follows.<br />

R. Resta: Macroscopic Polarization in Crystalline Dielectrics: the Geometric<br />

Phase Approach. Rev. Mod. Physics 66, 899–915 (1994).<br />

A. Debernardi, M. Bernasconi, M. Cardona, and M. Parrinello: Infrared Absorption<br />

in Amorphous Silicon from ab initio Molecular Dynamics. Appl.<br />

Phys. Lett. 71, 2692–2694 (1997).<br />

X. Gonze and C. Y. Lee: Dynamical Matrices, Born Effective Charges, Dielectric<br />

Permittivity Tensors, and Interatomic Force Constants from Density<br />

Functional Theory. Phys. Rev. B55, 10355–10368 (1997).<br />

F. Bernardini, V. Fiorentini, and D. Vanderbilt: Accurate Calculation of Polarization<br />

Related Quantities in Semiconductors. Phys. Rev. B63, 193201/1–4<br />

(2001).

Chapter 7 707<br />

S. Baroni, S. de Gironcoli, A. dal Corso, and P Giannozzi: Phonons and Related<br />

Properties from Density-Functional Perturbation Theory. Rev. Mod.<br />

Physics 73, 515–562 (2001).<br />

G. Y. Guo, S. Ishibashi, T. Tamura, and K. Terakura: Static Dielectric Response<br />

and Born Effective Charge of BN Nanotubes from ab initio Finite Electric<br />

Field Calculations. Phys. Rev. B75, 245403/1–7 (2007).<br />

H. Y. Wang, H. Xu, N. D. Zhang, and P. H. Zhang: The Dielectric and Dynamical<br />

Properties of Zinc-blende BN, AlN, and GaN from First-principle<br />

Calculation. Science in China Series G: Physics, Mechanics, Astronomy 51,<br />

1037–1045 (2008).<br />

General Reading<br />

V. G. Plekhanov: Applications of the Isotopic Effect in Solids (Springer Series<br />

in Materials Science) (Springer, Heidelberg, 2004).<br />

Chapter 7<br />

Emission Spectroscopies<br />

During the past decade photoluminescence spectroscopies have continued to<br />

play an important role in the characterization and in basic investigations of<br />

semiconductors. Luminescence has also found an increasing role in applications<br />

such as light emitting diodes, lasers and high efficiency solid state lighting.<br />

Considerable effort has been spent in the investigation of large band gap<br />

II-VI compounds, such as ZnO, and the group III nitrides. Isotopically pure<br />

semiconductors have been used to decrease the width of emission lines and<br />

thus the resolution of emission spectroscopies. A few relevant references are<br />

listed in the following:<br />

U. Kaufman, M. Kunzer, H. Obloh, M. Maier, Ch. Manz, A. Ramakrishnan,<br />

and B. Santic: Origin of Defect-Related Photoluminescence Bands in Doped<br />

and Nominally Undoped GaN. Phys. Rev. B59, 5561–5567 (1999).<br />

F. Rossi, and T. Kuhn: Theory of Ultrafast Phenomena in Photoexcited Semiconductors.<br />

Rev. Mod. Physics 74, 895–950 (2002).<br />

Q. X. Yu, B. Xu, Q. H. Wu, Y. Liao, G. Z. Wang, R. C. Fang, H. Y. Lee, and<br />

C. T. Lee: Optical Properties of ZnO/GaN heterostructure and its nearultraviolet<br />

Light-Emitting Diodes. Appl. Phys. Lett. 83, 4713–4715 (2003).<br />

D. Pelka and K. Patel: An Overview of LED Applications for General Illumination.<br />

Proceed. of SPIE Conference on Design of Efficient Illumination<br />

Systems 5186, 15–26 (2003).<br />

J. Y. Tsao: Solid State Lighting: Lamps, Chips and Materials for Tomorrow.<br />

IEEE Circuits and Dvices Magazine, 20, 28–37 (2004).

708 <strong>Appendix</strong> D<br />

B. K. Meyer, H. Alves, D. M. Hofmann, W. Kriegseis, D. Forster, F. Bertram, J.<br />

Christen, A. Hoffmann, M. Strassburg, M. Dworzak, U. Haboeck, and A. V.<br />

Rodina: Bound Exciton and donor-acceptor Pair Recombination in ZnO.<br />

Phys. Stat. Solidi (b) 241, 231–260 (2004).<br />

M. S. Jin, C. D. Kim, and W. T. Kim: Optical Properties of GaS: Ho 3 and<br />

GaS:Tm 3 Single Crystals. J. Korean Phys. Soc. 44, 920–924 (2004).<br />

F. J. Manjón, M. Mollar, B. Marí, N. Garro, A. Cantarero, R. Lauck, and M.<br />

Cardona: Effect of Isotopic Mass on Photoluminescence Spectra of – ‚-Zinc<br />

Sulfide. Solid State Commun. 133, 253–258 (2005).<br />

A. Yang, M. Steger, K. Karaiskaj, M. L. W. Thewalt, M. Cardona, K. M. Itoh,<br />

H. Reimann, N. V. Abrosimov, M. F. Churbanov, A. V. Gusev, A. D. Bulanov,<br />

A. K. Kaliteevskii, O. N. Godisov, P. Becker, H. J. Pohl, J. W. Ager III, and<br />

E. E. Haller: Optical Detection and Ionization of Donors in Specific Electronic<br />

and Nuclear Spin States. Phys. Rev. Lett. 97, 227401/1–4 (2006).<br />

M. L. Thewalt, A. Yang, M. Steger, D. Karaiskaj, M. Cardona, H. Riemann,<br />

and N. V. Abrosimov: Direct Observation of the Donor Nuclear Spin in a<br />

Near-Gap Bound Exciton Transition: 31 P in Highly Enriched 28 Si. J. Appl.<br />

Phys. 101, 081724/1–5 (2007).<br />

A. Yang, M. Steger, H. J. Lian, M. L. W. Thewalt, M. Uemura, A. Sagara, K. M.<br />

Itoh, E. E. Haller, J. W. Ager III, S. A. Lyon, M. Konuma, and M. Cardona,<br />

High-Resolution Photoluminescence Measurement of Isotopic-Mass<br />

Dependence of the Lattice Parameter of Silicon. Phys. Rev. B77, 113203/1–4<br />

(2008).<br />

Raman Spectroscopy<br />

Some of the recently developed important Raman techniques not covered in<br />

previous editions are: inelastic x-ray scattering (using monochromatized synchrotron<br />

radiation), time-dependent reflectivity induced by coherent phonons<br />

excited by femtosecond pulses (Raman scattering in the time domain), and<br />

spatially resolved Raman scattering using enhanced near-field in the vicinity<br />

of nanometer size scanning tips (known as Tip-enhanced Raman scattering or<br />

TERS). To measure the sample topology and size in TERS the scanning tips<br />

are typically controlled by an Atomic Force Microscopes (AFM). In terms of<br />

materials, carbon nanotubes and graphene, as well as semiconductor nanostructures<br />

and microcavities, have attracted considerable attention. TERS has<br />

become a very powerful technique for studying these nanostructures. The discovery<br />

of superconductivity in B-doped diamond, silicon, and SiC has again<br />

drawn attention to the Fano interference effect in the Raman spectra induced<br />

by the interaction between optical phonons and the continuum background<br />

of hole excitations. The book series Light Scattering in Solids, mentioned in<br />

the previous edition (vols. I-VI) has been continued with three new volumes<br />

(VII-IX, see references below). Last but not the least, ab initio calculations of<br />

Raman tensors have been performed. Appropriate references are given below:

Chapter 7 709<br />

W. Windl, K. Karch, P. Pavone, O. Schütt and D. Strauch: Full ab initio Calculations<br />

of second-order Raman spectra of Semiconductors. Int. J. of Quantum<br />

Chem. 56, 787–790 (1995).<br />

L. G. Quagliano, B. Jusserand and F. R. Ladan: The use of surface enhanced<br />

Raman scattering to investigate the surface of semiconductors. Proceedings<br />

of 22nd International Conference on the Physics of Semiconductors. Edited<br />

by D. J. Lockwood (World Scientific, Singapore, 1995) Vol. 1, pp. 505–508.<br />

G. Deinzer, and D. Strauch: Raman Tensor Calculated from the 2n+1 Theorem<br />

in Density Functional Theory. Phys. Rev. B66, 100301/1–3 (2002).<br />

D. Richards, R. G. Milner, F. Huang and F. Festy: Tip-enhanced Raman microscopy:<br />

practicalities and limitations. J. Raman Spect. 34, 663–667 (2003).<br />

D. S. Bulgarevich and M. Futamata: Apertureless tip-enhanced Raman microscopy<br />

with confocal epi-illumination/collection optics. Appl. Spect. 58,<br />

757–761 (2004).<br />

S. Piscanec, F. Mauri, A. C. Ferrari, M. Lazzeri, and J. Robertson: Ab Initio<br />

Resonant Raman Spectra of Diamond-like Carbons. Diamond & Related<br />

Materials 14, 1078–1083 (2005).<br />

M. Cardona and M. L. W. Thewalt: Isotope Effects on the Optical Spectra of<br />

Semiconductors. Rev. Mod. Phys. 77, 1173–1224 (2005).<br />

C. Aku-Leh, J. Zhao, R. Merlin, J. Menéndez, and M. Cardona: Long-Lived<br />

Optical Phonons in ZnO Studied with Impulsive Stimulated Raman Scattering.<br />

Phys. Rev. B71, 205211/1–4 (2005).<br />

P. Verma, T.-A. Yano, Y. Inouye and S. Kawata: Tip-enhanced near-field Raman<br />

scattering and imaging of carbon nanostructures. Proceed. of SPIE Conference,<br />

6324, 63240K/1–9 (2006).<br />

M. Becker, V. Sivakov, G. Andra, R Geiger, J. Schreiber, S. Hoffmann, J. Michler,<br />

A. P. Milenin, P. Werner and S.H. Christiansent: The SERS and TERS<br />

effects obtained by gold droplets on top of Si nanowires. Nano Letters, 7, 6<br />

(2006).<br />

O. Pagès, A. Chafi, D. Fristot, and A. V. Postnikov: (Ga, In)P: A Standard<br />

Alloy in the Classification of Phonon Mode Behavior. Phys. Rev. B73,<br />

165206/1–10 (2006).<br />

N. Garro, A. Cros, J. M. Llorens, A. García-Cristóbal, A. Cantarero, N.<br />

Gogneau, E. Sarigiannidou, E. Monroy, and B. Daudin: Resonant Raman<br />

Scattering in Self-Assembled GaN/AlN Quantum Dots. Phys. Rev B74,<br />

075305/1–8 (2006).<br />

M. Mohr, M. Machón, J. Maultzsch, C. Thomsen: Double-Resonant Raman<br />

Processes in Germanium: Group Theory and ab initio Calculations. Phys.<br />

Rev. B73, 035217 (2006)<br />

V. N. Popov, and P. Lambin: Resonant Raman Intensity of the Totally Symmetric<br />

Phonons of Single-Walled Carbon Nanotubes. Phys. Rev. B73, 165425/1–<br />

11 (2006).<br />

K. K. Kohli, G. Davies, N. Q. Vinh, D. West, S. K. Estreicher, T. Gregorkiewicz,<br />

I. Izedin, and K. M. Itoh: Isotope Dependence of the Lifetime of the<br />

1136 cm 1 Vibration of Oxygen in Silicon. Phys. Rev. Lett. 96, 225503/1–4<br />

(2006).

710 <strong>Appendix</strong> D<br />

K. G. Lee, D. S. Kim, K. J. Yee and H. S. Lee: Control of Coherent Optical<br />

Excitations in GaN Using Femtosecond Pulse Shaping. Phys. Rev. B74,<br />

113201/1–3 (2006).<br />

J.-R. Huntzinger, A. Mlaya, V. Paillard, A. Wellner, N. Combe, and C.<br />

Bonafos: Electron-Acoustic-Phonon Interaction and Resonant Raman Scattering<br />

in Ge Quantum Dots: Matrix and Quantum Confinement Effects.<br />

Phys. Rev. B74, 115308/1–12 (2006).<br />

A. Cros, N. Garro, A. Cantarero, J. Coraux, H. Renevier, and B. Daudin: Raman<br />

Scattering as a Tool for the Evaluation of Strain in GaN/AlN Quantum<br />

Dots: The Effect of Capping. Phys. Rev. B76, 165403/1–6 (2007).<br />

S. Nakashima, T. Mitani, T. Tomita, T. Kato. S. Nishizawa, H. Okumura, and<br />

H. Harima: Observation of Surface Polarity Dependent Phonons in SiC by<br />

Deep Ultraviolet Spectroscopy. Phys. Rev. B75, 115321/1–5 (2007).<br />

M. Mohr, J. Maultzsch, E. Dobardˇzić, S. Reich, I Milosević, M. Damnjanović,<br />

A. Bosak, M. Krisch, and C. Thomsen: Phonon Dispersion of Graphite by<br />

Inelastic x-Ray Scattering. Phys. Rev. B76, 035439/1–7 (2007).<br />

Y. Ezzahri, S. Grauby, J. M. Rampnoux, H. Michel, G. Pernot, W. Claeys, S.<br />

Dilhaire, C. Rossignol, G. Zeng, and A. Shakouri: Coherent Phonons in<br />

Si/SiGe Superlattices. Phys. Rev. B75, 195309/1–12 (2007)<br />

D. Graf, F. Molitor, K. Ensslin, C. Stampfer, A. Jungen, C. Hierold, and<br />

L. Wirtz: Raman Imaging of Graphene. Solid State Commun. 143, 44–46<br />

(2007).<br />

J. W. Pomeroy, M. Kuball, C. H. Swartz, T. H. Myers, H. Lu, and W. J. Schaff:<br />

Evidence for Phonon-Plasmon Interaction in InN by Raman Spectroscopy.<br />

Phys. Rev. B75, 035205/1–6 (2007).<br />

M. F. Pascual Winter, G. Rozas, A. Fainstein, B. Jusserand, B. Perrin, A.<br />

Huynh, P. O. Vaccaro, and S. Saravanan: Selective Optical Generation of Coherent<br />

Acoustic Nanocavity Modes. Phys. Rev. Lett. 98, 265501/1–4 (2007).<br />

V. R. D’Costa, J. Tolle, C. D. Poweleit, J. Kouvetakis, and J. Menéndez: Compositional<br />

Dependence of Raman Frequencies in Ternary Ge1xySixSny Alloys.<br />

Phys. Rev. B76, 035211/1–9 (2007).<br />

R. Matsui, P. Verma, T. Ichimura, Y. Inouye and S. Kawata: Nanoanalysis<br />

of crystalline properties of GaN thin film using tip-enhanced Raman spectroscopy.<br />

Appl. Phys. Lett. 90, 61906/1–3 (2007).<br />

C. Georgi, M. Hecker and E. Zschech: Raman intensity enhancement in<br />

silicon-on-insulator substrates by laser deflection at atomic force microscopy<br />

tips and particles. Appl. Phys. Lett. 90, 171102/1–3 (2007).<br />

X. L. Wu, S. J. Jiong, Y. M. Yang, J. F. Gong, H. T. Chen, J. Zhu, J. C. Shen,<br />

and P. K, Chu: Nanocrystal-Induced Line Narrowing of Surface Acoustic<br />

Phonons in the Raman Spectra of Embedded GexSi1x Alloy Nanocrystals.<br />

Phys. Rev. B78, 165319/1–5 (2008).<br />

R. Narula, and S. Reich: Double Resonant Raman Spectra in Graphene and<br />

Graphite: A Two-Dimensional Explanation of the Raman Amplitude. Phys.<br />

Rev. B78 165422/1–6 (2008).<br />

F. Pezzoli, E. Bonera, E. Grilli, M. Guzzi, S. Sanguinetti, D. Chrastina, G.<br />

Isella, H. von Känel, E. Wintersberger, J. Stangl, and G. Bauer: Phonon

Chapter 8 711<br />

Strain Shift Coefficients in Si1xGex Alloys. J. Appl. Phys. 103, 093521/1–4<br />

(2008).<br />

General Reading<br />

M. Cardona and G. Güntherodt (Eds.), Light Scattering in Solids VII: Crystal<br />

Field and Magnetic Excitations, (Springer, Heidelberg, 2000).<br />

M. Cardona and G. Güntherodt (Eds.), Light Scattering in Solids VIII:<br />

Fullerenes, Semiconductor Surfaces, Coherent Phonons, (Springer, Heidelberg,<br />

2000).<br />

M. Cardona and R. Merlin (Eds.), Light Scattering in Solids IX: Novel Materials<br />

and Techniques, (Springer, Heidelberg, 2007).<br />

V.G. Plekhanov, Applications of the Isotopic Effect in Solids (Springer, Heidelberg,<br />

2004).<br />

Chapter 8<br />

Photoelectron spectroscopy<br />

During the past two decades the number of electron synchrotrons and storage<br />

rings dedicated exclusively to applications of synchrotron radiation has<br />

proliferated. Most of these applications involve condensed matter physics, especially<br />

semiconductors. Most developed and a few developing countries (e.g.<br />

Brazil) have either domestic synchrotrons or easy access to one in a neighboring<br />

country. Their light and x-rays emission, once monochromatized, is particularly<br />

suitable for photoelectron spectroscopy. Although Chapter 8 discusses<br />

mostly bulk photoemission spectroscopy, a few pages are already devoted to<br />

surface effects. During the past decade emphasis has shifted from bulk to surface<br />

phenomena, a field in which ab initio electronic and vibronic calculations<br />

have been very helpful. The availability of synchrotrons has also made possible<br />

the development of a bulk-type spectroscopy in which electrons are resonantly<br />

excited from a core level to a conduction band. X-rays of a lower<br />

energy are then emitted through recombination of valence electrons with the<br />

hole left behind in the core. The efficiency of this Raman-like spectroscopy<br />

(called resonant x-ray emission spectroscopy) is rather limited and so is the<br />

corresponding resolution. Nevertheless, it allows one to map out the full band<br />

structures and even obtain information about their atomic and orbital compositions.<br />

As already mention in the past editions of this book, scanning tunneling<br />

microscopies and spectroscopies are useful techniques to elucidate surface<br />

properties. Some recent references are listed below.<br />

A. M. Frisch, W. G. Schmidt, J. Bernholc, M. Privstovsek, N. Esser, W. Richter:<br />

(2×4) GaP(001) Surfaces: Atomic Structure and Optical Anisotropy. Phys.<br />

Rev. B60, 2488–2494 (1999).

712 <strong>Appendix</strong> D<br />

J. Ristein, F. Maier, M. Riedel, J. B. Cui, L. Ley: Surface Electronic Properties<br />

of Diamond. Phys. Stat. Solidi A 181, 65–76 (2000).<br />

B. Voigtländer: Fundamental Processes in Si/Si and Ge/Si Epitaxy Studied by<br />

Scanning Tunneling Microscopy during Growth. Surf. Sci. Reports 43, 127–<br />

254 (2001).<br />

I. Mahboob, T. D. Veal, L. F. J. Piper, C. F. McConville, H. Lu, W. J. Schaff, J.<br />

Furthmüller, F. Bechstedt: Origin of Electron Accumulation at wurtzite InN<br />

surfaces. Phys. Rev. B69, 201307/1–4 (2004).<br />

I. Mahboob, T. D. Veal, C. F. McConville, H. Lu, and W. J. Schaff: Intrinsic<br />

Electron Accumulation at Clean InN Surfaces. Phys. Rev. Lett. 92, 036804/1–<br />

4 (2004).<br />

P. Rinke, A. Qteish, J. Neugebauer, C. Freysoldt, M. Scheffler: Combining<br />

GW Calculations with Exact-Exchange Density-Functional Theory: an Analysis<br />

of Valence Band Photoemission for Compound Semiconductors. New J.<br />

Phys. 7, 126/1–35 (2005).<br />

J. N. Crain, F. J. Himpsel: Low Dimensional Electronic States at Silicon Surfaces.<br />

Appl. Phys. A: Mat. Science and Processing 82, 431–438 (2006).<br />

L. Weinhardt, O. Fuchs, E. Umbach, C. Heske, A. Fleszar, W. Hanke, J. D.<br />

Denlinger: Resonant Inelastic Soft x-Ray Scattering, x-Ray Absorprion<br />

Spectroscopy and Density Functional theory Calculations of the Electronic<br />

Bulk Band Structure of CdS. Phys. Rev. B75, 165207/1–8 (2007).<br />

A. R. H. Preston, B. J. Ruck, L. F. J. Piper, A. DeMasi, K. E. Smith, A. Schleife,<br />

F. Fuchs, F. Bechstedt, J. Chai, S. M. Durbin: Band Structure of ZnO from<br />

Resonant x-Ray Emission Spectroscopy. Phys. Rev. B78, 155114/1–4 (2008).<br />

Core Levels and Core Level Shifts<br />

Electron emission from core levels is usually excited with far uv or x-ray radiation.<br />

Although investigations are sometimes still performed with conventional<br />

sources, most work is done now with monochromatized synchrotron radiation.<br />

Strong monochromaticity allows the determination of the natural line widths<br />

(not broadened by spectral resolution). Sometimes these widths are so narrow<br />

that the resolution of the contributions of the first few surface layers becomes<br />

possible (especially at low temperatures). Ab initio calculations of core level<br />

energies and shifts are also being performed. A few recent references follow:<br />

H. W. Yeom, Y. C. Chao, S. Terada, S. Hara, S. Yoshida, R. I. G. Uhrberg: Surface<br />

Core Levels of the 3C SiC(001)3×2 Surface: Atomic Origins and Surface<br />

Reconstruction. Phys Rev. B56, R15525–R15528 (1997).<br />

R. I. G. Uhrberg, T. Kaurila, Y. C. Chao: Low-Temperature Photoemission<br />

Study of the Surface Electronic Structure of Si(111)7×7. Phys. Rev. 58,<br />

R1730–R1733 (1998).<br />

P. De Padova, R. Larciprete, C. Quaresima, C. Ottaviani, B. Ressel, P. Perfetti:<br />

Identification of Si 2p Surface Core Level Shifts on the Sb/Si(001)-(2×1)<br />

interface. Phys. Rev. Letters 81, 2320–2323 (1998).

Chapter 9 713<br />

Z. J. Zhao, F. Liu, L. M. Qiu, L. Z. Zhao, S. K. Yan: Core Level Binding Energy<br />

Shifts Caused by Size Effect in Nanoparticles. Acta Physico-Chimica Sinica<br />

24, 1685–1688 (2008).<br />

Graphite and Graphene<br />

Recently it has been shown that by sticking adhesive tape on a graphite surface,it<br />

is possible to peel off isolated single hexagonal layers of carbon, the socalled<br />

graphene sheets. These are ideal two-dimensional samples. Their symmetry<br />

(with two atoms per two-dimensional primitive cell), demands degeneracy<br />

at the Fermi energy at the K-points of the two-dimensional Brillouin<br />

zone. The perfect single graphene layer can be called a semi-metal or a zerogap<br />

semiconductor. This fact has received considerable attention in the past<br />

5 years. A k · p expansion of the valence and conduction bands around this<br />

point results in Dirac-like particles of zero effective mass (see Problem 2.19).<br />

The interested reader should consult the following references in addition to<br />

those in Chapt. 1&9:<br />

K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelson, I. V.<br />

Grigorieva, S. V. Dubonos, A. A. Firsov: Two-Dimensional Gas of Massless<br />

Dirac Fermions in Graphene. Nature 438, 197–200 (2005).<br />

A. K. Geim and K. S. Novoselov: The Rise of Graphene. Nature Materials. 6,<br />

183–191 (2007).<br />

Chapter 9<br />

This chapter deals with the effect of confinement of electrons and phonons in<br />

semiconductors. At the time of first publication of this book the best way of<br />

demonstrating these confinement effects was to fabricate a nanometer thick<br />

layer of semiconductor, making a so called quantum well. Since then the<br />

field of creating nanometer scale semiconductor structures has “exploded”<br />

concomitantly with world-wide interest in nano-science and -technology. New<br />

terms like nanowires, quantum wires and quantum dots have appeared. We<br />

have tried to cover some of these new developments in subsequent editions. In<br />

the present edition we try to add new references to recent work in the area of<br />

nanostructured semiconductors relevant to the topics covered in various chapters.<br />

Due to the large number of publications which have appeared we find it<br />

necessary to limit ourselves to only a small number of selected papers.<br />

Confinement of electrons and holes in Quantum Wires and Quantum Dots<br />

Al. L. Efros, A. L. Efros: Interband absorption of light in a semiconductor<br />

sphere. Sov. Phys. Semicond. 16, 772–776 (1982).<br />

K. I. Kang, B. P. McGinnis, Sandalphon, Y. Z. Hu, S. W. Koch, N. Peyghambarian,<br />

A. Mysyrowicz, L. C. Liu, S. H. Risbud: Confinement-induced valenceband<br />

mixing in CdS quantum dots observed by two-photon spectroscopy.<br />

Phys. Rev. B45, 3465–3468 (1992).

714 <strong>Appendix</strong> D<br />

D. J. Norris, A. Sacra, C. B. Murray, M. G. Bawendi: Measurement of the Size<br />

Dependent Hole Spectrum in CdSe Quantum Dots. Phys. Rev. Lett. 72,<br />

2612–2615 (1994).<br />

A. I. Ekimov: Optical properties of oxide glasses doped by semiconductor<br />

nanocrystals. Radiation Effects and Defects in Solids, 134, 11–22 (1995).<br />

D. J. Norris, and M. G. Bawendi: Measurement and assignment of the sizedependent<br />

optical spectrum in CdSe quantum dots. Phys. Rev. B53, 16338–<br />

16346 (1996).<br />

M. H. Huang, S. Mao, H. Feick, H. Q. Yan, Y. Y. Wu, H. Kind, E. Weber, R.<br />

Russo, P. D. Yang: Room-temperature ultraviolet nanowire nanolasers. Science,<br />

292, 1897–1899 (2001).<br />

P. D. Yang: From nanowire lasers to quantum wire lasers. Proceedings of<br />

the SPIE – The International Society for Optical Engineering, 5349, 18–23<br />

(2004).<br />

Phonon modes and Electron-Phonon Interaction in Quantum Wires and<br />

Quantum Dots<br />

M. C. Klein, F. Hache, D. Ricard, C. Flytzanis: Size dependence of electronphonon<br />

coupling in semiconductor nanospheres: The case of CdSe. Phys.<br />

Rev. B42, 11123–11132 (1990).<br />

S. Nomura, K. Takayoshi: Exciton–LO-phonon couplings in spherical semiconductor<br />

microcrystallites. Phys. Rev. B45, 1305–1316 (1992).<br />

T. Takagahara: Electron-phonon interactions and excitonic dephasing in semiconductor<br />

nanocrystals. Phys. Rev. Lett. 71, 3577–3580 (1993).<br />

P. A. Knipp, T. L. Reinecke: Effects of boundary conditions on confined optical<br />

phonons in semiconductor nanostructures. Phys. Rev. B48, 18037–18042<br />

(1993).<br />

M. A. Stroscio, K. W. Kim, S. G. Yu, A. Ballato: Quantized acoustic phonon<br />

modes in quantum wires and quantum dots. J. Appl. Phys. 76, 4670–4675<br />

(1994).<br />

E. Roca, C. Trallero-Giner, M. Cardona: Polar optical vibrational modes in<br />

quantum dots. Phys. Rev. B49, 13704–13711 (1994).<br />

Al. L. Efros, V. A. Kharchenko, M. Rosen: Breaking the Phonon bottleneck<br />

in nanometer Quantum Dots: Role of Auger-like Processes. Sol. State Commun.<br />

93, 281–284 (1995).<br />

G. Tamulaitis, P. A. M. Rodrigues, P. Y. Yu: Screening of Longitudinal Optical<br />

Phonons by Carriers in Quantum Dots. Sol. State Commun. 95, 227–231<br />

(1995).<br />

T. Itoh, M. Nishijima, A. I. Ekimov, C. Gourdon, Al. L. Efros, M. Rosen: Polaron<br />

and Exciton-Phonon Complexes in CuCl Nanocrystals. Phys. Rev. Lett.<br />

74, 1645–1648 (1995).<br />

W. Cheng, S. F. Ren, P. Y. Yu: A Theoretical Investigation of the Surface Vibrational<br />

Modes in Germanium Nanocrystals. Phys. Rev. B68, 193309/1–4<br />

(2003).

Chapter 9 715<br />

S. F. Ren, W. Cheng, P. Y. Yu: Microscopic investigation of phonon modes in<br />

SiGe alloy nanocrystals. Phys. Rev. B69, 235327/1–8 (2004).<br />

Properties of Confined Excitons<br />

Y. Z. Hu, S. W. Koch, M. Lindberg, N. Peyghambarian: Theoretical and Experimental<br />

Results on Coulomb Effects in Semiconductor Quantum Dots. Phys.<br />

Stat. Sol. B 159, 249–257 (1990).<br />

M. G. Bawendi, W. L. Wilson, L. Rothberg, P. J. Carroll, T. M. Jedju, M. L.<br />

Steigerwald, L. E. Brus: Electronic structure and photoexcited-carrier dynamics<br />

in nanometer-size CdSe clusters. Phys. Rev. Lett. 65, 1623–1626<br />

(1990).<br />

K. Shum, W. B. Wang, R. R. Alfano, K. M. Jones. Observation of the 1P excitonic<br />

states in Cd(S,Se)-glass quantum dots. Phys. Rev. Lett. 68, 3904–3907<br />

(1992).<br />

J.-Y. Marzin, J.-M. Gérard, A. Izraël, and D. Barrier, G. Bastard: Photoluminescence<br />

of Single InAs Quantum Dots Obtained by Self-Organized Growth<br />

on GaAs. Phys. Rev. Lett. 73, 716–719 (1994).<br />

R. Rinaldi, R. Cingolani, M. Lepore, M. Ferrara, I. M. Catalano, F. Rossi,<br />

L. Rota, E. Molinari, P. Lugli, U. Marti, D. Martin, F. Morier-Gemoud, P.<br />

Ruterana, F. K. Reinhart: Exciton Binding Energy in GaAs V-Shaped Quantum<br />

Wires. Phys. Rev. Lett. 73, 2899–2902 (1994).<br />

C. R. M. de Oliveira, A. M. de Paula, F. O. Plentz Filho, J. A. Medeiros Neto,<br />

L. C. Barbosa, O. L. Alves, E. A. Menezes, J. M. M. Rios, H. L. Fragnito,<br />

C. H. Brito Cruz, C. L. Cesar: Probing of the quantum dot size distribution<br />

in CdTe-doped glasses by photoluminescence excitation spectroscopy. Appl.<br />

Phys. Lett. 66, 439–441 (1995).<br />

P. A. M. Rodrigues, G. Tamulaitis, P. Y. Yu, S. H. Risbud: Size selective Photoluminescence<br />

Excitation Spectroscopy in CdSe Nanocrystals. Sol. State Commun.<br />

94, 583–587 (1995).<br />

M. Bayer, O. Stern, A. Kuther, A. Forchel: Spectroscopic study of dark<br />

excitons in InxGa1xAs self-assembled quantum dots by a magnetic-fieldinduced<br />

symmetry breaking. Phys. Rev. B61, 7273–7276 (2000).<br />

K. L. Teo, S. H. Kwok, P. Y. Yu, S. Guha: Quantum Confinement of the Quasi-<br />

Two-Dimensional E1 Excitons in Ge Nanocrystals Studied by Resonant Raman<br />

Scattering. Phys. Rev. B62, 1584–1587 (2000).<br />

Raman Scattering in Quantum Wires and Quantum Dots<br />

A. Tanaka, S. Onari, and T. Arai: Raman scattering from CdSe microcrystals<br />

embedded in a germanate glass matrix. Phys. Rev. B45, 6587–6592 (1992).<br />

J. J. Shiang, I. M. Craig, A. P. Alivisatos: Resonance Raman Depolarization in<br />

CdSe nanocrystals. Z. Phys. D26, 358–360 (1993).<br />

L. Saviot, B. Champagnon, E. Duval, A. I. Ekimov: Size-selective resonant Raman<br />

scattering in CdS doped glasses. Phys. Rev. B57, 341–346 (1998).

716 <strong>Appendix</strong> D<br />

L. Saviot, B. Champagnon, E. Duval, A. I. Ekimov: Resonant low-frequency<br />

Raman scattering in CdS-doped glasses. J. Crystal Growth, 184–185, 370–373<br />

(1998).<br />

S. H. Kwok, P. Y. Yu, C. H. Tung, Y. H. Zhang, M. F. Li, C. S. Peng, J. M. Zhou:<br />

Confinement and Electron-Phonon Interactions of the E1 Exciton in Selforganized<br />

Ge Quantum Dots. Phys. Rev. B59, 4980–4984 (1999).<br />

W. Cheng, S. F. Ren, P. Y. Yu: A Microscopic Theory of the Low Frequency<br />

Raman Modes in Germanium Nanocrystals Phys. Rev. B71, 174305/1–10<br />

(2005); erratum: Phys. Rev. B72, 059901 (2005).<br />

S. P. Hepplestone, G. P. Srivastava: Lattice dynamics of ultrasmall silicon<br />

nanostructures. Appl. Phys. Lett., 87, 231906/1–3 (2005).<br />

J. Frechette, C. Carraro: Diameter-dependent modulation and polarization<br />

anisotropy in Raman scattering from individual nanowires. Phys. Rev. B74,<br />

161404/1–4 (2006).<br />

Y. Q. Chen, B. Peng, B. Wang: Raman spectra and temperature-dependent Raman<br />

scattering of silicon nanowires. J. Phys. Chem. C, 111, 5855–5858 (2007).<br />

M. J. Konstantinovic: Interplay between phonon confinement effect and anharmonicity<br />

in silicon nanowires. Physica E, 38, 109–111 (2007).<br />

Qi. J. Lu, K. W. Adu, H. R. Gutierrez, G. G. Chen, K.-K. Lew, P. Nimmatoori,<br />

X. Zhang, E. C. Dickey, J. M. Redwing, P. C. Eklund: Raman scattering from<br />

Si1xGex alloy nanowires. J. Phys. Chem. C, 112, 3209–15 (2008).<br />

Resonant Tunneling in Low Dimensional Devices<br />

S. Krishnamurthy, A.-B. Chen, A. Sher: I-V characteristics of resonant tunneling<br />

devices: Difference equation method. J. Appl. Phys. 84, 5037–5045<br />

(1998).<br />

A. G. Petukhov, D. O. Demchenko, A. N. Chantis: Electron spin polarization in<br />

resonant interband tunneling devices. Phys. Rev. B68, 125332/1–5 (2003).<br />

K. S. Chan: Rate enhancement in phonon-assisted resonant tunneling in quantum<br />

dots. J. Appl. Phys. 97, 16104/1–3 (2005).<br />

O. A. Tretiakov, K. A. Matveev: Decay of metastable current states in onedimensional<br />

resonant tunneling devices. Phys. Rev. B73, 115302/1–11 (2006).<br />

Quantum Transport in Carbon Nanotubes and Graphene<br />

D. H. Cobden, M. Bockrath, N. G. Chopra, A. Zettl, P. L. McEuen, A. Rinzler,<br />

A. Thess, R. E. Smalley: Transport spectroscopy of single-walled carbon<br />

nanotubes. Physica B 249–251, 132–135 (1998).<br />

J. Park, P. L. McEuen: Formation of a p-type quantum dot at the end of an<br />

n-type carbon nanotube. Appl. Phys. Lett. 79, 1363–1365 (2001).<br />

M. T. Woodside, P. L. McEuen: Scanned probe imaging of single-electron<br />

charge states in nanotube quantum dots. Science 296, 1098–1101 (2002).<br />

C. L. Kane, E. J. Mele: Quantum spin Hall effect in graphene. Phys. Rev. Lett.,<br />

95, 226801/1–4 (2005).

Chapter 9 717<br />

V. P. Gusynin, S. G. Sharapov: Unconventional integer quantum Hall effect in<br />

graphene. Phys. Rev. Lett., 95, 146801/1–4 (2005).<br />

Y. Zhang, Y. W. Tan, H. L. Stormer, P. Kim: Experimental observation of the<br />

quantum Hall effect and Berry’s phase in graphene. Nature, 438, 201–204<br />

(2005).<br />

Y. Zhang, Z. Jiang, J. P. Small, M. S. Purewal, Y.-W. Tan, M. Fazlollahi, J. D.<br />

Chudow, J. A. Jaszczak, H. L. Stormer, P. Kim: Landau-level splitting in<br />

graphene in high magnetic fields. Phys. Rev. Lett., 96, 136806/1–4 (2006).<br />

S. Y. Zhou, G.-H. Gweon, J. Graf, A. V. Federov, C. D. Spataru, R. D. Diehl,<br />

Y. Kopelevich, D.-H. Lee, S. G. Louie, A.Lanzara: First direct observation of<br />

Dirac fermions in graphite. Nature Physics, 2, 595–599 (2006).<br />

A. J. M. Giesbers, U. Zeitler, M. I. Katsnelson, L. A. Ponomarenko, T. M. G.<br />

Mohiuddin, J. C. Maan: Temperature dependence of the quantum Hall effect<br />

in graphene. Physica E, 40, 1089–1091 (2008).<br />

General Reading<br />

Barenham K., D. Vvedensky (ed): Low-Dimensional Semiconductor Structures<br />

(Cambridge University Press, 2001).<br />

Davies J. H.: The Physics of Low-Dimensional Semiconductors (Cambridge<br />

University Press, 1998).<br />

Yoffe A. D.: Semiconductor Quantum Dots And Related Systems: Electronic,<br />

Optical, Luminescence And Related Properties Of Low Dimensional Systems.<br />

Adv. Phys. 50, 1- 208 (2001).<br />

M. Di Ventra, S. Evoy, J. R. Heflin Jr., (Eds.): Introduction to Nanoscale<br />

Science and Technology Series: Nanostructure Science and Technology.<br />

(Springer, Heidelberg, 2004).<br />

R. Tsu: Superlattice to Nanoelectronics (Elsevier Science, 2005).

References 1<br />

Chapter 1<br />

1.1 J. I. Pankove, T. D. Moustakas (eds.): Gallium Nitride I, Semiconductors and<br />

Semimetals, Vol. 50 (Academic Press, San Diego 1998)<br />

S. Nakamura, G. Fasol: The Blue Laser Diode. GaN Based Light Emitters and<br />

Lasers (Springer, Berlin, Heidelberg 1997)<br />

1.2 L. Gao, Y. Y. Xue, F. Chen, Q. Xiong, R. L. Meng, D. Ramirez, C. W. Chu, J. H.<br />

Eggert, H. K. Mao: Superconductuvity up to 164 in HgBa2Ca m1CumO 2m2‰<br />

(m 1, 2, 3), under pressure. Phys. Rev. B50, 4260–4263 (1994)<br />

1.3 R. Saito, G. Dresselhaus and M. S. Dresselhaus: Physical Properties of Carbon<br />

Nanotubes (Imperial College Press, London 1998)<br />

1.4 J. Shinan, Z. Vardeny and Z. Kapati (ed.): Optical and Electronic Properties of<br />

Fullerenes and Fullerene-Band Materials (Marcel Dekker, New York, 1999)<br />

1.5 C. N. R. Rao and B. Raveau (ed.): Colossal Magnetoresistance, Charge Ordering<br />

and Related Properties of Manganese Oxides (World Scientific, Singapore,<br />

1998)<br />

1.6 T. Ruf, R. W. Henn, M. Asen-Palmer, E. Gmelin, M. Cardona, H.-J. Pohl, G. G.<br />

Devyatych, P.G. Sennikov: Thermal conductivity of isotopically enriched silicon.<br />

Solid State Commun. 115, 243 (2000)<br />

1.7 J. Czochralski: A new method for measuring the crystallization velocity of metals<br />

(in German). Z. Phys. Chem. 92, 219–221 (1918)<br />

1.8 O. Madelung, M. Schulz, H. Weiss (eds.): Landolt-Börnstein, Series III, Vol. 17c<br />

(Semiconductors) (Springer, Berlin, Heidelberg 1984) p. 29. This series contains<br />

comprehensive references on the growth techniques and properties of individual<br />

semiconductors up to 1984<br />

1.9 W. C. Dash: Growth of silicon crystals free of dislocations. J. Appl. Phys. 30,<br />

459 (1959)<br />

1.10 C. T. Foxon, B. A. Joyce: Growth of thin films and heterostructures of III–V compounds<br />

by molecular beam epitaxy, in Growth and Characterization of Semiconductors<br />

ed. by R. A. Stradling, P. C. Klipstein (Hilger, Bristol 1990) p. 35<br />

1.11 S. Nakamura and G. Fasol: The Blue Laser Diode: GaN Based Light Emitters<br />

and Lasers (Springer-Verlag, Berlin, 1997) p. 36–37<br />

1.12 I. N. Stranski and L. Krastanow: Sitzungsberichte d. Akad. d. Wissenschaften<br />

in Wien, Abt. 11B, Band 146, 797 (1937)<br />

1.13 D. W. Pashley: The Basics of Epitaxy, in Growth and Characterization of Semiconductors<br />

ed. by R. A. Stradling, P. C. Klipstein (Hilger, Bristol 1990) p. 1<br />

1.14 F. C. Frank and J. H. van der Merwe: One-dimensional dislocations I. Static<br />

theory, Proc. Royal Society A198, 205–216 (1949); One-dimensional disloca-<br />

1 In case several references are listed under one number, it is tacitly assumed that the<br />

first reference is a, the second one b, etc. The reference numbers highlighted in red correspond<br />

to proceedings of International Conferences on the Physics of Semiconductors<br />

(ICPS). See Preface to the Second Edition.

720 References<br />

tions II. Misfitting monolayers and oriented overgrowth, Proc. Royal Society<br />

A198, 216–225 (1949); One-dimensional dislocations III. Influence of the second<br />

harmonic term in the potential representation on the properties of the<br />

model, Proc. Royal Society A200, 125–134 (1949)<br />

1.15 See, for example, D. Bimberg, M. Grundmann, and N. N. Lebentsov: Growth,<br />

Spectroscopy, and Laser Application of Self-ordered III-V Quantum Dots.<br />

Bulletin of the Materials Research Society, 23, 31 (1998)<br />

1.16 J. Bohm, A. Lüdge, W. Schröder: Crystal Growth by Floating Zone Melting,<br />

in Handbook of Crystal Growth, Vol. 2 ed. by D. T. H. Hurle (North-Holland,<br />

Amsterdam, 1994) p. 213–258<br />

General Reading<br />

Bernard, J.C., M. Sugawara (ed.): Self-Assembled in GaAs/GaAs Quantum Dots. Volume<br />

60 of Semiconductors and Semimetals (Academic Press, New York, 1999)<br />

Bimberg, D., M. Grundmann and N. Ledentsov: Quantum Dot Heterostructures<br />

(John Wiley & Son, New York, 1999)<br />

Chernov A. A.: Modern Crystallography III – Crystal Growth, Springer Ser. Solid-<br />

State Sci., Vol. 36 (Springer, Berlin, Heidelberg 1984)<br />

Gilman J. J. (ed.): The Art and Science of Growing Crystals (Wiley, New York 1963)<br />

Hermann M. A., H. Sitter: Molecular Beam Epitaxy, 2nd edn., Springer Ser. Mater.<br />

Sci., Vol. 7 (Springer, Berlin, Heidelberg 1996)<br />

Kittel C.: Introduction to Solid State Physics, 7th edn. (Wiley, New York 1995)<br />

Laudies R. A.: The Growth of Single Crystals (Prentice-Hall, New York 1970)<br />

Matthews J. W. (ed.): Epitaxial Growth, Pts. a & b (Academic, New York 1975)<br />

Panish M. B., H. Temkin: Gas Source Molecular Beam Epitaxy, Springer Ser. Mater.<br />

Sci., Vol. 26 (Springer, Berlin, Heidelberg 1993)<br />

Williams, J. O.: Metal Organic Chemical Vapour Deposition (MOCVD) for the preparation<br />

of semiconductor materials and devices, in Growth and Characterization of<br />

Semiconductors, ed. by R. A. Stradling, P. C. Klipstein (Hilger, Bristol 1990) p. 17<br />

Chapter 2<br />

2.1 Quantum Theory of Real Materials (eds. Chelikowsky, J.R., Louie, S.G.)<br />

(Kluwer, Dordrecht, 1996)<br />

2.2 C. Kittel: Introduction to Solid State Physics, 7th edn. (Wiley, New York 1995)<br />

p. 37<br />

2.3 L. M. Falicov: Group Theory and its Physical Applications (Univ. Chicago<br />

Press, Chicago 1966)<br />

2.4 G. F. Koster: Space groups and their representations, in Solid State Physics 5,<br />

173–256 (Academic, New York 1957)<br />

2.5 G. Lucovsky, A comparison of the long wavelength optical phonons in trigonal<br />

Se and Te, Phys. Stat. Sol. (b) 49, 633 (1972)<br />

2.6 D. M. Greenaway, G. Harbeke: Optical Properties and Band Structure of Semiconductors<br />

(Pergamon, New York 1968) p. 44<br />

2.7 H. Jones: The Theory of Brillouin Zones and Electronic States in Crystals, 2nd<br />

edn. (North-Holland, Amsterdam 1975)<br />

2.8 M. L. Cohen, J. Chelikowsky: Electronic Structure and Optical Properties of<br />

Semiconductors, 2nd edn., Springer Ser. Solid-State Sci., Vol. 75 (Springer,<br />

Berlin, Heidelberg 1989)

References 721<br />

2.9 J. R. Chelikowsky, D. J. Chadi, M. L. Cohen: Calculated valence band densities<br />

of states and photoemission spectra of diamond and zinc-blende semiconductors.<br />

Phys. Rev. B 8, 2786–2794 (1973)<br />

2.10 C. Varea de Alvarez, J. P. Walter, R. W. Boyd, M. L. Cohen: Calculated band<br />

structures, optical constants and electronic charge densities for InAs and InSb.<br />

J. Chem. Phys. Solids 34, 337–345 (1973)<br />

2.11 P. Hohenberg, W. Kohn: Inhomogeneous electron gas. Phys. Rev. B 863, 136<br />

(1964)<br />

2.12 W. Kohn, L. Sham: Self-consistent equations including exchange and correlation<br />

effects. Phys. Rev. A 113, 140 (1965)<br />

2.13 M. S. Hybertsen, S. G. Louie: Electron correlation in semiconductors and insulators.<br />

Phys. Rev. B 34, 5390–5413 (1986)<br />

2.14 N. Trouillier, J. L. Martins: Efficient pseudopotentials for plane wave calculations.<br />

Phys. Rev. B 43, 1993–2006 (1991)<br />

2.15 E. O. Kane: Band structure of indium antimonide. J. Phys. Chem. Solids 1,<br />

249–261 (1957)<br />

2.16 M. Cardona, F. H. Pollak: Energy-band structure of germanium and silicon.<br />

Phys. Rev. 142, 530–543 (1966); see also Vol. 41B<br />

2.17 M. Cardona: Band parameters of semiconductors with zincblende, wurtzite,<br />

and germanium structure. J. Phys. Chem. Solids 24, 1543–1555 (1963); erratum:<br />

ibid. 26, 1351E (1965)<br />

2.18 O. Madelung, M. Schulz, H. Weiss (eds.): Landolt-Börnstein, Series III,<br />

Vol. 17a–h (Semiconductors) (Springer, Berlin, Heidelberg 1987)<br />

2.19 E. O. Kane: The k · p method. Semiconductors and Semimetals 1, 75–100 (Academic,<br />

New York 1966)<br />

2.20 M. Cardona, N. E. Christensen, G. Fasol: Relativistic band structure and<br />

spin-orbit splitting of zincblende-type semiconductors. Phys. Rev. B 38,<br />

1806–1827 (1988)<br />

2.21 G. Dresselhaus, A. F. Kip, C. Kittel: Cyclotron resonance of electrons and holes<br />

in silicon and germanium crystals. Phys. Rev. 98, 368–384 (1955)<br />

2.22 M. Willatzen, M. Cardona, N. E. Christensen: LMTO and k·p calculation of effective<br />

masses and band structure of semiconducting diamond. Phys. Rev. B50,<br />

18054 (1994)<br />

2.23 J. M. Luttinger: Quantum theory of cyclotron resonance in semiconductors:<br />

General theory. Phys. Rev. 102, 1030–1041 (1956)<br />

2.24 W. A. Harrison: Electronic Structure and the Properties of Solids: The Physics<br />

of the Chemical Bond (Dover, New York 1989)<br />

2.25 D. J. Chadi, M. L. Cohen: Tight-binding calculations of the valence bands of diamond<br />

and zincblende crystals. Phys. Stat. Solidi B 68, 405–419 (1975)<br />

2.26 W. A. Harrison: The physics of solid state chemistry, in Festkörperprobleme 17,<br />

135–155 (Vieweg, Braunschweig, FRG 1977)<br />

2.27 F. Herman: Recent progress in energy band theory, in Proc. Int’l Conf. on<br />

Physics of Semiconductors (Dunod, Paris 1964) pp. 3–22<br />

2.28 T. Dietl, W. Dobrowolski, J. Kosut, B. J. Kowalski, W. Szuskiewicz, Z. Wilamoski,<br />

A. M. Witowski: HgSe: Metal or Semiconductor? Phys. Rev. Lett. 81,<br />

1535 (1998);<br />

D. Eich, D. Hübner, R. Fink, E. Umbach, K. Ortner, C. R. Becker, G. Landwehr,<br />

A. Flezsar: Electronic structure of HgSe investigated by direct and inverse<br />

photoemission. Phys. Rev. B61, 12666–12669 (2000)<br />

2.29 T. N. Morgan: Symmetry of electron states in GaP. Phys. Rev. Lett. 21, 819–823<br />

(1968)

722 References<br />

2.30 R. M. Wentzcovitch, M. Cardona, M. L. Cohen, N. E. Christensen: X 1 and X3<br />

states of electrons and phonons in zincblende-type semiconductors. Solid State<br />

Commun. 67, 927–930 (1988)<br />

2.31 S. H. Wei, A. Zunger: Band gaps and spin-orbit splitting of ordered and disordered<br />

AlxGa 1xAs and GaAsxSb 1x alloys. Phys. Rev. B 39, 3279–3304 (1989)<br />

General Reading<br />

Group Theory and Applications<br />

Burns G.: Introduction to Group Theory and Applications (Academic, New York<br />

1977)<br />

Evarestov R. A., V. P. Smirnov: Site Symmetry in Crystals, Springer Ser. Solid-State<br />

Sci., Vol. 108 (Springer, Berlin, Heidelberg 1993)<br />

Falicov L. M.: Group Theory and Its Physical Applications (Univ. Chicago Press,<br />

Chicago 1966)<br />

Heine V.: Group Theory in Quantum Mechanics (Pergamon, New York 1960)<br />

Inui T., Y. Tanabe, Y. Onodera: Group Theory and Its Applications in Physics, 2nd<br />

edn. Springer Ser. Solid-State Sci., Vol. 78 (Springer, Berlin, Heidelberg 1996)<br />

Jones H.: Groups, Representations, and Physics (Hilger, Bristol 1990)<br />

Koster G. F.: Space groups and their representations. Solid State Physics 5, 173–256<br />

(Academic, New York 1957)<br />

Lax M.: Symmetry Principles in Solid State and Molecular Physics (Wiley, New York<br />

1974)<br />

Ludwig W., C. Falter: Symmetries in Physics, 2nd edn., Springer Ser. Solid-State Sci.,<br />

Vol. 64 (Springer, Berlin, Heidelberg 1996)<br />

Tinkham M.: Group Theory and Quantum Mechanics (McGraw-Hill, New York<br />

1964)<br />

Vainshtein B. K.: Fundamentals of Crystals, 2nd edn., Modern Crystallography, Vol. 1<br />

(Springer, Berlin, Heidelberg 1994)<br />

Electronic Band Structures<br />

Cohen M. L., Chelikowsky, J.: Electronic Structure and Optical Properties of Semiconductors,<br />

2nd edn., Springer Ser. Solid-State Sci., Vol. 75 (Springer, Berlin, Heidelberg<br />

1989)<br />

Greenaway D. L., Harbeke, G.: Optical Properties and Band Structure of Semiconductors<br />

(Pergamon, New York 1968)<br />

Harrison W. A.: Electronic Structure and the Properties of Solids: The Physics of the<br />

Chemical Bond (Dover, New York 1989)<br />

Jones H.: The Theory of Brillouin Zones and Electronic States in Crystals (North-<br />

Holland, Amsterdam 1962)<br />

Phillips J. C.: Covalent Bonding in Crystals, Molecules, and Polymers (Univ. Chicago<br />

Press, Chicago 1969)<br />

Chapter 3<br />

3.1 D. N. Talwar, M. Vandevyver, K. Kunc, M. Zigone: Lattice dynamics of zinc<br />

chalcogenides under compression: Phonon dispersion, mode Grüneisen, and<br />

thermal expansion. Phys. Rev. B 24, 741–753 (1981)

References 723<br />

A. Debernardi, M. Cardona: Isotope effects on the lattice constant by perturbation<br />

theory: an ab initio calculation, Phys. Rev. B 54, 11305–11310 (1996)<br />

3.2 H. Goldstein: Classical Mechanics (Addison-Wesley, Reading 1950) p. 329<br />

3.3 A. Debernardi: Phonon Linewidth in III–V semiconductors from density functional<br />

perturbation theory. Phys. Rev. B 57, 12847–12858 (1998)<br />

3.4 G. Nilsson, G. Nelin: Study of the homology between silicon and germanium<br />

by thermal-neutron spectroscopy. Phys. Rev. B 6, 3777–3786 (1972)<br />

3.5 W. Weber: Adiabatic bond charge model for the phonons in diamond, Si, Ge,<br />

and ·-Sn. Phys. Rev. B 15, 4789–4803 (1977)<br />

3.6 D. Strauch, B. Dorner: Phonon dispersion in GaAs. J. Phys.: Condens. Matter<br />

2, 1457–1474 (1990)<br />

3.7 T. Ruf, J. Serrano, M. Cardona, P. Pavone, M. Pabst, M. Krisch, M. D’Astuto,<br />

T. Suski, I. Grzegory and M. Leszczynski: Phonon Dispersion curves in<br />

wurtzite-structure GaN determined by inelastic x-ray scattering. Phys. Rev.<br />

Lett. 86, 906–909 (2001)<br />

3.8 R. Zallen, R. M. Martin, V. Natoli: Infrared Activity in Elemental Crystals.<br />

Phys. Rev. B49, 7032 (1994)<br />

3.9 M. Born, K. Huang: Dynamical Theory of Crystal Lattices (Oxford Univ. Press,<br />

Oxford 1988, reprint of the original 1954 edition)<br />

3.10 M. Born: The space lattice theory of diamond. Ann. Physik 44, 605–642 (1914)<br />

in German<br />

3.11 Y. C. Hsieh: The vibrational spectrum and the specific heat of germanium and<br />

silicon. J. Chem. Phys. 22, 306–311 (1954)<br />

3.12 F. Herman: Lattice vibrational spectrum of germanium. J. Phys. Chem. Solids<br />

8, 405–418 (1959)<br />

3.13 W. Cochran: Theory of the lattice vibrations of germanium. Proc. R. Soc. (London)<br />

Ser.A 253, 260–276 (1959)<br />

3.14 G. Dolling, R. A. Cowley: The thermodynamics and optical properties of germanium,<br />

silicon, diamond, and gallium arsenide, Proc. Phys. Soc. 88, 463–494<br />

(1966)<br />

3.15 J. C. Phillips: Covalent bonds in crystals. I. Elements of a structural theory.<br />

Phys. Rev. 166, 832–838 (1968); II. Partially ionic bonding. ibid. 168, 905–911<br />

(1968)<br />

3.16 M. J. P. Musgrave, J. A. Pople: A general valence force field for diamond. Proc.<br />

R. Soc. (London) Ser.A 268, 474–484 (1962)<br />

3.17 M. A. Nusimovici, J. L. Birman: Lattice dynamics of Wurtzite: CdS. Phys. Rev.<br />

156, 925–938 (1967)<br />

3.18 A. Debernardi, N. M. Pyka, A. Göbel, T. Ruf, R. Lauck, S. Kramp, M. Cardona:<br />

Lattice Dynamics of Wurtzite CdS, Solid State Commun. 103, 297–301 (1997)<br />

3.19 J. M. Rowe, R. M. Nicklow, D. L. Price, K. Zanio: Lattice dynamics of cadmium<br />

telluride. Phys. Rev. B 10, 671–675 (1974)<br />

3.20 F. Widulle, S. Kramp, N. M. Pyka, A. Göbel, T. Ruf, A. Debernardi, R. Lauck,<br />

M. Cardona: The phonon dispersion of wurtzite CdSe. Physica B263–264, 448–<br />

451 (1999)<br />

3.21 G. Lang, K. Karch, M. Schmitt, P. Pavone, A. P. Mayer, R. K. Wehner, D.<br />

Strauch: Anharmonic lineshift and linewidth of the Raman mode in Ge and<br />

Si. Phys. Rev. B59, 6182 (1999);<br />

S. Shobhana, D. Vanderbilt: Anharmonic self-energies of phonons in silicon.<br />

Phys. Rev. B43, 4541 (1991)<br />

3.22 P. N. Keating: Effect of invariance requirements on the elastic strain energy of<br />

crystals with application to the diamond structure. Phys. Rev. 145, 637–645 (1966)

724 References<br />

3.23 R. M. Martin: Elastic properties of ZnS structure semiconductors. Phys. Rev.<br />

B 1, 4005–4011 (1970)<br />

R. M. Martin: Dielectric screening model for lattice vibrations of diamondstructure<br />

crystals. Phys. Rev. 186, 871 (1969)<br />

3.24 J. Noolandi: Theory of crystal distortions in A II B IV C2 V and A 1 B III C2 VI chalcopyrite<br />

semiconductors. Phys. Rev. B 10, 2490–2494 (1974)<br />

3.25 S. Göttlicher, E. Wolfel: X-ray determination of the electron distribution in<br />

crystals (in German). Z. Elektrochem. 63, 891–901 (1959)<br />

3.26 L. W. Yang, P. Coppens: On the experimental electron distribution in silicon.<br />

Solid State Commun. 15, 1555–1559 (1974)<br />

3.27 J. Chelikowsky, M. L. Cohen: Nonlocal pseudopotential calculations for the<br />

electronic structure of eleven diamond and zincblende semiconductors. Phys.<br />

Rev. B 14, 556-582 (1976)<br />

3.28 P. Pavone, K. Karch, O. Schütt, W. Windl, D. Strauch, P. Gianozzi, S. Baroni:<br />

Ab initio lattice dynamics of diamond. Phys. Rev. B 48, 3156–3163 (1993)<br />

M. Schwoerer-Bohning, A. T. Macrauder, D. A. Arms: Phonon Dispersion<br />

in Diamond measured by inelastic X-ray scattering. Phys. Rev. Lett. 80,<br />

5572–5575 (1998)<br />

3.29 G. P. Srivastava: The Physics of Phonons (Hilger, Bristol 1990)<br />

3.30 A. Blacha, H. Presting, M. Cardona: Deformation potentials of k=0 states of<br />

tetrahedral semiconductors. Phys. Stat. Solidi b 126, 11–36 (1984)<br />

3.31 D. D. Nolte, W. Walukiewicz, E. E. Haller: Critical criterion for axial modes of<br />

defects in as-grown n-type GaAs. Phys. Rev. B 36, 9374–9377 (1987)<br />

3.32 M. Cardona, N. E. Christensen: Acoustic deformation potentials and heterostructure<br />

band offsets in semiconductors. Phys. Rev. B 35, 6182–6194 (1987)<br />

3.33 E. O. Kane: Strain effects on optical critical-point structure in diamond-type<br />

crystals. Phys. Rev. 178, 1368–1398 (1969)<br />

3.34 G. E. Pikus, G. L. Bir: Effect of deformation on the hole energy spectrum of<br />

germanium and silicon. Sov. Phys. – Solid State 1, 1502–1517 (1960)<br />

3.35 G. E. Pikus, G. L. Bir: Symmetry and Strain Induced Effects in Semiconductors<br />

(Wiley, New York 1974)<br />

3.36 E. L. Ivchenko and G. E. Pikus: Superlattices and other Heterostructures,<br />

(Springer, Heidelberg, 1997), p. 71<br />

3.37 C. Herring, E. Vogt: Transport and deformation-potential theory for manyvalley<br />

semiconductors with anisotropic scattering. Phys. Rev. 101, 944–961<br />

(1956)<br />

3.38 H. Brooks: Theory of the electrical properties of germanium and silicon. Advances<br />

in Electronics and Electron Physics 7, 85–182 (Academic, New York<br />

1955)<br />

3.39 J. F. Nye: Physical Properties of Crystals (Oxford Univ. Press, Oxford 1969)<br />

3.40 G. D. Mahan, J. J. Hopfield: Piezoelectric polaron effects in CdS. Phys. Rev.<br />

Lett. 12, 241–243 (1964)<br />

3.41 K. Hübner: Piezoelectricity in zincblende- and wurtzite-type crystals. Phys.<br />

Stat. Solidi B 57, 627–634 (1973)<br />

3.42 W. A. Harrison: Electronic Structure and the Properties of Solids: The Physics<br />

of the Chemical Bond (Dover, New York 1989) p. 224<br />

3.43 O. Madelung, M. Schulz, H. Weiss (eds.): Landolt-Börnstein, Series III, Vol. 22<br />

(Semiconductors), Subvolume a. Intrinsic Properties of Group IV Elements,<br />

III-V, II-VI and I-VII Compounds (Springer, Berlin, Heidelberg 1987)<br />

3.44 S. Adachi: GaAs, AlAs, and AlxGa 1xAs: Materials parameters for use in research<br />

and device applications. J. Appl. Phys. 58, R1–29 (1985)

References 725<br />

3.45 L. Kleinmann: Deformation potentials in Si: I. Uniaxial strain. Phys. Rev. 128,<br />

2614–2621 (1962)<br />

3.46 E. Anastassakis, M. Cardona: Internal strains and Raman-active optical<br />

phonons. Phys. Stat. Solidi B 104, 589–600 (1981)<br />

3.47 W. Plötz, P. Vogl: Theory of optical-phonon deformation potentials in tetrahedral<br />

semiconductors. Phys. Rev. B 24, 2025–2037 (1981)<br />

3.48 M. Cardona, M. Grimsditch, D. Olego: Theoretical and experimental determinations<br />

of Raman scattering cross sections in simple solids, in Light Scattering<br />

in Solids, ed. by J. L. Birman, H. Z. Cummins, K. K. Rebane (Plenum, New<br />

York 1979) pp. 249–256<br />

3.49 S. Zollner, S. Gopalan, M. Cardona: Intervalley deformation potentials and scattering<br />

rates in zincblende semiconductors. Appl. Phys. Lett. 54, 614–616 (1989)<br />

3.50 C. Carabatos, B. Prevot: Rigid ion model lattice dynamics of cuprite (Cu2O).<br />

Phys. Status Solid B 44, 701–712 (1971)<br />

3.51 P. Molinàs-Mata, M. Cardona: Planar force-constant models and internal strain<br />

parameter of Ge and Si. Phys. Rev. B 43, 9799–9809 (1991)<br />

3.52 P. Molinàs-Mata, A. J. Shields, M. Cardona: Phonons and internal stresses in<br />

IV-VI and III-V semiconductors: The planar bond-charge model. Phys. Rev.<br />

B 47, 1866–1875 (1993)<br />

3.53 C. H. Xu, C. Z. Wang, C. T. Chan, K. M. Ho: Theory of the thermal expansion<br />

of Si and Diamond. Phys. Rev. B43, 5024–5027 (1991)<br />

3.54 A. Debernardi and M. Cardona: Isotopic effects on the lattice constant in compound<br />

semiconductors by perturbation theory: an ab initio calculation. Phys.<br />

Rev. B54, 11305–11310 (1996)<br />

General Reading<br />

Lattice Dynamics<br />

Bilz, H., W. Kress: Phonon Dispersion Relations in Insulators, Springer Ser. Solid-<br />

State Sci., Vol. 10 (Springer, Berlin, Heidelberg 1979). This is touted as a “phonon<br />

atlas” by its authors. It presents a collection of phonon dispersion curves and densities<br />

of states for more than a hundred insulators, including all the well-known<br />

semiconductors.<br />

Born, M., K. Huang: Dynamical Theory of Crystal Lattices (Oxford Univ. Press,<br />

Oxford 1988), reprint of the original 1954 edition<br />

Horton G. K., Maradudin, A. A. (eds.): Dynamical Properties of Solids, Vols. 1–5<br />

(North-Holland, Amsterdam 1974)<br />

Sinha S. K.: Phonons in semiconductors. CRC Critical Reviews in Solid State Sciences<br />

3, 273–334 (1973)<br />

Srivastava G. P.: The Physics of Phonons (Hilger, Bristol 1990)<br />

Properties Related to Phonons<br />

Harrison W. A.: Electronic Structure and the Properties of Solids: The Physical of the<br />

Chemical Bond (Dover, New York, 1989)<br />

Kittel C.: Introduction to Solid State Physics, 7th edn. (Wiley, New York 1995) Chap. 4<br />

Madelung O.: Introduction to Solid-State Theory, Springer Ser. Solid-State Sci., Vol. 2<br />

(Springer, Berlin, Heidelberg 1978)<br />

Madelung O., Schulz, M.,